Author
others
View
3
Download
0
Embed Size (px)
Copyright Warning amp Restrictions
The copyright law of the United States (Title 17 United States Code) governs the making of photocopies or other
reproductions of copyrighted material
Under certain conditions specified in the law libraries and archives are authorized to furnish a photocopy or other
reproduction One of these specified conditions is that the photocopy or reproduction is not to be ldquoused for any
purpose other than private study scholarship or researchrdquo If a user makes a request for or later uses a photocopy or reproduction for purposes in excess of ldquofair userdquo that user
may be liable for copyright infringement
This institution reserves the right to refuse to accept a copying order if in its judgment fulfillment of the order
would involve violation of copyright law
Please Note The author retains the copyright while the New Jersey Institute of Technology reserves the right to
distribute this thesis or dissertation
Printing note If you do not wish to print this page then select ldquoPages from first page to last page rdquo on the print dialog screen
The Van Houten library has removed some of the personal information and all signatures from the approval page and biographical sketches of theses and dissertations in order to protect the identity of NJIT graduates and faculty
ABSTRACT
ANALYSIS OF TRANSPORT PROPERTIES OF A ZAZ GRAPHENE
NANORIBBON JUNCTION USING VARIOUS DOPANTS
by
Natasha Parikh
A 12 atom wide ZAZ Graphene Junction was simulated and its transport properties were
analyzed I-V curves calculated by nonequilibrium Greens function method combined
with the density functional theory under external bias showed varying semiconducting
characteristics Further the width of the junction also showed significant effects in the
determination of the semiconducting nature A theoretical study was performed on the
semiconducting characteristics by analyzing the I-V curve and transport coefficients in
the junction
ANALYSIS OF TRANSPORT PROPERTIES IN A ZAZ GRAPHENE
NANORIBBON JUNCTION USING VARIOUS DOPANTS
by
Natasha Parikh
A Thesis
Submitted to the Faculty of
New Jersey Institute of Technology
in Partial Fulfillment of the Requirements for the Degree of
Master of Science in Materials Science and Engineering
Interdisciplinary Program in Materials Science and Engineering
January 2014
APPROVAL PAGE
ANALYSIS OF TRANSPORT PROPERTIES IN A ZAZ GRAPHENE NANORIBBON JUNCTION USING VARIOUS DOPANTS
Natasha Parikh
Dr N M Ravindra Thesis Advisor Date Director of Material Science and Engineering Program NJIT Dr Keun H Ahn Committee Member Date Associate Professor of Physics NJIT Dr Tao Zhou Committee Member Date Associate Professor of Physics NJIT Dr Halina Opyrchal Committee Member Date Senior University Lecturer of Physics NJIT
BIOGRAPHICAL SKETCH
Author Natasha Parikh
Degree Master of Science
Date January 2014
Undergraduate and Graduate Education
bull Master of Science in Materials Science and EngineeringNew Jersey Institute of Technology Newark NJ 2014
bull Bachelor of Arts in Physics and Biological SciencesRutgers the State University of New Jersey New Brunswick NJ 2012
Major Materials Science and Engineering
iv
v
ACKNOWLEDGMENTS
I would like to express my gratitude to my supervisor Dr NM Ravindra for the useful
comments remarks and engagement throughout the learning process of this Mastersrsquo
thesis Furthermore I would like to thank Vijay Kasi Somayajula for introducing me to
the topic as well for the support I thank Dr Tao Zhou Dr Ken Ahn and Dr Halina
Opyrchal for serving on my thesis Committee I would like to thank my loved ones who
have supported me throughout the entire process both by keeping me harmonious and
helping me in putting pieces together
vi
TABLE OF CONTENTS
Chapter
Page
1 INTRODUCTIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
1
11 Graphene The New Carbonhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
1
12 Graphene Synthesishelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
3
121 Synthesis of Graphene on Nickel (Ni)helliphelliphelliphelliphelliphelliphelliphellip
5
122 Synthesis of Graphene on Copper (Cu)helliphelliphelliphelliphelliphelliphelliphellip
8
123 Transfer of Graphene Filmshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
8
124 Synthesis of Graphene Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
9
125 Doping in Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
10
126 Nitrogen (N) Doped Graphene Synthesis (Substitutional)hellip
12
13 Structure of Graphene Nanoribbon (GNR)helliphelliphelliphelliphelliphelliphelliphelliphelliphellip
13
14 Overview of Graphene Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
15
2 RESEARCH BACKGROUNDhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
21 Bandstructure of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
22 Transport Characteristics of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
20
23 Drude Theoryhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
22
24 Quantum Hall Effect (QHE)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
24
25 Resistivity and Resistancehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
27
26 Klein Tunnelinghelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
28
27 Quantum Hall Effect in Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
31
28 Thermoelectric Effecthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 34
vii
TABLE OF CONTENTS
(Continued)
Chapter Page
281 Seebeck Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
34
282 Peltier Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
36
29 Early Research ndash ab initio Studyhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
37
3 COMPUTATIONAL DETAILShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
31 Introductionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
311 Extended Huckel Theory helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
312 Introduction to NEGFhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
41
313 Electrostaticshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
42
314 Non-Equilibrium Greenrsquos Functionhelliphelliphelliphelliphelliphelliphelliphelliphellip
44
4 ATOMISTIX TOOLKIT DETAILShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
41 Introductionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
42 Device Structurehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
43 Transmission Spectrum Calculationhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
50
44 Calculating the Currenthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
51
45 Calculating the Transport Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
52
5 RESULTS AND DISCUSSIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
53
51 Band Structure Analysis helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
53
52 I-V Characteristics of GNR Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
59
53 Thermoelectric Propertieshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
63
6 CONCLUSIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 65
REFERENCEShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
66
viii
LIST OF FIGURES
Figure Page
11 (a) Chemical representation of Carbon (b) Graphite ore (c) Structure of
Graphite and a single layer Graphenhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
2
12 An optical image of Graphene flake obtained by exfoliation of
graphitehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
3
13 (a) Graphene formation on Nickel (b) Graphene atoms on Ni (111)
lattice (c)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
7
14 (a) SEM image of graphene on copper foil (b) High-resolution SEM
image of graphene on Cuhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
8
15 (a) Transfer process (b) Wafer-scale synthesis of graphene (c) Graphene
films transferred onto glass wafer (d) SiSiO2 with device patterned (e)
PET filmhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
9
16 (a) High-magnification image of the annealed sample showing that well-
defined zigzag armchair and zigzag-zigzag edges are formed (b) ) STM
image of an 8 nm wide bent junction connecting an armchair and a
zigzag graphene nanoribbon which was carved by STM
tipshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
10
17 Band structure of graphene before and after doping The image shows
shift towards the Fermi levelhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
11
18 Low resolution TEM image of N-doped graphene Background is the
lacey carbon TEM grid graphene sheet is crumpled with many
rippleshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
13
19 Zigzag and Armchair orientation of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphellip 13
110 Bandstructure of ZGNRhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 14
111 Bandstructure of AGNRhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 15
21 Left Real space Graphene lattice with basis vectors and Right
The first Brillouin zone of Graphene in reciprocal space with basis
vectors and K and Krsquo are responsible for massless transport at low
energyhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
ix
LIST OF FIGURES
(Continued)
Figure Page
22 Bandstructure of a graphene sheet showing a band gap of 0eVhelliphelliphellip 18
23 Band structure of Graphene calculated with the tight-binding modelhellip 19
24 The energy dispersion around the K pointhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 22
25 Electrons colliding with stationary ionshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 23
26 (a) 2D electrons in a perpendicular magnetic field Logitudinal resistance
measured across C5 and C6 Transverse resistance measured across C3
and C5 (b) Classical Hall resistance as a function on the magnetic field
25
27 Klein tunneling through an npn barrierhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 29
28 Electron trajectory considering the linear electrostatic potential U(x) = Fx 30
29 Electron like and hole like trajectories at same Ehelliphelliphelliphelliphelliphelliphelliphelliphellip 30
210 Quantum Hall effect in graphene 22
The Hall conductivity σxy and the
longitudinal resistivity of monolayer graphene as a function of carrier
density at B = 14T and T= 4K This shows half-integer QHE with chiral
index J= 1helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
32
211 (a) LL for Graphene bilayer (b) Schematics of Hall conductivity as a
function of nn0 for bilayer Graphene (solid line) and monolayer
Graphene (dotted line) (c) LL for monolayer Graphenehelliphelliphelliphelliphelliphelliphellip
33
212 Seebeck Effecthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 35
213 Transmission functions in units of (2e2h) for AZA structureshelliphelliphelliphellip 37
214 I-V curve for a 591nm long channel (Vbias=20mV)helliphelliphelliphelliphelliphelliphelliphellip 38
31 NEGF systemhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 42
41 Geometry of device configuration with two electrodeshelliphelliphelliphelliphelliphelliphellip 48
42 The electron distribution in a device configuration which illustrates a left
moving scattering state with origin in right electrodehelliphelliphelliphelliphelliphelliphelliphellip
48
x
LIST OF FIGURES
(Continued)
Figure Page
51 Band structure of AGNR widths (a) 4 atoms (b) 5 atomshelliphelliphelliphelliphelliphellip
53
52 Band structures of AGNR widths (a) 6 atoms (b) 7 atomshelliphelliphelliphelliphelliphellip 54
53 Band structure of AGNR widths (a) 8 atoms (b) 9 atomshelliphelliphelliphelliphelliphelliphellip 54
54 Band structures of AGNR widths (a) 10 atoms (b) 11 atomshelliphelliphelliphelliphellip 55
55 Band structure of AGNR with a width of 12 atomshelliphelliphelliphelliphelliphelliphelliphelliphellip 55
56 Variation in band gaps as the width (number of atoms) varieshelliphelliphelliphellip 55
57 Band structure of ZGNR width (a) 4 atoms (b) 6 atomshelliphelliphelliphelliphelliphelliphellip 56
58 Band structure of ZGNR width (a) 8atoms and (b) 10 atoms 57
59 Band structure of ZGNR with a width 12 atomshelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 57
510 Band structures of Doped AGNR (a) 4 N Doped (b) 4 B Doped (c)
2 N Doped (d) position of Nitrogen from (c)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
58
511 Current Vs Voltage graph for varying graphene width showing
conductivityhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
59
512 ZAZ GNR junction devicehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 60
513 I-V curve of Boron Doped ZAZ junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 61
514 I-V curve of Nitrogen Doped ZAZhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 62
515 Variation of Peltier effect coefficient with temperature for various doping 64
1
CHAPTER 1
INTRODUCTION
11 Graphene The New Carbon
Carbon (chemical symbol C atomic mass 1207amu) (Figure 11a) is a widely distributed
element in nature It is found abundantly in the sun stars comets and the atmospheres of
the planet Carbon can form up to four bonds it can bond with itself endlessly and with
most other elements in many different shapes making it a significant part of the
construction for many kinds of complex molecules1
Two allotropes of carbon are commonly used diamond and graphite (Figure
11b) The bonding structures of diamond and graphite contribute to the properties
individually In diamond all the p-orbitals are used forming a sp3
bonding whereas in
graphite only two orbitals are occupied allowing the unpaired bond for the transport of
electrons Each carbon atom in graphene possesses sp2 hybridization ie each carbon
atom is connected to three other carbon atoms via covalent bonds with a bond length of
142Å and an angle of 120deg between each bonded pair This makes graphite a better
conductor than diamond Graphite consists of many layers of 2D carbon lattices (Figure
11c) stacked on top of each other and held via Van der Waals forces A single layer of
graphite where carbon atoms are arranged in a honeycomb lattice is known as graphene
(Figure 11c)
2
Figure 11 (a) Chemical representation of Carbon (b) Graphite ore (c) Structure of
Graphite and a single layer Graphene2
Theoretical work on graphene was done specifically to study the other allotropes
The first study was done by Wallace in 1947 who calculated the band structure of
graphene3 Further the peculiar Landau levels were known by McClure in 1957 and the
relativistic Hofstadter butterfly by Ramal in 19853 Later in 1991 the invention of carbon
nanotubes by Iijima boosted the theoretical research on graphene3 Prior to the invention
of carbon nanotubes there were a few experimental papers on graphene growth via
various methods like intercalation of graphite (Shioyama 2001) free standing (Boehm
1962) epitaxial as well as graphene grown on metals (Bommel 1975 Land 1992 Itoh
1991)3 With all the various discoveries the electronic properties of graphene were not
studied until 2004 when Berger and Novoselov were able to access the electronic
properties with contact of graphene flakes3 (Figure 12)
3
Figure 12 An optical image of Graphene flake obtained by exfoliation of graphite3
The specific lattice structure of graphene possesses a number of unique electronic
properties making it an interesting material for theorists experimentalists and engineers
Utilization of graphene as a fundamental block of electronic devices requires
development of new theoretical methods for understanding the current propagations in
graphene constriction4
12 Graphene Synthesis
The discovery of graphene by mechanical exfoliation called the lsquoScotch tape methodrsquo led
to serious attempts towards the production of top quality graphene5 Graphene was first
exfoliated mechanically from graphite in 20046 The importance of high quality graphene
cannot be emphasized enough however electron transport has shown that defects play an
important role in hindering the transport properties of electrons (holes)7 The two
synthesizing methods for the large scale manufacture of graphene are chemical vapor
deposition (CVD) and silicon carbide (SiC) desorption method
4
Graphene can be synthesized by sublimation of silicon from SiC at high
temperature (1200degC) in high vacuum5 The major advantage of this method is that the
SiC provides an insulating substrate and no transfer of the graphene layer is needed Yet
the disadvantage of this method outweighs its advantages the high temperature is cost-
ineffective making it unsuitable for large scale manufacturing8 Also the crystal growth
face alters the properties of graphene Graphene grown on Si-terminated face has poor
homogeneity and is subjected to unintentional doping7 Conversely graphene grown on
C-terminated SiC has higher mobility and is often called lsquoturbostaticrsquo due to the
rotational disorder7
Unlike the SiC method the graphene produced via CVD method needs to be
transferred to a substrate making it difficult to maintain the quality of graphene Yet
CVD synthesized graphene has a larger grain size7 More research is being done on
various methods for synthesis of graphene The methods include direct chemical
synthesis ion implantation crystal sonification and lastly unzipping carbon nanotubes to
form graphene sheets9
Graphene and few-layer graphene have been grown by CVD from carbon
containing gases on catalytic metal surfaces andby surface segregation of C dissolved in
the bulk of such metals7 Growing graphene with CVD is a very attractive solution since
it is compatible with the existing semiconductor industry9 Graphene has been grown via
CVD process on metal substrates such as Nickel (Ni) and Copper (Cu)
5
121 Synthesis of Graphene on Nickel (Ni)
Polycrystalline Ni films are annealed in ArH2 atmosphere at 900-1000degC to increase
grain size and are then exposed to H2CH4 gas mixture10
In this step the hydrocarbon
decomposes and dissolves in Ni to form a solid solution Lastly the samples are cooled in
argon gas Ni has high carbon solubility at elevated temperatures and the solubility
decreases as temperature is reduced During the cooling process the carbon atoms diffuse
out from the Ni-C solid solution and precipitate on the Ni surface to form graphene films
(Figure 13a) Since Ni (111) has a lattice similar to the densely packed hexagonal lattice
of graphene (Figure 13b) they also have similar lattice constants and hence Ni surface
serves as an excellent lattice matched substrate for graphene growth11
The growth of graphene on Ni is based on carbon segregation and precipitation
process different segregation behavior is produced by different cooling rates which
affect the thickness and quality of graphene films12
Medium cooling rates lead to optimal
carbon segregation and produce few layers12
Graphene films grown on Ni are usually
continuous with monolayer and few layer regions Annealing of Ni substrates at elevated
temperatures in hydrogen atmosphere not only increases the single-crystalline Ni grain
size but also eliminates certain impurities in Ni thereby improving the graphene quality
Furthermore the graphene thickness can also be affected due to the amount of carbon
dissolved in the Ni films during the growth time
After synthesis the graphene can be transferred to other insulator substrates for
further characterization and applications Figure 13c shows the selected area electron
diffraction pattern of graphene film along the [001] direction which confirms the
graphene lattice structure shown After transfer to insulator substrates the geometry can
6
be retained as shown in Figure 13d Under optimal growth parameters graphene growth
is only limited by the Ni catalyst Lastly Figures 13e and 13f show the wafer-scale
graphene synthesis and transfer of graphene to a flexible transparent substrate
respectively
Though polycrystalline Ni is a good substrate the percentage and size of
graphene monolayer are still limited Researchers have hence tried other metal substrates
for graphene synthesis
7
Figure 13 (a) Graphene formation on Nickel (b) Graphene atoms on Ni (111) lattice
(c) Low magnification TEM image of graphene edges (d) Optical image of graphene
transferred from the Ni surface to SiO2Si substrate (e) Full-wafer scale deposition of
graphene layers on polycrystalline Ni (f) Transparent and flexible graphene films on
PDMS substrate10
8
122 Synthesis of Graphene on Copper (Cu)
Graphene films are grown on 25microm thick Cu foils in a hot wall furnace13
The Cu foil is
first annealed in hydrogen atmosphere at 1000degC and a mixture of H2CH4 is introduced
into the system to initiate graphene growth After a continuous graphene layer is formed
on the Cu foil the system is cooled to room temperature Figure 14a shows an SEM
image of graphene on Cu substrate indicating the Cu grains with contrast The Cu
surface steps are formed during thermal annealing and the darker flakes indicate multiple-
layer graphene (Figure 14b)10
The graphene wrinkles in Figure 14(b) originate from
different thermal expansion coefficient of graphene and Cu They go across the Cu grain
boundaries indicating that the graphene film is continuous
Figure 14 (a) SEM image of graphene on copper foil (b) High-resolution SEM image of
graphene on Cu10
123 Transfer of Graphene films
In order to facilitate the applications of graphene for electronic applications we need to
separate the graphene from the catalytic metal substrate Figure 15a shows the transfer
process of graphene Graphene is first coated with a thin layer of polymethyl
methacrylate (PMMA) and baked at 120degC to evaporate the solvent10
The metal layer is
then removed by Ni or Cu etchant leaving behind the PMMA graphene film The film is
then cleaned by deionized water and then transferred onto the target substrate After the
9
evaporation of water vapor the PMMA is removed by acetone leaving graphene film on
top of the target substrate Figure 15b shows a graphene wafer transferred from the
substrate onto glass and polyethylene terephthalate (PET) films
Figure 15 (a) Transfer process (b) Wafer-scale synthesis of graphene (c) Graphene
films transferred onto glass wafer (d) SiSiO2 with device patterned (e) PET film10
124 Synthesis of Graphene Junction
Graphene junctions with smooth armchair and zigzag edges are difficult to produce by
conventional methods such as mechanical exfoliation chemical exfoliation or lithography
etching14
The conventional methods can only produce rough edges Recently
Dresselhaus reported an edge reconstruction of graphene by Joule heating in a TEM-STM
10
(Figure16b) system15
An individual nanoribbon sample is attached to the sample holder
at one end and to the STM tip at the other end these ends also serve as the two
electrodes The structural transformation in the growth of graphene from armchair to zig-
zag is mainly attributed to the vaporization of carbon edges that reconstruct at high
temperatures in which resistive Joule heating and preferred current flow play an
important role This means that by controlling the flow of current a perfectly smooth
edged ribbon can be synthesized making graphene-based electronics possible16
Figure 16 (a) High-magnification image of the annealed sample showing that well-
defined zigzag armchair and zigzag-zigzag edges are formed (b) STM image of an 8 nm
wide bent junction connecting an armchair and a zigzag graphene nanoribbon which was
carved by STM tips14
125 Doping in Graphene
The doping of graphene can be roughly classified into two categories - electrical and
chemical Electrical doping involves changing gate voltages of graphene devices and
chemical doping uses chemical routes such as substitutional or interstitial This thesis
discusses chemical doping and the importance of doping sites by changing the dopant
Chemical doping is a common approach to tailor the electronic properties of
11
semiconductors Doping of graphene can cause its electronic properties to alter leading to
a metal-semiconductor transition The two means of doping graphene are interstitial and
substitutional In interstitial doping the dopant atoms or molecules are introduced as
adatoms or admolecules on the surface of graphene whereas in substitutional doping the
dopant atoms are replaced in the carbon lattice forming a bond in the lattice of
graphene16
Doping graphene results in the formation of n or p-type semiconductors
depending on the kind of dopant If the dopant is an electron donor it causes the Fermi
level to shift up resulting in n-type behavior of graphene Furthermore if the dopant is an
electron acceptor it causes the Fermi level to shift down resulting in a p-type behavior of
graphene (Figure 17)16
Figure 17 Band structure of graphene before and after doping The image shows shift
towards the Fermi level16
Graphene nanoribbons (GNR) can be made into a p- and n- type semiconductor
by doping with boron (B) and nitrogen (N) respectively In theory GNR p-n junction is
formed by doping GNR with B and N in different regions However experimentally
doping graphene with both these elements is very difficult due to the dopants reacting
with each other17
Hence most experimental studies use GNR doped by only one
12
element N-doped graphene was synthesized by Wei et al Wang and B-doped Graphene
was realized by Endo17
Many researchers have demonstrated interstitial doping of graphene by gas metal
and organic molecules16
The various gases and metals used are NO2 NH3 An-CH3 Na-
NH2 F4-TCNQ TPa TCNE and others16
Doping in graphene is hence possible by
electrons or holes in high concentration without deterioration of its mobility Interstitial
doping is highly sensitive due to most of the conducting channel being exposed to surface
absorbates and hence can be used in molecule detection
In substitutional doping the dopant atoms are included in the graphene lattice and
thus chemically bonded Substitutional doping is done via the CVD method using a
carbon and dopant source Substitutional doping opens up many applications in device
engineering making graphene a very good candidate as a semiconductor This study
involves the study of transport properties of graphene doped by substitution
126 Nitrogen (N) Doped Graphene Synthesis (Substitutional)
N-Doped graphene is prepared via a CVD process using a 25microm thick Cu film on a Si
substrate The substrate is placed in a quartz tube with the flow of hydrogen (20sccm) and
argon (100 sccm)18
When the center of the furnace reaches 800degC 60 sccm of CH4 and
60 sccm of NH3 is introduced into the flow as C source and N source respectively The
substrate is then moved to high temperature and after 10 min growth the sample is
cooled to room temperature under H2 ambient Figure 1 8 shows the growth of N-doped
graphene18
13
Figure 18 Low resolution TEM image of N-doped graphene Background is the lacey
carbon TEM grid graphene sheet is crumpled with many ripples18
13 Structure of Graphene Nanoribbon (GNR)
Graphene Nanoribbons (GNR) are strips of graphene with very thin width of lt50nm
GNRs can be terminated in three separate ways called zig-zag (0 n) armchair (m 0) and
chiral (m n) (Figure19) and this termination along the width of the ribbon dictates the
size of the band gap19
Figure 19 Zigzag and Armchair orientation of Graphene5
Due to their various edge structures GNRs exhibit different electronic properties
ranging from normal semiconductors to spin-polarized half metals which open the
possibility of GNRs as electronic devices19
14
Within a tight binding approach (AGNRs) could be metallic or semiconducting
depending on their ribbon width but all zigzag graphene nanoribbons (ZGNRs) are
metallic with a high density of electronic states at the edges Hence ZGNRs exhibit
characteristic edge effects which are not present in AGNRs These edge effects in
ZGNR create a flat band close to the Fermi level making the ZGNR edges more
reactive19
First-principles calculations show that the GNRs possess a non-zero direct
band gaps These gaps are small for ZGNR (Figure 110) caused due to spin ordering
effects at the edges For AGNRs the band gap arises from quantum confinement (Figure
111) effect that has larger magnitudes than ZGNR20
Figure 110 Band structure of ZGNR
15
Figure 111 Band structure of AGNR
For GNRs the band gap decreases as the ribbon width increases and in order to
create a semiconductor with a desirable band gap the nanoribbon width should be
adjusted accordingly This property of adjusting the band gap makes graphene an
excellent candidate for transistor switching By applying an electric field GNR can be
altered from an insulator to a conductor GNRs exhibit very intriguing properties and
have become one of the promising candidates for electronic applications
14 Overview of Graphene Junction
The invention of p-n junctions date back to 1940s which later resulted in the invention of
junction transistors One of the key technological reasons for success of the p-n junction
is mainly due to its ability to locally modulate the energy band gaps via an applied bias21
A graphene p-n junction is created via single layer of graphene in which the
carrier type and density in two adjacent regions are controlled by electrostatic gating8
For materials with a band gap the electric field can either switch lsquooffrsquo the current or
rectify it (p-n diode)22
Being a ldquogaplessrdquo material the off state is not achievable in
16
graphene In order to achieve an off state the gap can be created by doping graphene with
various elements (Group III or Group V) Doping allows p-n junctions to be
reconfigurable using a gate voltage to distinguish between graphene p- n regions within a
single sheet Many researchers have studied the electronic as well as transport properties
of doped graphene junctions
In 2009 Fangping OuYang studied the transport properties of T-shaped graphene
junctions using the ATK software and showed that the conductance depends on
geometric structures which can be controlled by selective doping23
Wei Yao in 2013
studied the transport properties in graphene p-n junctions and showed that the
rectification effect depends on boron doping density and position17
The study of transport properties in graphene p-n junctions is a recent
advancement The thesis discusses transport properties including the current-voltage (I-
V) characteristics of doped graphene junctions Moreover the software used is similar to
the software in use by current researchers since they have produced viable data using
ATK
17
CHAPTER 2
RESEARCH BACKGROUND
21 Band Structure of Graphene
The unique electronic properties of graphene were first predicted in 1946 Figure 21
shows a top view of the hexagonal arrangement of carbon atoms in real space as well as
the first Brillouin zone in reciprocal space
Figure 21 Left Real space graphene lattice with basis vectors and Right The
first Brillouin zone of graphene in reciprocal space with basis vectors and
K and
Krsquo are responsible for massless transport at low energy24
The real space basis vectors are radic
and
radic
The reciprocal space basis vectors are 1 2
0 0
4 1 3 4 1 3( )and ( )2 2 2 23 3
b x y b x ya a
where the magnitude of the basis vectors is |a0| = radic acc The distance between nearest
neighbor carbon atoms is acc=0142nm
18
The band structure can be calculated by solving the eigenvalues using the
dispersion relation E( )
1 2 3( ) 3 2cos 2cos 2cosE k t k a k a k a (21)
Transport properties of solids are closely related to the energy dispersion
relations E ( ) in the material and in particular to the behavior of E ( ) near the Fermi
level Graphene is a zero gap semimetal whose specific linear electronic band dispersion
near the Brillouin zone corners (Dirac points) gives rise to electrons and holes that
propagate as massless Fermions25
The valence and conduction bands do not overlap in
graphene they touch at the Fermi Level (Figure 22)
Figure 22 Band structure of a graphene sheet showing a band gap of 0eV
The low energy properties of graphene can be well described by making a linear
expansion of the band structure around the K and Krsquo This energy can be written as
19
E(k) = plusmnħvF|k (22)
where vF is the Fermi velocity of 1106ms given by
1F
Ev
k
ħ (23)
Figure 23 Band structure of graphene calculated with the tight-binding model
22
The Fermi surface of graphene consists of double cones with Fermi energy at the
intersection of these cones (Figure 23) The slope of the band is zero and hence the
effective mass of electrons in that region is zero which leads to an entirely new transport
mechanism in graphene26
20
22 Transport Characteristics of Graphene
Transport process usually involves a flow of charge or energy or both The flow is mainly
due to external perturbations such as electric field and temperature gradient The
relationship between forces and flow usually defines various transport coefficients that
are the characteristics of electrons and phonons in the material All modern electronics
are based on the ability to control the electronic properties of a material by applying
external voltage This is done by an electric field effect where the gate voltage changes
the carrier concentration of the material and consequently its conductivity The electric
field effect in graphene was reported by Novoselov in 2004 and is used in transport
measurements8
The electron-phonon interaction in graphene plays an important role in
understanding the photoemission spectra observed in graphene The electric field effect is
an alternative method for changing the charge carrier density in low dimensional systems
The electric field effect in graphene which was first reported by Novoselov et al in
2004 is widely used as a characterization tool in transport measurements25
The transport characteristics of the material are directly related to the
bandstructure of graphene The carriers in graphene lattice are free to move in two
dimensions In the carrier transport of graphene the carriers ndash electrons and holes ndash close
to the Dirac points are of importance The transport is described by a two component
wave function (Equation 24) which obeys the 2D Dirac-like equation for massless
particles27
21
-ivFσ nablaψ(r) = Eψ(r)
(24)
where σ is the 2D Pauli spin matrix In the continuum limit the above (Equation
24) corresponds to the effective low energy Dirac Hamiltonian (Equation 25)
0( )
0
x y
F F
x y
iH k k
i
k kv v
k k
(25)
The electronic band structure of the energy (E) versus wave vector (k) relation for
graphene is given by Equation 24
The two component wave function resembles the spin or wave function of
quantum electro dynamics (QED)27
Corresponding to the spin of particles in QED the
charge carriers of graphene can be attributed with a pseudospin σ The pseudospin is the
direct result of two different carbon sublattices corresponding to the bonding and
antibonding combinations27
22
Figure 24 The energy dispersion around the K point27
In Figure 24 the red and blue lines correspond to the antibonding and bonding
states respectively The pseudospin can have two values either in the direction of or
against the momentum It can be seen that the electrons with energy E travelling in the
positive direction originates from the same branch as a hole with energy ndashE travelling in
the negative direction giving it the same pseudospin This results in suppressed
backscattering and Klein tunneling The back scattering process requires the pseudospin
to flip which is possible in the presence of short range scatters that act differently on sub
lattices27
23 Drude Theory
The classical theory of metallic conductivity was presented by Drude in 1900 and was
elaborated by Lorentz in 190528
Drude treated the free electrons as classical ideal gas
meaning the electrons collide with stationary ions and not each other
23
Figure 25 Electrons colliding with stationary ions28
The Drude theory applied the kinetic theory of gases to a metal considered as a gas of
electrons The basic assumptions made by the Drude theory are28
When metallic elements are brought together to form a solid then the valence
electrons become freely moving through the metal whereas the ions remain intact
as nearly immobile positive particles
Between collisions the electrons move freely ie there is neither electron-
electron interaction nor electron-ion interaction
The scattering mechanism leads to instantaneous collisions of the electron with
the scatterers
The collisions are characterized by a relaxation time τ
The electrons achieve thermal equilibrium only through collisions the velocity
after a collision is randomly directed the speed is as appropriate to the
temperature
With the relaxation time Drude obtained the electrical conductivity expression
where n is the number of electrons per unit volume
σ = ne2τm
(25)
He also calculated the thermal conductivity and successfully provided the
theoretical basis for Wiedemann-Frantz law already established in 1853 which states that
24
the ratio of electrical and thermal conductivity of any metals is a universal constant at any
given temperature28
The Drude theory gives results which are qualitatively correct outside of the
quantum Hall regime28
In the Drude theory of the electrical conductivity of a metal an
electron is accelerated by the electric field for an average time τ before being scattered
by impurities lattice imperfections and phonons to a state which has zero average
velocity The average drift velocity of the electron is
d
eE mv (26)
It is assumed that all electrons drift together and hence the current density
j = -ne (27)
This Drude theory works well for fields below ~ 01T At stronger fields the Hall
resistivity becomes nearly constant over finite intervals of magnetic fields28
The QHE
reflects both novel disorder physics as well as novel interaction physics in the quantum
Hall regime
24 Quantum Hall Effect (QHE)
The discovery of QHE is a remarkable achievement in condensed matter physics The
Hall Effect was discovered by Edwin Hall in 187929
However the precise quantization
of the Hall conductance in units of e2h was not recognized until February 1980 Five
years later in 1985 Klaus von Klitzing was awarded the Nobel Prize in Physics for the
discovery of QHE29
The quantum Hall effect occurs in two-dimensional electron systems in the limit
of strong perpendicular magnetic field that stems from electronic transport
25
measurements where one drives a current I through the sample and where one measures
both the longitudinal and transverse resistance (Hall resistance) A longitudinal resistance
is a resistance measured between two contacts that may be connected by a line which
does not connect C1 and C430
Transverse resistance is measured between two contacts
connected by an imaginary line connecting C1 and C4 (Figure 26a)
Figure 26 (a) 2D electrons in a perpendicular magnetic field Logitudinal resistance
measured across C5 and C6 Transverse resistance measured across C3 and C5
(b) Classical Hall resistance as a function on the magnetic field30
Due to the existence of quantum Hall effect it is natural to expect that there exists
a classical Hall Effect Hall showed that the transverse resistance of a thin metallic plate
varies linearly with the strength B of the perpendicular magnetic field (Figure 26 b)
RH = Bqnel (28)
More quantitatively the classical Hall Effect can be understood within the Drude
model for diffusive transport in a metal Within this model one considers independent
26
charge carriers of momentum p described by the equation of motion
( )
b
dp p pe E B
dt m (29)
where E and B are the electric and magnetic field respectively The macroscopic
transport characteristics ie resistivity of the system are obtained from the static
solution of the equation of motion dpdt = 0 and one finds for 2D electrons with p =
(pxpy)
x
x yb
y
y xb
eBe
eBe
ppE
m
ppE
m
(210)
In the above expression characteristic frequency is visible as
C
b
eB
m (211)
This is known as cyclotron frequency as it characterizes the cyclotron motion of a
charged particle in a magnetic field30
With the Drude theory the conductivity can be
written as
j = -enelpmb (212)
and the mobility can be given as
micro = eτmb (213)
The transport properties in the limit of ωCτ-gt infin are entirely governed in the presence of
27
a magnetic field by the off-diagonal ie transverse components of
conductivityresistivity
The theory of quantum Hall effect subjects all physical properties of 2D electron
system in the limit where the magnetic field is strong so that the mixing of Landau levels
by disorder or electron-electron interaction is considered to be a weak perturbation30
This is known as the quantum Hall regime The ratios between the energy scales
corresponding to the two interactions are important The limit where disorder potential is
much stronger is referred to as integer quantum hall regime whereas the limit where the
interaction potential is much stronger is referred to as fractional quantum Hall regime
25 Resistivity and Resistance
The electronic transport in the framework of the Drude theory allows for the calculation
of conductivity or resistivity of a classical diffusive 2D electrons in a magnetic field30
The conductivity and conductance are related to one another but they depend on the
geometry of the conductor-the resistance R and hence the resistivity is given by
R = (LA)ρ (214)
where L is the length of the conductor and A is the cross section
For a d-dimensional conductor the cross section scales as Ld-1
such that the
scaling relation between the resistance and the resistivity is
R~ ρL2-d
(215)
From the dimension point of view resistance and resistivity are the same in 2D and the
resistance is scale-invariant Further the resistance of a 2D conductor depends in
general on the so-called aspect ratio LW via some factor f (LW)30
However for
transverse Hall resistance it is the length of the conductor that plays the role of cross
28
section such that the Hall resistivity and the Hall resistance truly coincide ie f=1 The
Quantum Hall effect is highly insensitive to the particular geometric properties of the
sample used in transport measurements Recently quantum Hall physics experienced the
discovery of ldquorelativisticrdquo quantum Hall effect in graphene The electrons in graphene
behave as if they were relativistic massless particles contributing to a very interesting
field of research30
26 Klein Tunneling
Klein tunneling in which relativistic particles penetrate through a potential barrier
without the exponential damping that is characteristic for nonrelativistic quantum
tunneling has never been observed for elementary particles The tunneling allows
transmission of a particle through a potential barrier higher than its kinetic energy
violating the principle of classical mechanics30
On the quantum scale the objects exhibit
wave-like characteristics in which the quanta move against a potential hill described by
their wave function This wave function represents the probability amplitude of finding
the object in a particular location The transmission of the object through the potential hill
is termed as tunneling When EltV then the ψ(x) over V is returned by ψrsquo(x) In quantum
mechanics an electron tunnels from the conduction into the valence band Such a
tunneling from an electron-like to hole-like state is called as Klein Tunneling in which the
electron avoids backscattering
In Figure 27 it is shown that an electron hitting a potential barrier is reflected
with 100 certainty In non-relativistic quantum mechanics the electrons can tunnel
through the barrier but the probability of tunneling exponentially decays with increasing
29
height and width of the barrier However in relativistic quantum mechanics the barrier
gets transparent even in the limit of infinite barrier height (Klein paradox)31
Figure 27 Klein tunneling through an npn barrier30
The Klein paradox in graphene can be understood in terms of electrons and holes
In graphene the massless carriers behave differently than ordinary carriers (with mass) in
the presence of an electric field A barrier which is repulsive for electrons will be
attractive for holes Since there are hole states inside the barrier with the same energy as
the electrons outside an electron arriving at the barrier can tunnel through it as a hole
before leaving again as an electron Klein tunneling for transport in graphene is that the
charge carriers cannot be confined by potential barriers The Klein tunneling effect has
been experimentally observed by Ando in 1998 in which the absence of backscattering
(Figure 28) is responsible for high conductivity in carbon nanotubes
30
Figure 28 Electron trajectory considering the linear electrostatic potential U(x) = Fx30
The electron is able to propagate through an infinitely high potential barrier since
it makes a transition from the conduction band to valence band In this transition from
conduction band to valence band its dynamics changes from electron-like to hole-like
The equation of motion is thus given by
2
2 2 2| | ( )
pdr E
dt E Up
p E U
v
v
at energy E (216)
This shows that in the conduction band (UltE) and in the valence band (UgtE)
In Klein tunneling the pairs of electron-like and hole-like trajectories at the same E and
py have turning points at dmin given by dmin=2v|py|F (Figure 29)
Figure 29 Electron like and hole like trajectories at same E21
31
The tunneling probability exponential dependence on dmin
2
min| |
( ) exp( ) exp( )2
y y
y
vT
F
p pdp
(217)
The applications of the Klein tunneling include Atomic clock Scanning tunneling
Microscope Tunnel diode Tunneling transistor and many more32
Since graphene
exhibits Klein tunneling it can be very useful to study the transport properties in
graphene and use it in such applications
27 Quantum Hall Effect in a Graphene
A monolayer graphene shows half-integer quantum Hall effects where the Hall
resistance is quantized at values of
2
1
xyh v eR
(218)
around filling factors
14( 1 2)Nv
(219)
where N is an integer e is the electron charge h is the Planckrsquos constant and the
factor 4 is due to spin and valley degeneracy QHE in graphene can be observed at room
temperature which is a very intriguing property (Figure 210) Graphene reveals
significant differences with respect to conventional 2D electron systems The Landau
quantization yields energy levels that disperse differently in graphene as well as
particular zero-energy level that is only half filled at the charge neutrality point (v=o)
32
Figure 210 Quantum Hall effect in graphene22
The Hall conductivity σxy and the
longitudinal resistivity of monolayer graphene as a function of carrier density at B = 14T
and T= 4K This shows half-integer QHE with chiral index J= 1
The QHE in graphene is not entirely similar to regular QHE since the charge
carriers in graphene are Dirac Fermions The charge carriers governed by
electrodynamics is given by (Equation 220) which does not apply for graphene and a
QED quantization of graphene electronic band structure is used
En = (n+12)ħω (220)
33
In the presence of magnetic field the nature of the Dirac Fermions in graphene
results in unevenly spaced Landau levels (LL) containing a distinctive LL at the electron-
hole degenerating a zero energy given by
2MG
MGFehn B
n vE (221)
The LL levels at high magnetic fields in MG are shown in Figure 211
Figure 211 (a) LL for Graphene bilayer (b) Schematics of Hall conductivity as a
function of nn0 for bilayer Graphene (solid line) and monolayer Graphene (dotted line)
(c) LL for monolayer Graphene33
It is found that the Hall resistance of a two dimensional electron system has
plateaus as a function of the number of electrons at low temperatures and strong magnetic
fields32
At large B the Dirac-like energy spectrum of graphene gives rise to a
characteristic series of QH plateaus in conductance reflecting the presence of a zero-
energy Landau level that include only odd multiples of 2e2h for uniform carrier density
in the sheet These plateaus of QH edge states at the edge of the sheet circulating in a
34
direction are determined by the direction of B and the carrier type33
This is why QHE in
graphene is known as Half-Integer Quantum Hall Effect
28 Thermoelectric Effect
Thermoelectricity refers to a class of phenomena in which a temperature difference
creates an electric potential or an electric potential creates a temperature difference The
principle of thermoelectric effect has been known for over 100 years Recently the
practical applications of thermoelectric effect have become more viable34
Thermoelectric effect is the direct conversion of temperature differences to
electric voltage and vice versa Joule heating is the heat generated whenever a voltage is
applied across a resistive material The Peltier-Seebeck effect is reversible whereas Joule
heating is not This effect can be used to generate electricity to measure temperature to
cool objects or to heat them Since the direction of heating and cooling is determined by
the sign of the applied voltage thermoelectric devices make very convenient temperature
controllers
281 Seebeck Coefficient
Thomas Johann Seebeck discovered that an emf appears in a circuit composed of two
dissimilar metals when the junction between the metals is held at different
temperatures34
The thermoelectric emf causes a continuous current in the circuit when a
complete loop is formed and the current is known as thermoelectric current This is
known as the Seebeck effect
35
Figure 212 Seebeck Effect34
As long as the two junctions are at different temperatures the thermoelectric emf
exists and the current will keep flowing between the hot and cold junction that are at
different temperatures The Seebeck effect is the conversion of temperature difference
directly into electricity The voltage developed in the circuit shown in Figure 212 is
proportional to the difference in temperature between the two junctions and is given by
V = α (T2-T1) (222)
This Seebeck effect is observed not only in metals but also in semiconductors
Here α is known as the Seebeck coefficient α measures the magnitude of an induced
thermoelectric voltage in response to the temperature difference across the material If the
temperature difference ∆T between the two ends of a material is small then the Seebeck
coefficient of a material is written by
α = ∆V∆T (223)
36
This can be expressed in terms of electric field as
α E∆T (224)
The units of Seebeck coefficient is given as VK The higher the Seebeck coefficient
value the better it is since it will create a very large voltage that can be used to provide
power
282 Peltier Coefficient
Peltier effect is the inverse of Seebeck effect involving a junction phenomenon There is
heat absorption or generation at the junctions depending on the direction of current flow
Heat generated by current flowing in one direction is absorbed if the current is reversed
The heat absorbed per second at a junction carrying current I is given by
Heat absorbed in t sec = πabIt (225)
Here πab is the Peltier coefficient and given by HIt Thus Peltier coefficient is
numerically equal to the applied potential difference expressed in Volts
Overall by studying the flow of electrons the values of Seebeck
coefficient and Peltier co-efficient can be estimated These values determine the various
applications of the materials In this thesis the Peltier and Seebeck coefficient of the
graphene junction and the new applications are discussed
37
29 Early Research ndash ab intio studies
In 2007 Androitis studied that the conducting properties of graphene nanoribbons and
junctions are strongly dependent on their size and geometric features35
He concluded that
there is no conductance for small AZA or ZAZ ribbons (Figure 213)
Figure 213 Transmission functions in units of (2e
2h) for AZA structures
35
Figure 213 shows that T (E) exhibits a negligible peak [T (E) = 001 in units of
2e2h] at E= -225 and 250eV However it was noted that when the width of the arm type
was increased T (E) at -225 and 250eV was 02035
Later in 2007 Qimin Yan used first principles methods to investigate the Current-
Voltage characteristics of GNR Transistors and the effect of edge doping He showed that
GNR field effect transistors can achieve high performance levels with ONOFF ratios on
the order of 103-10
436
Figure 214 is an I-V curve of AZA GNR-FET connected via
armchair metallic leads36
38
Figure 214 I-V curve for a 591nm long channel (Vbias=20mV)
36
In 2009 Fangping OuYang demonstrated the intrinsic transport properties and
effective B or N doping of the junctions by using first-principles quantum transport
simulations He concluded that the I-V characteristics of pure-carbon T-shaped junctions
exhibit metallic behavior and the current in the junction strongly depends on the height
of the stem23
He reported that the conductance of the devices depends on the geometric
structures which can be controlled by selective doping
In 2012 Wei Yao used the first principle calculations based on Density
Functional Theory (DFT) and Non-equilibrium Greens Function (NEGF) to study the
electronic as well as the transport properties of B-doped 6-GNR p-n junction His results
showed that the boron doping interval can influence the rectification effect at low bias
and also exhibit Negative Differential Resistance (NDR) phenomena at high positive
bias
39
CHAPTER 3
COMPUTATIONAL DETAILS
31 Introduction
The physical chemical electrical electronic and optical properties of a solid are
determined by their quantized electronic states The quantum states in low-dimensional
systems are produced due to the confinement of the carrier charges in one or two
dimensions Graphene is a conductor electrons are able to flow through graphene more
easily than through even copper The electrons can travel through the sheet of graphene
like mass-less particles as fast as just one hundredth that of the speed of light The ways
in which electrons behave in graphene make it very helpful to study their fundamental
physical properties Graphenersquos near perfect crystal lattice provides a very clean system
to experiment By restricting the electrons to only two dimensions they exhibit some
interesting properties such as the anomalous quantum Hall effect and Klein tunneling
In this chapter two theoretical concepts used for calculating the electronic structure
and the transport properties for graphene are described These include the Extended
Huckel Theory and Non-Equilibrium Greenrsquos Function (NEGF) method
311 Extended Huckel Theory
Erich Huumlckel was born in Germany on August 9th
1896 He studied mathematics and
physics in Berlin He is best known for his work in the field of chemistry and physics for
two contributions (1) Debye- Huumlckel theory of electrolytic solutions (2) Huumlckel
method of approximate molecular orbital calculations on electron systems In 1930 he
published his findings on systems in 1931 he generalized and expanded the system
40
theory to explain benzene Due to his poor communication skills his findings went
unrecognized for over 20 years It was in 1951 that his 4n + 2 rule was finally clarified by
Doering to show if C=C bonds would show aromaticity Huumlckel died on February 16th
1980 with very little worldwide recognition for his contributions to chemistry Today
chemistry students recognize his name and his contributions to the field are quite
substantial
One of the first semi-empirical methods to be developed was Huumlckel Molecular
Orbital Theory (HMO) HMO was developed to describe molecules containing
conjugated double bonds HMO considered only electrons in pi orbitals and ignored all
other electrons in a molecule The Extended Huumlckel Molecular Orbital Method (EH) was
developed out of the need to consider all valence electrons in a molecular orbital
calculation
By considering all the valence electrons chemists could determine molecular
structure compute energy barriers for bond rotations and determine energies and
structures of transition states for reactions By considering only the valence electrons the
computed energies could be used to choose between proposed transition states to clarify
reaction mechanisms The total valence electron wavefunction is described as a product
of the one-electron wave functions
1 2 3(1) (2) (3) ( )valence j n (31)
where n is the number of electrons and j identifies the molecular orbital Each
molecular orbital is written as a linear combination of atomic orbitals (LCAO)
1 12
N
j jr rrc j N
(32)
41
The energy of the jth
molecular orbital is given by a one-electron Schroumldinger
equation using an effective one electron Hamiltonian heff which expresses the interaction
of an electron with the rest of the molecule
eff j j jh (33)
This is the energy eigenvalue of jth
molecular orbital corresponding to the Eigen
function j The advantage of using this method is that the exact form of heff is not
required The total energy of the molecule is the sum of the single electron energies
j jj
E n (34)
where nj is the number of electrons in orbital j
In order to use the Extended Huckel method a set of calculation parameters and
approximations must be followed These parameters include the Basis set K-point and
the Brillouin Zone and lastly the Mesh cut-off
312 Introduction to NEGF
The Greenrsquos function is a function of two space-time coordinates From the knowledge of
this function one can calculate time-dependent expectation values such as currents and
densities electron addition and removal energies and the total energy of the system In
the absence of external fields the non-equilibrium Green function method reduces to the
equilibrium Green functions NEGF can be applied to both extended and finite systems
The generic system of NEGF consists of the electron dynamics of the channel described
by the Hamiltonian This channel consists of two contact reservoirs with respective
chemical potential μR and μL The NEGF assumes ballistic transport neglecting self-
42
energy from scattering The system is insulated from gate contacts whose effects are
realized via a 3D Poisson solver which solves for the potential at a given point in real
space based on electron density
22 ( ) [ ( ) ( )]D
qr N r n r
(35)
Figure 31 NEGF system
The system is easily expandable to systems with several contacts or gate
configurations by adding additional self-energy matrices to NEGF or additional sources
to the Poisson solver
313 Electrostatics
Electrostatic potential is created every time in the presence of a charge density due to an
induced electric field The Poissonrsquos equation correlates the electrostatic potential to
charge density as given in Equation 36
43
2( ( ) ( ) ( ) ( ))( )
( )( ) ( )
ADq p r n r r N rr
rr r
N
(36)
where ɛ(r) is the dielectric permittivity of the material ρ(r) n(r) ND(r) and NA(r) are the
hole electron donor and acceptor concentrations of the system respectively
Two types of boundary conditions are usually applied to the Poissonrsquos equation
Dirichlet boundary conditions
Φ (0) = F0 and Φ (L) = FL
von Neumann boundary conditions
00
( )
x
d x
dxB
and
( )L
x L
d x
dxB
For the transport problems with open boundary conditions the von Neumann
boundary conditions are used assuming that the potential vanishes at the boundary ie
B0=BL=0
The Poissonrsquos equation can hence be discretized on a grid as
2 ( )( )
( )
rx
r
= M (37)
where M is the matrix Φ and ρ are vectors containing the discretized values of
the electrostatic potential Φ and charge density ρ respectively
44
The Schroumldinger and Poisson equations are coupled since V(x) = -qΦ(x) is used
for the Schroumldinger to compute ρ(x) This self-consistent loop stops when the
convergence is reached
( )r
V(x) = -qΦ(x)
314 Non-Equilibrium Greenrsquos Function
Greenrsquos functions are a mathematical construction that are used to solve differential
equations subject to specific initial or boundary conditions They are named after the
British mathematician George Green The 1-D equation of L( )f( )=S( ) can be defined
by the Greenrsquos Function as given below
( ) ( ) ( )G x x f x x x (38)
The general Greenrsquos function is given by
( ) ( ) ( )f x dx G x x S x (39)
Applying the operator L( ) to the solution f( ) satisfies the original differential
equation The Greenrsquos Function G( ) is the propagator which propagates the influence
of a perturbation S( ) originally situated at the point to the point at which the
function f( ) is evaluated
The Greenrsquos Function G( ) can also be a correlation function If the points
and are strongly (weakly) correlated then S( ) will greatly (poorly) affect f( )
Poisson equation
2 ( )( )
( )
rr
r
Schroumldinger equation
2
2
( ( ) ) ( )
( )2
( ) | ( ) |
E H r E r S
H V rm
r dE E r
Figure 32 Self-consistent loop
45
The Schroumldinger equation with open boundaries can be written as
( )E H S (310)
Considering a 1-D and homogenous system ranging from =0 to L assuming
that Σ=0 and the form of equations is same before and after discretization then
22
2 0( ) ( ) ( )
2E x S x
m
dV
dx
(311)
The Greenrsquos function can hence be computed corresponding to the Schroumldinger
equation
22
2 0( ) ( ) ( )
2E G x x x x
m
dV
dx
(312)
Due to the delta-function at = a discontinuity is observed and hence the
Greens function is evaluated at boundary conditions
0
2
exp( ( )) x x 2 ( )( )
exp( ik(x x)) x x
ik x x m E VG x x k
A
A
(313)
By integrating the Schroumldinger equation twice and setting the lower and upper
integration boundaries to = -δ and = +δ the Greenrsquos Functions can be written as
2
( ) ( ) 0
( ) ( ) 2
x x x x
G x x G x x
dG x x dG x x m
dx dx
(314)
46
The coefficient A+ and A
- become
ik
mA A
(315)
The Greenrsquos Function takes a final form known as Retarded Greenrsquos Function and
is written as
( ) exp( | |)G x x i ik x xk
m (316)
And the wave function is
( ) ( ) ( )x dx G x x S x (317)
Retarded Greenrsquos Function propagates the wave functions generated by a source
or perturbation S from its origin at to any point
The retarded Greenrsquos Function as discretized Schroumldinger equation is written as
( )R RE H G I (318)
The wave function Φ can be calculated from the retarded Greenrsquos function and the
source vector as
Φ = GR∙S (319)
Overall in this section the Greenrsquos function approach in calculating the electron
dynamics is reviewed We defined the self-energy of each part of the system spectral
function and the probability current density the electric current is derived explicitly using
Non Equilibrium Greenrsquos function We will use this formalism to calculate the tunneling
phenomena in coupled quantum dots isolated or otherwise
47
CHAPTER 4
ATOMISTIX TOOLKIT DETAILS
41 Introduction
Virtual NanoLab (VNL) is a graphical user interface (GUI) that provides a group of
modeling tools the function of these tools involves the set-up investigation and the
study of nanoscale structures The quantum mechanical equations are solved by the
software by using the advanced software architecture and numerical methods to
implement ab initio calculations VNL simulates the electronic structure and calculates
the transport properties based on the two systems mentioned earlier NEGF and Extended
Huckel ATK is the main engine for computing the scripts and hence all the calculations
performed in VNL are done by ATK VNL is a user friendly software as it not only
allows creating a script but also helps to set up a virtual experiment
This thesis involves the use of VNL in order to study the effect of the width and
different orientations of the doped atoms Since the software allows for virtual
experiments it makes it much easier to study the I-V characteristics based on the change
in position of atoms
42 Device Structure
In this thesis AZA GNR p-n junction with boron doping (location) was created using the
ATK software which is based on NEGF and DFT Further the thesis discusses the
transport properties and the I-V curve of such junction
The input format of ATK is NanoLanguage which is an extension to Python
scripting language ATK uses the NEGF system for formalism of simulating device
48
Figure 41 Geometry of device configuration with two electrodes
37
The system is divided into three parts left central and right The implementation
relies on the screening approximation which assumes that the properties of the left and
right regions can be decribed by solving a bulk problem for fully periodic electrode cell37
This screening approximation is fulfilled when the electrode regions can be described by
an equilibrium electron distribution
Figure 42 The electron distribution in a device configuration which illustrates a left
moving scattering state with origin in right electrode37
The system assumes that in steady state the electron density of the central region
is constant in time and hence the electron density is calculated independently from each
electrode The electron density is given by the occupied eigenstates of the system
n(r) = nL(r) + n
R(r) (41)
49
The left and right densities are calculated by summing up the occupied scattering
states
nL(r) = sum
(42)
nR(r) = sum
(43)
The scattering states are usually calculated by first calculating the Bloch states in
the electrodes and then solving the Schroumldinger equation of the central region using the
Bloch state as matching boundary Instead of using the scattering states the ATK
software uses the NEGF method to calculate the non-equilibrium electron density
The electron density is given in terms of electron density matrix
D = DL + D
R (44)
The left density matrix is given by NEGF theory
DL = int
(45)
where
ρL(ɛ) =
(46)
ρL(ɛ) = is the special density matrix
Also if there is a non-equilibrium electron distribution in the central region then
the electron distribution in electrode is given by the Fermi function f with an electron
temperature TL
G(ɛ) =
(47)
G = retarded Green function
δ+ is an infinitesimal positive number and S H overlap the Hamiltonian matrices
L =
sum sum
(48)
50
L
is the broadening function of the left electrode given in terms of left electrode
self -energysum
43 Transmission Spectrum Calculations
Once the self-consistent non-equilibrium density matrix has been obtained the various
transport properties of the system can be calculated One of the most important properties
is the transmission spectrum from which the current and differential conductance can be
obtained
The transmission coefficient in ATK is obtained by the retarded Greens function
T(ɛ) = G(ɛ)ΓL(ɛ)G
ϯ(ɛ)Γ
R(ɛ) (49)
The transmission amplitude of individual scattering states may be obtained
through the Transmission Eigenvalues The ldquoTransmission Eigenvaluesrdquo is an analysis
which finds the eigenvalues of the transmission matrix
The transmission matrix at energy E and k-point is given by
Tnm(Ek) = sum (410)
where
= transmission amplitude from Bloch state ψn(k)
The transmission coefficient is given by the trace of transmission matrix
T(Ek) = sum (411)
Keeping in mind all quantities depend on the quantum numbers parametrically
Transmission eigenvalues sum up to the transmission coefficient
T = sum (412)
51
44 Calculating the Current
Current is calculated from the transmission coefficient using
I( ) ( )R L
L RL R
R LB B
eE f f dE
h
E EV V T T T
k kT T
(413)
where f is the Fermi function TRL is the electron temperature of the right or left
electrode and Tσ(E) is the transmission coefficient for the spin component σ
The chemical potentials of the left and right electrode given by
L
F R LR L
eVE
are defined relative to the Fermi level of the left electrode These chemical potential are
related to the applied bias and hencebiasR L
eV therefore bias L RV V V
The transmission spectrum itself is usually rather insensitive to temperature and is
used in self-consistent calculations but often depends strongly on the electrode voltages
Thus for an accurate estimate of the current the transmission spectrum should be
calculated self-consistently for each desired bias
ATK uses very precise method to calculate the transport properties of the system
Transmission spectra for various concentrations of boron doped graphene p-n junctions
are generated in this Chapter and various coefficients such as Seebeck Peltier and
Conductance are calculated
52
45 Calculating Transport coefficients
The linear response transport coefficient of an applied voltage difference or temperature
difference between the two electrodes is given by
Conductance
| dT 0
e
dI
dUG
(414)
Peltier coefficient
| d 0
Q
I
I
(415)
Seebeck coefficient
| 0
dUS I
dT T
(416)
These linear response coefficients are calculated by the Transport Coefficients To
perform these calculations the ATK uses the Electron Transmission Spectrum
53
CHAPTER 5
RESULTS AND DISCUSSION
51 Band Structure Analysis
The electronic bandstructure of GNR both doped and undoped are discussed in this
chapter
The armchair configuration of Pristine GNR (PGNR) has a band structure that is
dependent on its width This is explained by the fact that the sheet itself acts like a
potential well where the electrons are confined to form standing waves along Cr the
rolling vector albeit with slightly different boundary conditions (Cr = ma1 + na2
where m and n are integers and a1 and a2 are the unit cell vectors of graphene lattice) In
a GNR the two nodal points of the standing wave must be at the ribbon edge while in a
Single wall nanotube (SWNT) they can be anywhere ie a circumferential periodic
boundary condition
(a) (b)
Figure 51 Bandstructure of AGNR widths (a) 4 atoms (b) 5 atoms
54
(a) (b)
Figure 52 Bandstructure of AGNR widths (a) 6 atoms (b) 7 atoms
(a) (b)
Figure 53 Bandstructure of AGNR widths (a) 8 atoms (b) 9 atoms
55
(a) (b)
Figure 54 Bandstructure of AGNR widths (a) 10 atoms (b) 11 atoms
Figure 55 Bandstructure of AGNR with a width of 12 atoms
Figure 56 Variation in band gaps as the width (number of atoms) varies
0
05
1
15
2
25
0 2 4 6 8 10 12 14
Wdith vs Band Structure
eV
56
The band structure of 12 Atom AGNR is close to that of Ge (0626 eV) The
actual width of this nanoribbon is about 25 nm 12 AGNR has been fabricated
successfully and doped with various dopants Hence the 12 Atom AGNR has been chosen
to study the transport properties
A junction is created using ZGNR and AGNR To maintain the consistency in the
device analysis it is imperative that the band structure of ZGNR is also calculated From
the simulation it is evident that ZGNR-AGNR-ZGNR junction configuration displays the
Metal ndashSemiconductor-Metal configuration that is addressed in this work The Fermi
Level in all the Z-GNR nanoribbons of widths 4-12 lies within the conduction band
Figure 57 Band structure of ZGNR width (a) 4 atoms (b) 6 atoms
57
(a) (b)
Figure 58 Band structure of ZGNR width (a) 8 atoms and (b) 10 atoms
Figure 59 Band structure of ZGNR with a width of 12 atoms
In order to create viable junction that would show transistor properties doping of
the semiconductor part is necessary The 12 atom AGNR is doped with boron (p-type)
and nitrogen (n-type) - (Figure 510a) 4 N doped (Figure 510b) 4 B In both cases
the impurities lie on the edge of the atoms For 2 nitrogen doped GNR with the
58
impurities lying in the center of the ribbon the Fermi level is found to be in the
conduction band as shown in (Figure 510c) (Figure 510d) shows the position of N with
respect to the edge A very clear departure from the expected (the valence band extending
above Fermi level) is shown in (Figure 510a)
Figure 510 Band structures of Doped AGNR (a) 4 N Doped (b) 4 B Doped (c) 2
N Doped (d) position of Nitrogen from (c)
(a) (b)
(c) (d)
59
52 I-V Characteristics of GNR junction
In pristine graphene the chirality determines the conductivity as seen from the I-V curves
for various widths At certain widths the semiconducting properties are more
pronounced These widths determine the wavelengths of the standing waves which in
turn determine the sub-band locations in the E-k plot When the biasing potential
exceeds 012V the I-V curve shows linearity In case of the 8-atom wide PGNR the
band gap is about 03 eV and it is evident from the I-V plot that the On-State is + 033 V
The band gap of 10-atom and the 4-atom wide PGNR is large enough to show
semiconducting properties
Figure 511 Current Vs Voltage graph for varying graphene width showing
conductivity
-30000
-20000
-10000
0
10000
20000
30000
-3 -2 -1 0 1 2 3
Cu
rre
nt
(nA
)
Voltage (V) (bias)
Current (nA) Vs Voltage for varying graphene width
W=10
W=8
W=6
W=4
60
The ZAZ GNR Configurations show the properties of a semiconductor junction The 12
atom ZAZ structure is studied for its I-V characteristics In this Chapter undoped B-
doped N-Doped B and N Doped (P-N Junction) ZAZ junctions are simulated
Figure 512 ZAZ GNR junction device
61
The boron doped ZAZ junction I-V characteristics are shown below (Figure 513)
The impurity concentration is 2 and 4 Various device configurations are studied
Figure 513 I-V curve of Boron Doped ZAZ junction
-25000
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
25000
-205 -155 -105 -055 -005 045 095 145 195
Cu
rre
nt
(nA
)
VBias
2B_1G_R 2B_0G_R
4B_0G_L 4B_0G_C
4B_0G_R 4B_1G_L
4B_1G_C 4B_1G_R
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
-2 -1 0 1 2
Cu
ren
t(n
A)
VBias
4 B doped GNR Jn
62
Figure 514 I-V curve of Nitrogen Doped ZAZ
-25000
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
-2 -15 -1 -05 0 05 1 15 2
Cu
rre
nt(
nA
)
VBias
I-V Curve as function of Dopant location
2N_0G_L2N_0G_C2N_0G_R2N_1G2N_1G_C2N_1G_R
-15000
-10000
-5000
0
5000
10000
15000
-2 -1 0 1 2
Cu
rre
nt(
nA
)
VBias
2N_0G_C
2N_1G_C
63
Figure 513 and Figure 514 show the I-V characteristics of the GNR junction doped with
2 boron and nitrogen respectively The location of N and B is at the central region of
the edge of the GNR Both B doped and N doped GNR Junctions show significant
Negative Differential Resistance (NDR) This is more pronounced in case of nitrogen
doping Another interesting observation is increasing ohmic nature with the change in
location of the dopants Nitrogen doped device configuration exhibits a pronounced
semiconductor behavior and the NDR effect is observed to be minimal
53 Thermoelectric Properties
In this study the thermoelectric properties were simulated for the GNR Junctions that
displayed high NDR effect The variation in the Peltier coefficient with temperature is
shown as function of doping
When the concentration of nitrogen increases the dimensionless Figure of Merit
ZT seems to decrease considerably This is mostly explained by the decrease in both
conductivity and mobility of the electrons
ZT = S2σTk (51)
where S is the Seebeck coefficient σ is the electrical conductivity T is the
absolute temperature and k is the thermal conductivity
64
Figure 515 Variation of Peltier coefficient with temperature as function of
doping
Figure 515 shows the maximum Peltier coefficient for 2 boron This is
explained by the scattering by boron and the associated smallest mean free path
0
0001
0002
0003
0004
0005
0006
0007
0008
0009
001
250 270 290 310 330 350 370 390 410
ZT
T (K)
2B
4B
Undoped
2N
4N
65
CHAPTER 6
CONCLUSIONS
Graphene ZAZ junctions exhibit varying properties depending on the various structural
configurations In this thesis it was found that the transport properties of graphene
depend on their width the edge of GNR doping concentration and the type of dopant
used The calculations of the band structure contributed towards the determination of the
minimum length of GNR required for studying the transport properties The minimum
length had a band gap equivalent to that of germanium and hence the importance of the
width being 12 atoms wide This band gap indicated fluctuating changes when doped
with elements such as B and N The viable junction showing transistor properties was
hence created by doping the semiconductor part of ZAZ By doping the I-V
characteristics were studied which showed significant NDR which was more pronounced
in the case of nitrogen Also the changing positions of the dopants contributed towards
the I-V curve to be more ohmic The edge doping caused minimum NDR and
semiconductor behavior as compared to central doping Lastly the thermoelectric
properties were studied - the increasing concentration of N causes the Figure of Merit to
decline due to the decrease in conductivity as well as mobility of electrons
66
REFERENCES
1 Wikianswers What makes carbon unique
httpwikianswerscomQWhat_makes_carbon_so_unique (22 November)
2 Kopeliovich D D Graphite
httpwwwsubstechcomdokuwikidokuphpid=graphite (1128)
3 Barbier M Transport properties of nanostructures and superlattices on single layer and
bilayer graphene University Antwerpen Antwerpen 2012
4 Shylau A Electron transport interaction and spin in graphene and graphene
nanoribbons Linkoping Norrkoping 2012
5 HassJ R F T Li X Li Z Zong W A de Heer P N First E H Conrad C
AJeffrey and C Berger Applied Physics Letters 2006 89 (14) 143
6 Jones A Mechanical Exfoliation to Make Graphene and Visulization
httpcarbonchemwisceduFilesMechanicalExfoliationpdf (18 October)
7 Anteroinen J Structural and Electrical Characteristics of Graphene Field Effect
Transistors AALRO school of Electrical Engineering AALTO 2011
8 Novoselov K S A K G S V MorozovD JiangY Zhang S V Dubonos I V
Grigorieva A A Firsov Science 2004 306 (22)
9 Kosynkin D A L H A Sinitskii J R Lomeda A Dimiev K B Price and J M
Tour Nature 458 876
10 Yi Z Luyao Zhang Accounts of chemical research 46 (10) 2339
11 Eizenberg M B JM 1979 82 236
12 Yu Q K L J Siriponglert S Li H Chen Y P Pei S S Applied Physcis
Letters 2008 93 (113103)
13 Li X C W An J Kim S Nah J Yang D Piner R Velamakanni A Jung I
TutucE Banerjee S K Colombo L Ruoff R S Science 2009 324 1314
14 Schaefer H E Nanoscience Springer Berlin 2010
15 Levente Tapasztoacute G D Philippe Lambin amp Laacuteszloacute P Biroacute Nature Nanotechnology
2008 3 401
67
REFERENCES
16 Dacheng Wei Y L Advance Materials 2010 22 (30) 3241
17 Wei Yao K L Y GYGao Elsevier Solid State Communications 2013 153 52
18 Dacheng Wei Dagger Yunqi Liudagger Yu Wangdagger Hongliang ZhangdaggerDagger Liping HuangdaggerDagger
Yudagger a G NanoLetters 2009 9 (5) 1758
19 Nakada K M F G Dresselhaus and M S Dresselhaus PhysRevB 1996 54
(9858)
20 Son Y W C M L a L S G PhysRevLett 2006 97 (216803)
21 Raza H Graphene Nanoelectronics Springer 2012
22 Ryan W J Electronic Transport in Graphene p-n junctions Short Noise and
Nanoribbons Harvard University 2009
23 Fangping OuYang J X Rui Guo Hua Zhang and Hui Xu Nanotechnology 2009
20 6
24 Guo J Carbon nanotube electronicsModeling physics and applications Purdue
University West Lafayette IN 2005
25 Motta C S S-P MITrioni cond-matmes-hall 2012 7
26 B P Growing Graphene via Chemical Vapor Deposition Ponoma College Ponoma
2011
27 ZurichE Transport properties of three-terminal graphene devices University of
Science and Technology Norway 2008
28 Uichiro MIntroduction to the electron theory of metals
29 Robert Laughlin H S Additional background material on the Nobel Prize in Physics
1998 (410)
30 MarkGoerbig Quantum Hall Effects (11152013)
68
REFERENCES
31 Zurich E Transport properties of three-terminal graphene devices Norwegian
University of Science and Technology Norway 2008
32 Deepak R Klein Tunneling University og Tennessee Space Institute Tennessee
2011
33 Williams JR L D CMMarcus Quantum Hall Effect in a Gate-Controlled p-n
Junction in Graphene (1122013)
34 Avadhanulu MN P G K A Textbook of Engineering Physcis for BE BSc (Engg)
SChand New Delhi 1992
35 Andriotis A Applied Physics Letters 2007 91 (152105)
36 Qimin Yan B H dagger Jie Yudagger Fawei Zhengdagger Ji ZangDagger Jian Wudagger Bing-Lin Gu F
L Dagger and Wenhui Duandagger NanoLetters 2007 7 (6) 1473
37 Soler J M E A J D Gale A Garciacutea J Junquera P Ordejoacuten and D Saacutenchez-
Portal J Phys Condens Matter 2002 14 2745
The Van Houten library has removed some of the personal information and all signatures from the approval page and biographical sketches of theses and dissertations in order to protect the identity of NJIT graduates and faculty
ABSTRACT
ANALYSIS OF TRANSPORT PROPERTIES OF A ZAZ GRAPHENE
NANORIBBON JUNCTION USING VARIOUS DOPANTS
by
Natasha Parikh
A 12 atom wide ZAZ Graphene Junction was simulated and its transport properties were
analyzed I-V curves calculated by nonequilibrium Greens function method combined
with the density functional theory under external bias showed varying semiconducting
characteristics Further the width of the junction also showed significant effects in the
determination of the semiconducting nature A theoretical study was performed on the
semiconducting characteristics by analyzing the I-V curve and transport coefficients in
the junction
ANALYSIS OF TRANSPORT PROPERTIES IN A ZAZ GRAPHENE
NANORIBBON JUNCTION USING VARIOUS DOPANTS
by
Natasha Parikh
A Thesis
Submitted to the Faculty of
New Jersey Institute of Technology
in Partial Fulfillment of the Requirements for the Degree of
Master of Science in Materials Science and Engineering
Interdisciplinary Program in Materials Science and Engineering
January 2014
APPROVAL PAGE
ANALYSIS OF TRANSPORT PROPERTIES IN A ZAZ GRAPHENE NANORIBBON JUNCTION USING VARIOUS DOPANTS
Natasha Parikh
Dr N M Ravindra Thesis Advisor Date Director of Material Science and Engineering Program NJIT Dr Keun H Ahn Committee Member Date Associate Professor of Physics NJIT Dr Tao Zhou Committee Member Date Associate Professor of Physics NJIT Dr Halina Opyrchal Committee Member Date Senior University Lecturer of Physics NJIT
BIOGRAPHICAL SKETCH
Author Natasha Parikh
Degree Master of Science
Date January 2014
Undergraduate and Graduate Education
bull Master of Science in Materials Science and EngineeringNew Jersey Institute of Technology Newark NJ 2014
bull Bachelor of Arts in Physics and Biological SciencesRutgers the State University of New Jersey New Brunswick NJ 2012
Major Materials Science and Engineering
iv
v
ACKNOWLEDGMENTS
I would like to express my gratitude to my supervisor Dr NM Ravindra for the useful
comments remarks and engagement throughout the learning process of this Mastersrsquo
thesis Furthermore I would like to thank Vijay Kasi Somayajula for introducing me to
the topic as well for the support I thank Dr Tao Zhou Dr Ken Ahn and Dr Halina
Opyrchal for serving on my thesis Committee I would like to thank my loved ones who
have supported me throughout the entire process both by keeping me harmonious and
helping me in putting pieces together
vi
TABLE OF CONTENTS
Chapter
Page
1 INTRODUCTIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
1
11 Graphene The New Carbonhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
1
12 Graphene Synthesishelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
3
121 Synthesis of Graphene on Nickel (Ni)helliphelliphelliphelliphelliphelliphelliphellip
5
122 Synthesis of Graphene on Copper (Cu)helliphelliphelliphelliphelliphelliphelliphellip
8
123 Transfer of Graphene Filmshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
8
124 Synthesis of Graphene Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
9
125 Doping in Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
10
126 Nitrogen (N) Doped Graphene Synthesis (Substitutional)hellip
12
13 Structure of Graphene Nanoribbon (GNR)helliphelliphelliphelliphelliphelliphelliphelliphelliphellip
13
14 Overview of Graphene Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
15
2 RESEARCH BACKGROUNDhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
21 Bandstructure of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
22 Transport Characteristics of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
20
23 Drude Theoryhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
22
24 Quantum Hall Effect (QHE)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
24
25 Resistivity and Resistancehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
27
26 Klein Tunnelinghelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
28
27 Quantum Hall Effect in Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
31
28 Thermoelectric Effecthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 34
vii
TABLE OF CONTENTS
(Continued)
Chapter Page
281 Seebeck Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
34
282 Peltier Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
36
29 Early Research ndash ab initio Studyhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
37
3 COMPUTATIONAL DETAILShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
31 Introductionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
311 Extended Huckel Theory helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
312 Introduction to NEGFhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
41
313 Electrostaticshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
42
314 Non-Equilibrium Greenrsquos Functionhelliphelliphelliphelliphelliphelliphelliphelliphellip
44
4 ATOMISTIX TOOLKIT DETAILShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
41 Introductionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
42 Device Structurehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
43 Transmission Spectrum Calculationhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
50
44 Calculating the Currenthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
51
45 Calculating the Transport Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
52
5 RESULTS AND DISCUSSIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
53
51 Band Structure Analysis helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
53
52 I-V Characteristics of GNR Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
59
53 Thermoelectric Propertieshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
63
6 CONCLUSIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 65
REFERENCEShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
66
viii
LIST OF FIGURES
Figure Page
11 (a) Chemical representation of Carbon (b) Graphite ore (c) Structure of
Graphite and a single layer Graphenhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
2
12 An optical image of Graphene flake obtained by exfoliation of
graphitehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
3
13 (a) Graphene formation on Nickel (b) Graphene atoms on Ni (111)
lattice (c)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
7
14 (a) SEM image of graphene on copper foil (b) High-resolution SEM
image of graphene on Cuhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
8
15 (a) Transfer process (b) Wafer-scale synthesis of graphene (c) Graphene
films transferred onto glass wafer (d) SiSiO2 with device patterned (e)
PET filmhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
9
16 (a) High-magnification image of the annealed sample showing that well-
defined zigzag armchair and zigzag-zigzag edges are formed (b) ) STM
image of an 8 nm wide bent junction connecting an armchair and a
zigzag graphene nanoribbon which was carved by STM
tipshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
10
17 Band structure of graphene before and after doping The image shows
shift towards the Fermi levelhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
11
18 Low resolution TEM image of N-doped graphene Background is the
lacey carbon TEM grid graphene sheet is crumpled with many
rippleshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
13
19 Zigzag and Armchair orientation of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphellip 13
110 Bandstructure of ZGNRhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 14
111 Bandstructure of AGNRhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 15
21 Left Real space Graphene lattice with basis vectors and Right
The first Brillouin zone of Graphene in reciprocal space with basis
vectors and K and Krsquo are responsible for massless transport at low
energyhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
ix
LIST OF FIGURES
(Continued)
Figure Page
22 Bandstructure of a graphene sheet showing a band gap of 0eVhelliphelliphellip 18
23 Band structure of Graphene calculated with the tight-binding modelhellip 19
24 The energy dispersion around the K pointhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 22
25 Electrons colliding with stationary ionshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 23
26 (a) 2D electrons in a perpendicular magnetic field Logitudinal resistance
measured across C5 and C6 Transverse resistance measured across C3
and C5 (b) Classical Hall resistance as a function on the magnetic field
25
27 Klein tunneling through an npn barrierhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 29
28 Electron trajectory considering the linear electrostatic potential U(x) = Fx 30
29 Electron like and hole like trajectories at same Ehelliphelliphelliphelliphelliphelliphelliphelliphellip 30
210 Quantum Hall effect in graphene 22
The Hall conductivity σxy and the
longitudinal resistivity of monolayer graphene as a function of carrier
density at B = 14T and T= 4K This shows half-integer QHE with chiral
index J= 1helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
32
211 (a) LL for Graphene bilayer (b) Schematics of Hall conductivity as a
function of nn0 for bilayer Graphene (solid line) and monolayer
Graphene (dotted line) (c) LL for monolayer Graphenehelliphelliphelliphelliphelliphelliphellip
33
212 Seebeck Effecthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 35
213 Transmission functions in units of (2e2h) for AZA structureshelliphelliphelliphellip 37
214 I-V curve for a 591nm long channel (Vbias=20mV)helliphelliphelliphelliphelliphelliphelliphellip 38
31 NEGF systemhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 42
41 Geometry of device configuration with two electrodeshelliphelliphelliphelliphelliphelliphellip 48
42 The electron distribution in a device configuration which illustrates a left
moving scattering state with origin in right electrodehelliphelliphelliphelliphelliphelliphelliphellip
48
x
LIST OF FIGURES
(Continued)
Figure Page
51 Band structure of AGNR widths (a) 4 atoms (b) 5 atomshelliphelliphelliphelliphelliphellip
53
52 Band structures of AGNR widths (a) 6 atoms (b) 7 atomshelliphelliphelliphelliphelliphellip 54
53 Band structure of AGNR widths (a) 8 atoms (b) 9 atomshelliphelliphelliphelliphelliphelliphellip 54
54 Band structures of AGNR widths (a) 10 atoms (b) 11 atomshelliphelliphelliphelliphellip 55
55 Band structure of AGNR with a width of 12 atomshelliphelliphelliphelliphelliphelliphelliphelliphellip 55
56 Variation in band gaps as the width (number of atoms) varieshelliphelliphelliphellip 55
57 Band structure of ZGNR width (a) 4 atoms (b) 6 atomshelliphelliphelliphelliphelliphelliphellip 56
58 Band structure of ZGNR width (a) 8atoms and (b) 10 atoms 57
59 Band structure of ZGNR with a width 12 atomshelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 57
510 Band structures of Doped AGNR (a) 4 N Doped (b) 4 B Doped (c)
2 N Doped (d) position of Nitrogen from (c)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
58
511 Current Vs Voltage graph for varying graphene width showing
conductivityhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
59
512 ZAZ GNR junction devicehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 60
513 I-V curve of Boron Doped ZAZ junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 61
514 I-V curve of Nitrogen Doped ZAZhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 62
515 Variation of Peltier effect coefficient with temperature for various doping 64
1
CHAPTER 1
INTRODUCTION
11 Graphene The New Carbon
Carbon (chemical symbol C atomic mass 1207amu) (Figure 11a) is a widely distributed
element in nature It is found abundantly in the sun stars comets and the atmospheres of
the planet Carbon can form up to four bonds it can bond with itself endlessly and with
most other elements in many different shapes making it a significant part of the
construction for many kinds of complex molecules1
Two allotropes of carbon are commonly used diamond and graphite (Figure
11b) The bonding structures of diamond and graphite contribute to the properties
individually In diamond all the p-orbitals are used forming a sp3
bonding whereas in
graphite only two orbitals are occupied allowing the unpaired bond for the transport of
electrons Each carbon atom in graphene possesses sp2 hybridization ie each carbon
atom is connected to three other carbon atoms via covalent bonds with a bond length of
142Å and an angle of 120deg between each bonded pair This makes graphite a better
conductor than diamond Graphite consists of many layers of 2D carbon lattices (Figure
11c) stacked on top of each other and held via Van der Waals forces A single layer of
graphite where carbon atoms are arranged in a honeycomb lattice is known as graphene
(Figure 11c)
2
Figure 11 (a) Chemical representation of Carbon (b) Graphite ore (c) Structure of
Graphite and a single layer Graphene2
Theoretical work on graphene was done specifically to study the other allotropes
The first study was done by Wallace in 1947 who calculated the band structure of
graphene3 Further the peculiar Landau levels were known by McClure in 1957 and the
relativistic Hofstadter butterfly by Ramal in 19853 Later in 1991 the invention of carbon
nanotubes by Iijima boosted the theoretical research on graphene3 Prior to the invention
of carbon nanotubes there were a few experimental papers on graphene growth via
various methods like intercalation of graphite (Shioyama 2001) free standing (Boehm
1962) epitaxial as well as graphene grown on metals (Bommel 1975 Land 1992 Itoh
1991)3 With all the various discoveries the electronic properties of graphene were not
studied until 2004 when Berger and Novoselov were able to access the electronic
properties with contact of graphene flakes3 (Figure 12)
3
Figure 12 An optical image of Graphene flake obtained by exfoliation of graphite3
The specific lattice structure of graphene possesses a number of unique electronic
properties making it an interesting material for theorists experimentalists and engineers
Utilization of graphene as a fundamental block of electronic devices requires
development of new theoretical methods for understanding the current propagations in
graphene constriction4
12 Graphene Synthesis
The discovery of graphene by mechanical exfoliation called the lsquoScotch tape methodrsquo led
to serious attempts towards the production of top quality graphene5 Graphene was first
exfoliated mechanically from graphite in 20046 The importance of high quality graphene
cannot be emphasized enough however electron transport has shown that defects play an
important role in hindering the transport properties of electrons (holes)7 The two
synthesizing methods for the large scale manufacture of graphene are chemical vapor
deposition (CVD) and silicon carbide (SiC) desorption method
4
Graphene can be synthesized by sublimation of silicon from SiC at high
temperature (1200degC) in high vacuum5 The major advantage of this method is that the
SiC provides an insulating substrate and no transfer of the graphene layer is needed Yet
the disadvantage of this method outweighs its advantages the high temperature is cost-
ineffective making it unsuitable for large scale manufacturing8 Also the crystal growth
face alters the properties of graphene Graphene grown on Si-terminated face has poor
homogeneity and is subjected to unintentional doping7 Conversely graphene grown on
C-terminated SiC has higher mobility and is often called lsquoturbostaticrsquo due to the
rotational disorder7
Unlike the SiC method the graphene produced via CVD method needs to be
transferred to a substrate making it difficult to maintain the quality of graphene Yet
CVD synthesized graphene has a larger grain size7 More research is being done on
various methods for synthesis of graphene The methods include direct chemical
synthesis ion implantation crystal sonification and lastly unzipping carbon nanotubes to
form graphene sheets9
Graphene and few-layer graphene have been grown by CVD from carbon
containing gases on catalytic metal surfaces andby surface segregation of C dissolved in
the bulk of such metals7 Growing graphene with CVD is a very attractive solution since
it is compatible with the existing semiconductor industry9 Graphene has been grown via
CVD process on metal substrates such as Nickel (Ni) and Copper (Cu)
5
121 Synthesis of Graphene on Nickel (Ni)
Polycrystalline Ni films are annealed in ArH2 atmosphere at 900-1000degC to increase
grain size and are then exposed to H2CH4 gas mixture10
In this step the hydrocarbon
decomposes and dissolves in Ni to form a solid solution Lastly the samples are cooled in
argon gas Ni has high carbon solubility at elevated temperatures and the solubility
decreases as temperature is reduced During the cooling process the carbon atoms diffuse
out from the Ni-C solid solution and precipitate on the Ni surface to form graphene films
(Figure 13a) Since Ni (111) has a lattice similar to the densely packed hexagonal lattice
of graphene (Figure 13b) they also have similar lattice constants and hence Ni surface
serves as an excellent lattice matched substrate for graphene growth11
The growth of graphene on Ni is based on carbon segregation and precipitation
process different segregation behavior is produced by different cooling rates which
affect the thickness and quality of graphene films12
Medium cooling rates lead to optimal
carbon segregation and produce few layers12
Graphene films grown on Ni are usually
continuous with monolayer and few layer regions Annealing of Ni substrates at elevated
temperatures in hydrogen atmosphere not only increases the single-crystalline Ni grain
size but also eliminates certain impurities in Ni thereby improving the graphene quality
Furthermore the graphene thickness can also be affected due to the amount of carbon
dissolved in the Ni films during the growth time
After synthesis the graphene can be transferred to other insulator substrates for
further characterization and applications Figure 13c shows the selected area electron
diffraction pattern of graphene film along the [001] direction which confirms the
graphene lattice structure shown After transfer to insulator substrates the geometry can
6
be retained as shown in Figure 13d Under optimal growth parameters graphene growth
is only limited by the Ni catalyst Lastly Figures 13e and 13f show the wafer-scale
graphene synthesis and transfer of graphene to a flexible transparent substrate
respectively
Though polycrystalline Ni is a good substrate the percentage and size of
graphene monolayer are still limited Researchers have hence tried other metal substrates
for graphene synthesis
7
Figure 13 (a) Graphene formation on Nickel (b) Graphene atoms on Ni (111) lattice
(c) Low magnification TEM image of graphene edges (d) Optical image of graphene
transferred from the Ni surface to SiO2Si substrate (e) Full-wafer scale deposition of
graphene layers on polycrystalline Ni (f) Transparent and flexible graphene films on
PDMS substrate10
8
122 Synthesis of Graphene on Copper (Cu)
Graphene films are grown on 25microm thick Cu foils in a hot wall furnace13
The Cu foil is
first annealed in hydrogen atmosphere at 1000degC and a mixture of H2CH4 is introduced
into the system to initiate graphene growth After a continuous graphene layer is formed
on the Cu foil the system is cooled to room temperature Figure 14a shows an SEM
image of graphene on Cu substrate indicating the Cu grains with contrast The Cu
surface steps are formed during thermal annealing and the darker flakes indicate multiple-
layer graphene (Figure 14b)10
The graphene wrinkles in Figure 14(b) originate from
different thermal expansion coefficient of graphene and Cu They go across the Cu grain
boundaries indicating that the graphene film is continuous
Figure 14 (a) SEM image of graphene on copper foil (b) High-resolution SEM image of
graphene on Cu10
123 Transfer of Graphene films
In order to facilitate the applications of graphene for electronic applications we need to
separate the graphene from the catalytic metal substrate Figure 15a shows the transfer
process of graphene Graphene is first coated with a thin layer of polymethyl
methacrylate (PMMA) and baked at 120degC to evaporate the solvent10
The metal layer is
then removed by Ni or Cu etchant leaving behind the PMMA graphene film The film is
then cleaned by deionized water and then transferred onto the target substrate After the
9
evaporation of water vapor the PMMA is removed by acetone leaving graphene film on
top of the target substrate Figure 15b shows a graphene wafer transferred from the
substrate onto glass and polyethylene terephthalate (PET) films
Figure 15 (a) Transfer process (b) Wafer-scale synthesis of graphene (c) Graphene
films transferred onto glass wafer (d) SiSiO2 with device patterned (e) PET film10
124 Synthesis of Graphene Junction
Graphene junctions with smooth armchair and zigzag edges are difficult to produce by
conventional methods such as mechanical exfoliation chemical exfoliation or lithography
etching14
The conventional methods can only produce rough edges Recently
Dresselhaus reported an edge reconstruction of graphene by Joule heating in a TEM-STM
10
(Figure16b) system15
An individual nanoribbon sample is attached to the sample holder
at one end and to the STM tip at the other end these ends also serve as the two
electrodes The structural transformation in the growth of graphene from armchair to zig-
zag is mainly attributed to the vaporization of carbon edges that reconstruct at high
temperatures in which resistive Joule heating and preferred current flow play an
important role This means that by controlling the flow of current a perfectly smooth
edged ribbon can be synthesized making graphene-based electronics possible16
Figure 16 (a) High-magnification image of the annealed sample showing that well-
defined zigzag armchair and zigzag-zigzag edges are formed (b) STM image of an 8 nm
wide bent junction connecting an armchair and a zigzag graphene nanoribbon which was
carved by STM tips14
125 Doping in Graphene
The doping of graphene can be roughly classified into two categories - electrical and
chemical Electrical doping involves changing gate voltages of graphene devices and
chemical doping uses chemical routes such as substitutional or interstitial This thesis
discusses chemical doping and the importance of doping sites by changing the dopant
Chemical doping is a common approach to tailor the electronic properties of
11
semiconductors Doping of graphene can cause its electronic properties to alter leading to
a metal-semiconductor transition The two means of doping graphene are interstitial and
substitutional In interstitial doping the dopant atoms or molecules are introduced as
adatoms or admolecules on the surface of graphene whereas in substitutional doping the
dopant atoms are replaced in the carbon lattice forming a bond in the lattice of
graphene16
Doping graphene results in the formation of n or p-type semiconductors
depending on the kind of dopant If the dopant is an electron donor it causes the Fermi
level to shift up resulting in n-type behavior of graphene Furthermore if the dopant is an
electron acceptor it causes the Fermi level to shift down resulting in a p-type behavior of
graphene (Figure 17)16
Figure 17 Band structure of graphene before and after doping The image shows shift
towards the Fermi level16
Graphene nanoribbons (GNR) can be made into a p- and n- type semiconductor
by doping with boron (B) and nitrogen (N) respectively In theory GNR p-n junction is
formed by doping GNR with B and N in different regions However experimentally
doping graphene with both these elements is very difficult due to the dopants reacting
with each other17
Hence most experimental studies use GNR doped by only one
12
element N-doped graphene was synthesized by Wei et al Wang and B-doped Graphene
was realized by Endo17
Many researchers have demonstrated interstitial doping of graphene by gas metal
and organic molecules16
The various gases and metals used are NO2 NH3 An-CH3 Na-
NH2 F4-TCNQ TPa TCNE and others16
Doping in graphene is hence possible by
electrons or holes in high concentration without deterioration of its mobility Interstitial
doping is highly sensitive due to most of the conducting channel being exposed to surface
absorbates and hence can be used in molecule detection
In substitutional doping the dopant atoms are included in the graphene lattice and
thus chemically bonded Substitutional doping is done via the CVD method using a
carbon and dopant source Substitutional doping opens up many applications in device
engineering making graphene a very good candidate as a semiconductor This study
involves the study of transport properties of graphene doped by substitution
126 Nitrogen (N) Doped Graphene Synthesis (Substitutional)
N-Doped graphene is prepared via a CVD process using a 25microm thick Cu film on a Si
substrate The substrate is placed in a quartz tube with the flow of hydrogen (20sccm) and
argon (100 sccm)18
When the center of the furnace reaches 800degC 60 sccm of CH4 and
60 sccm of NH3 is introduced into the flow as C source and N source respectively The
substrate is then moved to high temperature and after 10 min growth the sample is
cooled to room temperature under H2 ambient Figure 1 8 shows the growth of N-doped
graphene18
13
Figure 18 Low resolution TEM image of N-doped graphene Background is the lacey
carbon TEM grid graphene sheet is crumpled with many ripples18
13 Structure of Graphene Nanoribbon (GNR)
Graphene Nanoribbons (GNR) are strips of graphene with very thin width of lt50nm
GNRs can be terminated in three separate ways called zig-zag (0 n) armchair (m 0) and
chiral (m n) (Figure19) and this termination along the width of the ribbon dictates the
size of the band gap19
Figure 19 Zigzag and Armchair orientation of Graphene5
Due to their various edge structures GNRs exhibit different electronic properties
ranging from normal semiconductors to spin-polarized half metals which open the
possibility of GNRs as electronic devices19
14
Within a tight binding approach (AGNRs) could be metallic or semiconducting
depending on their ribbon width but all zigzag graphene nanoribbons (ZGNRs) are
metallic with a high density of electronic states at the edges Hence ZGNRs exhibit
characteristic edge effects which are not present in AGNRs These edge effects in
ZGNR create a flat band close to the Fermi level making the ZGNR edges more
reactive19
First-principles calculations show that the GNRs possess a non-zero direct
band gaps These gaps are small for ZGNR (Figure 110) caused due to spin ordering
effects at the edges For AGNRs the band gap arises from quantum confinement (Figure
111) effect that has larger magnitudes than ZGNR20
Figure 110 Band structure of ZGNR
15
Figure 111 Band structure of AGNR
For GNRs the band gap decreases as the ribbon width increases and in order to
create a semiconductor with a desirable band gap the nanoribbon width should be
adjusted accordingly This property of adjusting the band gap makes graphene an
excellent candidate for transistor switching By applying an electric field GNR can be
altered from an insulator to a conductor GNRs exhibit very intriguing properties and
have become one of the promising candidates for electronic applications
14 Overview of Graphene Junction
The invention of p-n junctions date back to 1940s which later resulted in the invention of
junction transistors One of the key technological reasons for success of the p-n junction
is mainly due to its ability to locally modulate the energy band gaps via an applied bias21
A graphene p-n junction is created via single layer of graphene in which the
carrier type and density in two adjacent regions are controlled by electrostatic gating8
For materials with a band gap the electric field can either switch lsquooffrsquo the current or
rectify it (p-n diode)22
Being a ldquogaplessrdquo material the off state is not achievable in
16
graphene In order to achieve an off state the gap can be created by doping graphene with
various elements (Group III or Group V) Doping allows p-n junctions to be
reconfigurable using a gate voltage to distinguish between graphene p- n regions within a
single sheet Many researchers have studied the electronic as well as transport properties
of doped graphene junctions
In 2009 Fangping OuYang studied the transport properties of T-shaped graphene
junctions using the ATK software and showed that the conductance depends on
geometric structures which can be controlled by selective doping23
Wei Yao in 2013
studied the transport properties in graphene p-n junctions and showed that the
rectification effect depends on boron doping density and position17
The study of transport properties in graphene p-n junctions is a recent
advancement The thesis discusses transport properties including the current-voltage (I-
V) characteristics of doped graphene junctions Moreover the software used is similar to
the software in use by current researchers since they have produced viable data using
ATK
17
CHAPTER 2
RESEARCH BACKGROUND
21 Band Structure of Graphene
The unique electronic properties of graphene were first predicted in 1946 Figure 21
shows a top view of the hexagonal arrangement of carbon atoms in real space as well as
the first Brillouin zone in reciprocal space
Figure 21 Left Real space graphene lattice with basis vectors and Right The
first Brillouin zone of graphene in reciprocal space with basis vectors and
K and
Krsquo are responsible for massless transport at low energy24
The real space basis vectors are radic
and
radic
The reciprocal space basis vectors are 1 2
0 0
4 1 3 4 1 3( )and ( )2 2 2 23 3
b x y b x ya a
where the magnitude of the basis vectors is |a0| = radic acc The distance between nearest
neighbor carbon atoms is acc=0142nm
18
The band structure can be calculated by solving the eigenvalues using the
dispersion relation E( )
1 2 3( ) 3 2cos 2cos 2cosE k t k a k a k a (21)
Transport properties of solids are closely related to the energy dispersion
relations E ( ) in the material and in particular to the behavior of E ( ) near the Fermi
level Graphene is a zero gap semimetal whose specific linear electronic band dispersion
near the Brillouin zone corners (Dirac points) gives rise to electrons and holes that
propagate as massless Fermions25
The valence and conduction bands do not overlap in
graphene they touch at the Fermi Level (Figure 22)
Figure 22 Band structure of a graphene sheet showing a band gap of 0eV
The low energy properties of graphene can be well described by making a linear
expansion of the band structure around the K and Krsquo This energy can be written as
19
E(k) = plusmnħvF|k (22)
where vF is the Fermi velocity of 1106ms given by
1F
Ev
k
ħ (23)
Figure 23 Band structure of graphene calculated with the tight-binding model
22
The Fermi surface of graphene consists of double cones with Fermi energy at the
intersection of these cones (Figure 23) The slope of the band is zero and hence the
effective mass of electrons in that region is zero which leads to an entirely new transport
mechanism in graphene26
20
22 Transport Characteristics of Graphene
Transport process usually involves a flow of charge or energy or both The flow is mainly
due to external perturbations such as electric field and temperature gradient The
relationship between forces and flow usually defines various transport coefficients that
are the characteristics of electrons and phonons in the material All modern electronics
are based on the ability to control the electronic properties of a material by applying
external voltage This is done by an electric field effect where the gate voltage changes
the carrier concentration of the material and consequently its conductivity The electric
field effect in graphene was reported by Novoselov in 2004 and is used in transport
measurements8
The electron-phonon interaction in graphene plays an important role in
understanding the photoemission spectra observed in graphene The electric field effect is
an alternative method for changing the charge carrier density in low dimensional systems
The electric field effect in graphene which was first reported by Novoselov et al in
2004 is widely used as a characterization tool in transport measurements25
The transport characteristics of the material are directly related to the
bandstructure of graphene The carriers in graphene lattice are free to move in two
dimensions In the carrier transport of graphene the carriers ndash electrons and holes ndash close
to the Dirac points are of importance The transport is described by a two component
wave function (Equation 24) which obeys the 2D Dirac-like equation for massless
particles27
21
-ivFσ nablaψ(r) = Eψ(r)
(24)
where σ is the 2D Pauli spin matrix In the continuum limit the above (Equation
24) corresponds to the effective low energy Dirac Hamiltonian (Equation 25)
0( )
0
x y
F F
x y
iH k k
i
k kv v
k k
(25)
The electronic band structure of the energy (E) versus wave vector (k) relation for
graphene is given by Equation 24
The two component wave function resembles the spin or wave function of
quantum electro dynamics (QED)27
Corresponding to the spin of particles in QED the
charge carriers of graphene can be attributed with a pseudospin σ The pseudospin is the
direct result of two different carbon sublattices corresponding to the bonding and
antibonding combinations27
22
Figure 24 The energy dispersion around the K point27
In Figure 24 the red and blue lines correspond to the antibonding and bonding
states respectively The pseudospin can have two values either in the direction of or
against the momentum It can be seen that the electrons with energy E travelling in the
positive direction originates from the same branch as a hole with energy ndashE travelling in
the negative direction giving it the same pseudospin This results in suppressed
backscattering and Klein tunneling The back scattering process requires the pseudospin
to flip which is possible in the presence of short range scatters that act differently on sub
lattices27
23 Drude Theory
The classical theory of metallic conductivity was presented by Drude in 1900 and was
elaborated by Lorentz in 190528
Drude treated the free electrons as classical ideal gas
meaning the electrons collide with stationary ions and not each other
23
Figure 25 Electrons colliding with stationary ions28
The Drude theory applied the kinetic theory of gases to a metal considered as a gas of
electrons The basic assumptions made by the Drude theory are28
When metallic elements are brought together to form a solid then the valence
electrons become freely moving through the metal whereas the ions remain intact
as nearly immobile positive particles
Between collisions the electrons move freely ie there is neither electron-
electron interaction nor electron-ion interaction
The scattering mechanism leads to instantaneous collisions of the electron with
the scatterers
The collisions are characterized by a relaxation time τ
The electrons achieve thermal equilibrium only through collisions the velocity
after a collision is randomly directed the speed is as appropriate to the
temperature
With the relaxation time Drude obtained the electrical conductivity expression
where n is the number of electrons per unit volume
σ = ne2τm
(25)
He also calculated the thermal conductivity and successfully provided the
theoretical basis for Wiedemann-Frantz law already established in 1853 which states that
24
the ratio of electrical and thermal conductivity of any metals is a universal constant at any
given temperature28
The Drude theory gives results which are qualitatively correct outside of the
quantum Hall regime28
In the Drude theory of the electrical conductivity of a metal an
electron is accelerated by the electric field for an average time τ before being scattered
by impurities lattice imperfections and phonons to a state which has zero average
velocity The average drift velocity of the electron is
d
eE mv (26)
It is assumed that all electrons drift together and hence the current density
j = -ne (27)
This Drude theory works well for fields below ~ 01T At stronger fields the Hall
resistivity becomes nearly constant over finite intervals of magnetic fields28
The QHE
reflects both novel disorder physics as well as novel interaction physics in the quantum
Hall regime
24 Quantum Hall Effect (QHE)
The discovery of QHE is a remarkable achievement in condensed matter physics The
Hall Effect was discovered by Edwin Hall in 187929
However the precise quantization
of the Hall conductance in units of e2h was not recognized until February 1980 Five
years later in 1985 Klaus von Klitzing was awarded the Nobel Prize in Physics for the
discovery of QHE29
The quantum Hall effect occurs in two-dimensional electron systems in the limit
of strong perpendicular magnetic field that stems from electronic transport
25
measurements where one drives a current I through the sample and where one measures
both the longitudinal and transverse resistance (Hall resistance) A longitudinal resistance
is a resistance measured between two contacts that may be connected by a line which
does not connect C1 and C430
Transverse resistance is measured between two contacts
connected by an imaginary line connecting C1 and C4 (Figure 26a)
Figure 26 (a) 2D electrons in a perpendicular magnetic field Logitudinal resistance
measured across C5 and C6 Transverse resistance measured across C3 and C5
(b) Classical Hall resistance as a function on the magnetic field30
Due to the existence of quantum Hall effect it is natural to expect that there exists
a classical Hall Effect Hall showed that the transverse resistance of a thin metallic plate
varies linearly with the strength B of the perpendicular magnetic field (Figure 26 b)
RH = Bqnel (28)
More quantitatively the classical Hall Effect can be understood within the Drude
model for diffusive transport in a metal Within this model one considers independent
26
charge carriers of momentum p described by the equation of motion
( )
b
dp p pe E B
dt m (29)
where E and B are the electric and magnetic field respectively The macroscopic
transport characteristics ie resistivity of the system are obtained from the static
solution of the equation of motion dpdt = 0 and one finds for 2D electrons with p =
(pxpy)
x
x yb
y
y xb
eBe
eBe
ppE
m
ppE
m
(210)
In the above expression characteristic frequency is visible as
C
b
eB
m (211)
This is known as cyclotron frequency as it characterizes the cyclotron motion of a
charged particle in a magnetic field30
With the Drude theory the conductivity can be
written as
j = -enelpmb (212)
and the mobility can be given as
micro = eτmb (213)
The transport properties in the limit of ωCτ-gt infin are entirely governed in the presence of
27
a magnetic field by the off-diagonal ie transverse components of
conductivityresistivity
The theory of quantum Hall effect subjects all physical properties of 2D electron
system in the limit where the magnetic field is strong so that the mixing of Landau levels
by disorder or electron-electron interaction is considered to be a weak perturbation30
This is known as the quantum Hall regime The ratios between the energy scales
corresponding to the two interactions are important The limit where disorder potential is
much stronger is referred to as integer quantum hall regime whereas the limit where the
interaction potential is much stronger is referred to as fractional quantum Hall regime
25 Resistivity and Resistance
The electronic transport in the framework of the Drude theory allows for the calculation
of conductivity or resistivity of a classical diffusive 2D electrons in a magnetic field30
The conductivity and conductance are related to one another but they depend on the
geometry of the conductor-the resistance R and hence the resistivity is given by
R = (LA)ρ (214)
where L is the length of the conductor and A is the cross section
For a d-dimensional conductor the cross section scales as Ld-1
such that the
scaling relation between the resistance and the resistivity is
R~ ρL2-d
(215)
From the dimension point of view resistance and resistivity are the same in 2D and the
resistance is scale-invariant Further the resistance of a 2D conductor depends in
general on the so-called aspect ratio LW via some factor f (LW)30
However for
transverse Hall resistance it is the length of the conductor that plays the role of cross
28
section such that the Hall resistivity and the Hall resistance truly coincide ie f=1 The
Quantum Hall effect is highly insensitive to the particular geometric properties of the
sample used in transport measurements Recently quantum Hall physics experienced the
discovery of ldquorelativisticrdquo quantum Hall effect in graphene The electrons in graphene
behave as if they were relativistic massless particles contributing to a very interesting
field of research30
26 Klein Tunneling
Klein tunneling in which relativistic particles penetrate through a potential barrier
without the exponential damping that is characteristic for nonrelativistic quantum
tunneling has never been observed for elementary particles The tunneling allows
transmission of a particle through a potential barrier higher than its kinetic energy
violating the principle of classical mechanics30
On the quantum scale the objects exhibit
wave-like characteristics in which the quanta move against a potential hill described by
their wave function This wave function represents the probability amplitude of finding
the object in a particular location The transmission of the object through the potential hill
is termed as tunneling When EltV then the ψ(x) over V is returned by ψrsquo(x) In quantum
mechanics an electron tunnels from the conduction into the valence band Such a
tunneling from an electron-like to hole-like state is called as Klein Tunneling in which the
electron avoids backscattering
In Figure 27 it is shown that an electron hitting a potential barrier is reflected
with 100 certainty In non-relativistic quantum mechanics the electrons can tunnel
through the barrier but the probability of tunneling exponentially decays with increasing
29
height and width of the barrier However in relativistic quantum mechanics the barrier
gets transparent even in the limit of infinite barrier height (Klein paradox)31
Figure 27 Klein tunneling through an npn barrier30
The Klein paradox in graphene can be understood in terms of electrons and holes
In graphene the massless carriers behave differently than ordinary carriers (with mass) in
the presence of an electric field A barrier which is repulsive for electrons will be
attractive for holes Since there are hole states inside the barrier with the same energy as
the electrons outside an electron arriving at the barrier can tunnel through it as a hole
before leaving again as an electron Klein tunneling for transport in graphene is that the
charge carriers cannot be confined by potential barriers The Klein tunneling effect has
been experimentally observed by Ando in 1998 in which the absence of backscattering
(Figure 28) is responsible for high conductivity in carbon nanotubes
30
Figure 28 Electron trajectory considering the linear electrostatic potential U(x) = Fx30
The electron is able to propagate through an infinitely high potential barrier since
it makes a transition from the conduction band to valence band In this transition from
conduction band to valence band its dynamics changes from electron-like to hole-like
The equation of motion is thus given by
2
2 2 2| | ( )
pdr E
dt E Up
p E U
v
v
at energy E (216)
This shows that in the conduction band (UltE) and in the valence band (UgtE)
In Klein tunneling the pairs of electron-like and hole-like trajectories at the same E and
py have turning points at dmin given by dmin=2v|py|F (Figure 29)
Figure 29 Electron like and hole like trajectories at same E21
31
The tunneling probability exponential dependence on dmin
2
min| |
( ) exp( ) exp( )2
y y
y
vT
F
p pdp
(217)
The applications of the Klein tunneling include Atomic clock Scanning tunneling
Microscope Tunnel diode Tunneling transistor and many more32
Since graphene
exhibits Klein tunneling it can be very useful to study the transport properties in
graphene and use it in such applications
27 Quantum Hall Effect in a Graphene
A monolayer graphene shows half-integer quantum Hall effects where the Hall
resistance is quantized at values of
2
1
xyh v eR
(218)
around filling factors
14( 1 2)Nv
(219)
where N is an integer e is the electron charge h is the Planckrsquos constant and the
factor 4 is due to spin and valley degeneracy QHE in graphene can be observed at room
temperature which is a very intriguing property (Figure 210) Graphene reveals
significant differences with respect to conventional 2D electron systems The Landau
quantization yields energy levels that disperse differently in graphene as well as
particular zero-energy level that is only half filled at the charge neutrality point (v=o)
32
Figure 210 Quantum Hall effect in graphene22
The Hall conductivity σxy and the
longitudinal resistivity of monolayer graphene as a function of carrier density at B = 14T
and T= 4K This shows half-integer QHE with chiral index J= 1
The QHE in graphene is not entirely similar to regular QHE since the charge
carriers in graphene are Dirac Fermions The charge carriers governed by
electrodynamics is given by (Equation 220) which does not apply for graphene and a
QED quantization of graphene electronic band structure is used
En = (n+12)ħω (220)
33
In the presence of magnetic field the nature of the Dirac Fermions in graphene
results in unevenly spaced Landau levels (LL) containing a distinctive LL at the electron-
hole degenerating a zero energy given by
2MG
MGFehn B
n vE (221)
The LL levels at high magnetic fields in MG are shown in Figure 211
Figure 211 (a) LL for Graphene bilayer (b) Schematics of Hall conductivity as a
function of nn0 for bilayer Graphene (solid line) and monolayer Graphene (dotted line)
(c) LL for monolayer Graphene33
It is found that the Hall resistance of a two dimensional electron system has
plateaus as a function of the number of electrons at low temperatures and strong magnetic
fields32
At large B the Dirac-like energy spectrum of graphene gives rise to a
characteristic series of QH plateaus in conductance reflecting the presence of a zero-
energy Landau level that include only odd multiples of 2e2h for uniform carrier density
in the sheet These plateaus of QH edge states at the edge of the sheet circulating in a
34
direction are determined by the direction of B and the carrier type33
This is why QHE in
graphene is known as Half-Integer Quantum Hall Effect
28 Thermoelectric Effect
Thermoelectricity refers to a class of phenomena in which a temperature difference
creates an electric potential or an electric potential creates a temperature difference The
principle of thermoelectric effect has been known for over 100 years Recently the
practical applications of thermoelectric effect have become more viable34
Thermoelectric effect is the direct conversion of temperature differences to
electric voltage and vice versa Joule heating is the heat generated whenever a voltage is
applied across a resistive material The Peltier-Seebeck effect is reversible whereas Joule
heating is not This effect can be used to generate electricity to measure temperature to
cool objects or to heat them Since the direction of heating and cooling is determined by
the sign of the applied voltage thermoelectric devices make very convenient temperature
controllers
281 Seebeck Coefficient
Thomas Johann Seebeck discovered that an emf appears in a circuit composed of two
dissimilar metals when the junction between the metals is held at different
temperatures34
The thermoelectric emf causes a continuous current in the circuit when a
complete loop is formed and the current is known as thermoelectric current This is
known as the Seebeck effect
35
Figure 212 Seebeck Effect34
As long as the two junctions are at different temperatures the thermoelectric emf
exists and the current will keep flowing between the hot and cold junction that are at
different temperatures The Seebeck effect is the conversion of temperature difference
directly into electricity The voltage developed in the circuit shown in Figure 212 is
proportional to the difference in temperature between the two junctions and is given by
V = α (T2-T1) (222)
This Seebeck effect is observed not only in metals but also in semiconductors
Here α is known as the Seebeck coefficient α measures the magnitude of an induced
thermoelectric voltage in response to the temperature difference across the material If the
temperature difference ∆T between the two ends of a material is small then the Seebeck
coefficient of a material is written by
α = ∆V∆T (223)
36
This can be expressed in terms of electric field as
α E∆T (224)
The units of Seebeck coefficient is given as VK The higher the Seebeck coefficient
value the better it is since it will create a very large voltage that can be used to provide
power
282 Peltier Coefficient
Peltier effect is the inverse of Seebeck effect involving a junction phenomenon There is
heat absorption or generation at the junctions depending on the direction of current flow
Heat generated by current flowing in one direction is absorbed if the current is reversed
The heat absorbed per second at a junction carrying current I is given by
Heat absorbed in t sec = πabIt (225)
Here πab is the Peltier coefficient and given by HIt Thus Peltier coefficient is
numerically equal to the applied potential difference expressed in Volts
Overall by studying the flow of electrons the values of Seebeck
coefficient and Peltier co-efficient can be estimated These values determine the various
applications of the materials In this thesis the Peltier and Seebeck coefficient of the
graphene junction and the new applications are discussed
37
29 Early Research ndash ab intio studies
In 2007 Androitis studied that the conducting properties of graphene nanoribbons and
junctions are strongly dependent on their size and geometric features35
He concluded that
there is no conductance for small AZA or ZAZ ribbons (Figure 213)
Figure 213 Transmission functions in units of (2e
2h) for AZA structures
35
Figure 213 shows that T (E) exhibits a negligible peak [T (E) = 001 in units of
2e2h] at E= -225 and 250eV However it was noted that when the width of the arm type
was increased T (E) at -225 and 250eV was 02035
Later in 2007 Qimin Yan used first principles methods to investigate the Current-
Voltage characteristics of GNR Transistors and the effect of edge doping He showed that
GNR field effect transistors can achieve high performance levels with ONOFF ratios on
the order of 103-10
436
Figure 214 is an I-V curve of AZA GNR-FET connected via
armchair metallic leads36
38
Figure 214 I-V curve for a 591nm long channel (Vbias=20mV)
36
In 2009 Fangping OuYang demonstrated the intrinsic transport properties and
effective B or N doping of the junctions by using first-principles quantum transport
simulations He concluded that the I-V characteristics of pure-carbon T-shaped junctions
exhibit metallic behavior and the current in the junction strongly depends on the height
of the stem23
He reported that the conductance of the devices depends on the geometric
structures which can be controlled by selective doping
In 2012 Wei Yao used the first principle calculations based on Density
Functional Theory (DFT) and Non-equilibrium Greens Function (NEGF) to study the
electronic as well as the transport properties of B-doped 6-GNR p-n junction His results
showed that the boron doping interval can influence the rectification effect at low bias
and also exhibit Negative Differential Resistance (NDR) phenomena at high positive
bias
39
CHAPTER 3
COMPUTATIONAL DETAILS
31 Introduction
The physical chemical electrical electronic and optical properties of a solid are
determined by their quantized electronic states The quantum states in low-dimensional
systems are produced due to the confinement of the carrier charges in one or two
dimensions Graphene is a conductor electrons are able to flow through graphene more
easily than through even copper The electrons can travel through the sheet of graphene
like mass-less particles as fast as just one hundredth that of the speed of light The ways
in which electrons behave in graphene make it very helpful to study their fundamental
physical properties Graphenersquos near perfect crystal lattice provides a very clean system
to experiment By restricting the electrons to only two dimensions they exhibit some
interesting properties such as the anomalous quantum Hall effect and Klein tunneling
In this chapter two theoretical concepts used for calculating the electronic structure
and the transport properties for graphene are described These include the Extended
Huckel Theory and Non-Equilibrium Greenrsquos Function (NEGF) method
311 Extended Huckel Theory
Erich Huumlckel was born in Germany on August 9th
1896 He studied mathematics and
physics in Berlin He is best known for his work in the field of chemistry and physics for
two contributions (1) Debye- Huumlckel theory of electrolytic solutions (2) Huumlckel
method of approximate molecular orbital calculations on electron systems In 1930 he
published his findings on systems in 1931 he generalized and expanded the system
40
theory to explain benzene Due to his poor communication skills his findings went
unrecognized for over 20 years It was in 1951 that his 4n + 2 rule was finally clarified by
Doering to show if C=C bonds would show aromaticity Huumlckel died on February 16th
1980 with very little worldwide recognition for his contributions to chemistry Today
chemistry students recognize his name and his contributions to the field are quite
substantial
One of the first semi-empirical methods to be developed was Huumlckel Molecular
Orbital Theory (HMO) HMO was developed to describe molecules containing
conjugated double bonds HMO considered only electrons in pi orbitals and ignored all
other electrons in a molecule The Extended Huumlckel Molecular Orbital Method (EH) was
developed out of the need to consider all valence electrons in a molecular orbital
calculation
By considering all the valence electrons chemists could determine molecular
structure compute energy barriers for bond rotations and determine energies and
structures of transition states for reactions By considering only the valence electrons the
computed energies could be used to choose between proposed transition states to clarify
reaction mechanisms The total valence electron wavefunction is described as a product
of the one-electron wave functions
1 2 3(1) (2) (3) ( )valence j n (31)
where n is the number of electrons and j identifies the molecular orbital Each
molecular orbital is written as a linear combination of atomic orbitals (LCAO)
1 12
N
j jr rrc j N
(32)
41
The energy of the jth
molecular orbital is given by a one-electron Schroumldinger
equation using an effective one electron Hamiltonian heff which expresses the interaction
of an electron with the rest of the molecule
eff j j jh (33)
This is the energy eigenvalue of jth
molecular orbital corresponding to the Eigen
function j The advantage of using this method is that the exact form of heff is not
required The total energy of the molecule is the sum of the single electron energies
j jj
E n (34)
where nj is the number of electrons in orbital j
In order to use the Extended Huckel method a set of calculation parameters and
approximations must be followed These parameters include the Basis set K-point and
the Brillouin Zone and lastly the Mesh cut-off
312 Introduction to NEGF
The Greenrsquos function is a function of two space-time coordinates From the knowledge of
this function one can calculate time-dependent expectation values such as currents and
densities electron addition and removal energies and the total energy of the system In
the absence of external fields the non-equilibrium Green function method reduces to the
equilibrium Green functions NEGF can be applied to both extended and finite systems
The generic system of NEGF consists of the electron dynamics of the channel described
by the Hamiltonian This channel consists of two contact reservoirs with respective
chemical potential μR and μL The NEGF assumes ballistic transport neglecting self-
42
energy from scattering The system is insulated from gate contacts whose effects are
realized via a 3D Poisson solver which solves for the potential at a given point in real
space based on electron density
22 ( ) [ ( ) ( )]D
qr N r n r
(35)
Figure 31 NEGF system
The system is easily expandable to systems with several contacts or gate
configurations by adding additional self-energy matrices to NEGF or additional sources
to the Poisson solver
313 Electrostatics
Electrostatic potential is created every time in the presence of a charge density due to an
induced electric field The Poissonrsquos equation correlates the electrostatic potential to
charge density as given in Equation 36
43
2( ( ) ( ) ( ) ( ))( )
( )( ) ( )
ADq p r n r r N rr
rr r
N
(36)
where ɛ(r) is the dielectric permittivity of the material ρ(r) n(r) ND(r) and NA(r) are the
hole electron donor and acceptor concentrations of the system respectively
Two types of boundary conditions are usually applied to the Poissonrsquos equation
Dirichlet boundary conditions
Φ (0) = F0 and Φ (L) = FL
von Neumann boundary conditions
00
( )
x
d x
dxB
and
( )L
x L
d x
dxB
For the transport problems with open boundary conditions the von Neumann
boundary conditions are used assuming that the potential vanishes at the boundary ie
B0=BL=0
The Poissonrsquos equation can hence be discretized on a grid as
2 ( )( )
( )
rx
r
= M (37)
where M is the matrix Φ and ρ are vectors containing the discretized values of
the electrostatic potential Φ and charge density ρ respectively
44
The Schroumldinger and Poisson equations are coupled since V(x) = -qΦ(x) is used
for the Schroumldinger to compute ρ(x) This self-consistent loop stops when the
convergence is reached
( )r
V(x) = -qΦ(x)
314 Non-Equilibrium Greenrsquos Function
Greenrsquos functions are a mathematical construction that are used to solve differential
equations subject to specific initial or boundary conditions They are named after the
British mathematician George Green The 1-D equation of L( )f( )=S( ) can be defined
by the Greenrsquos Function as given below
( ) ( ) ( )G x x f x x x (38)
The general Greenrsquos function is given by
( ) ( ) ( )f x dx G x x S x (39)
Applying the operator L( ) to the solution f( ) satisfies the original differential
equation The Greenrsquos Function G( ) is the propagator which propagates the influence
of a perturbation S( ) originally situated at the point to the point at which the
function f( ) is evaluated
The Greenrsquos Function G( ) can also be a correlation function If the points
and are strongly (weakly) correlated then S( ) will greatly (poorly) affect f( )
Poisson equation
2 ( )( )
( )
rr
r
Schroumldinger equation
2
2
( ( ) ) ( )
( )2
( ) | ( ) |
E H r E r S
H V rm
r dE E r
Figure 32 Self-consistent loop
45
The Schroumldinger equation with open boundaries can be written as
( )E H S (310)
Considering a 1-D and homogenous system ranging from =0 to L assuming
that Σ=0 and the form of equations is same before and after discretization then
22
2 0( ) ( ) ( )
2E x S x
m
dV
dx
(311)
The Greenrsquos function can hence be computed corresponding to the Schroumldinger
equation
22
2 0( ) ( ) ( )
2E G x x x x
m
dV
dx
(312)
Due to the delta-function at = a discontinuity is observed and hence the
Greens function is evaluated at boundary conditions
0
2
exp( ( )) x x 2 ( )( )
exp( ik(x x)) x x
ik x x m E VG x x k
A
A
(313)
By integrating the Schroumldinger equation twice and setting the lower and upper
integration boundaries to = -δ and = +δ the Greenrsquos Functions can be written as
2
( ) ( ) 0
( ) ( ) 2
x x x x
G x x G x x
dG x x dG x x m
dx dx
(314)
46
The coefficient A+ and A
- become
ik
mA A
(315)
The Greenrsquos Function takes a final form known as Retarded Greenrsquos Function and
is written as
( ) exp( | |)G x x i ik x xk
m (316)
And the wave function is
( ) ( ) ( )x dx G x x S x (317)
Retarded Greenrsquos Function propagates the wave functions generated by a source
or perturbation S from its origin at to any point
The retarded Greenrsquos Function as discretized Schroumldinger equation is written as
( )R RE H G I (318)
The wave function Φ can be calculated from the retarded Greenrsquos function and the
source vector as
Φ = GR∙S (319)
Overall in this section the Greenrsquos function approach in calculating the electron
dynamics is reviewed We defined the self-energy of each part of the system spectral
function and the probability current density the electric current is derived explicitly using
Non Equilibrium Greenrsquos function We will use this formalism to calculate the tunneling
phenomena in coupled quantum dots isolated or otherwise
47
CHAPTER 4
ATOMISTIX TOOLKIT DETAILS
41 Introduction
Virtual NanoLab (VNL) is a graphical user interface (GUI) that provides a group of
modeling tools the function of these tools involves the set-up investigation and the
study of nanoscale structures The quantum mechanical equations are solved by the
software by using the advanced software architecture and numerical methods to
implement ab initio calculations VNL simulates the electronic structure and calculates
the transport properties based on the two systems mentioned earlier NEGF and Extended
Huckel ATK is the main engine for computing the scripts and hence all the calculations
performed in VNL are done by ATK VNL is a user friendly software as it not only
allows creating a script but also helps to set up a virtual experiment
This thesis involves the use of VNL in order to study the effect of the width and
different orientations of the doped atoms Since the software allows for virtual
experiments it makes it much easier to study the I-V characteristics based on the change
in position of atoms
42 Device Structure
In this thesis AZA GNR p-n junction with boron doping (location) was created using the
ATK software which is based on NEGF and DFT Further the thesis discusses the
transport properties and the I-V curve of such junction
The input format of ATK is NanoLanguage which is an extension to Python
scripting language ATK uses the NEGF system for formalism of simulating device
48
Figure 41 Geometry of device configuration with two electrodes
37
The system is divided into three parts left central and right The implementation
relies on the screening approximation which assumes that the properties of the left and
right regions can be decribed by solving a bulk problem for fully periodic electrode cell37
This screening approximation is fulfilled when the electrode regions can be described by
an equilibrium electron distribution
Figure 42 The electron distribution in a device configuration which illustrates a left
moving scattering state with origin in right electrode37
The system assumes that in steady state the electron density of the central region
is constant in time and hence the electron density is calculated independently from each
electrode The electron density is given by the occupied eigenstates of the system
n(r) = nL(r) + n
R(r) (41)
49
The left and right densities are calculated by summing up the occupied scattering
states
nL(r) = sum
(42)
nR(r) = sum
(43)
The scattering states are usually calculated by first calculating the Bloch states in
the electrodes and then solving the Schroumldinger equation of the central region using the
Bloch state as matching boundary Instead of using the scattering states the ATK
software uses the NEGF method to calculate the non-equilibrium electron density
The electron density is given in terms of electron density matrix
D = DL + D
R (44)
The left density matrix is given by NEGF theory
DL = int
(45)
where
ρL(ɛ) =
(46)
ρL(ɛ) = is the special density matrix
Also if there is a non-equilibrium electron distribution in the central region then
the electron distribution in electrode is given by the Fermi function f with an electron
temperature TL
G(ɛ) =
(47)
G = retarded Green function
δ+ is an infinitesimal positive number and S H overlap the Hamiltonian matrices
L =
sum sum
(48)
50
L
is the broadening function of the left electrode given in terms of left electrode
self -energysum
43 Transmission Spectrum Calculations
Once the self-consistent non-equilibrium density matrix has been obtained the various
transport properties of the system can be calculated One of the most important properties
is the transmission spectrum from which the current and differential conductance can be
obtained
The transmission coefficient in ATK is obtained by the retarded Greens function
T(ɛ) = G(ɛ)ΓL(ɛ)G
ϯ(ɛ)Γ
R(ɛ) (49)
The transmission amplitude of individual scattering states may be obtained
through the Transmission Eigenvalues The ldquoTransmission Eigenvaluesrdquo is an analysis
which finds the eigenvalues of the transmission matrix
The transmission matrix at energy E and k-point is given by
Tnm(Ek) = sum (410)
where
= transmission amplitude from Bloch state ψn(k)
The transmission coefficient is given by the trace of transmission matrix
T(Ek) = sum (411)
Keeping in mind all quantities depend on the quantum numbers parametrically
Transmission eigenvalues sum up to the transmission coefficient
T = sum (412)
51
44 Calculating the Current
Current is calculated from the transmission coefficient using
I( ) ( )R L
L RL R
R LB B
eE f f dE
h
E EV V T T T
k kT T
(413)
where f is the Fermi function TRL is the electron temperature of the right or left
electrode and Tσ(E) is the transmission coefficient for the spin component σ
The chemical potentials of the left and right electrode given by
L
F R LR L
eVE
are defined relative to the Fermi level of the left electrode These chemical potential are
related to the applied bias and hencebiasR L
eV therefore bias L RV V V
The transmission spectrum itself is usually rather insensitive to temperature and is
used in self-consistent calculations but often depends strongly on the electrode voltages
Thus for an accurate estimate of the current the transmission spectrum should be
calculated self-consistently for each desired bias
ATK uses very precise method to calculate the transport properties of the system
Transmission spectra for various concentrations of boron doped graphene p-n junctions
are generated in this Chapter and various coefficients such as Seebeck Peltier and
Conductance are calculated
52
45 Calculating Transport coefficients
The linear response transport coefficient of an applied voltage difference or temperature
difference between the two electrodes is given by
Conductance
| dT 0
e
dI
dUG
(414)
Peltier coefficient
| d 0
Q
I
I
(415)
Seebeck coefficient
| 0
dUS I
dT T
(416)
These linear response coefficients are calculated by the Transport Coefficients To
perform these calculations the ATK uses the Electron Transmission Spectrum
53
CHAPTER 5
RESULTS AND DISCUSSION
51 Band Structure Analysis
The electronic bandstructure of GNR both doped and undoped are discussed in this
chapter
The armchair configuration of Pristine GNR (PGNR) has a band structure that is
dependent on its width This is explained by the fact that the sheet itself acts like a
potential well where the electrons are confined to form standing waves along Cr the
rolling vector albeit with slightly different boundary conditions (Cr = ma1 + na2
where m and n are integers and a1 and a2 are the unit cell vectors of graphene lattice) In
a GNR the two nodal points of the standing wave must be at the ribbon edge while in a
Single wall nanotube (SWNT) they can be anywhere ie a circumferential periodic
boundary condition
(a) (b)
Figure 51 Bandstructure of AGNR widths (a) 4 atoms (b) 5 atoms
54
(a) (b)
Figure 52 Bandstructure of AGNR widths (a) 6 atoms (b) 7 atoms
(a) (b)
Figure 53 Bandstructure of AGNR widths (a) 8 atoms (b) 9 atoms
55
(a) (b)
Figure 54 Bandstructure of AGNR widths (a) 10 atoms (b) 11 atoms
Figure 55 Bandstructure of AGNR with a width of 12 atoms
Figure 56 Variation in band gaps as the width (number of atoms) varies
0
05
1
15
2
25
0 2 4 6 8 10 12 14
Wdith vs Band Structure
eV
56
The band structure of 12 Atom AGNR is close to that of Ge (0626 eV) The
actual width of this nanoribbon is about 25 nm 12 AGNR has been fabricated
successfully and doped with various dopants Hence the 12 Atom AGNR has been chosen
to study the transport properties
A junction is created using ZGNR and AGNR To maintain the consistency in the
device analysis it is imperative that the band structure of ZGNR is also calculated From
the simulation it is evident that ZGNR-AGNR-ZGNR junction configuration displays the
Metal ndashSemiconductor-Metal configuration that is addressed in this work The Fermi
Level in all the Z-GNR nanoribbons of widths 4-12 lies within the conduction band
Figure 57 Band structure of ZGNR width (a) 4 atoms (b) 6 atoms
57
(a) (b)
Figure 58 Band structure of ZGNR width (a) 8 atoms and (b) 10 atoms
Figure 59 Band structure of ZGNR with a width of 12 atoms
In order to create viable junction that would show transistor properties doping of
the semiconductor part is necessary The 12 atom AGNR is doped with boron (p-type)
and nitrogen (n-type) - (Figure 510a) 4 N doped (Figure 510b) 4 B In both cases
the impurities lie on the edge of the atoms For 2 nitrogen doped GNR with the
58
impurities lying in the center of the ribbon the Fermi level is found to be in the
conduction band as shown in (Figure 510c) (Figure 510d) shows the position of N with
respect to the edge A very clear departure from the expected (the valence band extending
above Fermi level) is shown in (Figure 510a)
Figure 510 Band structures of Doped AGNR (a) 4 N Doped (b) 4 B Doped (c) 2
N Doped (d) position of Nitrogen from (c)
(a) (b)
(c) (d)
59
52 I-V Characteristics of GNR junction
In pristine graphene the chirality determines the conductivity as seen from the I-V curves
for various widths At certain widths the semiconducting properties are more
pronounced These widths determine the wavelengths of the standing waves which in
turn determine the sub-band locations in the E-k plot When the biasing potential
exceeds 012V the I-V curve shows linearity In case of the 8-atom wide PGNR the
band gap is about 03 eV and it is evident from the I-V plot that the On-State is + 033 V
The band gap of 10-atom and the 4-atom wide PGNR is large enough to show
semiconducting properties
Figure 511 Current Vs Voltage graph for varying graphene width showing
conductivity
-30000
-20000
-10000
0
10000
20000
30000
-3 -2 -1 0 1 2 3
Cu
rre
nt
(nA
)
Voltage (V) (bias)
Current (nA) Vs Voltage for varying graphene width
W=10
W=8
W=6
W=4
60
The ZAZ GNR Configurations show the properties of a semiconductor junction The 12
atom ZAZ structure is studied for its I-V characteristics In this Chapter undoped B-
doped N-Doped B and N Doped (P-N Junction) ZAZ junctions are simulated
Figure 512 ZAZ GNR junction device
61
The boron doped ZAZ junction I-V characteristics are shown below (Figure 513)
The impurity concentration is 2 and 4 Various device configurations are studied
Figure 513 I-V curve of Boron Doped ZAZ junction
-25000
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
25000
-205 -155 -105 -055 -005 045 095 145 195
Cu
rre
nt
(nA
)
VBias
2B_1G_R 2B_0G_R
4B_0G_L 4B_0G_C
4B_0G_R 4B_1G_L
4B_1G_C 4B_1G_R
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
-2 -1 0 1 2
Cu
ren
t(n
A)
VBias
4 B doped GNR Jn
62
Figure 514 I-V curve of Nitrogen Doped ZAZ
-25000
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
-2 -15 -1 -05 0 05 1 15 2
Cu
rre
nt(
nA
)
VBias
I-V Curve as function of Dopant location
2N_0G_L2N_0G_C2N_0G_R2N_1G2N_1G_C2N_1G_R
-15000
-10000
-5000
0
5000
10000
15000
-2 -1 0 1 2
Cu
rre
nt(
nA
)
VBias
2N_0G_C
2N_1G_C
63
Figure 513 and Figure 514 show the I-V characteristics of the GNR junction doped with
2 boron and nitrogen respectively The location of N and B is at the central region of
the edge of the GNR Both B doped and N doped GNR Junctions show significant
Negative Differential Resistance (NDR) This is more pronounced in case of nitrogen
doping Another interesting observation is increasing ohmic nature with the change in
location of the dopants Nitrogen doped device configuration exhibits a pronounced
semiconductor behavior and the NDR effect is observed to be minimal
53 Thermoelectric Properties
In this study the thermoelectric properties were simulated for the GNR Junctions that
displayed high NDR effect The variation in the Peltier coefficient with temperature is
shown as function of doping
When the concentration of nitrogen increases the dimensionless Figure of Merit
ZT seems to decrease considerably This is mostly explained by the decrease in both
conductivity and mobility of the electrons
ZT = S2σTk (51)
where S is the Seebeck coefficient σ is the electrical conductivity T is the
absolute temperature and k is the thermal conductivity
64
Figure 515 Variation of Peltier coefficient with temperature as function of
doping
Figure 515 shows the maximum Peltier coefficient for 2 boron This is
explained by the scattering by boron and the associated smallest mean free path
0
0001
0002
0003
0004
0005
0006
0007
0008
0009
001
250 270 290 310 330 350 370 390 410
ZT
T (K)
2B
4B
Undoped
2N
4N
65
CHAPTER 6
CONCLUSIONS
Graphene ZAZ junctions exhibit varying properties depending on the various structural
configurations In this thesis it was found that the transport properties of graphene
depend on their width the edge of GNR doping concentration and the type of dopant
used The calculations of the band structure contributed towards the determination of the
minimum length of GNR required for studying the transport properties The minimum
length had a band gap equivalent to that of germanium and hence the importance of the
width being 12 atoms wide This band gap indicated fluctuating changes when doped
with elements such as B and N The viable junction showing transistor properties was
hence created by doping the semiconductor part of ZAZ By doping the I-V
characteristics were studied which showed significant NDR which was more pronounced
in the case of nitrogen Also the changing positions of the dopants contributed towards
the I-V curve to be more ohmic The edge doping caused minimum NDR and
semiconductor behavior as compared to central doping Lastly the thermoelectric
properties were studied - the increasing concentration of N causes the Figure of Merit to
decline due to the decrease in conductivity as well as mobility of electrons
66
REFERENCES
1 Wikianswers What makes carbon unique
httpwikianswerscomQWhat_makes_carbon_so_unique (22 November)
2 Kopeliovich D D Graphite
httpwwwsubstechcomdokuwikidokuphpid=graphite (1128)
3 Barbier M Transport properties of nanostructures and superlattices on single layer and
bilayer graphene University Antwerpen Antwerpen 2012
4 Shylau A Electron transport interaction and spin in graphene and graphene
nanoribbons Linkoping Norrkoping 2012
5 HassJ R F T Li X Li Z Zong W A de Heer P N First E H Conrad C
AJeffrey and C Berger Applied Physics Letters 2006 89 (14) 143
6 Jones A Mechanical Exfoliation to Make Graphene and Visulization
httpcarbonchemwisceduFilesMechanicalExfoliationpdf (18 October)
7 Anteroinen J Structural and Electrical Characteristics of Graphene Field Effect
Transistors AALRO school of Electrical Engineering AALTO 2011
8 Novoselov K S A K G S V MorozovD JiangY Zhang S V Dubonos I V
Grigorieva A A Firsov Science 2004 306 (22)
9 Kosynkin D A L H A Sinitskii J R Lomeda A Dimiev K B Price and J M
Tour Nature 458 876
10 Yi Z Luyao Zhang Accounts of chemical research 46 (10) 2339
11 Eizenberg M B JM 1979 82 236
12 Yu Q K L J Siriponglert S Li H Chen Y P Pei S S Applied Physcis
Letters 2008 93 (113103)
13 Li X C W An J Kim S Nah J Yang D Piner R Velamakanni A Jung I
TutucE Banerjee S K Colombo L Ruoff R S Science 2009 324 1314
14 Schaefer H E Nanoscience Springer Berlin 2010
15 Levente Tapasztoacute G D Philippe Lambin amp Laacuteszloacute P Biroacute Nature Nanotechnology
2008 3 401
67
REFERENCES
16 Dacheng Wei Y L Advance Materials 2010 22 (30) 3241
17 Wei Yao K L Y GYGao Elsevier Solid State Communications 2013 153 52
18 Dacheng Wei Dagger Yunqi Liudagger Yu Wangdagger Hongliang ZhangdaggerDagger Liping HuangdaggerDagger
Yudagger a G NanoLetters 2009 9 (5) 1758
19 Nakada K M F G Dresselhaus and M S Dresselhaus PhysRevB 1996 54
(9858)
20 Son Y W C M L a L S G PhysRevLett 2006 97 (216803)
21 Raza H Graphene Nanoelectronics Springer 2012
22 Ryan W J Electronic Transport in Graphene p-n junctions Short Noise and
Nanoribbons Harvard University 2009
23 Fangping OuYang J X Rui Guo Hua Zhang and Hui Xu Nanotechnology 2009
20 6
24 Guo J Carbon nanotube electronicsModeling physics and applications Purdue
University West Lafayette IN 2005
25 Motta C S S-P MITrioni cond-matmes-hall 2012 7
26 B P Growing Graphene via Chemical Vapor Deposition Ponoma College Ponoma
2011
27 ZurichE Transport properties of three-terminal graphene devices University of
Science and Technology Norway 2008
28 Uichiro MIntroduction to the electron theory of metals
29 Robert Laughlin H S Additional background material on the Nobel Prize in Physics
1998 (410)
30 MarkGoerbig Quantum Hall Effects (11152013)
68
REFERENCES
31 Zurich E Transport properties of three-terminal graphene devices Norwegian
University of Science and Technology Norway 2008
32 Deepak R Klein Tunneling University og Tennessee Space Institute Tennessee
2011
33 Williams JR L D CMMarcus Quantum Hall Effect in a Gate-Controlled p-n
Junction in Graphene (1122013)
34 Avadhanulu MN P G K A Textbook of Engineering Physcis for BE BSc (Engg)
SChand New Delhi 1992
35 Andriotis A Applied Physics Letters 2007 91 (152105)
36 Qimin Yan B H dagger Jie Yudagger Fawei Zhengdagger Ji ZangDagger Jian Wudagger Bing-Lin Gu F
L Dagger and Wenhui Duandagger NanoLetters 2007 7 (6) 1473
37 Soler J M E A J D Gale A Garciacutea J Junquera P Ordejoacuten and D Saacutenchez-
Portal J Phys Condens Matter 2002 14 2745
ABSTRACT
ANALYSIS OF TRANSPORT PROPERTIES OF A ZAZ GRAPHENE
NANORIBBON JUNCTION USING VARIOUS DOPANTS
by
Natasha Parikh
A 12 atom wide ZAZ Graphene Junction was simulated and its transport properties were
analyzed I-V curves calculated by nonequilibrium Greens function method combined
with the density functional theory under external bias showed varying semiconducting
characteristics Further the width of the junction also showed significant effects in the
determination of the semiconducting nature A theoretical study was performed on the
semiconducting characteristics by analyzing the I-V curve and transport coefficients in
the junction
ANALYSIS OF TRANSPORT PROPERTIES IN A ZAZ GRAPHENE
NANORIBBON JUNCTION USING VARIOUS DOPANTS
by
Natasha Parikh
A Thesis
Submitted to the Faculty of
New Jersey Institute of Technology
in Partial Fulfillment of the Requirements for the Degree of
Master of Science in Materials Science and Engineering
Interdisciplinary Program in Materials Science and Engineering
January 2014
APPROVAL PAGE
ANALYSIS OF TRANSPORT PROPERTIES IN A ZAZ GRAPHENE NANORIBBON JUNCTION USING VARIOUS DOPANTS
Natasha Parikh
Dr N M Ravindra Thesis Advisor Date Director of Material Science and Engineering Program NJIT Dr Keun H Ahn Committee Member Date Associate Professor of Physics NJIT Dr Tao Zhou Committee Member Date Associate Professor of Physics NJIT Dr Halina Opyrchal Committee Member Date Senior University Lecturer of Physics NJIT
BIOGRAPHICAL SKETCH
Author Natasha Parikh
Degree Master of Science
Date January 2014
Undergraduate and Graduate Education
bull Master of Science in Materials Science and EngineeringNew Jersey Institute of Technology Newark NJ 2014
bull Bachelor of Arts in Physics and Biological SciencesRutgers the State University of New Jersey New Brunswick NJ 2012
Major Materials Science and Engineering
iv
v
ACKNOWLEDGMENTS
I would like to express my gratitude to my supervisor Dr NM Ravindra for the useful
comments remarks and engagement throughout the learning process of this Mastersrsquo
thesis Furthermore I would like to thank Vijay Kasi Somayajula for introducing me to
the topic as well for the support I thank Dr Tao Zhou Dr Ken Ahn and Dr Halina
Opyrchal for serving on my thesis Committee I would like to thank my loved ones who
have supported me throughout the entire process both by keeping me harmonious and
helping me in putting pieces together
vi
TABLE OF CONTENTS
Chapter
Page
1 INTRODUCTIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
1
11 Graphene The New Carbonhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
1
12 Graphene Synthesishelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
3
121 Synthesis of Graphene on Nickel (Ni)helliphelliphelliphelliphelliphelliphelliphellip
5
122 Synthesis of Graphene on Copper (Cu)helliphelliphelliphelliphelliphelliphelliphellip
8
123 Transfer of Graphene Filmshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
8
124 Synthesis of Graphene Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
9
125 Doping in Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
10
126 Nitrogen (N) Doped Graphene Synthesis (Substitutional)hellip
12
13 Structure of Graphene Nanoribbon (GNR)helliphelliphelliphelliphelliphelliphelliphelliphelliphellip
13
14 Overview of Graphene Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
15
2 RESEARCH BACKGROUNDhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
21 Bandstructure of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
22 Transport Characteristics of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
20
23 Drude Theoryhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
22
24 Quantum Hall Effect (QHE)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
24
25 Resistivity and Resistancehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
27
26 Klein Tunnelinghelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
28
27 Quantum Hall Effect in Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
31
28 Thermoelectric Effecthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 34
vii
TABLE OF CONTENTS
(Continued)
Chapter Page
281 Seebeck Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
34
282 Peltier Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
36
29 Early Research ndash ab initio Studyhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
37
3 COMPUTATIONAL DETAILShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
31 Introductionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
311 Extended Huckel Theory helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
312 Introduction to NEGFhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
41
313 Electrostaticshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
42
314 Non-Equilibrium Greenrsquos Functionhelliphelliphelliphelliphelliphelliphelliphelliphellip
44
4 ATOMISTIX TOOLKIT DETAILShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
41 Introductionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
42 Device Structurehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
43 Transmission Spectrum Calculationhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
50
44 Calculating the Currenthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
51
45 Calculating the Transport Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
52
5 RESULTS AND DISCUSSIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
53
51 Band Structure Analysis helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
53
52 I-V Characteristics of GNR Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
59
53 Thermoelectric Propertieshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
63
6 CONCLUSIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 65
REFERENCEShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
66
viii
LIST OF FIGURES
Figure Page
11 (a) Chemical representation of Carbon (b) Graphite ore (c) Structure of
Graphite and a single layer Graphenhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
2
12 An optical image of Graphene flake obtained by exfoliation of
graphitehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
3
13 (a) Graphene formation on Nickel (b) Graphene atoms on Ni (111)
lattice (c)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
7
14 (a) SEM image of graphene on copper foil (b) High-resolution SEM
image of graphene on Cuhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
8
15 (a) Transfer process (b) Wafer-scale synthesis of graphene (c) Graphene
films transferred onto glass wafer (d) SiSiO2 with device patterned (e)
PET filmhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
9
16 (a) High-magnification image of the annealed sample showing that well-
defined zigzag armchair and zigzag-zigzag edges are formed (b) ) STM
image of an 8 nm wide bent junction connecting an armchair and a
zigzag graphene nanoribbon which was carved by STM
tipshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
10
17 Band structure of graphene before and after doping The image shows
shift towards the Fermi levelhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
11
18 Low resolution TEM image of N-doped graphene Background is the
lacey carbon TEM grid graphene sheet is crumpled with many
rippleshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
13
19 Zigzag and Armchair orientation of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphellip 13
110 Bandstructure of ZGNRhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 14
111 Bandstructure of AGNRhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 15
21 Left Real space Graphene lattice with basis vectors and Right
The first Brillouin zone of Graphene in reciprocal space with basis
vectors and K and Krsquo are responsible for massless transport at low
energyhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
ix
LIST OF FIGURES
(Continued)
Figure Page
22 Bandstructure of a graphene sheet showing a band gap of 0eVhelliphelliphellip 18
23 Band structure of Graphene calculated with the tight-binding modelhellip 19
24 The energy dispersion around the K pointhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 22
25 Electrons colliding with stationary ionshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 23
26 (a) 2D electrons in a perpendicular magnetic field Logitudinal resistance
measured across C5 and C6 Transverse resistance measured across C3
and C5 (b) Classical Hall resistance as a function on the magnetic field
25
27 Klein tunneling through an npn barrierhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 29
28 Electron trajectory considering the linear electrostatic potential U(x) = Fx 30
29 Electron like and hole like trajectories at same Ehelliphelliphelliphelliphelliphelliphelliphelliphellip 30
210 Quantum Hall effect in graphene 22
The Hall conductivity σxy and the
longitudinal resistivity of monolayer graphene as a function of carrier
density at B = 14T and T= 4K This shows half-integer QHE with chiral
index J= 1helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
32
211 (a) LL for Graphene bilayer (b) Schematics of Hall conductivity as a
function of nn0 for bilayer Graphene (solid line) and monolayer
Graphene (dotted line) (c) LL for monolayer Graphenehelliphelliphelliphelliphelliphelliphellip
33
212 Seebeck Effecthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 35
213 Transmission functions in units of (2e2h) for AZA structureshelliphelliphelliphellip 37
214 I-V curve for a 591nm long channel (Vbias=20mV)helliphelliphelliphelliphelliphelliphelliphellip 38
31 NEGF systemhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 42
41 Geometry of device configuration with two electrodeshelliphelliphelliphelliphelliphelliphellip 48
42 The electron distribution in a device configuration which illustrates a left
moving scattering state with origin in right electrodehelliphelliphelliphelliphelliphelliphelliphellip
48
x
LIST OF FIGURES
(Continued)
Figure Page
51 Band structure of AGNR widths (a) 4 atoms (b) 5 atomshelliphelliphelliphelliphelliphellip
53
52 Band structures of AGNR widths (a) 6 atoms (b) 7 atomshelliphelliphelliphelliphelliphellip 54
53 Band structure of AGNR widths (a) 8 atoms (b) 9 atomshelliphelliphelliphelliphelliphelliphellip 54
54 Band structures of AGNR widths (a) 10 atoms (b) 11 atomshelliphelliphelliphelliphellip 55
55 Band structure of AGNR with a width of 12 atomshelliphelliphelliphelliphelliphelliphelliphelliphellip 55
56 Variation in band gaps as the width (number of atoms) varieshelliphelliphelliphellip 55
57 Band structure of ZGNR width (a) 4 atoms (b) 6 atomshelliphelliphelliphelliphelliphelliphellip 56
58 Band structure of ZGNR width (a) 8atoms and (b) 10 atoms 57
59 Band structure of ZGNR with a width 12 atomshelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 57
510 Band structures of Doped AGNR (a) 4 N Doped (b) 4 B Doped (c)
2 N Doped (d) position of Nitrogen from (c)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
58
511 Current Vs Voltage graph for varying graphene width showing
conductivityhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
59
512 ZAZ GNR junction devicehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 60
513 I-V curve of Boron Doped ZAZ junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 61
514 I-V curve of Nitrogen Doped ZAZhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 62
515 Variation of Peltier effect coefficient with temperature for various doping 64
1
CHAPTER 1
INTRODUCTION
11 Graphene The New Carbon
Carbon (chemical symbol C atomic mass 1207amu) (Figure 11a) is a widely distributed
element in nature It is found abundantly in the sun stars comets and the atmospheres of
the planet Carbon can form up to four bonds it can bond with itself endlessly and with
most other elements in many different shapes making it a significant part of the
construction for many kinds of complex molecules1
Two allotropes of carbon are commonly used diamond and graphite (Figure
11b) The bonding structures of diamond and graphite contribute to the properties
individually In diamond all the p-orbitals are used forming a sp3
bonding whereas in
graphite only two orbitals are occupied allowing the unpaired bond for the transport of
electrons Each carbon atom in graphene possesses sp2 hybridization ie each carbon
atom is connected to three other carbon atoms via covalent bonds with a bond length of
142Å and an angle of 120deg between each bonded pair This makes graphite a better
conductor than diamond Graphite consists of many layers of 2D carbon lattices (Figure
11c) stacked on top of each other and held via Van der Waals forces A single layer of
graphite where carbon atoms are arranged in a honeycomb lattice is known as graphene
(Figure 11c)
2
Figure 11 (a) Chemical representation of Carbon (b) Graphite ore (c) Structure of
Graphite and a single layer Graphene2
Theoretical work on graphene was done specifically to study the other allotropes
The first study was done by Wallace in 1947 who calculated the band structure of
graphene3 Further the peculiar Landau levels were known by McClure in 1957 and the
relativistic Hofstadter butterfly by Ramal in 19853 Later in 1991 the invention of carbon
nanotubes by Iijima boosted the theoretical research on graphene3 Prior to the invention
of carbon nanotubes there were a few experimental papers on graphene growth via
various methods like intercalation of graphite (Shioyama 2001) free standing (Boehm
1962) epitaxial as well as graphene grown on metals (Bommel 1975 Land 1992 Itoh
1991)3 With all the various discoveries the electronic properties of graphene were not
studied until 2004 when Berger and Novoselov were able to access the electronic
properties with contact of graphene flakes3 (Figure 12)
3
Figure 12 An optical image of Graphene flake obtained by exfoliation of graphite3
The specific lattice structure of graphene possesses a number of unique electronic
properties making it an interesting material for theorists experimentalists and engineers
Utilization of graphene as a fundamental block of electronic devices requires
development of new theoretical methods for understanding the current propagations in
graphene constriction4
12 Graphene Synthesis
The discovery of graphene by mechanical exfoliation called the lsquoScotch tape methodrsquo led
to serious attempts towards the production of top quality graphene5 Graphene was first
exfoliated mechanically from graphite in 20046 The importance of high quality graphene
cannot be emphasized enough however electron transport has shown that defects play an
important role in hindering the transport properties of electrons (holes)7 The two
synthesizing methods for the large scale manufacture of graphene are chemical vapor
deposition (CVD) and silicon carbide (SiC) desorption method
4
Graphene can be synthesized by sublimation of silicon from SiC at high
temperature (1200degC) in high vacuum5 The major advantage of this method is that the
SiC provides an insulating substrate and no transfer of the graphene layer is needed Yet
the disadvantage of this method outweighs its advantages the high temperature is cost-
ineffective making it unsuitable for large scale manufacturing8 Also the crystal growth
face alters the properties of graphene Graphene grown on Si-terminated face has poor
homogeneity and is subjected to unintentional doping7 Conversely graphene grown on
C-terminated SiC has higher mobility and is often called lsquoturbostaticrsquo due to the
rotational disorder7
Unlike the SiC method the graphene produced via CVD method needs to be
transferred to a substrate making it difficult to maintain the quality of graphene Yet
CVD synthesized graphene has a larger grain size7 More research is being done on
various methods for synthesis of graphene The methods include direct chemical
synthesis ion implantation crystal sonification and lastly unzipping carbon nanotubes to
form graphene sheets9
Graphene and few-layer graphene have been grown by CVD from carbon
containing gases on catalytic metal surfaces andby surface segregation of C dissolved in
the bulk of such metals7 Growing graphene with CVD is a very attractive solution since
it is compatible with the existing semiconductor industry9 Graphene has been grown via
CVD process on metal substrates such as Nickel (Ni) and Copper (Cu)
5
121 Synthesis of Graphene on Nickel (Ni)
Polycrystalline Ni films are annealed in ArH2 atmosphere at 900-1000degC to increase
grain size and are then exposed to H2CH4 gas mixture10
In this step the hydrocarbon
decomposes and dissolves in Ni to form a solid solution Lastly the samples are cooled in
argon gas Ni has high carbon solubility at elevated temperatures and the solubility
decreases as temperature is reduced During the cooling process the carbon atoms diffuse
out from the Ni-C solid solution and precipitate on the Ni surface to form graphene films
(Figure 13a) Since Ni (111) has a lattice similar to the densely packed hexagonal lattice
of graphene (Figure 13b) they also have similar lattice constants and hence Ni surface
serves as an excellent lattice matched substrate for graphene growth11
The growth of graphene on Ni is based on carbon segregation and precipitation
process different segregation behavior is produced by different cooling rates which
affect the thickness and quality of graphene films12
Medium cooling rates lead to optimal
carbon segregation and produce few layers12
Graphene films grown on Ni are usually
continuous with monolayer and few layer regions Annealing of Ni substrates at elevated
temperatures in hydrogen atmosphere not only increases the single-crystalline Ni grain
size but also eliminates certain impurities in Ni thereby improving the graphene quality
Furthermore the graphene thickness can also be affected due to the amount of carbon
dissolved in the Ni films during the growth time
After synthesis the graphene can be transferred to other insulator substrates for
further characterization and applications Figure 13c shows the selected area electron
diffraction pattern of graphene film along the [001] direction which confirms the
graphene lattice structure shown After transfer to insulator substrates the geometry can
6
be retained as shown in Figure 13d Under optimal growth parameters graphene growth
is only limited by the Ni catalyst Lastly Figures 13e and 13f show the wafer-scale
graphene synthesis and transfer of graphene to a flexible transparent substrate
respectively
Though polycrystalline Ni is a good substrate the percentage and size of
graphene monolayer are still limited Researchers have hence tried other metal substrates
for graphene synthesis
7
Figure 13 (a) Graphene formation on Nickel (b) Graphene atoms on Ni (111) lattice
(c) Low magnification TEM image of graphene edges (d) Optical image of graphene
transferred from the Ni surface to SiO2Si substrate (e) Full-wafer scale deposition of
graphene layers on polycrystalline Ni (f) Transparent and flexible graphene films on
PDMS substrate10
8
122 Synthesis of Graphene on Copper (Cu)
Graphene films are grown on 25microm thick Cu foils in a hot wall furnace13
The Cu foil is
first annealed in hydrogen atmosphere at 1000degC and a mixture of H2CH4 is introduced
into the system to initiate graphene growth After a continuous graphene layer is formed
on the Cu foil the system is cooled to room temperature Figure 14a shows an SEM
image of graphene on Cu substrate indicating the Cu grains with contrast The Cu
surface steps are formed during thermal annealing and the darker flakes indicate multiple-
layer graphene (Figure 14b)10
The graphene wrinkles in Figure 14(b) originate from
different thermal expansion coefficient of graphene and Cu They go across the Cu grain
boundaries indicating that the graphene film is continuous
Figure 14 (a) SEM image of graphene on copper foil (b) High-resolution SEM image of
graphene on Cu10
123 Transfer of Graphene films
In order to facilitate the applications of graphene for electronic applications we need to
separate the graphene from the catalytic metal substrate Figure 15a shows the transfer
process of graphene Graphene is first coated with a thin layer of polymethyl
methacrylate (PMMA) and baked at 120degC to evaporate the solvent10
The metal layer is
then removed by Ni or Cu etchant leaving behind the PMMA graphene film The film is
then cleaned by deionized water and then transferred onto the target substrate After the
9
evaporation of water vapor the PMMA is removed by acetone leaving graphene film on
top of the target substrate Figure 15b shows a graphene wafer transferred from the
substrate onto glass and polyethylene terephthalate (PET) films
Figure 15 (a) Transfer process (b) Wafer-scale synthesis of graphene (c) Graphene
films transferred onto glass wafer (d) SiSiO2 with device patterned (e) PET film10
124 Synthesis of Graphene Junction
Graphene junctions with smooth armchair and zigzag edges are difficult to produce by
conventional methods such as mechanical exfoliation chemical exfoliation or lithography
etching14
The conventional methods can only produce rough edges Recently
Dresselhaus reported an edge reconstruction of graphene by Joule heating in a TEM-STM
10
(Figure16b) system15
An individual nanoribbon sample is attached to the sample holder
at one end and to the STM tip at the other end these ends also serve as the two
electrodes The structural transformation in the growth of graphene from armchair to zig-
zag is mainly attributed to the vaporization of carbon edges that reconstruct at high
temperatures in which resistive Joule heating and preferred current flow play an
important role This means that by controlling the flow of current a perfectly smooth
edged ribbon can be synthesized making graphene-based electronics possible16
Figure 16 (a) High-magnification image of the annealed sample showing that well-
defined zigzag armchair and zigzag-zigzag edges are formed (b) STM image of an 8 nm
wide bent junction connecting an armchair and a zigzag graphene nanoribbon which was
carved by STM tips14
125 Doping in Graphene
The doping of graphene can be roughly classified into two categories - electrical and
chemical Electrical doping involves changing gate voltages of graphene devices and
chemical doping uses chemical routes such as substitutional or interstitial This thesis
discusses chemical doping and the importance of doping sites by changing the dopant
Chemical doping is a common approach to tailor the electronic properties of
11
semiconductors Doping of graphene can cause its electronic properties to alter leading to
a metal-semiconductor transition The two means of doping graphene are interstitial and
substitutional In interstitial doping the dopant atoms or molecules are introduced as
adatoms or admolecules on the surface of graphene whereas in substitutional doping the
dopant atoms are replaced in the carbon lattice forming a bond in the lattice of
graphene16
Doping graphene results in the formation of n or p-type semiconductors
depending on the kind of dopant If the dopant is an electron donor it causes the Fermi
level to shift up resulting in n-type behavior of graphene Furthermore if the dopant is an
electron acceptor it causes the Fermi level to shift down resulting in a p-type behavior of
graphene (Figure 17)16
Figure 17 Band structure of graphene before and after doping The image shows shift
towards the Fermi level16
Graphene nanoribbons (GNR) can be made into a p- and n- type semiconductor
by doping with boron (B) and nitrogen (N) respectively In theory GNR p-n junction is
formed by doping GNR with B and N in different regions However experimentally
doping graphene with both these elements is very difficult due to the dopants reacting
with each other17
Hence most experimental studies use GNR doped by only one
12
element N-doped graphene was synthesized by Wei et al Wang and B-doped Graphene
was realized by Endo17
Many researchers have demonstrated interstitial doping of graphene by gas metal
and organic molecules16
The various gases and metals used are NO2 NH3 An-CH3 Na-
NH2 F4-TCNQ TPa TCNE and others16
Doping in graphene is hence possible by
electrons or holes in high concentration without deterioration of its mobility Interstitial
doping is highly sensitive due to most of the conducting channel being exposed to surface
absorbates and hence can be used in molecule detection
In substitutional doping the dopant atoms are included in the graphene lattice and
thus chemically bonded Substitutional doping is done via the CVD method using a
carbon and dopant source Substitutional doping opens up many applications in device
engineering making graphene a very good candidate as a semiconductor This study
involves the study of transport properties of graphene doped by substitution
126 Nitrogen (N) Doped Graphene Synthesis (Substitutional)
N-Doped graphene is prepared via a CVD process using a 25microm thick Cu film on a Si
substrate The substrate is placed in a quartz tube with the flow of hydrogen (20sccm) and
argon (100 sccm)18
When the center of the furnace reaches 800degC 60 sccm of CH4 and
60 sccm of NH3 is introduced into the flow as C source and N source respectively The
substrate is then moved to high temperature and after 10 min growth the sample is
cooled to room temperature under H2 ambient Figure 1 8 shows the growth of N-doped
graphene18
13
Figure 18 Low resolution TEM image of N-doped graphene Background is the lacey
carbon TEM grid graphene sheet is crumpled with many ripples18
13 Structure of Graphene Nanoribbon (GNR)
Graphene Nanoribbons (GNR) are strips of graphene with very thin width of lt50nm
GNRs can be terminated in three separate ways called zig-zag (0 n) armchair (m 0) and
chiral (m n) (Figure19) and this termination along the width of the ribbon dictates the
size of the band gap19
Figure 19 Zigzag and Armchair orientation of Graphene5
Due to their various edge structures GNRs exhibit different electronic properties
ranging from normal semiconductors to spin-polarized half metals which open the
possibility of GNRs as electronic devices19
14
Within a tight binding approach (AGNRs) could be metallic or semiconducting
depending on their ribbon width but all zigzag graphene nanoribbons (ZGNRs) are
metallic with a high density of electronic states at the edges Hence ZGNRs exhibit
characteristic edge effects which are not present in AGNRs These edge effects in
ZGNR create a flat band close to the Fermi level making the ZGNR edges more
reactive19
First-principles calculations show that the GNRs possess a non-zero direct
band gaps These gaps are small for ZGNR (Figure 110) caused due to spin ordering
effects at the edges For AGNRs the band gap arises from quantum confinement (Figure
111) effect that has larger magnitudes than ZGNR20
Figure 110 Band structure of ZGNR
15
Figure 111 Band structure of AGNR
For GNRs the band gap decreases as the ribbon width increases and in order to
create a semiconductor with a desirable band gap the nanoribbon width should be
adjusted accordingly This property of adjusting the band gap makes graphene an
excellent candidate for transistor switching By applying an electric field GNR can be
altered from an insulator to a conductor GNRs exhibit very intriguing properties and
have become one of the promising candidates for electronic applications
14 Overview of Graphene Junction
The invention of p-n junctions date back to 1940s which later resulted in the invention of
junction transistors One of the key technological reasons for success of the p-n junction
is mainly due to its ability to locally modulate the energy band gaps via an applied bias21
A graphene p-n junction is created via single layer of graphene in which the
carrier type and density in two adjacent regions are controlled by electrostatic gating8
For materials with a band gap the electric field can either switch lsquooffrsquo the current or
rectify it (p-n diode)22
Being a ldquogaplessrdquo material the off state is not achievable in
16
graphene In order to achieve an off state the gap can be created by doping graphene with
various elements (Group III or Group V) Doping allows p-n junctions to be
reconfigurable using a gate voltage to distinguish between graphene p- n regions within a
single sheet Many researchers have studied the electronic as well as transport properties
of doped graphene junctions
In 2009 Fangping OuYang studied the transport properties of T-shaped graphene
junctions using the ATK software and showed that the conductance depends on
geometric structures which can be controlled by selective doping23
Wei Yao in 2013
studied the transport properties in graphene p-n junctions and showed that the
rectification effect depends on boron doping density and position17
The study of transport properties in graphene p-n junctions is a recent
advancement The thesis discusses transport properties including the current-voltage (I-
V) characteristics of doped graphene junctions Moreover the software used is similar to
the software in use by current researchers since they have produced viable data using
ATK
17
CHAPTER 2
RESEARCH BACKGROUND
21 Band Structure of Graphene
The unique electronic properties of graphene were first predicted in 1946 Figure 21
shows a top view of the hexagonal arrangement of carbon atoms in real space as well as
the first Brillouin zone in reciprocal space
Figure 21 Left Real space graphene lattice with basis vectors and Right The
first Brillouin zone of graphene in reciprocal space with basis vectors and
K and
Krsquo are responsible for massless transport at low energy24
The real space basis vectors are radic
and
radic
The reciprocal space basis vectors are 1 2
0 0
4 1 3 4 1 3( )and ( )2 2 2 23 3
b x y b x ya a
where the magnitude of the basis vectors is |a0| = radic acc The distance between nearest
neighbor carbon atoms is acc=0142nm
18
The band structure can be calculated by solving the eigenvalues using the
dispersion relation E( )
1 2 3( ) 3 2cos 2cos 2cosE k t k a k a k a (21)
Transport properties of solids are closely related to the energy dispersion
relations E ( ) in the material and in particular to the behavior of E ( ) near the Fermi
level Graphene is a zero gap semimetal whose specific linear electronic band dispersion
near the Brillouin zone corners (Dirac points) gives rise to electrons and holes that
propagate as massless Fermions25
The valence and conduction bands do not overlap in
graphene they touch at the Fermi Level (Figure 22)
Figure 22 Band structure of a graphene sheet showing a band gap of 0eV
The low energy properties of graphene can be well described by making a linear
expansion of the band structure around the K and Krsquo This energy can be written as
19
E(k) = plusmnħvF|k (22)
where vF is the Fermi velocity of 1106ms given by
1F
Ev
k
ħ (23)
Figure 23 Band structure of graphene calculated with the tight-binding model
22
The Fermi surface of graphene consists of double cones with Fermi energy at the
intersection of these cones (Figure 23) The slope of the band is zero and hence the
effective mass of electrons in that region is zero which leads to an entirely new transport
mechanism in graphene26
20
22 Transport Characteristics of Graphene
Transport process usually involves a flow of charge or energy or both The flow is mainly
due to external perturbations such as electric field and temperature gradient The
relationship between forces and flow usually defines various transport coefficients that
are the characteristics of electrons and phonons in the material All modern electronics
are based on the ability to control the electronic properties of a material by applying
external voltage This is done by an electric field effect where the gate voltage changes
the carrier concentration of the material and consequently its conductivity The electric
field effect in graphene was reported by Novoselov in 2004 and is used in transport
measurements8
The electron-phonon interaction in graphene plays an important role in
understanding the photoemission spectra observed in graphene The electric field effect is
an alternative method for changing the charge carrier density in low dimensional systems
The electric field effect in graphene which was first reported by Novoselov et al in
2004 is widely used as a characterization tool in transport measurements25
The transport characteristics of the material are directly related to the
bandstructure of graphene The carriers in graphene lattice are free to move in two
dimensions In the carrier transport of graphene the carriers ndash electrons and holes ndash close
to the Dirac points are of importance The transport is described by a two component
wave function (Equation 24) which obeys the 2D Dirac-like equation for massless
particles27
21
-ivFσ nablaψ(r) = Eψ(r)
(24)
where σ is the 2D Pauli spin matrix In the continuum limit the above (Equation
24) corresponds to the effective low energy Dirac Hamiltonian (Equation 25)
0( )
0
x y
F F
x y
iH k k
i
k kv v
k k
(25)
The electronic band structure of the energy (E) versus wave vector (k) relation for
graphene is given by Equation 24
The two component wave function resembles the spin or wave function of
quantum electro dynamics (QED)27
Corresponding to the spin of particles in QED the
charge carriers of graphene can be attributed with a pseudospin σ The pseudospin is the
direct result of two different carbon sublattices corresponding to the bonding and
antibonding combinations27
22
Figure 24 The energy dispersion around the K point27
In Figure 24 the red and blue lines correspond to the antibonding and bonding
states respectively The pseudospin can have two values either in the direction of or
against the momentum It can be seen that the electrons with energy E travelling in the
positive direction originates from the same branch as a hole with energy ndashE travelling in
the negative direction giving it the same pseudospin This results in suppressed
backscattering and Klein tunneling The back scattering process requires the pseudospin
to flip which is possible in the presence of short range scatters that act differently on sub
lattices27
23 Drude Theory
The classical theory of metallic conductivity was presented by Drude in 1900 and was
elaborated by Lorentz in 190528
Drude treated the free electrons as classical ideal gas
meaning the electrons collide with stationary ions and not each other
23
Figure 25 Electrons colliding with stationary ions28
The Drude theory applied the kinetic theory of gases to a metal considered as a gas of
electrons The basic assumptions made by the Drude theory are28
When metallic elements are brought together to form a solid then the valence
electrons become freely moving through the metal whereas the ions remain intact
as nearly immobile positive particles
Between collisions the electrons move freely ie there is neither electron-
electron interaction nor electron-ion interaction
The scattering mechanism leads to instantaneous collisions of the electron with
the scatterers
The collisions are characterized by a relaxation time τ
The electrons achieve thermal equilibrium only through collisions the velocity
after a collision is randomly directed the speed is as appropriate to the
temperature
With the relaxation time Drude obtained the electrical conductivity expression
where n is the number of electrons per unit volume
σ = ne2τm
(25)
He also calculated the thermal conductivity and successfully provided the
theoretical basis for Wiedemann-Frantz law already established in 1853 which states that
24
the ratio of electrical and thermal conductivity of any metals is a universal constant at any
given temperature28
The Drude theory gives results which are qualitatively correct outside of the
quantum Hall regime28
In the Drude theory of the electrical conductivity of a metal an
electron is accelerated by the electric field for an average time τ before being scattered
by impurities lattice imperfections and phonons to a state which has zero average
velocity The average drift velocity of the electron is
d
eE mv (26)
It is assumed that all electrons drift together and hence the current density
j = -ne (27)
This Drude theory works well for fields below ~ 01T At stronger fields the Hall
resistivity becomes nearly constant over finite intervals of magnetic fields28
The QHE
reflects both novel disorder physics as well as novel interaction physics in the quantum
Hall regime
24 Quantum Hall Effect (QHE)
The discovery of QHE is a remarkable achievement in condensed matter physics The
Hall Effect was discovered by Edwin Hall in 187929
However the precise quantization
of the Hall conductance in units of e2h was not recognized until February 1980 Five
years later in 1985 Klaus von Klitzing was awarded the Nobel Prize in Physics for the
discovery of QHE29
The quantum Hall effect occurs in two-dimensional electron systems in the limit
of strong perpendicular magnetic field that stems from electronic transport
25
measurements where one drives a current I through the sample and where one measures
both the longitudinal and transverse resistance (Hall resistance) A longitudinal resistance
is a resistance measured between two contacts that may be connected by a line which
does not connect C1 and C430
Transverse resistance is measured between two contacts
connected by an imaginary line connecting C1 and C4 (Figure 26a)
Figure 26 (a) 2D electrons in a perpendicular magnetic field Logitudinal resistance
measured across C5 and C6 Transverse resistance measured across C3 and C5
(b) Classical Hall resistance as a function on the magnetic field30
Due to the existence of quantum Hall effect it is natural to expect that there exists
a classical Hall Effect Hall showed that the transverse resistance of a thin metallic plate
varies linearly with the strength B of the perpendicular magnetic field (Figure 26 b)
RH = Bqnel (28)
More quantitatively the classical Hall Effect can be understood within the Drude
model for diffusive transport in a metal Within this model one considers independent
26
charge carriers of momentum p described by the equation of motion
( )
b
dp p pe E B
dt m (29)
where E and B are the electric and magnetic field respectively The macroscopic
transport characteristics ie resistivity of the system are obtained from the static
solution of the equation of motion dpdt = 0 and one finds for 2D electrons with p =
(pxpy)
x
x yb
y
y xb
eBe
eBe
ppE
m
ppE
m
(210)
In the above expression characteristic frequency is visible as
C
b
eB
m (211)
This is known as cyclotron frequency as it characterizes the cyclotron motion of a
charged particle in a magnetic field30
With the Drude theory the conductivity can be
written as
j = -enelpmb (212)
and the mobility can be given as
micro = eτmb (213)
The transport properties in the limit of ωCτ-gt infin are entirely governed in the presence of
27
a magnetic field by the off-diagonal ie transverse components of
conductivityresistivity
The theory of quantum Hall effect subjects all physical properties of 2D electron
system in the limit where the magnetic field is strong so that the mixing of Landau levels
by disorder or electron-electron interaction is considered to be a weak perturbation30
This is known as the quantum Hall regime The ratios between the energy scales
corresponding to the two interactions are important The limit where disorder potential is
much stronger is referred to as integer quantum hall regime whereas the limit where the
interaction potential is much stronger is referred to as fractional quantum Hall regime
25 Resistivity and Resistance
The electronic transport in the framework of the Drude theory allows for the calculation
of conductivity or resistivity of a classical diffusive 2D electrons in a magnetic field30
The conductivity and conductance are related to one another but they depend on the
geometry of the conductor-the resistance R and hence the resistivity is given by
R = (LA)ρ (214)
where L is the length of the conductor and A is the cross section
For a d-dimensional conductor the cross section scales as Ld-1
such that the
scaling relation between the resistance and the resistivity is
R~ ρL2-d
(215)
From the dimension point of view resistance and resistivity are the same in 2D and the
resistance is scale-invariant Further the resistance of a 2D conductor depends in
general on the so-called aspect ratio LW via some factor f (LW)30
However for
transverse Hall resistance it is the length of the conductor that plays the role of cross
28
section such that the Hall resistivity and the Hall resistance truly coincide ie f=1 The
Quantum Hall effect is highly insensitive to the particular geometric properties of the
sample used in transport measurements Recently quantum Hall physics experienced the
discovery of ldquorelativisticrdquo quantum Hall effect in graphene The electrons in graphene
behave as if they were relativistic massless particles contributing to a very interesting
field of research30
26 Klein Tunneling
Klein tunneling in which relativistic particles penetrate through a potential barrier
without the exponential damping that is characteristic for nonrelativistic quantum
tunneling has never been observed for elementary particles The tunneling allows
transmission of a particle through a potential barrier higher than its kinetic energy
violating the principle of classical mechanics30
On the quantum scale the objects exhibit
wave-like characteristics in which the quanta move against a potential hill described by
their wave function This wave function represents the probability amplitude of finding
the object in a particular location The transmission of the object through the potential hill
is termed as tunneling When EltV then the ψ(x) over V is returned by ψrsquo(x) In quantum
mechanics an electron tunnels from the conduction into the valence band Such a
tunneling from an electron-like to hole-like state is called as Klein Tunneling in which the
electron avoids backscattering
In Figure 27 it is shown that an electron hitting a potential barrier is reflected
with 100 certainty In non-relativistic quantum mechanics the electrons can tunnel
through the barrier but the probability of tunneling exponentially decays with increasing
29
height and width of the barrier However in relativistic quantum mechanics the barrier
gets transparent even in the limit of infinite barrier height (Klein paradox)31
Figure 27 Klein tunneling through an npn barrier30
The Klein paradox in graphene can be understood in terms of electrons and holes
In graphene the massless carriers behave differently than ordinary carriers (with mass) in
the presence of an electric field A barrier which is repulsive for electrons will be
attractive for holes Since there are hole states inside the barrier with the same energy as
the electrons outside an electron arriving at the barrier can tunnel through it as a hole
before leaving again as an electron Klein tunneling for transport in graphene is that the
charge carriers cannot be confined by potential barriers The Klein tunneling effect has
been experimentally observed by Ando in 1998 in which the absence of backscattering
(Figure 28) is responsible for high conductivity in carbon nanotubes
30
Figure 28 Electron trajectory considering the linear electrostatic potential U(x) = Fx30
The electron is able to propagate through an infinitely high potential barrier since
it makes a transition from the conduction band to valence band In this transition from
conduction band to valence band its dynamics changes from electron-like to hole-like
The equation of motion is thus given by
2
2 2 2| | ( )
pdr E
dt E Up
p E U
v
v
at energy E (216)
This shows that in the conduction band (UltE) and in the valence band (UgtE)
In Klein tunneling the pairs of electron-like and hole-like trajectories at the same E and
py have turning points at dmin given by dmin=2v|py|F (Figure 29)
Figure 29 Electron like and hole like trajectories at same E21
31
The tunneling probability exponential dependence on dmin
2
min| |
( ) exp( ) exp( )2
y y
y
vT
F
p pdp
(217)
The applications of the Klein tunneling include Atomic clock Scanning tunneling
Microscope Tunnel diode Tunneling transistor and many more32
Since graphene
exhibits Klein tunneling it can be very useful to study the transport properties in
graphene and use it in such applications
27 Quantum Hall Effect in a Graphene
A monolayer graphene shows half-integer quantum Hall effects where the Hall
resistance is quantized at values of
2
1
xyh v eR
(218)
around filling factors
14( 1 2)Nv
(219)
where N is an integer e is the electron charge h is the Planckrsquos constant and the
factor 4 is due to spin and valley degeneracy QHE in graphene can be observed at room
temperature which is a very intriguing property (Figure 210) Graphene reveals
significant differences with respect to conventional 2D electron systems The Landau
quantization yields energy levels that disperse differently in graphene as well as
particular zero-energy level that is only half filled at the charge neutrality point (v=o)
32
Figure 210 Quantum Hall effect in graphene22
The Hall conductivity σxy and the
longitudinal resistivity of monolayer graphene as a function of carrier density at B = 14T
and T= 4K This shows half-integer QHE with chiral index J= 1
The QHE in graphene is not entirely similar to regular QHE since the charge
carriers in graphene are Dirac Fermions The charge carriers governed by
electrodynamics is given by (Equation 220) which does not apply for graphene and a
QED quantization of graphene electronic band structure is used
En = (n+12)ħω (220)
33
In the presence of magnetic field the nature of the Dirac Fermions in graphene
results in unevenly spaced Landau levels (LL) containing a distinctive LL at the electron-
hole degenerating a zero energy given by
2MG
MGFehn B
n vE (221)
The LL levels at high magnetic fields in MG are shown in Figure 211
Figure 211 (a) LL for Graphene bilayer (b) Schematics of Hall conductivity as a
function of nn0 for bilayer Graphene (solid line) and monolayer Graphene (dotted line)
(c) LL for monolayer Graphene33
It is found that the Hall resistance of a two dimensional electron system has
plateaus as a function of the number of electrons at low temperatures and strong magnetic
fields32
At large B the Dirac-like energy spectrum of graphene gives rise to a
characteristic series of QH plateaus in conductance reflecting the presence of a zero-
energy Landau level that include only odd multiples of 2e2h for uniform carrier density
in the sheet These plateaus of QH edge states at the edge of the sheet circulating in a
34
direction are determined by the direction of B and the carrier type33
This is why QHE in
graphene is known as Half-Integer Quantum Hall Effect
28 Thermoelectric Effect
Thermoelectricity refers to a class of phenomena in which a temperature difference
creates an electric potential or an electric potential creates a temperature difference The
principle of thermoelectric effect has been known for over 100 years Recently the
practical applications of thermoelectric effect have become more viable34
Thermoelectric effect is the direct conversion of temperature differences to
electric voltage and vice versa Joule heating is the heat generated whenever a voltage is
applied across a resistive material The Peltier-Seebeck effect is reversible whereas Joule
heating is not This effect can be used to generate electricity to measure temperature to
cool objects or to heat them Since the direction of heating and cooling is determined by
the sign of the applied voltage thermoelectric devices make very convenient temperature
controllers
281 Seebeck Coefficient
Thomas Johann Seebeck discovered that an emf appears in a circuit composed of two
dissimilar metals when the junction between the metals is held at different
temperatures34
The thermoelectric emf causes a continuous current in the circuit when a
complete loop is formed and the current is known as thermoelectric current This is
known as the Seebeck effect
35
Figure 212 Seebeck Effect34
As long as the two junctions are at different temperatures the thermoelectric emf
exists and the current will keep flowing between the hot and cold junction that are at
different temperatures The Seebeck effect is the conversion of temperature difference
directly into electricity The voltage developed in the circuit shown in Figure 212 is
proportional to the difference in temperature between the two junctions and is given by
V = α (T2-T1) (222)
This Seebeck effect is observed not only in metals but also in semiconductors
Here α is known as the Seebeck coefficient α measures the magnitude of an induced
thermoelectric voltage in response to the temperature difference across the material If the
temperature difference ∆T between the two ends of a material is small then the Seebeck
coefficient of a material is written by
α = ∆V∆T (223)
36
This can be expressed in terms of electric field as
α E∆T (224)
The units of Seebeck coefficient is given as VK The higher the Seebeck coefficient
value the better it is since it will create a very large voltage that can be used to provide
power
282 Peltier Coefficient
Peltier effect is the inverse of Seebeck effect involving a junction phenomenon There is
heat absorption or generation at the junctions depending on the direction of current flow
Heat generated by current flowing in one direction is absorbed if the current is reversed
The heat absorbed per second at a junction carrying current I is given by
Heat absorbed in t sec = πabIt (225)
Here πab is the Peltier coefficient and given by HIt Thus Peltier coefficient is
numerically equal to the applied potential difference expressed in Volts
Overall by studying the flow of electrons the values of Seebeck
coefficient and Peltier co-efficient can be estimated These values determine the various
applications of the materials In this thesis the Peltier and Seebeck coefficient of the
graphene junction and the new applications are discussed
37
29 Early Research ndash ab intio studies
In 2007 Androitis studied that the conducting properties of graphene nanoribbons and
junctions are strongly dependent on their size and geometric features35
He concluded that
there is no conductance for small AZA or ZAZ ribbons (Figure 213)
Figure 213 Transmission functions in units of (2e
2h) for AZA structures
35
Figure 213 shows that T (E) exhibits a negligible peak [T (E) = 001 in units of
2e2h] at E= -225 and 250eV However it was noted that when the width of the arm type
was increased T (E) at -225 and 250eV was 02035
Later in 2007 Qimin Yan used first principles methods to investigate the Current-
Voltage characteristics of GNR Transistors and the effect of edge doping He showed that
GNR field effect transistors can achieve high performance levels with ONOFF ratios on
the order of 103-10
436
Figure 214 is an I-V curve of AZA GNR-FET connected via
armchair metallic leads36
38
Figure 214 I-V curve for a 591nm long channel (Vbias=20mV)
36
In 2009 Fangping OuYang demonstrated the intrinsic transport properties and
effective B or N doping of the junctions by using first-principles quantum transport
simulations He concluded that the I-V characteristics of pure-carbon T-shaped junctions
exhibit metallic behavior and the current in the junction strongly depends on the height
of the stem23
He reported that the conductance of the devices depends on the geometric
structures which can be controlled by selective doping
In 2012 Wei Yao used the first principle calculations based on Density
Functional Theory (DFT) and Non-equilibrium Greens Function (NEGF) to study the
electronic as well as the transport properties of B-doped 6-GNR p-n junction His results
showed that the boron doping interval can influence the rectification effect at low bias
and also exhibit Negative Differential Resistance (NDR) phenomena at high positive
bias
39
CHAPTER 3
COMPUTATIONAL DETAILS
31 Introduction
The physical chemical electrical electronic and optical properties of a solid are
determined by their quantized electronic states The quantum states in low-dimensional
systems are produced due to the confinement of the carrier charges in one or two
dimensions Graphene is a conductor electrons are able to flow through graphene more
easily than through even copper The electrons can travel through the sheet of graphene
like mass-less particles as fast as just one hundredth that of the speed of light The ways
in which electrons behave in graphene make it very helpful to study their fundamental
physical properties Graphenersquos near perfect crystal lattice provides a very clean system
to experiment By restricting the electrons to only two dimensions they exhibit some
interesting properties such as the anomalous quantum Hall effect and Klein tunneling
In this chapter two theoretical concepts used for calculating the electronic structure
and the transport properties for graphene are described These include the Extended
Huckel Theory and Non-Equilibrium Greenrsquos Function (NEGF) method
311 Extended Huckel Theory
Erich Huumlckel was born in Germany on August 9th
1896 He studied mathematics and
physics in Berlin He is best known for his work in the field of chemistry and physics for
two contributions (1) Debye- Huumlckel theory of electrolytic solutions (2) Huumlckel
method of approximate molecular orbital calculations on electron systems In 1930 he
published his findings on systems in 1931 he generalized and expanded the system
40
theory to explain benzene Due to his poor communication skills his findings went
unrecognized for over 20 years It was in 1951 that his 4n + 2 rule was finally clarified by
Doering to show if C=C bonds would show aromaticity Huumlckel died on February 16th
1980 with very little worldwide recognition for his contributions to chemistry Today
chemistry students recognize his name and his contributions to the field are quite
substantial
One of the first semi-empirical methods to be developed was Huumlckel Molecular
Orbital Theory (HMO) HMO was developed to describe molecules containing
conjugated double bonds HMO considered only electrons in pi orbitals and ignored all
other electrons in a molecule The Extended Huumlckel Molecular Orbital Method (EH) was
developed out of the need to consider all valence electrons in a molecular orbital
calculation
By considering all the valence electrons chemists could determine molecular
structure compute energy barriers for bond rotations and determine energies and
structures of transition states for reactions By considering only the valence electrons the
computed energies could be used to choose between proposed transition states to clarify
reaction mechanisms The total valence electron wavefunction is described as a product
of the one-electron wave functions
1 2 3(1) (2) (3) ( )valence j n (31)
where n is the number of electrons and j identifies the molecular orbital Each
molecular orbital is written as a linear combination of atomic orbitals (LCAO)
1 12
N
j jr rrc j N
(32)
41
The energy of the jth
molecular orbital is given by a one-electron Schroumldinger
equation using an effective one electron Hamiltonian heff which expresses the interaction
of an electron with the rest of the molecule
eff j j jh (33)
This is the energy eigenvalue of jth
molecular orbital corresponding to the Eigen
function j The advantage of using this method is that the exact form of heff is not
required The total energy of the molecule is the sum of the single electron energies
j jj
E n (34)
where nj is the number of electrons in orbital j
In order to use the Extended Huckel method a set of calculation parameters and
approximations must be followed These parameters include the Basis set K-point and
the Brillouin Zone and lastly the Mesh cut-off
312 Introduction to NEGF
The Greenrsquos function is a function of two space-time coordinates From the knowledge of
this function one can calculate time-dependent expectation values such as currents and
densities electron addition and removal energies and the total energy of the system In
the absence of external fields the non-equilibrium Green function method reduces to the
equilibrium Green functions NEGF can be applied to both extended and finite systems
The generic system of NEGF consists of the electron dynamics of the channel described
by the Hamiltonian This channel consists of two contact reservoirs with respective
chemical potential μR and μL The NEGF assumes ballistic transport neglecting self-
42
energy from scattering The system is insulated from gate contacts whose effects are
realized via a 3D Poisson solver which solves for the potential at a given point in real
space based on electron density
22 ( ) [ ( ) ( )]D
qr N r n r
(35)
Figure 31 NEGF system
The system is easily expandable to systems with several contacts or gate
configurations by adding additional self-energy matrices to NEGF or additional sources
to the Poisson solver
313 Electrostatics
Electrostatic potential is created every time in the presence of a charge density due to an
induced electric field The Poissonrsquos equation correlates the electrostatic potential to
charge density as given in Equation 36
43
2( ( ) ( ) ( ) ( ))( )
( )( ) ( )
ADq p r n r r N rr
rr r
N
(36)
where ɛ(r) is the dielectric permittivity of the material ρ(r) n(r) ND(r) and NA(r) are the
hole electron donor and acceptor concentrations of the system respectively
Two types of boundary conditions are usually applied to the Poissonrsquos equation
Dirichlet boundary conditions
Φ (0) = F0 and Φ (L) = FL
von Neumann boundary conditions
00
( )
x
d x
dxB
and
( )L
x L
d x
dxB
For the transport problems with open boundary conditions the von Neumann
boundary conditions are used assuming that the potential vanishes at the boundary ie
B0=BL=0
The Poissonrsquos equation can hence be discretized on a grid as
2 ( )( )
( )
rx
r
= M (37)
where M is the matrix Φ and ρ are vectors containing the discretized values of
the electrostatic potential Φ and charge density ρ respectively
44
The Schroumldinger and Poisson equations are coupled since V(x) = -qΦ(x) is used
for the Schroumldinger to compute ρ(x) This self-consistent loop stops when the
convergence is reached
( )r
V(x) = -qΦ(x)
314 Non-Equilibrium Greenrsquos Function
Greenrsquos functions are a mathematical construction that are used to solve differential
equations subject to specific initial or boundary conditions They are named after the
British mathematician George Green The 1-D equation of L( )f( )=S( ) can be defined
by the Greenrsquos Function as given below
( ) ( ) ( )G x x f x x x (38)
The general Greenrsquos function is given by
( ) ( ) ( )f x dx G x x S x (39)
Applying the operator L( ) to the solution f( ) satisfies the original differential
equation The Greenrsquos Function G( ) is the propagator which propagates the influence
of a perturbation S( ) originally situated at the point to the point at which the
function f( ) is evaluated
The Greenrsquos Function G( ) can also be a correlation function If the points
and are strongly (weakly) correlated then S( ) will greatly (poorly) affect f( )
Poisson equation
2 ( )( )
( )
rr
r
Schroumldinger equation
2
2
( ( ) ) ( )
( )2
( ) | ( ) |
E H r E r S
H V rm
r dE E r
Figure 32 Self-consistent loop
45
The Schroumldinger equation with open boundaries can be written as
( )E H S (310)
Considering a 1-D and homogenous system ranging from =0 to L assuming
that Σ=0 and the form of equations is same before and after discretization then
22
2 0( ) ( ) ( )
2E x S x
m
dV
dx
(311)
The Greenrsquos function can hence be computed corresponding to the Schroumldinger
equation
22
2 0( ) ( ) ( )
2E G x x x x
m
dV
dx
(312)
Due to the delta-function at = a discontinuity is observed and hence the
Greens function is evaluated at boundary conditions
0
2
exp( ( )) x x 2 ( )( )
exp( ik(x x)) x x
ik x x m E VG x x k
A
A
(313)
By integrating the Schroumldinger equation twice and setting the lower and upper
integration boundaries to = -δ and = +δ the Greenrsquos Functions can be written as
2
( ) ( ) 0
( ) ( ) 2
x x x x
G x x G x x
dG x x dG x x m
dx dx
(314)
46
The coefficient A+ and A
- become
ik
mA A
(315)
The Greenrsquos Function takes a final form known as Retarded Greenrsquos Function and
is written as
( ) exp( | |)G x x i ik x xk
m (316)
And the wave function is
( ) ( ) ( )x dx G x x S x (317)
Retarded Greenrsquos Function propagates the wave functions generated by a source
or perturbation S from its origin at to any point
The retarded Greenrsquos Function as discretized Schroumldinger equation is written as
( )R RE H G I (318)
The wave function Φ can be calculated from the retarded Greenrsquos function and the
source vector as
Φ = GR∙S (319)
Overall in this section the Greenrsquos function approach in calculating the electron
dynamics is reviewed We defined the self-energy of each part of the system spectral
function and the probability current density the electric current is derived explicitly using
Non Equilibrium Greenrsquos function We will use this formalism to calculate the tunneling
phenomena in coupled quantum dots isolated or otherwise
47
CHAPTER 4
ATOMISTIX TOOLKIT DETAILS
41 Introduction
Virtual NanoLab (VNL) is a graphical user interface (GUI) that provides a group of
modeling tools the function of these tools involves the set-up investigation and the
study of nanoscale structures The quantum mechanical equations are solved by the
software by using the advanced software architecture and numerical methods to
implement ab initio calculations VNL simulates the electronic structure and calculates
the transport properties based on the two systems mentioned earlier NEGF and Extended
Huckel ATK is the main engine for computing the scripts and hence all the calculations
performed in VNL are done by ATK VNL is a user friendly software as it not only
allows creating a script but also helps to set up a virtual experiment
This thesis involves the use of VNL in order to study the effect of the width and
different orientations of the doped atoms Since the software allows for virtual
experiments it makes it much easier to study the I-V characteristics based on the change
in position of atoms
42 Device Structure
In this thesis AZA GNR p-n junction with boron doping (location) was created using the
ATK software which is based on NEGF and DFT Further the thesis discusses the
transport properties and the I-V curve of such junction
The input format of ATK is NanoLanguage which is an extension to Python
scripting language ATK uses the NEGF system for formalism of simulating device
48
Figure 41 Geometry of device configuration with two electrodes
37
The system is divided into three parts left central and right The implementation
relies on the screening approximation which assumes that the properties of the left and
right regions can be decribed by solving a bulk problem for fully periodic electrode cell37
This screening approximation is fulfilled when the electrode regions can be described by
an equilibrium electron distribution
Figure 42 The electron distribution in a device configuration which illustrates a left
moving scattering state with origin in right electrode37
The system assumes that in steady state the electron density of the central region
is constant in time and hence the electron density is calculated independently from each
electrode The electron density is given by the occupied eigenstates of the system
n(r) = nL(r) + n
R(r) (41)
49
The left and right densities are calculated by summing up the occupied scattering
states
nL(r) = sum
(42)
nR(r) = sum
(43)
The scattering states are usually calculated by first calculating the Bloch states in
the electrodes and then solving the Schroumldinger equation of the central region using the
Bloch state as matching boundary Instead of using the scattering states the ATK
software uses the NEGF method to calculate the non-equilibrium electron density
The electron density is given in terms of electron density matrix
D = DL + D
R (44)
The left density matrix is given by NEGF theory
DL = int
(45)
where
ρL(ɛ) =
(46)
ρL(ɛ) = is the special density matrix
Also if there is a non-equilibrium electron distribution in the central region then
the electron distribution in electrode is given by the Fermi function f with an electron
temperature TL
G(ɛ) =
(47)
G = retarded Green function
δ+ is an infinitesimal positive number and S H overlap the Hamiltonian matrices
L =
sum sum
(48)
50
L
is the broadening function of the left electrode given in terms of left electrode
self -energysum
43 Transmission Spectrum Calculations
Once the self-consistent non-equilibrium density matrix has been obtained the various
transport properties of the system can be calculated One of the most important properties
is the transmission spectrum from which the current and differential conductance can be
obtained
The transmission coefficient in ATK is obtained by the retarded Greens function
T(ɛ) = G(ɛ)ΓL(ɛ)G
ϯ(ɛ)Γ
R(ɛ) (49)
The transmission amplitude of individual scattering states may be obtained
through the Transmission Eigenvalues The ldquoTransmission Eigenvaluesrdquo is an analysis
which finds the eigenvalues of the transmission matrix
The transmission matrix at energy E and k-point is given by
Tnm(Ek) = sum (410)
where
= transmission amplitude from Bloch state ψn(k)
The transmission coefficient is given by the trace of transmission matrix
T(Ek) = sum (411)
Keeping in mind all quantities depend on the quantum numbers parametrically
Transmission eigenvalues sum up to the transmission coefficient
T = sum (412)
51
44 Calculating the Current
Current is calculated from the transmission coefficient using
I( ) ( )R L
L RL R
R LB B
eE f f dE
h
E EV V T T T
k kT T
(413)
where f is the Fermi function TRL is the electron temperature of the right or left
electrode and Tσ(E) is the transmission coefficient for the spin component σ
The chemical potentials of the left and right electrode given by
L
F R LR L
eVE
are defined relative to the Fermi level of the left electrode These chemical potential are
related to the applied bias and hencebiasR L
eV therefore bias L RV V V
The transmission spectrum itself is usually rather insensitive to temperature and is
used in self-consistent calculations but often depends strongly on the electrode voltages
Thus for an accurate estimate of the current the transmission spectrum should be
calculated self-consistently for each desired bias
ATK uses very precise method to calculate the transport properties of the system
Transmission spectra for various concentrations of boron doped graphene p-n junctions
are generated in this Chapter and various coefficients such as Seebeck Peltier and
Conductance are calculated
52
45 Calculating Transport coefficients
The linear response transport coefficient of an applied voltage difference or temperature
difference between the two electrodes is given by
Conductance
| dT 0
e
dI
dUG
(414)
Peltier coefficient
| d 0
Q
I
I
(415)
Seebeck coefficient
| 0
dUS I
dT T
(416)
These linear response coefficients are calculated by the Transport Coefficients To
perform these calculations the ATK uses the Electron Transmission Spectrum
53
CHAPTER 5
RESULTS AND DISCUSSION
51 Band Structure Analysis
The electronic bandstructure of GNR both doped and undoped are discussed in this
chapter
The armchair configuration of Pristine GNR (PGNR) has a band structure that is
dependent on its width This is explained by the fact that the sheet itself acts like a
potential well where the electrons are confined to form standing waves along Cr the
rolling vector albeit with slightly different boundary conditions (Cr = ma1 + na2
where m and n are integers and a1 and a2 are the unit cell vectors of graphene lattice) In
a GNR the two nodal points of the standing wave must be at the ribbon edge while in a
Single wall nanotube (SWNT) they can be anywhere ie a circumferential periodic
boundary condition
(a) (b)
Figure 51 Bandstructure of AGNR widths (a) 4 atoms (b) 5 atoms
54
(a) (b)
Figure 52 Bandstructure of AGNR widths (a) 6 atoms (b) 7 atoms
(a) (b)
Figure 53 Bandstructure of AGNR widths (a) 8 atoms (b) 9 atoms
55
(a) (b)
Figure 54 Bandstructure of AGNR widths (a) 10 atoms (b) 11 atoms
Figure 55 Bandstructure of AGNR with a width of 12 atoms
Figure 56 Variation in band gaps as the width (number of atoms) varies
0
05
1
15
2
25
0 2 4 6 8 10 12 14
Wdith vs Band Structure
eV
56
The band structure of 12 Atom AGNR is close to that of Ge (0626 eV) The
actual width of this nanoribbon is about 25 nm 12 AGNR has been fabricated
successfully and doped with various dopants Hence the 12 Atom AGNR has been chosen
to study the transport properties
A junction is created using ZGNR and AGNR To maintain the consistency in the
device analysis it is imperative that the band structure of ZGNR is also calculated From
the simulation it is evident that ZGNR-AGNR-ZGNR junction configuration displays the
Metal ndashSemiconductor-Metal configuration that is addressed in this work The Fermi
Level in all the Z-GNR nanoribbons of widths 4-12 lies within the conduction band
Figure 57 Band structure of ZGNR width (a) 4 atoms (b) 6 atoms
57
(a) (b)
Figure 58 Band structure of ZGNR width (a) 8 atoms and (b) 10 atoms
Figure 59 Band structure of ZGNR with a width of 12 atoms
In order to create viable junction that would show transistor properties doping of
the semiconductor part is necessary The 12 atom AGNR is doped with boron (p-type)
and nitrogen (n-type) - (Figure 510a) 4 N doped (Figure 510b) 4 B In both cases
the impurities lie on the edge of the atoms For 2 nitrogen doped GNR with the
58
impurities lying in the center of the ribbon the Fermi level is found to be in the
conduction band as shown in (Figure 510c) (Figure 510d) shows the position of N with
respect to the edge A very clear departure from the expected (the valence band extending
above Fermi level) is shown in (Figure 510a)
Figure 510 Band structures of Doped AGNR (a) 4 N Doped (b) 4 B Doped (c) 2
N Doped (d) position of Nitrogen from (c)
(a) (b)
(c) (d)
59
52 I-V Characteristics of GNR junction
In pristine graphene the chirality determines the conductivity as seen from the I-V curves
for various widths At certain widths the semiconducting properties are more
pronounced These widths determine the wavelengths of the standing waves which in
turn determine the sub-band locations in the E-k plot When the biasing potential
exceeds 012V the I-V curve shows linearity In case of the 8-atom wide PGNR the
band gap is about 03 eV and it is evident from the I-V plot that the On-State is + 033 V
The band gap of 10-atom and the 4-atom wide PGNR is large enough to show
semiconducting properties
Figure 511 Current Vs Voltage graph for varying graphene width showing
conductivity
-30000
-20000
-10000
0
10000
20000
30000
-3 -2 -1 0 1 2 3
Cu
rre
nt
(nA
)
Voltage (V) (bias)
Current (nA) Vs Voltage for varying graphene width
W=10
W=8
W=6
W=4
60
The ZAZ GNR Configurations show the properties of a semiconductor junction The 12
atom ZAZ structure is studied for its I-V characteristics In this Chapter undoped B-
doped N-Doped B and N Doped (P-N Junction) ZAZ junctions are simulated
Figure 512 ZAZ GNR junction device
61
The boron doped ZAZ junction I-V characteristics are shown below (Figure 513)
The impurity concentration is 2 and 4 Various device configurations are studied
Figure 513 I-V curve of Boron Doped ZAZ junction
-25000
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
25000
-205 -155 -105 -055 -005 045 095 145 195
Cu
rre
nt
(nA
)
VBias
2B_1G_R 2B_0G_R
4B_0G_L 4B_0G_C
4B_0G_R 4B_1G_L
4B_1G_C 4B_1G_R
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
-2 -1 0 1 2
Cu
ren
t(n
A)
VBias
4 B doped GNR Jn
62
Figure 514 I-V curve of Nitrogen Doped ZAZ
-25000
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
-2 -15 -1 -05 0 05 1 15 2
Cu
rre
nt(
nA
)
VBias
I-V Curve as function of Dopant location
2N_0G_L2N_0G_C2N_0G_R2N_1G2N_1G_C2N_1G_R
-15000
-10000
-5000
0
5000
10000
15000
-2 -1 0 1 2
Cu
rre
nt(
nA
)
VBias
2N_0G_C
2N_1G_C
63
Figure 513 and Figure 514 show the I-V characteristics of the GNR junction doped with
2 boron and nitrogen respectively The location of N and B is at the central region of
the edge of the GNR Both B doped and N doped GNR Junctions show significant
Negative Differential Resistance (NDR) This is more pronounced in case of nitrogen
doping Another interesting observation is increasing ohmic nature with the change in
location of the dopants Nitrogen doped device configuration exhibits a pronounced
semiconductor behavior and the NDR effect is observed to be minimal
53 Thermoelectric Properties
In this study the thermoelectric properties were simulated for the GNR Junctions that
displayed high NDR effect The variation in the Peltier coefficient with temperature is
shown as function of doping
When the concentration of nitrogen increases the dimensionless Figure of Merit
ZT seems to decrease considerably This is mostly explained by the decrease in both
conductivity and mobility of the electrons
ZT = S2σTk (51)
where S is the Seebeck coefficient σ is the electrical conductivity T is the
absolute temperature and k is the thermal conductivity
64
Figure 515 Variation of Peltier coefficient with temperature as function of
doping
Figure 515 shows the maximum Peltier coefficient for 2 boron This is
explained by the scattering by boron and the associated smallest mean free path
0
0001
0002
0003
0004
0005
0006
0007
0008
0009
001
250 270 290 310 330 350 370 390 410
ZT
T (K)
2B
4B
Undoped
2N
4N
65
CHAPTER 6
CONCLUSIONS
Graphene ZAZ junctions exhibit varying properties depending on the various structural
configurations In this thesis it was found that the transport properties of graphene
depend on their width the edge of GNR doping concentration and the type of dopant
used The calculations of the band structure contributed towards the determination of the
minimum length of GNR required for studying the transport properties The minimum
length had a band gap equivalent to that of germanium and hence the importance of the
width being 12 atoms wide This band gap indicated fluctuating changes when doped
with elements such as B and N The viable junction showing transistor properties was
hence created by doping the semiconductor part of ZAZ By doping the I-V
characteristics were studied which showed significant NDR which was more pronounced
in the case of nitrogen Also the changing positions of the dopants contributed towards
the I-V curve to be more ohmic The edge doping caused minimum NDR and
semiconductor behavior as compared to central doping Lastly the thermoelectric
properties were studied - the increasing concentration of N causes the Figure of Merit to
decline due to the decrease in conductivity as well as mobility of electrons
66
REFERENCES
1 Wikianswers What makes carbon unique
httpwikianswerscomQWhat_makes_carbon_so_unique (22 November)
2 Kopeliovich D D Graphite
httpwwwsubstechcomdokuwikidokuphpid=graphite (1128)
3 Barbier M Transport properties of nanostructures and superlattices on single layer and
bilayer graphene University Antwerpen Antwerpen 2012
4 Shylau A Electron transport interaction and spin in graphene and graphene
nanoribbons Linkoping Norrkoping 2012
5 HassJ R F T Li X Li Z Zong W A de Heer P N First E H Conrad C
AJeffrey and C Berger Applied Physics Letters 2006 89 (14) 143
6 Jones A Mechanical Exfoliation to Make Graphene and Visulization
httpcarbonchemwisceduFilesMechanicalExfoliationpdf (18 October)
7 Anteroinen J Structural and Electrical Characteristics of Graphene Field Effect
Transistors AALRO school of Electrical Engineering AALTO 2011
8 Novoselov K S A K G S V MorozovD JiangY Zhang S V Dubonos I V
Grigorieva A A Firsov Science 2004 306 (22)
9 Kosynkin D A L H A Sinitskii J R Lomeda A Dimiev K B Price and J M
Tour Nature 458 876
10 Yi Z Luyao Zhang Accounts of chemical research 46 (10) 2339
11 Eizenberg M B JM 1979 82 236
12 Yu Q K L J Siriponglert S Li H Chen Y P Pei S S Applied Physcis
Letters 2008 93 (113103)
13 Li X C W An J Kim S Nah J Yang D Piner R Velamakanni A Jung I
TutucE Banerjee S K Colombo L Ruoff R S Science 2009 324 1314
14 Schaefer H E Nanoscience Springer Berlin 2010
15 Levente Tapasztoacute G D Philippe Lambin amp Laacuteszloacute P Biroacute Nature Nanotechnology
2008 3 401
67
REFERENCES
16 Dacheng Wei Y L Advance Materials 2010 22 (30) 3241
17 Wei Yao K L Y GYGao Elsevier Solid State Communications 2013 153 52
18 Dacheng Wei Dagger Yunqi Liudagger Yu Wangdagger Hongliang ZhangdaggerDagger Liping HuangdaggerDagger
Yudagger a G NanoLetters 2009 9 (5) 1758
19 Nakada K M F G Dresselhaus and M S Dresselhaus PhysRevB 1996 54
(9858)
20 Son Y W C M L a L S G PhysRevLett 2006 97 (216803)
21 Raza H Graphene Nanoelectronics Springer 2012
22 Ryan W J Electronic Transport in Graphene p-n junctions Short Noise and
Nanoribbons Harvard University 2009
23 Fangping OuYang J X Rui Guo Hua Zhang and Hui Xu Nanotechnology 2009
20 6
24 Guo J Carbon nanotube electronicsModeling physics and applications Purdue
University West Lafayette IN 2005
25 Motta C S S-P MITrioni cond-matmes-hall 2012 7
26 B P Growing Graphene via Chemical Vapor Deposition Ponoma College Ponoma
2011
27 ZurichE Transport properties of three-terminal graphene devices University of
Science and Technology Norway 2008
28 Uichiro MIntroduction to the electron theory of metals
29 Robert Laughlin H S Additional background material on the Nobel Prize in Physics
1998 (410)
30 MarkGoerbig Quantum Hall Effects (11152013)
68
REFERENCES
31 Zurich E Transport properties of three-terminal graphene devices Norwegian
University of Science and Technology Norway 2008
32 Deepak R Klein Tunneling University og Tennessee Space Institute Tennessee
2011
33 Williams JR L D CMMarcus Quantum Hall Effect in a Gate-Controlled p-n
Junction in Graphene (1122013)
34 Avadhanulu MN P G K A Textbook of Engineering Physcis for BE BSc (Engg)
SChand New Delhi 1992
35 Andriotis A Applied Physics Letters 2007 91 (152105)
36 Qimin Yan B H dagger Jie Yudagger Fawei Zhengdagger Ji ZangDagger Jian Wudagger Bing-Lin Gu F
L Dagger and Wenhui Duandagger NanoLetters 2007 7 (6) 1473
37 Soler J M E A J D Gale A Garciacutea J Junquera P Ordejoacuten and D Saacutenchez-
Portal J Phys Condens Matter 2002 14 2745
ANALYSIS OF TRANSPORT PROPERTIES IN A ZAZ GRAPHENE
NANORIBBON JUNCTION USING VARIOUS DOPANTS
by
Natasha Parikh
A Thesis
Submitted to the Faculty of
New Jersey Institute of Technology
in Partial Fulfillment of the Requirements for the Degree of
Master of Science in Materials Science and Engineering
Interdisciplinary Program in Materials Science and Engineering
January 2014
APPROVAL PAGE
ANALYSIS OF TRANSPORT PROPERTIES IN A ZAZ GRAPHENE NANORIBBON JUNCTION USING VARIOUS DOPANTS
Natasha Parikh
Dr N M Ravindra Thesis Advisor Date Director of Material Science and Engineering Program NJIT Dr Keun H Ahn Committee Member Date Associate Professor of Physics NJIT Dr Tao Zhou Committee Member Date Associate Professor of Physics NJIT Dr Halina Opyrchal Committee Member Date Senior University Lecturer of Physics NJIT
BIOGRAPHICAL SKETCH
Author Natasha Parikh
Degree Master of Science
Date January 2014
Undergraduate and Graduate Education
bull Master of Science in Materials Science and EngineeringNew Jersey Institute of Technology Newark NJ 2014
bull Bachelor of Arts in Physics and Biological SciencesRutgers the State University of New Jersey New Brunswick NJ 2012
Major Materials Science and Engineering
iv
v
ACKNOWLEDGMENTS
I would like to express my gratitude to my supervisor Dr NM Ravindra for the useful
comments remarks and engagement throughout the learning process of this Mastersrsquo
thesis Furthermore I would like to thank Vijay Kasi Somayajula for introducing me to
the topic as well for the support I thank Dr Tao Zhou Dr Ken Ahn and Dr Halina
Opyrchal for serving on my thesis Committee I would like to thank my loved ones who
have supported me throughout the entire process both by keeping me harmonious and
helping me in putting pieces together
vi
TABLE OF CONTENTS
Chapter
Page
1 INTRODUCTIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
1
11 Graphene The New Carbonhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
1
12 Graphene Synthesishelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
3
121 Synthesis of Graphene on Nickel (Ni)helliphelliphelliphelliphelliphelliphelliphellip
5
122 Synthesis of Graphene on Copper (Cu)helliphelliphelliphelliphelliphelliphelliphellip
8
123 Transfer of Graphene Filmshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
8
124 Synthesis of Graphene Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
9
125 Doping in Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
10
126 Nitrogen (N) Doped Graphene Synthesis (Substitutional)hellip
12
13 Structure of Graphene Nanoribbon (GNR)helliphelliphelliphelliphelliphelliphelliphelliphelliphellip
13
14 Overview of Graphene Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
15
2 RESEARCH BACKGROUNDhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
21 Bandstructure of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
22 Transport Characteristics of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
20
23 Drude Theoryhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
22
24 Quantum Hall Effect (QHE)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
24
25 Resistivity and Resistancehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
27
26 Klein Tunnelinghelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
28
27 Quantum Hall Effect in Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
31
28 Thermoelectric Effecthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 34
vii
TABLE OF CONTENTS
(Continued)
Chapter Page
281 Seebeck Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
34
282 Peltier Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
36
29 Early Research ndash ab initio Studyhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
37
3 COMPUTATIONAL DETAILShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
31 Introductionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
311 Extended Huckel Theory helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
312 Introduction to NEGFhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
41
313 Electrostaticshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
42
314 Non-Equilibrium Greenrsquos Functionhelliphelliphelliphelliphelliphelliphelliphelliphellip
44
4 ATOMISTIX TOOLKIT DETAILShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
41 Introductionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
42 Device Structurehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
43 Transmission Spectrum Calculationhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
50
44 Calculating the Currenthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
51
45 Calculating the Transport Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
52
5 RESULTS AND DISCUSSIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
53
51 Band Structure Analysis helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
53
52 I-V Characteristics of GNR Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
59
53 Thermoelectric Propertieshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
63
6 CONCLUSIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 65
REFERENCEShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
66
viii
LIST OF FIGURES
Figure Page
11 (a) Chemical representation of Carbon (b) Graphite ore (c) Structure of
Graphite and a single layer Graphenhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
2
12 An optical image of Graphene flake obtained by exfoliation of
graphitehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
3
13 (a) Graphene formation on Nickel (b) Graphene atoms on Ni (111)
lattice (c)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
7
14 (a) SEM image of graphene on copper foil (b) High-resolution SEM
image of graphene on Cuhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
8
15 (a) Transfer process (b) Wafer-scale synthesis of graphene (c) Graphene
films transferred onto glass wafer (d) SiSiO2 with device patterned (e)
PET filmhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
9
16 (a) High-magnification image of the annealed sample showing that well-
defined zigzag armchair and zigzag-zigzag edges are formed (b) ) STM
image of an 8 nm wide bent junction connecting an armchair and a
zigzag graphene nanoribbon which was carved by STM
tipshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
10
17 Band structure of graphene before and after doping The image shows
shift towards the Fermi levelhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
11
18 Low resolution TEM image of N-doped graphene Background is the
lacey carbon TEM grid graphene sheet is crumpled with many
rippleshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
13
19 Zigzag and Armchair orientation of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphellip 13
110 Bandstructure of ZGNRhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 14
111 Bandstructure of AGNRhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 15
21 Left Real space Graphene lattice with basis vectors and Right
The first Brillouin zone of Graphene in reciprocal space with basis
vectors and K and Krsquo are responsible for massless transport at low
energyhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
ix
LIST OF FIGURES
(Continued)
Figure Page
22 Bandstructure of a graphene sheet showing a band gap of 0eVhelliphelliphellip 18
23 Band structure of Graphene calculated with the tight-binding modelhellip 19
24 The energy dispersion around the K pointhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 22
25 Electrons colliding with stationary ionshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 23
26 (a) 2D electrons in a perpendicular magnetic field Logitudinal resistance
measured across C5 and C6 Transverse resistance measured across C3
and C5 (b) Classical Hall resistance as a function on the magnetic field
25
27 Klein tunneling through an npn barrierhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 29
28 Electron trajectory considering the linear electrostatic potential U(x) = Fx 30
29 Electron like and hole like trajectories at same Ehelliphelliphelliphelliphelliphelliphelliphelliphellip 30
210 Quantum Hall effect in graphene 22
The Hall conductivity σxy and the
longitudinal resistivity of monolayer graphene as a function of carrier
density at B = 14T and T= 4K This shows half-integer QHE with chiral
index J= 1helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
32
211 (a) LL for Graphene bilayer (b) Schematics of Hall conductivity as a
function of nn0 for bilayer Graphene (solid line) and monolayer
Graphene (dotted line) (c) LL for monolayer Graphenehelliphelliphelliphelliphelliphelliphellip
33
212 Seebeck Effecthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 35
213 Transmission functions in units of (2e2h) for AZA structureshelliphelliphelliphellip 37
214 I-V curve for a 591nm long channel (Vbias=20mV)helliphelliphelliphelliphelliphelliphelliphellip 38
31 NEGF systemhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 42
41 Geometry of device configuration with two electrodeshelliphelliphelliphelliphelliphelliphellip 48
42 The electron distribution in a device configuration which illustrates a left
moving scattering state with origin in right electrodehelliphelliphelliphelliphelliphelliphelliphellip
48
x
LIST OF FIGURES
(Continued)
Figure Page
51 Band structure of AGNR widths (a) 4 atoms (b) 5 atomshelliphelliphelliphelliphelliphellip
53
52 Band structures of AGNR widths (a) 6 atoms (b) 7 atomshelliphelliphelliphelliphelliphellip 54
53 Band structure of AGNR widths (a) 8 atoms (b) 9 atomshelliphelliphelliphelliphelliphelliphellip 54
54 Band structures of AGNR widths (a) 10 atoms (b) 11 atomshelliphelliphelliphelliphellip 55
55 Band structure of AGNR with a width of 12 atomshelliphelliphelliphelliphelliphelliphelliphelliphellip 55
56 Variation in band gaps as the width (number of atoms) varieshelliphelliphelliphellip 55
57 Band structure of ZGNR width (a) 4 atoms (b) 6 atomshelliphelliphelliphelliphelliphelliphellip 56
58 Band structure of ZGNR width (a) 8atoms and (b) 10 atoms 57
59 Band structure of ZGNR with a width 12 atomshelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 57
510 Band structures of Doped AGNR (a) 4 N Doped (b) 4 B Doped (c)
2 N Doped (d) position of Nitrogen from (c)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
58
511 Current Vs Voltage graph for varying graphene width showing
conductivityhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
59
512 ZAZ GNR junction devicehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 60
513 I-V curve of Boron Doped ZAZ junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 61
514 I-V curve of Nitrogen Doped ZAZhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 62
515 Variation of Peltier effect coefficient with temperature for various doping 64
1
CHAPTER 1
INTRODUCTION
11 Graphene The New Carbon
Carbon (chemical symbol C atomic mass 1207amu) (Figure 11a) is a widely distributed
element in nature It is found abundantly in the sun stars comets and the atmospheres of
the planet Carbon can form up to four bonds it can bond with itself endlessly and with
most other elements in many different shapes making it a significant part of the
construction for many kinds of complex molecules1
Two allotropes of carbon are commonly used diamond and graphite (Figure
11b) The bonding structures of diamond and graphite contribute to the properties
individually In diamond all the p-orbitals are used forming a sp3
bonding whereas in
graphite only two orbitals are occupied allowing the unpaired bond for the transport of
electrons Each carbon atom in graphene possesses sp2 hybridization ie each carbon
atom is connected to three other carbon atoms via covalent bonds with a bond length of
142Å and an angle of 120deg between each bonded pair This makes graphite a better
conductor than diamond Graphite consists of many layers of 2D carbon lattices (Figure
11c) stacked on top of each other and held via Van der Waals forces A single layer of
graphite where carbon atoms are arranged in a honeycomb lattice is known as graphene
(Figure 11c)
2
Figure 11 (a) Chemical representation of Carbon (b) Graphite ore (c) Structure of
Graphite and a single layer Graphene2
Theoretical work on graphene was done specifically to study the other allotropes
The first study was done by Wallace in 1947 who calculated the band structure of
graphene3 Further the peculiar Landau levels were known by McClure in 1957 and the
relativistic Hofstadter butterfly by Ramal in 19853 Later in 1991 the invention of carbon
nanotubes by Iijima boosted the theoretical research on graphene3 Prior to the invention
of carbon nanotubes there were a few experimental papers on graphene growth via
various methods like intercalation of graphite (Shioyama 2001) free standing (Boehm
1962) epitaxial as well as graphene grown on metals (Bommel 1975 Land 1992 Itoh
1991)3 With all the various discoveries the electronic properties of graphene were not
studied until 2004 when Berger and Novoselov were able to access the electronic
properties with contact of graphene flakes3 (Figure 12)
3
Figure 12 An optical image of Graphene flake obtained by exfoliation of graphite3
The specific lattice structure of graphene possesses a number of unique electronic
properties making it an interesting material for theorists experimentalists and engineers
Utilization of graphene as a fundamental block of electronic devices requires
development of new theoretical methods for understanding the current propagations in
graphene constriction4
12 Graphene Synthesis
The discovery of graphene by mechanical exfoliation called the lsquoScotch tape methodrsquo led
to serious attempts towards the production of top quality graphene5 Graphene was first
exfoliated mechanically from graphite in 20046 The importance of high quality graphene
cannot be emphasized enough however electron transport has shown that defects play an
important role in hindering the transport properties of electrons (holes)7 The two
synthesizing methods for the large scale manufacture of graphene are chemical vapor
deposition (CVD) and silicon carbide (SiC) desorption method
4
Graphene can be synthesized by sublimation of silicon from SiC at high
temperature (1200degC) in high vacuum5 The major advantage of this method is that the
SiC provides an insulating substrate and no transfer of the graphene layer is needed Yet
the disadvantage of this method outweighs its advantages the high temperature is cost-
ineffective making it unsuitable for large scale manufacturing8 Also the crystal growth
face alters the properties of graphene Graphene grown on Si-terminated face has poor
homogeneity and is subjected to unintentional doping7 Conversely graphene grown on
C-terminated SiC has higher mobility and is often called lsquoturbostaticrsquo due to the
rotational disorder7
Unlike the SiC method the graphene produced via CVD method needs to be
transferred to a substrate making it difficult to maintain the quality of graphene Yet
CVD synthesized graphene has a larger grain size7 More research is being done on
various methods for synthesis of graphene The methods include direct chemical
synthesis ion implantation crystal sonification and lastly unzipping carbon nanotubes to
form graphene sheets9
Graphene and few-layer graphene have been grown by CVD from carbon
containing gases on catalytic metal surfaces andby surface segregation of C dissolved in
the bulk of such metals7 Growing graphene with CVD is a very attractive solution since
it is compatible with the existing semiconductor industry9 Graphene has been grown via
CVD process on metal substrates such as Nickel (Ni) and Copper (Cu)
5
121 Synthesis of Graphene on Nickel (Ni)
Polycrystalline Ni films are annealed in ArH2 atmosphere at 900-1000degC to increase
grain size and are then exposed to H2CH4 gas mixture10
In this step the hydrocarbon
decomposes and dissolves in Ni to form a solid solution Lastly the samples are cooled in
argon gas Ni has high carbon solubility at elevated temperatures and the solubility
decreases as temperature is reduced During the cooling process the carbon atoms diffuse
out from the Ni-C solid solution and precipitate on the Ni surface to form graphene films
(Figure 13a) Since Ni (111) has a lattice similar to the densely packed hexagonal lattice
of graphene (Figure 13b) they also have similar lattice constants and hence Ni surface
serves as an excellent lattice matched substrate for graphene growth11
The growth of graphene on Ni is based on carbon segregation and precipitation
process different segregation behavior is produced by different cooling rates which
affect the thickness and quality of graphene films12
Medium cooling rates lead to optimal
carbon segregation and produce few layers12
Graphene films grown on Ni are usually
continuous with monolayer and few layer regions Annealing of Ni substrates at elevated
temperatures in hydrogen atmosphere not only increases the single-crystalline Ni grain
size but also eliminates certain impurities in Ni thereby improving the graphene quality
Furthermore the graphene thickness can also be affected due to the amount of carbon
dissolved in the Ni films during the growth time
After synthesis the graphene can be transferred to other insulator substrates for
further characterization and applications Figure 13c shows the selected area electron
diffraction pattern of graphene film along the [001] direction which confirms the
graphene lattice structure shown After transfer to insulator substrates the geometry can
6
be retained as shown in Figure 13d Under optimal growth parameters graphene growth
is only limited by the Ni catalyst Lastly Figures 13e and 13f show the wafer-scale
graphene synthesis and transfer of graphene to a flexible transparent substrate
respectively
Though polycrystalline Ni is a good substrate the percentage and size of
graphene monolayer are still limited Researchers have hence tried other metal substrates
for graphene synthesis
7
Figure 13 (a) Graphene formation on Nickel (b) Graphene atoms on Ni (111) lattice
(c) Low magnification TEM image of graphene edges (d) Optical image of graphene
transferred from the Ni surface to SiO2Si substrate (e) Full-wafer scale deposition of
graphene layers on polycrystalline Ni (f) Transparent and flexible graphene films on
PDMS substrate10
8
122 Synthesis of Graphene on Copper (Cu)
Graphene films are grown on 25microm thick Cu foils in a hot wall furnace13
The Cu foil is
first annealed in hydrogen atmosphere at 1000degC and a mixture of H2CH4 is introduced
into the system to initiate graphene growth After a continuous graphene layer is formed
on the Cu foil the system is cooled to room temperature Figure 14a shows an SEM
image of graphene on Cu substrate indicating the Cu grains with contrast The Cu
surface steps are formed during thermal annealing and the darker flakes indicate multiple-
layer graphene (Figure 14b)10
The graphene wrinkles in Figure 14(b) originate from
different thermal expansion coefficient of graphene and Cu They go across the Cu grain
boundaries indicating that the graphene film is continuous
Figure 14 (a) SEM image of graphene on copper foil (b) High-resolution SEM image of
graphene on Cu10
123 Transfer of Graphene films
In order to facilitate the applications of graphene for electronic applications we need to
separate the graphene from the catalytic metal substrate Figure 15a shows the transfer
process of graphene Graphene is first coated with a thin layer of polymethyl
methacrylate (PMMA) and baked at 120degC to evaporate the solvent10
The metal layer is
then removed by Ni or Cu etchant leaving behind the PMMA graphene film The film is
then cleaned by deionized water and then transferred onto the target substrate After the
9
evaporation of water vapor the PMMA is removed by acetone leaving graphene film on
top of the target substrate Figure 15b shows a graphene wafer transferred from the
substrate onto glass and polyethylene terephthalate (PET) films
Figure 15 (a) Transfer process (b) Wafer-scale synthesis of graphene (c) Graphene
films transferred onto glass wafer (d) SiSiO2 with device patterned (e) PET film10
124 Synthesis of Graphene Junction
Graphene junctions with smooth armchair and zigzag edges are difficult to produce by
conventional methods such as mechanical exfoliation chemical exfoliation or lithography
etching14
The conventional methods can only produce rough edges Recently
Dresselhaus reported an edge reconstruction of graphene by Joule heating in a TEM-STM
10
(Figure16b) system15
An individual nanoribbon sample is attached to the sample holder
at one end and to the STM tip at the other end these ends also serve as the two
electrodes The structural transformation in the growth of graphene from armchair to zig-
zag is mainly attributed to the vaporization of carbon edges that reconstruct at high
temperatures in which resistive Joule heating and preferred current flow play an
important role This means that by controlling the flow of current a perfectly smooth
edged ribbon can be synthesized making graphene-based electronics possible16
Figure 16 (a) High-magnification image of the annealed sample showing that well-
defined zigzag armchair and zigzag-zigzag edges are formed (b) STM image of an 8 nm
wide bent junction connecting an armchair and a zigzag graphene nanoribbon which was
carved by STM tips14
125 Doping in Graphene
The doping of graphene can be roughly classified into two categories - electrical and
chemical Electrical doping involves changing gate voltages of graphene devices and
chemical doping uses chemical routes such as substitutional or interstitial This thesis
discusses chemical doping and the importance of doping sites by changing the dopant
Chemical doping is a common approach to tailor the electronic properties of
11
semiconductors Doping of graphene can cause its electronic properties to alter leading to
a metal-semiconductor transition The two means of doping graphene are interstitial and
substitutional In interstitial doping the dopant atoms or molecules are introduced as
adatoms or admolecules on the surface of graphene whereas in substitutional doping the
dopant atoms are replaced in the carbon lattice forming a bond in the lattice of
graphene16
Doping graphene results in the formation of n or p-type semiconductors
depending on the kind of dopant If the dopant is an electron donor it causes the Fermi
level to shift up resulting in n-type behavior of graphene Furthermore if the dopant is an
electron acceptor it causes the Fermi level to shift down resulting in a p-type behavior of
graphene (Figure 17)16
Figure 17 Band structure of graphene before and after doping The image shows shift
towards the Fermi level16
Graphene nanoribbons (GNR) can be made into a p- and n- type semiconductor
by doping with boron (B) and nitrogen (N) respectively In theory GNR p-n junction is
formed by doping GNR with B and N in different regions However experimentally
doping graphene with both these elements is very difficult due to the dopants reacting
with each other17
Hence most experimental studies use GNR doped by only one
12
element N-doped graphene was synthesized by Wei et al Wang and B-doped Graphene
was realized by Endo17
Many researchers have demonstrated interstitial doping of graphene by gas metal
and organic molecules16
The various gases and metals used are NO2 NH3 An-CH3 Na-
NH2 F4-TCNQ TPa TCNE and others16
Doping in graphene is hence possible by
electrons or holes in high concentration without deterioration of its mobility Interstitial
doping is highly sensitive due to most of the conducting channel being exposed to surface
absorbates and hence can be used in molecule detection
In substitutional doping the dopant atoms are included in the graphene lattice and
thus chemically bonded Substitutional doping is done via the CVD method using a
carbon and dopant source Substitutional doping opens up many applications in device
engineering making graphene a very good candidate as a semiconductor This study
involves the study of transport properties of graphene doped by substitution
126 Nitrogen (N) Doped Graphene Synthesis (Substitutional)
N-Doped graphene is prepared via a CVD process using a 25microm thick Cu film on a Si
substrate The substrate is placed in a quartz tube with the flow of hydrogen (20sccm) and
argon (100 sccm)18
When the center of the furnace reaches 800degC 60 sccm of CH4 and
60 sccm of NH3 is introduced into the flow as C source and N source respectively The
substrate is then moved to high temperature and after 10 min growth the sample is
cooled to room temperature under H2 ambient Figure 1 8 shows the growth of N-doped
graphene18
13
Figure 18 Low resolution TEM image of N-doped graphene Background is the lacey
carbon TEM grid graphene sheet is crumpled with many ripples18
13 Structure of Graphene Nanoribbon (GNR)
Graphene Nanoribbons (GNR) are strips of graphene with very thin width of lt50nm
GNRs can be terminated in three separate ways called zig-zag (0 n) armchair (m 0) and
chiral (m n) (Figure19) and this termination along the width of the ribbon dictates the
size of the band gap19
Figure 19 Zigzag and Armchair orientation of Graphene5
Due to their various edge structures GNRs exhibit different electronic properties
ranging from normal semiconductors to spin-polarized half metals which open the
possibility of GNRs as electronic devices19
14
Within a tight binding approach (AGNRs) could be metallic or semiconducting
depending on their ribbon width but all zigzag graphene nanoribbons (ZGNRs) are
metallic with a high density of electronic states at the edges Hence ZGNRs exhibit
characteristic edge effects which are not present in AGNRs These edge effects in
ZGNR create a flat band close to the Fermi level making the ZGNR edges more
reactive19
First-principles calculations show that the GNRs possess a non-zero direct
band gaps These gaps are small for ZGNR (Figure 110) caused due to spin ordering
effects at the edges For AGNRs the band gap arises from quantum confinement (Figure
111) effect that has larger magnitudes than ZGNR20
Figure 110 Band structure of ZGNR
15
Figure 111 Band structure of AGNR
For GNRs the band gap decreases as the ribbon width increases and in order to
create a semiconductor with a desirable band gap the nanoribbon width should be
adjusted accordingly This property of adjusting the band gap makes graphene an
excellent candidate for transistor switching By applying an electric field GNR can be
altered from an insulator to a conductor GNRs exhibit very intriguing properties and
have become one of the promising candidates for electronic applications
14 Overview of Graphene Junction
The invention of p-n junctions date back to 1940s which later resulted in the invention of
junction transistors One of the key technological reasons for success of the p-n junction
is mainly due to its ability to locally modulate the energy band gaps via an applied bias21
A graphene p-n junction is created via single layer of graphene in which the
carrier type and density in two adjacent regions are controlled by electrostatic gating8
For materials with a band gap the electric field can either switch lsquooffrsquo the current or
rectify it (p-n diode)22
Being a ldquogaplessrdquo material the off state is not achievable in
16
graphene In order to achieve an off state the gap can be created by doping graphene with
various elements (Group III or Group V) Doping allows p-n junctions to be
reconfigurable using a gate voltage to distinguish between graphene p- n regions within a
single sheet Many researchers have studied the electronic as well as transport properties
of doped graphene junctions
In 2009 Fangping OuYang studied the transport properties of T-shaped graphene
junctions using the ATK software and showed that the conductance depends on
geometric structures which can be controlled by selective doping23
Wei Yao in 2013
studied the transport properties in graphene p-n junctions and showed that the
rectification effect depends on boron doping density and position17
The study of transport properties in graphene p-n junctions is a recent
advancement The thesis discusses transport properties including the current-voltage (I-
V) characteristics of doped graphene junctions Moreover the software used is similar to
the software in use by current researchers since they have produced viable data using
ATK
17
CHAPTER 2
RESEARCH BACKGROUND
21 Band Structure of Graphene
The unique electronic properties of graphene were first predicted in 1946 Figure 21
shows a top view of the hexagonal arrangement of carbon atoms in real space as well as
the first Brillouin zone in reciprocal space
Figure 21 Left Real space graphene lattice with basis vectors and Right The
first Brillouin zone of graphene in reciprocal space with basis vectors and
K and
Krsquo are responsible for massless transport at low energy24
The real space basis vectors are radic
and
radic
The reciprocal space basis vectors are 1 2
0 0
4 1 3 4 1 3( )and ( )2 2 2 23 3
b x y b x ya a
where the magnitude of the basis vectors is |a0| = radic acc The distance between nearest
neighbor carbon atoms is acc=0142nm
18
The band structure can be calculated by solving the eigenvalues using the
dispersion relation E( )
1 2 3( ) 3 2cos 2cos 2cosE k t k a k a k a (21)
Transport properties of solids are closely related to the energy dispersion
relations E ( ) in the material and in particular to the behavior of E ( ) near the Fermi
level Graphene is a zero gap semimetal whose specific linear electronic band dispersion
near the Brillouin zone corners (Dirac points) gives rise to electrons and holes that
propagate as massless Fermions25
The valence and conduction bands do not overlap in
graphene they touch at the Fermi Level (Figure 22)
Figure 22 Band structure of a graphene sheet showing a band gap of 0eV
The low energy properties of graphene can be well described by making a linear
expansion of the band structure around the K and Krsquo This energy can be written as
19
E(k) = plusmnħvF|k (22)
where vF is the Fermi velocity of 1106ms given by
1F
Ev
k
ħ (23)
Figure 23 Band structure of graphene calculated with the tight-binding model
22
The Fermi surface of graphene consists of double cones with Fermi energy at the
intersection of these cones (Figure 23) The slope of the band is zero and hence the
effective mass of electrons in that region is zero which leads to an entirely new transport
mechanism in graphene26
20
22 Transport Characteristics of Graphene
Transport process usually involves a flow of charge or energy or both The flow is mainly
due to external perturbations such as electric field and temperature gradient The
relationship between forces and flow usually defines various transport coefficients that
are the characteristics of electrons and phonons in the material All modern electronics
are based on the ability to control the electronic properties of a material by applying
external voltage This is done by an electric field effect where the gate voltage changes
the carrier concentration of the material and consequently its conductivity The electric
field effect in graphene was reported by Novoselov in 2004 and is used in transport
measurements8
The electron-phonon interaction in graphene plays an important role in
understanding the photoemission spectra observed in graphene The electric field effect is
an alternative method for changing the charge carrier density in low dimensional systems
The electric field effect in graphene which was first reported by Novoselov et al in
2004 is widely used as a characterization tool in transport measurements25
The transport characteristics of the material are directly related to the
bandstructure of graphene The carriers in graphene lattice are free to move in two
dimensions In the carrier transport of graphene the carriers ndash electrons and holes ndash close
to the Dirac points are of importance The transport is described by a two component
wave function (Equation 24) which obeys the 2D Dirac-like equation for massless
particles27
21
-ivFσ nablaψ(r) = Eψ(r)
(24)
where σ is the 2D Pauli spin matrix In the continuum limit the above (Equation
24) corresponds to the effective low energy Dirac Hamiltonian (Equation 25)
0( )
0
x y
F F
x y
iH k k
i
k kv v
k k
(25)
The electronic band structure of the energy (E) versus wave vector (k) relation for
graphene is given by Equation 24
The two component wave function resembles the spin or wave function of
quantum electro dynamics (QED)27
Corresponding to the spin of particles in QED the
charge carriers of graphene can be attributed with a pseudospin σ The pseudospin is the
direct result of two different carbon sublattices corresponding to the bonding and
antibonding combinations27
22
Figure 24 The energy dispersion around the K point27
In Figure 24 the red and blue lines correspond to the antibonding and bonding
states respectively The pseudospin can have two values either in the direction of or
against the momentum It can be seen that the electrons with energy E travelling in the
positive direction originates from the same branch as a hole with energy ndashE travelling in
the negative direction giving it the same pseudospin This results in suppressed
backscattering and Klein tunneling The back scattering process requires the pseudospin
to flip which is possible in the presence of short range scatters that act differently on sub
lattices27
23 Drude Theory
The classical theory of metallic conductivity was presented by Drude in 1900 and was
elaborated by Lorentz in 190528
Drude treated the free electrons as classical ideal gas
meaning the electrons collide with stationary ions and not each other
23
Figure 25 Electrons colliding with stationary ions28
The Drude theory applied the kinetic theory of gases to a metal considered as a gas of
electrons The basic assumptions made by the Drude theory are28
When metallic elements are brought together to form a solid then the valence
electrons become freely moving through the metal whereas the ions remain intact
as nearly immobile positive particles
Between collisions the electrons move freely ie there is neither electron-
electron interaction nor electron-ion interaction
The scattering mechanism leads to instantaneous collisions of the electron with
the scatterers
The collisions are characterized by a relaxation time τ
The electrons achieve thermal equilibrium only through collisions the velocity
after a collision is randomly directed the speed is as appropriate to the
temperature
With the relaxation time Drude obtained the electrical conductivity expression
where n is the number of electrons per unit volume
σ = ne2τm
(25)
He also calculated the thermal conductivity and successfully provided the
theoretical basis for Wiedemann-Frantz law already established in 1853 which states that
24
the ratio of electrical and thermal conductivity of any metals is a universal constant at any
given temperature28
The Drude theory gives results which are qualitatively correct outside of the
quantum Hall regime28
In the Drude theory of the electrical conductivity of a metal an
electron is accelerated by the electric field for an average time τ before being scattered
by impurities lattice imperfections and phonons to a state which has zero average
velocity The average drift velocity of the electron is
d
eE mv (26)
It is assumed that all electrons drift together and hence the current density
j = -ne (27)
This Drude theory works well for fields below ~ 01T At stronger fields the Hall
resistivity becomes nearly constant over finite intervals of magnetic fields28
The QHE
reflects both novel disorder physics as well as novel interaction physics in the quantum
Hall regime
24 Quantum Hall Effect (QHE)
The discovery of QHE is a remarkable achievement in condensed matter physics The
Hall Effect was discovered by Edwin Hall in 187929
However the precise quantization
of the Hall conductance in units of e2h was not recognized until February 1980 Five
years later in 1985 Klaus von Klitzing was awarded the Nobel Prize in Physics for the
discovery of QHE29
The quantum Hall effect occurs in two-dimensional electron systems in the limit
of strong perpendicular magnetic field that stems from electronic transport
25
measurements where one drives a current I through the sample and where one measures
both the longitudinal and transverse resistance (Hall resistance) A longitudinal resistance
is a resistance measured between two contacts that may be connected by a line which
does not connect C1 and C430
Transverse resistance is measured between two contacts
connected by an imaginary line connecting C1 and C4 (Figure 26a)
Figure 26 (a) 2D electrons in a perpendicular magnetic field Logitudinal resistance
measured across C5 and C6 Transverse resistance measured across C3 and C5
(b) Classical Hall resistance as a function on the magnetic field30
Due to the existence of quantum Hall effect it is natural to expect that there exists
a classical Hall Effect Hall showed that the transverse resistance of a thin metallic plate
varies linearly with the strength B of the perpendicular magnetic field (Figure 26 b)
RH = Bqnel (28)
More quantitatively the classical Hall Effect can be understood within the Drude
model for diffusive transport in a metal Within this model one considers independent
26
charge carriers of momentum p described by the equation of motion
( )
b
dp p pe E B
dt m (29)
where E and B are the electric and magnetic field respectively The macroscopic
transport characteristics ie resistivity of the system are obtained from the static
solution of the equation of motion dpdt = 0 and one finds for 2D electrons with p =
(pxpy)
x
x yb
y
y xb
eBe
eBe
ppE
m
ppE
m
(210)
In the above expression characteristic frequency is visible as
C
b
eB
m (211)
This is known as cyclotron frequency as it characterizes the cyclotron motion of a
charged particle in a magnetic field30
With the Drude theory the conductivity can be
written as
j = -enelpmb (212)
and the mobility can be given as
micro = eτmb (213)
The transport properties in the limit of ωCτ-gt infin are entirely governed in the presence of
27
a magnetic field by the off-diagonal ie transverse components of
conductivityresistivity
The theory of quantum Hall effect subjects all physical properties of 2D electron
system in the limit where the magnetic field is strong so that the mixing of Landau levels
by disorder or electron-electron interaction is considered to be a weak perturbation30
This is known as the quantum Hall regime The ratios between the energy scales
corresponding to the two interactions are important The limit where disorder potential is
much stronger is referred to as integer quantum hall regime whereas the limit where the
interaction potential is much stronger is referred to as fractional quantum Hall regime
25 Resistivity and Resistance
The electronic transport in the framework of the Drude theory allows for the calculation
of conductivity or resistivity of a classical diffusive 2D electrons in a magnetic field30
The conductivity and conductance are related to one another but they depend on the
geometry of the conductor-the resistance R and hence the resistivity is given by
R = (LA)ρ (214)
where L is the length of the conductor and A is the cross section
For a d-dimensional conductor the cross section scales as Ld-1
such that the
scaling relation between the resistance and the resistivity is
R~ ρL2-d
(215)
From the dimension point of view resistance and resistivity are the same in 2D and the
resistance is scale-invariant Further the resistance of a 2D conductor depends in
general on the so-called aspect ratio LW via some factor f (LW)30
However for
transverse Hall resistance it is the length of the conductor that plays the role of cross
28
section such that the Hall resistivity and the Hall resistance truly coincide ie f=1 The
Quantum Hall effect is highly insensitive to the particular geometric properties of the
sample used in transport measurements Recently quantum Hall physics experienced the
discovery of ldquorelativisticrdquo quantum Hall effect in graphene The electrons in graphene
behave as if they were relativistic massless particles contributing to a very interesting
field of research30
26 Klein Tunneling
Klein tunneling in which relativistic particles penetrate through a potential barrier
without the exponential damping that is characteristic for nonrelativistic quantum
tunneling has never been observed for elementary particles The tunneling allows
transmission of a particle through a potential barrier higher than its kinetic energy
violating the principle of classical mechanics30
On the quantum scale the objects exhibit
wave-like characteristics in which the quanta move against a potential hill described by
their wave function This wave function represents the probability amplitude of finding
the object in a particular location The transmission of the object through the potential hill
is termed as tunneling When EltV then the ψ(x) over V is returned by ψrsquo(x) In quantum
mechanics an electron tunnels from the conduction into the valence band Such a
tunneling from an electron-like to hole-like state is called as Klein Tunneling in which the
electron avoids backscattering
In Figure 27 it is shown that an electron hitting a potential barrier is reflected
with 100 certainty In non-relativistic quantum mechanics the electrons can tunnel
through the barrier but the probability of tunneling exponentially decays with increasing
29
height and width of the barrier However in relativistic quantum mechanics the barrier
gets transparent even in the limit of infinite barrier height (Klein paradox)31
Figure 27 Klein tunneling through an npn barrier30
The Klein paradox in graphene can be understood in terms of electrons and holes
In graphene the massless carriers behave differently than ordinary carriers (with mass) in
the presence of an electric field A barrier which is repulsive for electrons will be
attractive for holes Since there are hole states inside the barrier with the same energy as
the electrons outside an electron arriving at the barrier can tunnel through it as a hole
before leaving again as an electron Klein tunneling for transport in graphene is that the
charge carriers cannot be confined by potential barriers The Klein tunneling effect has
been experimentally observed by Ando in 1998 in which the absence of backscattering
(Figure 28) is responsible for high conductivity in carbon nanotubes
30
Figure 28 Electron trajectory considering the linear electrostatic potential U(x) = Fx30
The electron is able to propagate through an infinitely high potential barrier since
it makes a transition from the conduction band to valence band In this transition from
conduction band to valence band its dynamics changes from electron-like to hole-like
The equation of motion is thus given by
2
2 2 2| | ( )
pdr E
dt E Up
p E U
v
v
at energy E (216)
This shows that in the conduction band (UltE) and in the valence band (UgtE)
In Klein tunneling the pairs of electron-like and hole-like trajectories at the same E and
py have turning points at dmin given by dmin=2v|py|F (Figure 29)
Figure 29 Electron like and hole like trajectories at same E21
31
The tunneling probability exponential dependence on dmin
2
min| |
( ) exp( ) exp( )2
y y
y
vT
F
p pdp
(217)
The applications of the Klein tunneling include Atomic clock Scanning tunneling
Microscope Tunnel diode Tunneling transistor and many more32
Since graphene
exhibits Klein tunneling it can be very useful to study the transport properties in
graphene and use it in such applications
27 Quantum Hall Effect in a Graphene
A monolayer graphene shows half-integer quantum Hall effects where the Hall
resistance is quantized at values of
2
1
xyh v eR
(218)
around filling factors
14( 1 2)Nv
(219)
where N is an integer e is the electron charge h is the Planckrsquos constant and the
factor 4 is due to spin and valley degeneracy QHE in graphene can be observed at room
temperature which is a very intriguing property (Figure 210) Graphene reveals
significant differences with respect to conventional 2D electron systems The Landau
quantization yields energy levels that disperse differently in graphene as well as
particular zero-energy level that is only half filled at the charge neutrality point (v=o)
32
Figure 210 Quantum Hall effect in graphene22
The Hall conductivity σxy and the
longitudinal resistivity of monolayer graphene as a function of carrier density at B = 14T
and T= 4K This shows half-integer QHE with chiral index J= 1
The QHE in graphene is not entirely similar to regular QHE since the charge
carriers in graphene are Dirac Fermions The charge carriers governed by
electrodynamics is given by (Equation 220) which does not apply for graphene and a
QED quantization of graphene electronic band structure is used
En = (n+12)ħω (220)
33
In the presence of magnetic field the nature of the Dirac Fermions in graphene
results in unevenly spaced Landau levels (LL) containing a distinctive LL at the electron-
hole degenerating a zero energy given by
2MG
MGFehn B
n vE (221)
The LL levels at high magnetic fields in MG are shown in Figure 211
Figure 211 (a) LL for Graphene bilayer (b) Schematics of Hall conductivity as a
function of nn0 for bilayer Graphene (solid line) and monolayer Graphene (dotted line)
(c) LL for monolayer Graphene33
It is found that the Hall resistance of a two dimensional electron system has
plateaus as a function of the number of electrons at low temperatures and strong magnetic
fields32
At large B the Dirac-like energy spectrum of graphene gives rise to a
characteristic series of QH plateaus in conductance reflecting the presence of a zero-
energy Landau level that include only odd multiples of 2e2h for uniform carrier density
in the sheet These plateaus of QH edge states at the edge of the sheet circulating in a
34
direction are determined by the direction of B and the carrier type33
This is why QHE in
graphene is known as Half-Integer Quantum Hall Effect
28 Thermoelectric Effect
Thermoelectricity refers to a class of phenomena in which a temperature difference
creates an electric potential or an electric potential creates a temperature difference The
principle of thermoelectric effect has been known for over 100 years Recently the
practical applications of thermoelectric effect have become more viable34
Thermoelectric effect is the direct conversion of temperature differences to
electric voltage and vice versa Joule heating is the heat generated whenever a voltage is
applied across a resistive material The Peltier-Seebeck effect is reversible whereas Joule
heating is not This effect can be used to generate electricity to measure temperature to
cool objects or to heat them Since the direction of heating and cooling is determined by
the sign of the applied voltage thermoelectric devices make very convenient temperature
controllers
281 Seebeck Coefficient
Thomas Johann Seebeck discovered that an emf appears in a circuit composed of two
dissimilar metals when the junction between the metals is held at different
temperatures34
The thermoelectric emf causes a continuous current in the circuit when a
complete loop is formed and the current is known as thermoelectric current This is
known as the Seebeck effect
35
Figure 212 Seebeck Effect34
As long as the two junctions are at different temperatures the thermoelectric emf
exists and the current will keep flowing between the hot and cold junction that are at
different temperatures The Seebeck effect is the conversion of temperature difference
directly into electricity The voltage developed in the circuit shown in Figure 212 is
proportional to the difference in temperature between the two junctions and is given by
V = α (T2-T1) (222)
This Seebeck effect is observed not only in metals but also in semiconductors
Here α is known as the Seebeck coefficient α measures the magnitude of an induced
thermoelectric voltage in response to the temperature difference across the material If the
temperature difference ∆T between the two ends of a material is small then the Seebeck
coefficient of a material is written by
α = ∆V∆T (223)
36
This can be expressed in terms of electric field as
α E∆T (224)
The units of Seebeck coefficient is given as VK The higher the Seebeck coefficient
value the better it is since it will create a very large voltage that can be used to provide
power
282 Peltier Coefficient
Peltier effect is the inverse of Seebeck effect involving a junction phenomenon There is
heat absorption or generation at the junctions depending on the direction of current flow
Heat generated by current flowing in one direction is absorbed if the current is reversed
The heat absorbed per second at a junction carrying current I is given by
Heat absorbed in t sec = πabIt (225)
Here πab is the Peltier coefficient and given by HIt Thus Peltier coefficient is
numerically equal to the applied potential difference expressed in Volts
Overall by studying the flow of electrons the values of Seebeck
coefficient and Peltier co-efficient can be estimated These values determine the various
applications of the materials In this thesis the Peltier and Seebeck coefficient of the
graphene junction and the new applications are discussed
37
29 Early Research ndash ab intio studies
In 2007 Androitis studied that the conducting properties of graphene nanoribbons and
junctions are strongly dependent on their size and geometric features35
He concluded that
there is no conductance for small AZA or ZAZ ribbons (Figure 213)
Figure 213 Transmission functions in units of (2e
2h) for AZA structures
35
Figure 213 shows that T (E) exhibits a negligible peak [T (E) = 001 in units of
2e2h] at E= -225 and 250eV However it was noted that when the width of the arm type
was increased T (E) at -225 and 250eV was 02035
Later in 2007 Qimin Yan used first principles methods to investigate the Current-
Voltage characteristics of GNR Transistors and the effect of edge doping He showed that
GNR field effect transistors can achieve high performance levels with ONOFF ratios on
the order of 103-10
436
Figure 214 is an I-V curve of AZA GNR-FET connected via
armchair metallic leads36
38
Figure 214 I-V curve for a 591nm long channel (Vbias=20mV)
36
In 2009 Fangping OuYang demonstrated the intrinsic transport properties and
effective B or N doping of the junctions by using first-principles quantum transport
simulations He concluded that the I-V characteristics of pure-carbon T-shaped junctions
exhibit metallic behavior and the current in the junction strongly depends on the height
of the stem23
He reported that the conductance of the devices depends on the geometric
structures which can be controlled by selective doping
In 2012 Wei Yao used the first principle calculations based on Density
Functional Theory (DFT) and Non-equilibrium Greens Function (NEGF) to study the
electronic as well as the transport properties of B-doped 6-GNR p-n junction His results
showed that the boron doping interval can influence the rectification effect at low bias
and also exhibit Negative Differential Resistance (NDR) phenomena at high positive
bias
39
CHAPTER 3
COMPUTATIONAL DETAILS
31 Introduction
The physical chemical electrical electronic and optical properties of a solid are
determined by their quantized electronic states The quantum states in low-dimensional
systems are produced due to the confinement of the carrier charges in one or two
dimensions Graphene is a conductor electrons are able to flow through graphene more
easily than through even copper The electrons can travel through the sheet of graphene
like mass-less particles as fast as just one hundredth that of the speed of light The ways
in which electrons behave in graphene make it very helpful to study their fundamental
physical properties Graphenersquos near perfect crystal lattice provides a very clean system
to experiment By restricting the electrons to only two dimensions they exhibit some
interesting properties such as the anomalous quantum Hall effect and Klein tunneling
In this chapter two theoretical concepts used for calculating the electronic structure
and the transport properties for graphene are described These include the Extended
Huckel Theory and Non-Equilibrium Greenrsquos Function (NEGF) method
311 Extended Huckel Theory
Erich Huumlckel was born in Germany on August 9th
1896 He studied mathematics and
physics in Berlin He is best known for his work in the field of chemistry and physics for
two contributions (1) Debye- Huumlckel theory of electrolytic solutions (2) Huumlckel
method of approximate molecular orbital calculations on electron systems In 1930 he
published his findings on systems in 1931 he generalized and expanded the system
40
theory to explain benzene Due to his poor communication skills his findings went
unrecognized for over 20 years It was in 1951 that his 4n + 2 rule was finally clarified by
Doering to show if C=C bonds would show aromaticity Huumlckel died on February 16th
1980 with very little worldwide recognition for his contributions to chemistry Today
chemistry students recognize his name and his contributions to the field are quite
substantial
One of the first semi-empirical methods to be developed was Huumlckel Molecular
Orbital Theory (HMO) HMO was developed to describe molecules containing
conjugated double bonds HMO considered only electrons in pi orbitals and ignored all
other electrons in a molecule The Extended Huumlckel Molecular Orbital Method (EH) was
developed out of the need to consider all valence electrons in a molecular orbital
calculation
By considering all the valence electrons chemists could determine molecular
structure compute energy barriers for bond rotations and determine energies and
structures of transition states for reactions By considering only the valence electrons the
computed energies could be used to choose between proposed transition states to clarify
reaction mechanisms The total valence electron wavefunction is described as a product
of the one-electron wave functions
1 2 3(1) (2) (3) ( )valence j n (31)
where n is the number of electrons and j identifies the molecular orbital Each
molecular orbital is written as a linear combination of atomic orbitals (LCAO)
1 12
N
j jr rrc j N
(32)
41
The energy of the jth
molecular orbital is given by a one-electron Schroumldinger
equation using an effective one electron Hamiltonian heff which expresses the interaction
of an electron with the rest of the molecule
eff j j jh (33)
This is the energy eigenvalue of jth
molecular orbital corresponding to the Eigen
function j The advantage of using this method is that the exact form of heff is not
required The total energy of the molecule is the sum of the single electron energies
j jj
E n (34)
where nj is the number of electrons in orbital j
In order to use the Extended Huckel method a set of calculation parameters and
approximations must be followed These parameters include the Basis set K-point and
the Brillouin Zone and lastly the Mesh cut-off
312 Introduction to NEGF
The Greenrsquos function is a function of two space-time coordinates From the knowledge of
this function one can calculate time-dependent expectation values such as currents and
densities electron addition and removal energies and the total energy of the system In
the absence of external fields the non-equilibrium Green function method reduces to the
equilibrium Green functions NEGF can be applied to both extended and finite systems
The generic system of NEGF consists of the electron dynamics of the channel described
by the Hamiltonian This channel consists of two contact reservoirs with respective
chemical potential μR and μL The NEGF assumes ballistic transport neglecting self-
42
energy from scattering The system is insulated from gate contacts whose effects are
realized via a 3D Poisson solver which solves for the potential at a given point in real
space based on electron density
22 ( ) [ ( ) ( )]D
qr N r n r
(35)
Figure 31 NEGF system
The system is easily expandable to systems with several contacts or gate
configurations by adding additional self-energy matrices to NEGF or additional sources
to the Poisson solver
313 Electrostatics
Electrostatic potential is created every time in the presence of a charge density due to an
induced electric field The Poissonrsquos equation correlates the electrostatic potential to
charge density as given in Equation 36
43
2( ( ) ( ) ( ) ( ))( )
( )( ) ( )
ADq p r n r r N rr
rr r
N
(36)
where ɛ(r) is the dielectric permittivity of the material ρ(r) n(r) ND(r) and NA(r) are the
hole electron donor and acceptor concentrations of the system respectively
Two types of boundary conditions are usually applied to the Poissonrsquos equation
Dirichlet boundary conditions
Φ (0) = F0 and Φ (L) = FL
von Neumann boundary conditions
00
( )
x
d x
dxB
and
( )L
x L
d x
dxB
For the transport problems with open boundary conditions the von Neumann
boundary conditions are used assuming that the potential vanishes at the boundary ie
B0=BL=0
The Poissonrsquos equation can hence be discretized on a grid as
2 ( )( )
( )
rx
r
= M (37)
where M is the matrix Φ and ρ are vectors containing the discretized values of
the electrostatic potential Φ and charge density ρ respectively
44
The Schroumldinger and Poisson equations are coupled since V(x) = -qΦ(x) is used
for the Schroumldinger to compute ρ(x) This self-consistent loop stops when the
convergence is reached
( )r
V(x) = -qΦ(x)
314 Non-Equilibrium Greenrsquos Function
Greenrsquos functions are a mathematical construction that are used to solve differential
equations subject to specific initial or boundary conditions They are named after the
British mathematician George Green The 1-D equation of L( )f( )=S( ) can be defined
by the Greenrsquos Function as given below
( ) ( ) ( )G x x f x x x (38)
The general Greenrsquos function is given by
( ) ( ) ( )f x dx G x x S x (39)
Applying the operator L( ) to the solution f( ) satisfies the original differential
equation The Greenrsquos Function G( ) is the propagator which propagates the influence
of a perturbation S( ) originally situated at the point to the point at which the
function f( ) is evaluated
The Greenrsquos Function G( ) can also be a correlation function If the points
and are strongly (weakly) correlated then S( ) will greatly (poorly) affect f( )
Poisson equation
2 ( )( )
( )
rr
r
Schroumldinger equation
2
2
( ( ) ) ( )
( )2
( ) | ( ) |
E H r E r S
H V rm
r dE E r
Figure 32 Self-consistent loop
45
The Schroumldinger equation with open boundaries can be written as
( )E H S (310)
Considering a 1-D and homogenous system ranging from =0 to L assuming
that Σ=0 and the form of equations is same before and after discretization then
22
2 0( ) ( ) ( )
2E x S x
m
dV
dx
(311)
The Greenrsquos function can hence be computed corresponding to the Schroumldinger
equation
22
2 0( ) ( ) ( )
2E G x x x x
m
dV
dx
(312)
Due to the delta-function at = a discontinuity is observed and hence the
Greens function is evaluated at boundary conditions
0
2
exp( ( )) x x 2 ( )( )
exp( ik(x x)) x x
ik x x m E VG x x k
A
A
(313)
By integrating the Schroumldinger equation twice and setting the lower and upper
integration boundaries to = -δ and = +δ the Greenrsquos Functions can be written as
2
( ) ( ) 0
( ) ( ) 2
x x x x
G x x G x x
dG x x dG x x m
dx dx
(314)
46
The coefficient A+ and A
- become
ik
mA A
(315)
The Greenrsquos Function takes a final form known as Retarded Greenrsquos Function and
is written as
( ) exp( | |)G x x i ik x xk
m (316)
And the wave function is
( ) ( ) ( )x dx G x x S x (317)
Retarded Greenrsquos Function propagates the wave functions generated by a source
or perturbation S from its origin at to any point
The retarded Greenrsquos Function as discretized Schroumldinger equation is written as
( )R RE H G I (318)
The wave function Φ can be calculated from the retarded Greenrsquos function and the
source vector as
Φ = GR∙S (319)
Overall in this section the Greenrsquos function approach in calculating the electron
dynamics is reviewed We defined the self-energy of each part of the system spectral
function and the probability current density the electric current is derived explicitly using
Non Equilibrium Greenrsquos function We will use this formalism to calculate the tunneling
phenomena in coupled quantum dots isolated or otherwise
47
CHAPTER 4
ATOMISTIX TOOLKIT DETAILS
41 Introduction
Virtual NanoLab (VNL) is a graphical user interface (GUI) that provides a group of
modeling tools the function of these tools involves the set-up investigation and the
study of nanoscale structures The quantum mechanical equations are solved by the
software by using the advanced software architecture and numerical methods to
implement ab initio calculations VNL simulates the electronic structure and calculates
the transport properties based on the two systems mentioned earlier NEGF and Extended
Huckel ATK is the main engine for computing the scripts and hence all the calculations
performed in VNL are done by ATK VNL is a user friendly software as it not only
allows creating a script but also helps to set up a virtual experiment
This thesis involves the use of VNL in order to study the effect of the width and
different orientations of the doped atoms Since the software allows for virtual
experiments it makes it much easier to study the I-V characteristics based on the change
in position of atoms
42 Device Structure
In this thesis AZA GNR p-n junction with boron doping (location) was created using the
ATK software which is based on NEGF and DFT Further the thesis discusses the
transport properties and the I-V curve of such junction
The input format of ATK is NanoLanguage which is an extension to Python
scripting language ATK uses the NEGF system for formalism of simulating device
48
Figure 41 Geometry of device configuration with two electrodes
37
The system is divided into three parts left central and right The implementation
relies on the screening approximation which assumes that the properties of the left and
right regions can be decribed by solving a bulk problem for fully periodic electrode cell37
This screening approximation is fulfilled when the electrode regions can be described by
an equilibrium electron distribution
Figure 42 The electron distribution in a device configuration which illustrates a left
moving scattering state with origin in right electrode37
The system assumes that in steady state the electron density of the central region
is constant in time and hence the electron density is calculated independently from each
electrode The electron density is given by the occupied eigenstates of the system
n(r) = nL(r) + n
R(r) (41)
49
The left and right densities are calculated by summing up the occupied scattering
states
nL(r) = sum
(42)
nR(r) = sum
(43)
The scattering states are usually calculated by first calculating the Bloch states in
the electrodes and then solving the Schroumldinger equation of the central region using the
Bloch state as matching boundary Instead of using the scattering states the ATK
software uses the NEGF method to calculate the non-equilibrium electron density
The electron density is given in terms of electron density matrix
D = DL + D
R (44)
The left density matrix is given by NEGF theory
DL = int
(45)
where
ρL(ɛ) =
(46)
ρL(ɛ) = is the special density matrix
Also if there is a non-equilibrium electron distribution in the central region then
the electron distribution in electrode is given by the Fermi function f with an electron
temperature TL
G(ɛ) =
(47)
G = retarded Green function
δ+ is an infinitesimal positive number and S H overlap the Hamiltonian matrices
L =
sum sum
(48)
50
L
is the broadening function of the left electrode given in terms of left electrode
self -energysum
43 Transmission Spectrum Calculations
Once the self-consistent non-equilibrium density matrix has been obtained the various
transport properties of the system can be calculated One of the most important properties
is the transmission spectrum from which the current and differential conductance can be
obtained
The transmission coefficient in ATK is obtained by the retarded Greens function
T(ɛ) = G(ɛ)ΓL(ɛ)G
ϯ(ɛ)Γ
R(ɛ) (49)
The transmission amplitude of individual scattering states may be obtained
through the Transmission Eigenvalues The ldquoTransmission Eigenvaluesrdquo is an analysis
which finds the eigenvalues of the transmission matrix
The transmission matrix at energy E and k-point is given by
Tnm(Ek) = sum (410)
where
= transmission amplitude from Bloch state ψn(k)
The transmission coefficient is given by the trace of transmission matrix
T(Ek) = sum (411)
Keeping in mind all quantities depend on the quantum numbers parametrically
Transmission eigenvalues sum up to the transmission coefficient
T = sum (412)
51
44 Calculating the Current
Current is calculated from the transmission coefficient using
I( ) ( )R L
L RL R
R LB B
eE f f dE
h
E EV V T T T
k kT T
(413)
where f is the Fermi function TRL is the electron temperature of the right or left
electrode and Tσ(E) is the transmission coefficient for the spin component σ
The chemical potentials of the left and right electrode given by
L
F R LR L
eVE
are defined relative to the Fermi level of the left electrode These chemical potential are
related to the applied bias and hencebiasR L
eV therefore bias L RV V V
The transmission spectrum itself is usually rather insensitive to temperature and is
used in self-consistent calculations but often depends strongly on the electrode voltages
Thus for an accurate estimate of the current the transmission spectrum should be
calculated self-consistently for each desired bias
ATK uses very precise method to calculate the transport properties of the system
Transmission spectra for various concentrations of boron doped graphene p-n junctions
are generated in this Chapter and various coefficients such as Seebeck Peltier and
Conductance are calculated
52
45 Calculating Transport coefficients
The linear response transport coefficient of an applied voltage difference or temperature
difference between the two electrodes is given by
Conductance
| dT 0
e
dI
dUG
(414)
Peltier coefficient
| d 0
Q
I
I
(415)
Seebeck coefficient
| 0
dUS I
dT T
(416)
These linear response coefficients are calculated by the Transport Coefficients To
perform these calculations the ATK uses the Electron Transmission Spectrum
53
CHAPTER 5
RESULTS AND DISCUSSION
51 Band Structure Analysis
The electronic bandstructure of GNR both doped and undoped are discussed in this
chapter
The armchair configuration of Pristine GNR (PGNR) has a band structure that is
dependent on its width This is explained by the fact that the sheet itself acts like a
potential well where the electrons are confined to form standing waves along Cr the
rolling vector albeit with slightly different boundary conditions (Cr = ma1 + na2
where m and n are integers and a1 and a2 are the unit cell vectors of graphene lattice) In
a GNR the two nodal points of the standing wave must be at the ribbon edge while in a
Single wall nanotube (SWNT) they can be anywhere ie a circumferential periodic
boundary condition
(a) (b)
Figure 51 Bandstructure of AGNR widths (a) 4 atoms (b) 5 atoms
54
(a) (b)
Figure 52 Bandstructure of AGNR widths (a) 6 atoms (b) 7 atoms
(a) (b)
Figure 53 Bandstructure of AGNR widths (a) 8 atoms (b) 9 atoms
55
(a) (b)
Figure 54 Bandstructure of AGNR widths (a) 10 atoms (b) 11 atoms
Figure 55 Bandstructure of AGNR with a width of 12 atoms
Figure 56 Variation in band gaps as the width (number of atoms) varies
0
05
1
15
2
25
0 2 4 6 8 10 12 14
Wdith vs Band Structure
eV
56
The band structure of 12 Atom AGNR is close to that of Ge (0626 eV) The
actual width of this nanoribbon is about 25 nm 12 AGNR has been fabricated
successfully and doped with various dopants Hence the 12 Atom AGNR has been chosen
to study the transport properties
A junction is created using ZGNR and AGNR To maintain the consistency in the
device analysis it is imperative that the band structure of ZGNR is also calculated From
the simulation it is evident that ZGNR-AGNR-ZGNR junction configuration displays the
Metal ndashSemiconductor-Metal configuration that is addressed in this work The Fermi
Level in all the Z-GNR nanoribbons of widths 4-12 lies within the conduction band
Figure 57 Band structure of ZGNR width (a) 4 atoms (b) 6 atoms
57
(a) (b)
Figure 58 Band structure of ZGNR width (a) 8 atoms and (b) 10 atoms
Figure 59 Band structure of ZGNR with a width of 12 atoms
In order to create viable junction that would show transistor properties doping of
the semiconductor part is necessary The 12 atom AGNR is doped with boron (p-type)
and nitrogen (n-type) - (Figure 510a) 4 N doped (Figure 510b) 4 B In both cases
the impurities lie on the edge of the atoms For 2 nitrogen doped GNR with the
58
impurities lying in the center of the ribbon the Fermi level is found to be in the
conduction band as shown in (Figure 510c) (Figure 510d) shows the position of N with
respect to the edge A very clear departure from the expected (the valence band extending
above Fermi level) is shown in (Figure 510a)
Figure 510 Band structures of Doped AGNR (a) 4 N Doped (b) 4 B Doped (c) 2
N Doped (d) position of Nitrogen from (c)
(a) (b)
(c) (d)
59
52 I-V Characteristics of GNR junction
In pristine graphene the chirality determines the conductivity as seen from the I-V curves
for various widths At certain widths the semiconducting properties are more
pronounced These widths determine the wavelengths of the standing waves which in
turn determine the sub-band locations in the E-k plot When the biasing potential
exceeds 012V the I-V curve shows linearity In case of the 8-atom wide PGNR the
band gap is about 03 eV and it is evident from the I-V plot that the On-State is + 033 V
The band gap of 10-atom and the 4-atom wide PGNR is large enough to show
semiconducting properties
Figure 511 Current Vs Voltage graph for varying graphene width showing
conductivity
-30000
-20000
-10000
0
10000
20000
30000
-3 -2 -1 0 1 2 3
Cu
rre
nt
(nA
)
Voltage (V) (bias)
Current (nA) Vs Voltage for varying graphene width
W=10
W=8
W=6
W=4
60
The ZAZ GNR Configurations show the properties of a semiconductor junction The 12
atom ZAZ structure is studied for its I-V characteristics In this Chapter undoped B-
doped N-Doped B and N Doped (P-N Junction) ZAZ junctions are simulated
Figure 512 ZAZ GNR junction device
61
The boron doped ZAZ junction I-V characteristics are shown below (Figure 513)
The impurity concentration is 2 and 4 Various device configurations are studied
Figure 513 I-V curve of Boron Doped ZAZ junction
-25000
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
25000
-205 -155 -105 -055 -005 045 095 145 195
Cu
rre
nt
(nA
)
VBias
2B_1G_R 2B_0G_R
4B_0G_L 4B_0G_C
4B_0G_R 4B_1G_L
4B_1G_C 4B_1G_R
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
-2 -1 0 1 2
Cu
ren
t(n
A)
VBias
4 B doped GNR Jn
62
Figure 514 I-V curve of Nitrogen Doped ZAZ
-25000
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
-2 -15 -1 -05 0 05 1 15 2
Cu
rre
nt(
nA
)
VBias
I-V Curve as function of Dopant location
2N_0G_L2N_0G_C2N_0G_R2N_1G2N_1G_C2N_1G_R
-15000
-10000
-5000
0
5000
10000
15000
-2 -1 0 1 2
Cu
rre
nt(
nA
)
VBias
2N_0G_C
2N_1G_C
63
Figure 513 and Figure 514 show the I-V characteristics of the GNR junction doped with
2 boron and nitrogen respectively The location of N and B is at the central region of
the edge of the GNR Both B doped and N doped GNR Junctions show significant
Negative Differential Resistance (NDR) This is more pronounced in case of nitrogen
doping Another interesting observation is increasing ohmic nature with the change in
location of the dopants Nitrogen doped device configuration exhibits a pronounced
semiconductor behavior and the NDR effect is observed to be minimal
53 Thermoelectric Properties
In this study the thermoelectric properties were simulated for the GNR Junctions that
displayed high NDR effect The variation in the Peltier coefficient with temperature is
shown as function of doping
When the concentration of nitrogen increases the dimensionless Figure of Merit
ZT seems to decrease considerably This is mostly explained by the decrease in both
conductivity and mobility of the electrons
ZT = S2σTk (51)
where S is the Seebeck coefficient σ is the electrical conductivity T is the
absolute temperature and k is the thermal conductivity
64
Figure 515 Variation of Peltier coefficient with temperature as function of
doping
Figure 515 shows the maximum Peltier coefficient for 2 boron This is
explained by the scattering by boron and the associated smallest mean free path
0
0001
0002
0003
0004
0005
0006
0007
0008
0009
001
250 270 290 310 330 350 370 390 410
ZT
T (K)
2B
4B
Undoped
2N
4N
65
CHAPTER 6
CONCLUSIONS
Graphene ZAZ junctions exhibit varying properties depending on the various structural
configurations In this thesis it was found that the transport properties of graphene
depend on their width the edge of GNR doping concentration and the type of dopant
used The calculations of the band structure contributed towards the determination of the
minimum length of GNR required for studying the transport properties The minimum
length had a band gap equivalent to that of germanium and hence the importance of the
width being 12 atoms wide This band gap indicated fluctuating changes when doped
with elements such as B and N The viable junction showing transistor properties was
hence created by doping the semiconductor part of ZAZ By doping the I-V
characteristics were studied which showed significant NDR which was more pronounced
in the case of nitrogen Also the changing positions of the dopants contributed towards
the I-V curve to be more ohmic The edge doping caused minimum NDR and
semiconductor behavior as compared to central doping Lastly the thermoelectric
properties were studied - the increasing concentration of N causes the Figure of Merit to
decline due to the decrease in conductivity as well as mobility of electrons
66
REFERENCES
1 Wikianswers What makes carbon unique
httpwikianswerscomQWhat_makes_carbon_so_unique (22 November)
2 Kopeliovich D D Graphite
httpwwwsubstechcomdokuwikidokuphpid=graphite (1128)
3 Barbier M Transport properties of nanostructures and superlattices on single layer and
bilayer graphene University Antwerpen Antwerpen 2012
4 Shylau A Electron transport interaction and spin in graphene and graphene
nanoribbons Linkoping Norrkoping 2012
5 HassJ R F T Li X Li Z Zong W A de Heer P N First E H Conrad C
AJeffrey and C Berger Applied Physics Letters 2006 89 (14) 143
6 Jones A Mechanical Exfoliation to Make Graphene and Visulization
httpcarbonchemwisceduFilesMechanicalExfoliationpdf (18 October)
7 Anteroinen J Structural and Electrical Characteristics of Graphene Field Effect
Transistors AALRO school of Electrical Engineering AALTO 2011
8 Novoselov K S A K G S V MorozovD JiangY Zhang S V Dubonos I V
Grigorieva A A Firsov Science 2004 306 (22)
9 Kosynkin D A L H A Sinitskii J R Lomeda A Dimiev K B Price and J M
Tour Nature 458 876
10 Yi Z Luyao Zhang Accounts of chemical research 46 (10) 2339
11 Eizenberg M B JM 1979 82 236
12 Yu Q K L J Siriponglert S Li H Chen Y P Pei S S Applied Physcis
Letters 2008 93 (113103)
13 Li X C W An J Kim S Nah J Yang D Piner R Velamakanni A Jung I
TutucE Banerjee S K Colombo L Ruoff R S Science 2009 324 1314
14 Schaefer H E Nanoscience Springer Berlin 2010
15 Levente Tapasztoacute G D Philippe Lambin amp Laacuteszloacute P Biroacute Nature Nanotechnology
2008 3 401
67
REFERENCES
16 Dacheng Wei Y L Advance Materials 2010 22 (30) 3241
17 Wei Yao K L Y GYGao Elsevier Solid State Communications 2013 153 52
18 Dacheng Wei Dagger Yunqi Liudagger Yu Wangdagger Hongliang ZhangdaggerDagger Liping HuangdaggerDagger
Yudagger a G NanoLetters 2009 9 (5) 1758
19 Nakada K M F G Dresselhaus and M S Dresselhaus PhysRevB 1996 54
(9858)
20 Son Y W C M L a L S G PhysRevLett 2006 97 (216803)
21 Raza H Graphene Nanoelectronics Springer 2012
22 Ryan W J Electronic Transport in Graphene p-n junctions Short Noise and
Nanoribbons Harvard University 2009
23 Fangping OuYang J X Rui Guo Hua Zhang and Hui Xu Nanotechnology 2009
20 6
24 Guo J Carbon nanotube electronicsModeling physics and applications Purdue
University West Lafayette IN 2005
25 Motta C S S-P MITrioni cond-matmes-hall 2012 7
26 B P Growing Graphene via Chemical Vapor Deposition Ponoma College Ponoma
2011
27 ZurichE Transport properties of three-terminal graphene devices University of
Science and Technology Norway 2008
28 Uichiro MIntroduction to the electron theory of metals
29 Robert Laughlin H S Additional background material on the Nobel Prize in Physics
1998 (410)
30 MarkGoerbig Quantum Hall Effects (11152013)
68
REFERENCES
31 Zurich E Transport properties of three-terminal graphene devices Norwegian
University of Science and Technology Norway 2008
32 Deepak R Klein Tunneling University og Tennessee Space Institute Tennessee
2011
33 Williams JR L D CMMarcus Quantum Hall Effect in a Gate-Controlled p-n
Junction in Graphene (1122013)
34 Avadhanulu MN P G K A Textbook of Engineering Physcis for BE BSc (Engg)
SChand New Delhi 1992
35 Andriotis A Applied Physics Letters 2007 91 (152105)
36 Qimin Yan B H dagger Jie Yudagger Fawei Zhengdagger Ji ZangDagger Jian Wudagger Bing-Lin Gu F
L Dagger and Wenhui Duandagger NanoLetters 2007 7 (6) 1473
37 Soler J M E A J D Gale A Garciacutea J Junquera P Ordejoacuten and D Saacutenchez-
Portal J Phys Condens Matter 2002 14 2745
APPROVAL PAGE
ANALYSIS OF TRANSPORT PROPERTIES IN A ZAZ GRAPHENE NANORIBBON JUNCTION USING VARIOUS DOPANTS
Natasha Parikh
Dr N M Ravindra Thesis Advisor Date Director of Material Science and Engineering Program NJIT Dr Keun H Ahn Committee Member Date Associate Professor of Physics NJIT Dr Tao Zhou Committee Member Date Associate Professor of Physics NJIT Dr Halina Opyrchal Committee Member Date Senior University Lecturer of Physics NJIT
BIOGRAPHICAL SKETCH
Author Natasha Parikh
Degree Master of Science
Date January 2014
Undergraduate and Graduate Education
bull Master of Science in Materials Science and EngineeringNew Jersey Institute of Technology Newark NJ 2014
bull Bachelor of Arts in Physics and Biological SciencesRutgers the State University of New Jersey New Brunswick NJ 2012
Major Materials Science and Engineering
iv
v
ACKNOWLEDGMENTS
I would like to express my gratitude to my supervisor Dr NM Ravindra for the useful
comments remarks and engagement throughout the learning process of this Mastersrsquo
thesis Furthermore I would like to thank Vijay Kasi Somayajula for introducing me to
the topic as well for the support I thank Dr Tao Zhou Dr Ken Ahn and Dr Halina
Opyrchal for serving on my thesis Committee I would like to thank my loved ones who
have supported me throughout the entire process both by keeping me harmonious and
helping me in putting pieces together
vi
TABLE OF CONTENTS
Chapter
Page
1 INTRODUCTIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
1
11 Graphene The New Carbonhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
1
12 Graphene Synthesishelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
3
121 Synthesis of Graphene on Nickel (Ni)helliphelliphelliphelliphelliphelliphelliphellip
5
122 Synthesis of Graphene on Copper (Cu)helliphelliphelliphelliphelliphelliphelliphellip
8
123 Transfer of Graphene Filmshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
8
124 Synthesis of Graphene Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
9
125 Doping in Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
10
126 Nitrogen (N) Doped Graphene Synthesis (Substitutional)hellip
12
13 Structure of Graphene Nanoribbon (GNR)helliphelliphelliphelliphelliphelliphelliphelliphelliphellip
13
14 Overview of Graphene Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
15
2 RESEARCH BACKGROUNDhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
21 Bandstructure of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
22 Transport Characteristics of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
20
23 Drude Theoryhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
22
24 Quantum Hall Effect (QHE)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
24
25 Resistivity and Resistancehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
27
26 Klein Tunnelinghelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
28
27 Quantum Hall Effect in Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
31
28 Thermoelectric Effecthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 34
vii
TABLE OF CONTENTS
(Continued)
Chapter Page
281 Seebeck Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
34
282 Peltier Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
36
29 Early Research ndash ab initio Studyhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
37
3 COMPUTATIONAL DETAILShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
31 Introductionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
311 Extended Huckel Theory helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
312 Introduction to NEGFhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
41
313 Electrostaticshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
42
314 Non-Equilibrium Greenrsquos Functionhelliphelliphelliphelliphelliphelliphelliphelliphellip
44
4 ATOMISTIX TOOLKIT DETAILShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
41 Introductionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
42 Device Structurehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
43 Transmission Spectrum Calculationhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
50
44 Calculating the Currenthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
51
45 Calculating the Transport Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
52
5 RESULTS AND DISCUSSIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
53
51 Band Structure Analysis helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
53
52 I-V Characteristics of GNR Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
59
53 Thermoelectric Propertieshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
63
6 CONCLUSIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 65
REFERENCEShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
66
viii
LIST OF FIGURES
Figure Page
11 (a) Chemical representation of Carbon (b) Graphite ore (c) Structure of
Graphite and a single layer Graphenhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
2
12 An optical image of Graphene flake obtained by exfoliation of
graphitehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
3
13 (a) Graphene formation on Nickel (b) Graphene atoms on Ni (111)
lattice (c)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
7
14 (a) SEM image of graphene on copper foil (b) High-resolution SEM
image of graphene on Cuhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
8
15 (a) Transfer process (b) Wafer-scale synthesis of graphene (c) Graphene
films transferred onto glass wafer (d) SiSiO2 with device patterned (e)
PET filmhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
9
16 (a) High-magnification image of the annealed sample showing that well-
defined zigzag armchair and zigzag-zigzag edges are formed (b) ) STM
image of an 8 nm wide bent junction connecting an armchair and a
zigzag graphene nanoribbon which was carved by STM
tipshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
10
17 Band structure of graphene before and after doping The image shows
shift towards the Fermi levelhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
11
18 Low resolution TEM image of N-doped graphene Background is the
lacey carbon TEM grid graphene sheet is crumpled with many
rippleshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
13
19 Zigzag and Armchair orientation of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphellip 13
110 Bandstructure of ZGNRhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 14
111 Bandstructure of AGNRhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 15
21 Left Real space Graphene lattice with basis vectors and Right
The first Brillouin zone of Graphene in reciprocal space with basis
vectors and K and Krsquo are responsible for massless transport at low
energyhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
ix
LIST OF FIGURES
(Continued)
Figure Page
22 Bandstructure of a graphene sheet showing a band gap of 0eVhelliphelliphellip 18
23 Band structure of Graphene calculated with the tight-binding modelhellip 19
24 The energy dispersion around the K pointhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 22
25 Electrons colliding with stationary ionshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 23
26 (a) 2D electrons in a perpendicular magnetic field Logitudinal resistance
measured across C5 and C6 Transverse resistance measured across C3
and C5 (b) Classical Hall resistance as a function on the magnetic field
25
27 Klein tunneling through an npn barrierhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 29
28 Electron trajectory considering the linear electrostatic potential U(x) = Fx 30
29 Electron like and hole like trajectories at same Ehelliphelliphelliphelliphelliphelliphelliphelliphellip 30
210 Quantum Hall effect in graphene 22
The Hall conductivity σxy and the
longitudinal resistivity of monolayer graphene as a function of carrier
density at B = 14T and T= 4K This shows half-integer QHE with chiral
index J= 1helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
32
211 (a) LL for Graphene bilayer (b) Schematics of Hall conductivity as a
function of nn0 for bilayer Graphene (solid line) and monolayer
Graphene (dotted line) (c) LL for monolayer Graphenehelliphelliphelliphelliphelliphelliphellip
33
212 Seebeck Effecthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 35
213 Transmission functions in units of (2e2h) for AZA structureshelliphelliphelliphellip 37
214 I-V curve for a 591nm long channel (Vbias=20mV)helliphelliphelliphelliphelliphelliphelliphellip 38
31 NEGF systemhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 42
41 Geometry of device configuration with two electrodeshelliphelliphelliphelliphelliphelliphellip 48
42 The electron distribution in a device configuration which illustrates a left
moving scattering state with origin in right electrodehelliphelliphelliphelliphelliphelliphelliphellip
48
x
LIST OF FIGURES
(Continued)
Figure Page
51 Band structure of AGNR widths (a) 4 atoms (b) 5 atomshelliphelliphelliphelliphelliphellip
53
52 Band structures of AGNR widths (a) 6 atoms (b) 7 atomshelliphelliphelliphelliphelliphellip 54
53 Band structure of AGNR widths (a) 8 atoms (b) 9 atomshelliphelliphelliphelliphelliphelliphellip 54
54 Band structures of AGNR widths (a) 10 atoms (b) 11 atomshelliphelliphelliphelliphellip 55
55 Band structure of AGNR with a width of 12 atomshelliphelliphelliphelliphelliphelliphelliphelliphellip 55
56 Variation in band gaps as the width (number of atoms) varieshelliphelliphelliphellip 55
57 Band structure of ZGNR width (a) 4 atoms (b) 6 atomshelliphelliphelliphelliphelliphelliphellip 56
58 Band structure of ZGNR width (a) 8atoms and (b) 10 atoms 57
59 Band structure of ZGNR with a width 12 atomshelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 57
510 Band structures of Doped AGNR (a) 4 N Doped (b) 4 B Doped (c)
2 N Doped (d) position of Nitrogen from (c)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
58
511 Current Vs Voltage graph for varying graphene width showing
conductivityhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
59
512 ZAZ GNR junction devicehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 60
513 I-V curve of Boron Doped ZAZ junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 61
514 I-V curve of Nitrogen Doped ZAZhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 62
515 Variation of Peltier effect coefficient with temperature for various doping 64
1
CHAPTER 1
INTRODUCTION
11 Graphene The New Carbon
Carbon (chemical symbol C atomic mass 1207amu) (Figure 11a) is a widely distributed
element in nature It is found abundantly in the sun stars comets and the atmospheres of
the planet Carbon can form up to four bonds it can bond with itself endlessly and with
most other elements in many different shapes making it a significant part of the
construction for many kinds of complex molecules1
Two allotropes of carbon are commonly used diamond and graphite (Figure
11b) The bonding structures of diamond and graphite contribute to the properties
individually In diamond all the p-orbitals are used forming a sp3
bonding whereas in
graphite only two orbitals are occupied allowing the unpaired bond for the transport of
electrons Each carbon atom in graphene possesses sp2 hybridization ie each carbon
atom is connected to three other carbon atoms via covalent bonds with a bond length of
142Å and an angle of 120deg between each bonded pair This makes graphite a better
conductor than diamond Graphite consists of many layers of 2D carbon lattices (Figure
11c) stacked on top of each other and held via Van der Waals forces A single layer of
graphite where carbon atoms are arranged in a honeycomb lattice is known as graphene
(Figure 11c)
2
Figure 11 (a) Chemical representation of Carbon (b) Graphite ore (c) Structure of
Graphite and a single layer Graphene2
Theoretical work on graphene was done specifically to study the other allotropes
The first study was done by Wallace in 1947 who calculated the band structure of
graphene3 Further the peculiar Landau levels were known by McClure in 1957 and the
relativistic Hofstadter butterfly by Ramal in 19853 Later in 1991 the invention of carbon
nanotubes by Iijima boosted the theoretical research on graphene3 Prior to the invention
of carbon nanotubes there were a few experimental papers on graphene growth via
various methods like intercalation of graphite (Shioyama 2001) free standing (Boehm
1962) epitaxial as well as graphene grown on metals (Bommel 1975 Land 1992 Itoh
1991)3 With all the various discoveries the electronic properties of graphene were not
studied until 2004 when Berger and Novoselov were able to access the electronic
properties with contact of graphene flakes3 (Figure 12)
3
Figure 12 An optical image of Graphene flake obtained by exfoliation of graphite3
The specific lattice structure of graphene possesses a number of unique electronic
properties making it an interesting material for theorists experimentalists and engineers
Utilization of graphene as a fundamental block of electronic devices requires
development of new theoretical methods for understanding the current propagations in
graphene constriction4
12 Graphene Synthesis
The discovery of graphene by mechanical exfoliation called the lsquoScotch tape methodrsquo led
to serious attempts towards the production of top quality graphene5 Graphene was first
exfoliated mechanically from graphite in 20046 The importance of high quality graphene
cannot be emphasized enough however electron transport has shown that defects play an
important role in hindering the transport properties of electrons (holes)7 The two
synthesizing methods for the large scale manufacture of graphene are chemical vapor
deposition (CVD) and silicon carbide (SiC) desorption method
4
Graphene can be synthesized by sublimation of silicon from SiC at high
temperature (1200degC) in high vacuum5 The major advantage of this method is that the
SiC provides an insulating substrate and no transfer of the graphene layer is needed Yet
the disadvantage of this method outweighs its advantages the high temperature is cost-
ineffective making it unsuitable for large scale manufacturing8 Also the crystal growth
face alters the properties of graphene Graphene grown on Si-terminated face has poor
homogeneity and is subjected to unintentional doping7 Conversely graphene grown on
C-terminated SiC has higher mobility and is often called lsquoturbostaticrsquo due to the
rotational disorder7
Unlike the SiC method the graphene produced via CVD method needs to be
transferred to a substrate making it difficult to maintain the quality of graphene Yet
CVD synthesized graphene has a larger grain size7 More research is being done on
various methods for synthesis of graphene The methods include direct chemical
synthesis ion implantation crystal sonification and lastly unzipping carbon nanotubes to
form graphene sheets9
Graphene and few-layer graphene have been grown by CVD from carbon
containing gases on catalytic metal surfaces andby surface segregation of C dissolved in
the bulk of such metals7 Growing graphene with CVD is a very attractive solution since
it is compatible with the existing semiconductor industry9 Graphene has been grown via
CVD process on metal substrates such as Nickel (Ni) and Copper (Cu)
5
121 Synthesis of Graphene on Nickel (Ni)
Polycrystalline Ni films are annealed in ArH2 atmosphere at 900-1000degC to increase
grain size and are then exposed to H2CH4 gas mixture10
In this step the hydrocarbon
decomposes and dissolves in Ni to form a solid solution Lastly the samples are cooled in
argon gas Ni has high carbon solubility at elevated temperatures and the solubility
decreases as temperature is reduced During the cooling process the carbon atoms diffuse
out from the Ni-C solid solution and precipitate on the Ni surface to form graphene films
(Figure 13a) Since Ni (111) has a lattice similar to the densely packed hexagonal lattice
of graphene (Figure 13b) they also have similar lattice constants and hence Ni surface
serves as an excellent lattice matched substrate for graphene growth11
The growth of graphene on Ni is based on carbon segregation and precipitation
process different segregation behavior is produced by different cooling rates which
affect the thickness and quality of graphene films12
Medium cooling rates lead to optimal
carbon segregation and produce few layers12
Graphene films grown on Ni are usually
continuous with monolayer and few layer regions Annealing of Ni substrates at elevated
temperatures in hydrogen atmosphere not only increases the single-crystalline Ni grain
size but also eliminates certain impurities in Ni thereby improving the graphene quality
Furthermore the graphene thickness can also be affected due to the amount of carbon
dissolved in the Ni films during the growth time
After synthesis the graphene can be transferred to other insulator substrates for
further characterization and applications Figure 13c shows the selected area electron
diffraction pattern of graphene film along the [001] direction which confirms the
graphene lattice structure shown After transfer to insulator substrates the geometry can
6
be retained as shown in Figure 13d Under optimal growth parameters graphene growth
is only limited by the Ni catalyst Lastly Figures 13e and 13f show the wafer-scale
graphene synthesis and transfer of graphene to a flexible transparent substrate
respectively
Though polycrystalline Ni is a good substrate the percentage and size of
graphene monolayer are still limited Researchers have hence tried other metal substrates
for graphene synthesis
7
Figure 13 (a) Graphene formation on Nickel (b) Graphene atoms on Ni (111) lattice
(c) Low magnification TEM image of graphene edges (d) Optical image of graphene
transferred from the Ni surface to SiO2Si substrate (e) Full-wafer scale deposition of
graphene layers on polycrystalline Ni (f) Transparent and flexible graphene films on
PDMS substrate10
8
122 Synthesis of Graphene on Copper (Cu)
Graphene films are grown on 25microm thick Cu foils in a hot wall furnace13
The Cu foil is
first annealed in hydrogen atmosphere at 1000degC and a mixture of H2CH4 is introduced
into the system to initiate graphene growth After a continuous graphene layer is formed
on the Cu foil the system is cooled to room temperature Figure 14a shows an SEM
image of graphene on Cu substrate indicating the Cu grains with contrast The Cu
surface steps are formed during thermal annealing and the darker flakes indicate multiple-
layer graphene (Figure 14b)10
The graphene wrinkles in Figure 14(b) originate from
different thermal expansion coefficient of graphene and Cu They go across the Cu grain
boundaries indicating that the graphene film is continuous
Figure 14 (a) SEM image of graphene on copper foil (b) High-resolution SEM image of
graphene on Cu10
123 Transfer of Graphene films
In order to facilitate the applications of graphene for electronic applications we need to
separate the graphene from the catalytic metal substrate Figure 15a shows the transfer
process of graphene Graphene is first coated with a thin layer of polymethyl
methacrylate (PMMA) and baked at 120degC to evaporate the solvent10
The metal layer is
then removed by Ni or Cu etchant leaving behind the PMMA graphene film The film is
then cleaned by deionized water and then transferred onto the target substrate After the
9
evaporation of water vapor the PMMA is removed by acetone leaving graphene film on
top of the target substrate Figure 15b shows a graphene wafer transferred from the
substrate onto glass and polyethylene terephthalate (PET) films
Figure 15 (a) Transfer process (b) Wafer-scale synthesis of graphene (c) Graphene
films transferred onto glass wafer (d) SiSiO2 with device patterned (e) PET film10
124 Synthesis of Graphene Junction
Graphene junctions with smooth armchair and zigzag edges are difficult to produce by
conventional methods such as mechanical exfoliation chemical exfoliation or lithography
etching14
The conventional methods can only produce rough edges Recently
Dresselhaus reported an edge reconstruction of graphene by Joule heating in a TEM-STM
10
(Figure16b) system15
An individual nanoribbon sample is attached to the sample holder
at one end and to the STM tip at the other end these ends also serve as the two
electrodes The structural transformation in the growth of graphene from armchair to zig-
zag is mainly attributed to the vaporization of carbon edges that reconstruct at high
temperatures in which resistive Joule heating and preferred current flow play an
important role This means that by controlling the flow of current a perfectly smooth
edged ribbon can be synthesized making graphene-based electronics possible16
Figure 16 (a) High-magnification image of the annealed sample showing that well-
defined zigzag armchair and zigzag-zigzag edges are formed (b) STM image of an 8 nm
wide bent junction connecting an armchair and a zigzag graphene nanoribbon which was
carved by STM tips14
125 Doping in Graphene
The doping of graphene can be roughly classified into two categories - electrical and
chemical Electrical doping involves changing gate voltages of graphene devices and
chemical doping uses chemical routes such as substitutional or interstitial This thesis
discusses chemical doping and the importance of doping sites by changing the dopant
Chemical doping is a common approach to tailor the electronic properties of
11
semiconductors Doping of graphene can cause its electronic properties to alter leading to
a metal-semiconductor transition The two means of doping graphene are interstitial and
substitutional In interstitial doping the dopant atoms or molecules are introduced as
adatoms or admolecules on the surface of graphene whereas in substitutional doping the
dopant atoms are replaced in the carbon lattice forming a bond in the lattice of
graphene16
Doping graphene results in the formation of n or p-type semiconductors
depending on the kind of dopant If the dopant is an electron donor it causes the Fermi
level to shift up resulting in n-type behavior of graphene Furthermore if the dopant is an
electron acceptor it causes the Fermi level to shift down resulting in a p-type behavior of
graphene (Figure 17)16
Figure 17 Band structure of graphene before and after doping The image shows shift
towards the Fermi level16
Graphene nanoribbons (GNR) can be made into a p- and n- type semiconductor
by doping with boron (B) and nitrogen (N) respectively In theory GNR p-n junction is
formed by doping GNR with B and N in different regions However experimentally
doping graphene with both these elements is very difficult due to the dopants reacting
with each other17
Hence most experimental studies use GNR doped by only one
12
element N-doped graphene was synthesized by Wei et al Wang and B-doped Graphene
was realized by Endo17
Many researchers have demonstrated interstitial doping of graphene by gas metal
and organic molecules16
The various gases and metals used are NO2 NH3 An-CH3 Na-
NH2 F4-TCNQ TPa TCNE and others16
Doping in graphene is hence possible by
electrons or holes in high concentration without deterioration of its mobility Interstitial
doping is highly sensitive due to most of the conducting channel being exposed to surface
absorbates and hence can be used in molecule detection
In substitutional doping the dopant atoms are included in the graphene lattice and
thus chemically bonded Substitutional doping is done via the CVD method using a
carbon and dopant source Substitutional doping opens up many applications in device
engineering making graphene a very good candidate as a semiconductor This study
involves the study of transport properties of graphene doped by substitution
126 Nitrogen (N) Doped Graphene Synthesis (Substitutional)
N-Doped graphene is prepared via a CVD process using a 25microm thick Cu film on a Si
substrate The substrate is placed in a quartz tube with the flow of hydrogen (20sccm) and
argon (100 sccm)18
When the center of the furnace reaches 800degC 60 sccm of CH4 and
60 sccm of NH3 is introduced into the flow as C source and N source respectively The
substrate is then moved to high temperature and after 10 min growth the sample is
cooled to room temperature under H2 ambient Figure 1 8 shows the growth of N-doped
graphene18
13
Figure 18 Low resolution TEM image of N-doped graphene Background is the lacey
carbon TEM grid graphene sheet is crumpled with many ripples18
13 Structure of Graphene Nanoribbon (GNR)
Graphene Nanoribbons (GNR) are strips of graphene with very thin width of lt50nm
GNRs can be terminated in three separate ways called zig-zag (0 n) armchair (m 0) and
chiral (m n) (Figure19) and this termination along the width of the ribbon dictates the
size of the band gap19
Figure 19 Zigzag and Armchair orientation of Graphene5
Due to their various edge structures GNRs exhibit different electronic properties
ranging from normal semiconductors to spin-polarized half metals which open the
possibility of GNRs as electronic devices19
14
Within a tight binding approach (AGNRs) could be metallic or semiconducting
depending on their ribbon width but all zigzag graphene nanoribbons (ZGNRs) are
metallic with a high density of electronic states at the edges Hence ZGNRs exhibit
characteristic edge effects which are not present in AGNRs These edge effects in
ZGNR create a flat band close to the Fermi level making the ZGNR edges more
reactive19
First-principles calculations show that the GNRs possess a non-zero direct
band gaps These gaps are small for ZGNR (Figure 110) caused due to spin ordering
effects at the edges For AGNRs the band gap arises from quantum confinement (Figure
111) effect that has larger magnitudes than ZGNR20
Figure 110 Band structure of ZGNR
15
Figure 111 Band structure of AGNR
For GNRs the band gap decreases as the ribbon width increases and in order to
create a semiconductor with a desirable band gap the nanoribbon width should be
adjusted accordingly This property of adjusting the band gap makes graphene an
excellent candidate for transistor switching By applying an electric field GNR can be
altered from an insulator to a conductor GNRs exhibit very intriguing properties and
have become one of the promising candidates for electronic applications
14 Overview of Graphene Junction
The invention of p-n junctions date back to 1940s which later resulted in the invention of
junction transistors One of the key technological reasons for success of the p-n junction
is mainly due to its ability to locally modulate the energy band gaps via an applied bias21
A graphene p-n junction is created via single layer of graphene in which the
carrier type and density in two adjacent regions are controlled by electrostatic gating8
For materials with a band gap the electric field can either switch lsquooffrsquo the current or
rectify it (p-n diode)22
Being a ldquogaplessrdquo material the off state is not achievable in
16
graphene In order to achieve an off state the gap can be created by doping graphene with
various elements (Group III or Group V) Doping allows p-n junctions to be
reconfigurable using a gate voltage to distinguish between graphene p- n regions within a
single sheet Many researchers have studied the electronic as well as transport properties
of doped graphene junctions
In 2009 Fangping OuYang studied the transport properties of T-shaped graphene
junctions using the ATK software and showed that the conductance depends on
geometric structures which can be controlled by selective doping23
Wei Yao in 2013
studied the transport properties in graphene p-n junctions and showed that the
rectification effect depends on boron doping density and position17
The study of transport properties in graphene p-n junctions is a recent
advancement The thesis discusses transport properties including the current-voltage (I-
V) characteristics of doped graphene junctions Moreover the software used is similar to
the software in use by current researchers since they have produced viable data using
ATK
17
CHAPTER 2
RESEARCH BACKGROUND
21 Band Structure of Graphene
The unique electronic properties of graphene were first predicted in 1946 Figure 21
shows a top view of the hexagonal arrangement of carbon atoms in real space as well as
the first Brillouin zone in reciprocal space
Figure 21 Left Real space graphene lattice with basis vectors and Right The
first Brillouin zone of graphene in reciprocal space with basis vectors and
K and
Krsquo are responsible for massless transport at low energy24
The real space basis vectors are radic
and
radic
The reciprocal space basis vectors are 1 2
0 0
4 1 3 4 1 3( )and ( )2 2 2 23 3
b x y b x ya a
where the magnitude of the basis vectors is |a0| = radic acc The distance between nearest
neighbor carbon atoms is acc=0142nm
18
The band structure can be calculated by solving the eigenvalues using the
dispersion relation E( )
1 2 3( ) 3 2cos 2cos 2cosE k t k a k a k a (21)
Transport properties of solids are closely related to the energy dispersion
relations E ( ) in the material and in particular to the behavior of E ( ) near the Fermi
level Graphene is a zero gap semimetal whose specific linear electronic band dispersion
near the Brillouin zone corners (Dirac points) gives rise to electrons and holes that
propagate as massless Fermions25
The valence and conduction bands do not overlap in
graphene they touch at the Fermi Level (Figure 22)
Figure 22 Band structure of a graphene sheet showing a band gap of 0eV
The low energy properties of graphene can be well described by making a linear
expansion of the band structure around the K and Krsquo This energy can be written as
19
E(k) = plusmnħvF|k (22)
where vF is the Fermi velocity of 1106ms given by
1F
Ev
k
ħ (23)
Figure 23 Band structure of graphene calculated with the tight-binding model
22
The Fermi surface of graphene consists of double cones with Fermi energy at the
intersection of these cones (Figure 23) The slope of the band is zero and hence the
effective mass of electrons in that region is zero which leads to an entirely new transport
mechanism in graphene26
20
22 Transport Characteristics of Graphene
Transport process usually involves a flow of charge or energy or both The flow is mainly
due to external perturbations such as electric field and temperature gradient The
relationship between forces and flow usually defines various transport coefficients that
are the characteristics of electrons and phonons in the material All modern electronics
are based on the ability to control the electronic properties of a material by applying
external voltage This is done by an electric field effect where the gate voltage changes
the carrier concentration of the material and consequently its conductivity The electric
field effect in graphene was reported by Novoselov in 2004 and is used in transport
measurements8
The electron-phonon interaction in graphene plays an important role in
understanding the photoemission spectra observed in graphene The electric field effect is
an alternative method for changing the charge carrier density in low dimensional systems
The electric field effect in graphene which was first reported by Novoselov et al in
2004 is widely used as a characterization tool in transport measurements25
The transport characteristics of the material are directly related to the
bandstructure of graphene The carriers in graphene lattice are free to move in two
dimensions In the carrier transport of graphene the carriers ndash electrons and holes ndash close
to the Dirac points are of importance The transport is described by a two component
wave function (Equation 24) which obeys the 2D Dirac-like equation for massless
particles27
21
-ivFσ nablaψ(r) = Eψ(r)
(24)
where σ is the 2D Pauli spin matrix In the continuum limit the above (Equation
24) corresponds to the effective low energy Dirac Hamiltonian (Equation 25)
0( )
0
x y
F F
x y
iH k k
i
k kv v
k k
(25)
The electronic band structure of the energy (E) versus wave vector (k) relation for
graphene is given by Equation 24
The two component wave function resembles the spin or wave function of
quantum electro dynamics (QED)27
Corresponding to the spin of particles in QED the
charge carriers of graphene can be attributed with a pseudospin σ The pseudospin is the
direct result of two different carbon sublattices corresponding to the bonding and
antibonding combinations27
22
Figure 24 The energy dispersion around the K point27
In Figure 24 the red and blue lines correspond to the antibonding and bonding
states respectively The pseudospin can have two values either in the direction of or
against the momentum It can be seen that the electrons with energy E travelling in the
positive direction originates from the same branch as a hole with energy ndashE travelling in
the negative direction giving it the same pseudospin This results in suppressed
backscattering and Klein tunneling The back scattering process requires the pseudospin
to flip which is possible in the presence of short range scatters that act differently on sub
lattices27
23 Drude Theory
The classical theory of metallic conductivity was presented by Drude in 1900 and was
elaborated by Lorentz in 190528
Drude treated the free electrons as classical ideal gas
meaning the electrons collide with stationary ions and not each other
23
Figure 25 Electrons colliding with stationary ions28
The Drude theory applied the kinetic theory of gases to a metal considered as a gas of
electrons The basic assumptions made by the Drude theory are28
When metallic elements are brought together to form a solid then the valence
electrons become freely moving through the metal whereas the ions remain intact
as nearly immobile positive particles
Between collisions the electrons move freely ie there is neither electron-
electron interaction nor electron-ion interaction
The scattering mechanism leads to instantaneous collisions of the electron with
the scatterers
The collisions are characterized by a relaxation time τ
The electrons achieve thermal equilibrium only through collisions the velocity
after a collision is randomly directed the speed is as appropriate to the
temperature
With the relaxation time Drude obtained the electrical conductivity expression
where n is the number of electrons per unit volume
σ = ne2τm
(25)
He also calculated the thermal conductivity and successfully provided the
theoretical basis for Wiedemann-Frantz law already established in 1853 which states that
24
the ratio of electrical and thermal conductivity of any metals is a universal constant at any
given temperature28
The Drude theory gives results which are qualitatively correct outside of the
quantum Hall regime28
In the Drude theory of the electrical conductivity of a metal an
electron is accelerated by the electric field for an average time τ before being scattered
by impurities lattice imperfections and phonons to a state which has zero average
velocity The average drift velocity of the electron is
d
eE mv (26)
It is assumed that all electrons drift together and hence the current density
j = -ne (27)
This Drude theory works well for fields below ~ 01T At stronger fields the Hall
resistivity becomes nearly constant over finite intervals of magnetic fields28
The QHE
reflects both novel disorder physics as well as novel interaction physics in the quantum
Hall regime
24 Quantum Hall Effect (QHE)
The discovery of QHE is a remarkable achievement in condensed matter physics The
Hall Effect was discovered by Edwin Hall in 187929
However the precise quantization
of the Hall conductance in units of e2h was not recognized until February 1980 Five
years later in 1985 Klaus von Klitzing was awarded the Nobel Prize in Physics for the
discovery of QHE29
The quantum Hall effect occurs in two-dimensional electron systems in the limit
of strong perpendicular magnetic field that stems from electronic transport
25
measurements where one drives a current I through the sample and where one measures
both the longitudinal and transverse resistance (Hall resistance) A longitudinal resistance
is a resistance measured between two contacts that may be connected by a line which
does not connect C1 and C430
Transverse resistance is measured between two contacts
connected by an imaginary line connecting C1 and C4 (Figure 26a)
Figure 26 (a) 2D electrons in a perpendicular magnetic field Logitudinal resistance
measured across C5 and C6 Transverse resistance measured across C3 and C5
(b) Classical Hall resistance as a function on the magnetic field30
Due to the existence of quantum Hall effect it is natural to expect that there exists
a classical Hall Effect Hall showed that the transverse resistance of a thin metallic plate
varies linearly with the strength B of the perpendicular magnetic field (Figure 26 b)
RH = Bqnel (28)
More quantitatively the classical Hall Effect can be understood within the Drude
model for diffusive transport in a metal Within this model one considers independent
26
charge carriers of momentum p described by the equation of motion
( )
b
dp p pe E B
dt m (29)
where E and B are the electric and magnetic field respectively The macroscopic
transport characteristics ie resistivity of the system are obtained from the static
solution of the equation of motion dpdt = 0 and one finds for 2D electrons with p =
(pxpy)
x
x yb
y
y xb
eBe
eBe
ppE
m
ppE
m
(210)
In the above expression characteristic frequency is visible as
C
b
eB
m (211)
This is known as cyclotron frequency as it characterizes the cyclotron motion of a
charged particle in a magnetic field30
With the Drude theory the conductivity can be
written as
j = -enelpmb (212)
and the mobility can be given as
micro = eτmb (213)
The transport properties in the limit of ωCτ-gt infin are entirely governed in the presence of
27
a magnetic field by the off-diagonal ie transverse components of
conductivityresistivity
The theory of quantum Hall effect subjects all physical properties of 2D electron
system in the limit where the magnetic field is strong so that the mixing of Landau levels
by disorder or electron-electron interaction is considered to be a weak perturbation30
This is known as the quantum Hall regime The ratios between the energy scales
corresponding to the two interactions are important The limit where disorder potential is
much stronger is referred to as integer quantum hall regime whereas the limit where the
interaction potential is much stronger is referred to as fractional quantum Hall regime
25 Resistivity and Resistance
The electronic transport in the framework of the Drude theory allows for the calculation
of conductivity or resistivity of a classical diffusive 2D electrons in a magnetic field30
The conductivity and conductance are related to one another but they depend on the
geometry of the conductor-the resistance R and hence the resistivity is given by
R = (LA)ρ (214)
where L is the length of the conductor and A is the cross section
For a d-dimensional conductor the cross section scales as Ld-1
such that the
scaling relation between the resistance and the resistivity is
R~ ρL2-d
(215)
From the dimension point of view resistance and resistivity are the same in 2D and the
resistance is scale-invariant Further the resistance of a 2D conductor depends in
general on the so-called aspect ratio LW via some factor f (LW)30
However for
transverse Hall resistance it is the length of the conductor that plays the role of cross
28
section such that the Hall resistivity and the Hall resistance truly coincide ie f=1 The
Quantum Hall effect is highly insensitive to the particular geometric properties of the
sample used in transport measurements Recently quantum Hall physics experienced the
discovery of ldquorelativisticrdquo quantum Hall effect in graphene The electrons in graphene
behave as if they were relativistic massless particles contributing to a very interesting
field of research30
26 Klein Tunneling
Klein tunneling in which relativistic particles penetrate through a potential barrier
without the exponential damping that is characteristic for nonrelativistic quantum
tunneling has never been observed for elementary particles The tunneling allows
transmission of a particle through a potential barrier higher than its kinetic energy
violating the principle of classical mechanics30
On the quantum scale the objects exhibit
wave-like characteristics in which the quanta move against a potential hill described by
their wave function This wave function represents the probability amplitude of finding
the object in a particular location The transmission of the object through the potential hill
is termed as tunneling When EltV then the ψ(x) over V is returned by ψrsquo(x) In quantum
mechanics an electron tunnels from the conduction into the valence band Such a
tunneling from an electron-like to hole-like state is called as Klein Tunneling in which the
electron avoids backscattering
In Figure 27 it is shown that an electron hitting a potential barrier is reflected
with 100 certainty In non-relativistic quantum mechanics the electrons can tunnel
through the barrier but the probability of tunneling exponentially decays with increasing
29
height and width of the barrier However in relativistic quantum mechanics the barrier
gets transparent even in the limit of infinite barrier height (Klein paradox)31
Figure 27 Klein tunneling through an npn barrier30
The Klein paradox in graphene can be understood in terms of electrons and holes
In graphene the massless carriers behave differently than ordinary carriers (with mass) in
the presence of an electric field A barrier which is repulsive for electrons will be
attractive for holes Since there are hole states inside the barrier with the same energy as
the electrons outside an electron arriving at the barrier can tunnel through it as a hole
before leaving again as an electron Klein tunneling for transport in graphene is that the
charge carriers cannot be confined by potential barriers The Klein tunneling effect has
been experimentally observed by Ando in 1998 in which the absence of backscattering
(Figure 28) is responsible for high conductivity in carbon nanotubes
30
Figure 28 Electron trajectory considering the linear electrostatic potential U(x) = Fx30
The electron is able to propagate through an infinitely high potential barrier since
it makes a transition from the conduction band to valence band In this transition from
conduction band to valence band its dynamics changes from electron-like to hole-like
The equation of motion is thus given by
2
2 2 2| | ( )
pdr E
dt E Up
p E U
v
v
at energy E (216)
This shows that in the conduction band (UltE) and in the valence band (UgtE)
In Klein tunneling the pairs of electron-like and hole-like trajectories at the same E and
py have turning points at dmin given by dmin=2v|py|F (Figure 29)
Figure 29 Electron like and hole like trajectories at same E21
31
The tunneling probability exponential dependence on dmin
2
min| |
( ) exp( ) exp( )2
y y
y
vT
F
p pdp
(217)
The applications of the Klein tunneling include Atomic clock Scanning tunneling
Microscope Tunnel diode Tunneling transistor and many more32
Since graphene
exhibits Klein tunneling it can be very useful to study the transport properties in
graphene and use it in such applications
27 Quantum Hall Effect in a Graphene
A monolayer graphene shows half-integer quantum Hall effects where the Hall
resistance is quantized at values of
2
1
xyh v eR
(218)
around filling factors
14( 1 2)Nv
(219)
where N is an integer e is the electron charge h is the Planckrsquos constant and the
factor 4 is due to spin and valley degeneracy QHE in graphene can be observed at room
temperature which is a very intriguing property (Figure 210) Graphene reveals
significant differences with respect to conventional 2D electron systems The Landau
quantization yields energy levels that disperse differently in graphene as well as
particular zero-energy level that is only half filled at the charge neutrality point (v=o)
32
Figure 210 Quantum Hall effect in graphene22
The Hall conductivity σxy and the
longitudinal resistivity of monolayer graphene as a function of carrier density at B = 14T
and T= 4K This shows half-integer QHE with chiral index J= 1
The QHE in graphene is not entirely similar to regular QHE since the charge
carriers in graphene are Dirac Fermions The charge carriers governed by
electrodynamics is given by (Equation 220) which does not apply for graphene and a
QED quantization of graphene electronic band structure is used
En = (n+12)ħω (220)
33
In the presence of magnetic field the nature of the Dirac Fermions in graphene
results in unevenly spaced Landau levels (LL) containing a distinctive LL at the electron-
hole degenerating a zero energy given by
2MG
MGFehn B
n vE (221)
The LL levels at high magnetic fields in MG are shown in Figure 211
Figure 211 (a) LL for Graphene bilayer (b) Schematics of Hall conductivity as a
function of nn0 for bilayer Graphene (solid line) and monolayer Graphene (dotted line)
(c) LL for monolayer Graphene33
It is found that the Hall resistance of a two dimensional electron system has
plateaus as a function of the number of electrons at low temperatures and strong magnetic
fields32
At large B the Dirac-like energy spectrum of graphene gives rise to a
characteristic series of QH plateaus in conductance reflecting the presence of a zero-
energy Landau level that include only odd multiples of 2e2h for uniform carrier density
in the sheet These plateaus of QH edge states at the edge of the sheet circulating in a
34
direction are determined by the direction of B and the carrier type33
This is why QHE in
graphene is known as Half-Integer Quantum Hall Effect
28 Thermoelectric Effect
Thermoelectricity refers to a class of phenomena in which a temperature difference
creates an electric potential or an electric potential creates a temperature difference The
principle of thermoelectric effect has been known for over 100 years Recently the
practical applications of thermoelectric effect have become more viable34
Thermoelectric effect is the direct conversion of temperature differences to
electric voltage and vice versa Joule heating is the heat generated whenever a voltage is
applied across a resistive material The Peltier-Seebeck effect is reversible whereas Joule
heating is not This effect can be used to generate electricity to measure temperature to
cool objects or to heat them Since the direction of heating and cooling is determined by
the sign of the applied voltage thermoelectric devices make very convenient temperature
controllers
281 Seebeck Coefficient
Thomas Johann Seebeck discovered that an emf appears in a circuit composed of two
dissimilar metals when the junction between the metals is held at different
temperatures34
The thermoelectric emf causes a continuous current in the circuit when a
complete loop is formed and the current is known as thermoelectric current This is
known as the Seebeck effect
35
Figure 212 Seebeck Effect34
As long as the two junctions are at different temperatures the thermoelectric emf
exists and the current will keep flowing between the hot and cold junction that are at
different temperatures The Seebeck effect is the conversion of temperature difference
directly into electricity The voltage developed in the circuit shown in Figure 212 is
proportional to the difference in temperature between the two junctions and is given by
V = α (T2-T1) (222)
This Seebeck effect is observed not only in metals but also in semiconductors
Here α is known as the Seebeck coefficient α measures the magnitude of an induced
thermoelectric voltage in response to the temperature difference across the material If the
temperature difference ∆T between the two ends of a material is small then the Seebeck
coefficient of a material is written by
α = ∆V∆T (223)
36
This can be expressed in terms of electric field as
α E∆T (224)
The units of Seebeck coefficient is given as VK The higher the Seebeck coefficient
value the better it is since it will create a very large voltage that can be used to provide
power
282 Peltier Coefficient
Peltier effect is the inverse of Seebeck effect involving a junction phenomenon There is
heat absorption or generation at the junctions depending on the direction of current flow
Heat generated by current flowing in one direction is absorbed if the current is reversed
The heat absorbed per second at a junction carrying current I is given by
Heat absorbed in t sec = πabIt (225)
Here πab is the Peltier coefficient and given by HIt Thus Peltier coefficient is
numerically equal to the applied potential difference expressed in Volts
Overall by studying the flow of electrons the values of Seebeck
coefficient and Peltier co-efficient can be estimated These values determine the various
applications of the materials In this thesis the Peltier and Seebeck coefficient of the
graphene junction and the new applications are discussed
37
29 Early Research ndash ab intio studies
In 2007 Androitis studied that the conducting properties of graphene nanoribbons and
junctions are strongly dependent on their size and geometric features35
He concluded that
there is no conductance for small AZA or ZAZ ribbons (Figure 213)
Figure 213 Transmission functions in units of (2e
2h) for AZA structures
35
Figure 213 shows that T (E) exhibits a negligible peak [T (E) = 001 in units of
2e2h] at E= -225 and 250eV However it was noted that when the width of the arm type
was increased T (E) at -225 and 250eV was 02035
Later in 2007 Qimin Yan used first principles methods to investigate the Current-
Voltage characteristics of GNR Transistors and the effect of edge doping He showed that
GNR field effect transistors can achieve high performance levels with ONOFF ratios on
the order of 103-10
436
Figure 214 is an I-V curve of AZA GNR-FET connected via
armchair metallic leads36
38
Figure 214 I-V curve for a 591nm long channel (Vbias=20mV)
36
In 2009 Fangping OuYang demonstrated the intrinsic transport properties and
effective B or N doping of the junctions by using first-principles quantum transport
simulations He concluded that the I-V characteristics of pure-carbon T-shaped junctions
exhibit metallic behavior and the current in the junction strongly depends on the height
of the stem23
He reported that the conductance of the devices depends on the geometric
structures which can be controlled by selective doping
In 2012 Wei Yao used the first principle calculations based on Density
Functional Theory (DFT) and Non-equilibrium Greens Function (NEGF) to study the
electronic as well as the transport properties of B-doped 6-GNR p-n junction His results
showed that the boron doping interval can influence the rectification effect at low bias
and also exhibit Negative Differential Resistance (NDR) phenomena at high positive
bias
39
CHAPTER 3
COMPUTATIONAL DETAILS
31 Introduction
The physical chemical electrical electronic and optical properties of a solid are
determined by their quantized electronic states The quantum states in low-dimensional
systems are produced due to the confinement of the carrier charges in one or two
dimensions Graphene is a conductor electrons are able to flow through graphene more
easily than through even copper The electrons can travel through the sheet of graphene
like mass-less particles as fast as just one hundredth that of the speed of light The ways
in which electrons behave in graphene make it very helpful to study their fundamental
physical properties Graphenersquos near perfect crystal lattice provides a very clean system
to experiment By restricting the electrons to only two dimensions they exhibit some
interesting properties such as the anomalous quantum Hall effect and Klein tunneling
In this chapter two theoretical concepts used for calculating the electronic structure
and the transport properties for graphene are described These include the Extended
Huckel Theory and Non-Equilibrium Greenrsquos Function (NEGF) method
311 Extended Huckel Theory
Erich Huumlckel was born in Germany on August 9th
1896 He studied mathematics and
physics in Berlin He is best known for his work in the field of chemistry and physics for
two contributions (1) Debye- Huumlckel theory of electrolytic solutions (2) Huumlckel
method of approximate molecular orbital calculations on electron systems In 1930 he
published his findings on systems in 1931 he generalized and expanded the system
40
theory to explain benzene Due to his poor communication skills his findings went
unrecognized for over 20 years It was in 1951 that his 4n + 2 rule was finally clarified by
Doering to show if C=C bonds would show aromaticity Huumlckel died on February 16th
1980 with very little worldwide recognition for his contributions to chemistry Today
chemistry students recognize his name and his contributions to the field are quite
substantial
One of the first semi-empirical methods to be developed was Huumlckel Molecular
Orbital Theory (HMO) HMO was developed to describe molecules containing
conjugated double bonds HMO considered only electrons in pi orbitals and ignored all
other electrons in a molecule The Extended Huumlckel Molecular Orbital Method (EH) was
developed out of the need to consider all valence electrons in a molecular orbital
calculation
By considering all the valence electrons chemists could determine molecular
structure compute energy barriers for bond rotations and determine energies and
structures of transition states for reactions By considering only the valence electrons the
computed energies could be used to choose between proposed transition states to clarify
reaction mechanisms The total valence electron wavefunction is described as a product
of the one-electron wave functions
1 2 3(1) (2) (3) ( )valence j n (31)
where n is the number of electrons and j identifies the molecular orbital Each
molecular orbital is written as a linear combination of atomic orbitals (LCAO)
1 12
N
j jr rrc j N
(32)
41
The energy of the jth
molecular orbital is given by a one-electron Schroumldinger
equation using an effective one electron Hamiltonian heff which expresses the interaction
of an electron with the rest of the molecule
eff j j jh (33)
This is the energy eigenvalue of jth
molecular orbital corresponding to the Eigen
function j The advantage of using this method is that the exact form of heff is not
required The total energy of the molecule is the sum of the single electron energies
j jj
E n (34)
where nj is the number of electrons in orbital j
In order to use the Extended Huckel method a set of calculation parameters and
approximations must be followed These parameters include the Basis set K-point and
the Brillouin Zone and lastly the Mesh cut-off
312 Introduction to NEGF
The Greenrsquos function is a function of two space-time coordinates From the knowledge of
this function one can calculate time-dependent expectation values such as currents and
densities electron addition and removal energies and the total energy of the system In
the absence of external fields the non-equilibrium Green function method reduces to the
equilibrium Green functions NEGF can be applied to both extended and finite systems
The generic system of NEGF consists of the electron dynamics of the channel described
by the Hamiltonian This channel consists of two contact reservoirs with respective
chemical potential μR and μL The NEGF assumes ballistic transport neglecting self-
42
energy from scattering The system is insulated from gate contacts whose effects are
realized via a 3D Poisson solver which solves for the potential at a given point in real
space based on electron density
22 ( ) [ ( ) ( )]D
qr N r n r
(35)
Figure 31 NEGF system
The system is easily expandable to systems with several contacts or gate
configurations by adding additional self-energy matrices to NEGF or additional sources
to the Poisson solver
313 Electrostatics
Electrostatic potential is created every time in the presence of a charge density due to an
induced electric field The Poissonrsquos equation correlates the electrostatic potential to
charge density as given in Equation 36
43
2( ( ) ( ) ( ) ( ))( )
( )( ) ( )
ADq p r n r r N rr
rr r
N
(36)
where ɛ(r) is the dielectric permittivity of the material ρ(r) n(r) ND(r) and NA(r) are the
hole electron donor and acceptor concentrations of the system respectively
Two types of boundary conditions are usually applied to the Poissonrsquos equation
Dirichlet boundary conditions
Φ (0) = F0 and Φ (L) = FL
von Neumann boundary conditions
00
( )
x
d x
dxB
and
( )L
x L
d x
dxB
For the transport problems with open boundary conditions the von Neumann
boundary conditions are used assuming that the potential vanishes at the boundary ie
B0=BL=0
The Poissonrsquos equation can hence be discretized on a grid as
2 ( )( )
( )
rx
r
= M (37)
where M is the matrix Φ and ρ are vectors containing the discretized values of
the electrostatic potential Φ and charge density ρ respectively
44
The Schroumldinger and Poisson equations are coupled since V(x) = -qΦ(x) is used
for the Schroumldinger to compute ρ(x) This self-consistent loop stops when the
convergence is reached
( )r
V(x) = -qΦ(x)
314 Non-Equilibrium Greenrsquos Function
Greenrsquos functions are a mathematical construction that are used to solve differential
equations subject to specific initial or boundary conditions They are named after the
British mathematician George Green The 1-D equation of L( )f( )=S( ) can be defined
by the Greenrsquos Function as given below
( ) ( ) ( )G x x f x x x (38)
The general Greenrsquos function is given by
( ) ( ) ( )f x dx G x x S x (39)
Applying the operator L( ) to the solution f( ) satisfies the original differential
equation The Greenrsquos Function G( ) is the propagator which propagates the influence
of a perturbation S( ) originally situated at the point to the point at which the
function f( ) is evaluated
The Greenrsquos Function G( ) can also be a correlation function If the points
and are strongly (weakly) correlated then S( ) will greatly (poorly) affect f( )
Poisson equation
2 ( )( )
( )
rr
r
Schroumldinger equation
2
2
( ( ) ) ( )
( )2
( ) | ( ) |
E H r E r S
H V rm
r dE E r
Figure 32 Self-consistent loop
45
The Schroumldinger equation with open boundaries can be written as
( )E H S (310)
Considering a 1-D and homogenous system ranging from =0 to L assuming
that Σ=0 and the form of equations is same before and after discretization then
22
2 0( ) ( ) ( )
2E x S x
m
dV
dx
(311)
The Greenrsquos function can hence be computed corresponding to the Schroumldinger
equation
22
2 0( ) ( ) ( )
2E G x x x x
m
dV
dx
(312)
Due to the delta-function at = a discontinuity is observed and hence the
Greens function is evaluated at boundary conditions
0
2
exp( ( )) x x 2 ( )( )
exp( ik(x x)) x x
ik x x m E VG x x k
A
A
(313)
By integrating the Schroumldinger equation twice and setting the lower and upper
integration boundaries to = -δ and = +δ the Greenrsquos Functions can be written as
2
( ) ( ) 0
( ) ( ) 2
x x x x
G x x G x x
dG x x dG x x m
dx dx
(314)
46
The coefficient A+ and A
- become
ik
mA A
(315)
The Greenrsquos Function takes a final form known as Retarded Greenrsquos Function and
is written as
( ) exp( | |)G x x i ik x xk
m (316)
And the wave function is
( ) ( ) ( )x dx G x x S x (317)
Retarded Greenrsquos Function propagates the wave functions generated by a source
or perturbation S from its origin at to any point
The retarded Greenrsquos Function as discretized Schroumldinger equation is written as
( )R RE H G I (318)
The wave function Φ can be calculated from the retarded Greenrsquos function and the
source vector as
Φ = GR∙S (319)
Overall in this section the Greenrsquos function approach in calculating the electron
dynamics is reviewed We defined the self-energy of each part of the system spectral
function and the probability current density the electric current is derived explicitly using
Non Equilibrium Greenrsquos function We will use this formalism to calculate the tunneling
phenomena in coupled quantum dots isolated or otherwise
47
CHAPTER 4
ATOMISTIX TOOLKIT DETAILS
41 Introduction
Virtual NanoLab (VNL) is a graphical user interface (GUI) that provides a group of
modeling tools the function of these tools involves the set-up investigation and the
study of nanoscale structures The quantum mechanical equations are solved by the
software by using the advanced software architecture and numerical methods to
implement ab initio calculations VNL simulates the electronic structure and calculates
the transport properties based on the two systems mentioned earlier NEGF and Extended
Huckel ATK is the main engine for computing the scripts and hence all the calculations
performed in VNL are done by ATK VNL is a user friendly software as it not only
allows creating a script but also helps to set up a virtual experiment
This thesis involves the use of VNL in order to study the effect of the width and
different orientations of the doped atoms Since the software allows for virtual
experiments it makes it much easier to study the I-V characteristics based on the change
in position of atoms
42 Device Structure
In this thesis AZA GNR p-n junction with boron doping (location) was created using the
ATK software which is based on NEGF and DFT Further the thesis discusses the
transport properties and the I-V curve of such junction
The input format of ATK is NanoLanguage which is an extension to Python
scripting language ATK uses the NEGF system for formalism of simulating device
48
Figure 41 Geometry of device configuration with two electrodes
37
The system is divided into three parts left central and right The implementation
relies on the screening approximation which assumes that the properties of the left and
right regions can be decribed by solving a bulk problem for fully periodic electrode cell37
This screening approximation is fulfilled when the electrode regions can be described by
an equilibrium electron distribution
Figure 42 The electron distribution in a device configuration which illustrates a left
moving scattering state with origin in right electrode37
The system assumes that in steady state the electron density of the central region
is constant in time and hence the electron density is calculated independently from each
electrode The electron density is given by the occupied eigenstates of the system
n(r) = nL(r) + n
R(r) (41)
49
The left and right densities are calculated by summing up the occupied scattering
states
nL(r) = sum
(42)
nR(r) = sum
(43)
The scattering states are usually calculated by first calculating the Bloch states in
the electrodes and then solving the Schroumldinger equation of the central region using the
Bloch state as matching boundary Instead of using the scattering states the ATK
software uses the NEGF method to calculate the non-equilibrium electron density
The electron density is given in terms of electron density matrix
D = DL + D
R (44)
The left density matrix is given by NEGF theory
DL = int
(45)
where
ρL(ɛ) =
(46)
ρL(ɛ) = is the special density matrix
Also if there is a non-equilibrium electron distribution in the central region then
the electron distribution in electrode is given by the Fermi function f with an electron
temperature TL
G(ɛ) =
(47)
G = retarded Green function
δ+ is an infinitesimal positive number and S H overlap the Hamiltonian matrices
L =
sum sum
(48)
50
L
is the broadening function of the left electrode given in terms of left electrode
self -energysum
43 Transmission Spectrum Calculations
Once the self-consistent non-equilibrium density matrix has been obtained the various
transport properties of the system can be calculated One of the most important properties
is the transmission spectrum from which the current and differential conductance can be
obtained
The transmission coefficient in ATK is obtained by the retarded Greens function
T(ɛ) = G(ɛ)ΓL(ɛ)G
ϯ(ɛ)Γ
R(ɛ) (49)
The transmission amplitude of individual scattering states may be obtained
through the Transmission Eigenvalues The ldquoTransmission Eigenvaluesrdquo is an analysis
which finds the eigenvalues of the transmission matrix
The transmission matrix at energy E and k-point is given by
Tnm(Ek) = sum (410)
where
= transmission amplitude from Bloch state ψn(k)
The transmission coefficient is given by the trace of transmission matrix
T(Ek) = sum (411)
Keeping in mind all quantities depend on the quantum numbers parametrically
Transmission eigenvalues sum up to the transmission coefficient
T = sum (412)
51
44 Calculating the Current
Current is calculated from the transmission coefficient using
I( ) ( )R L
L RL R
R LB B
eE f f dE
h
E EV V T T T
k kT T
(413)
where f is the Fermi function TRL is the electron temperature of the right or left
electrode and Tσ(E) is the transmission coefficient for the spin component σ
The chemical potentials of the left and right electrode given by
L
F R LR L
eVE
are defined relative to the Fermi level of the left electrode These chemical potential are
related to the applied bias and hencebiasR L
eV therefore bias L RV V V
The transmission spectrum itself is usually rather insensitive to temperature and is
used in self-consistent calculations but often depends strongly on the electrode voltages
Thus for an accurate estimate of the current the transmission spectrum should be
calculated self-consistently for each desired bias
ATK uses very precise method to calculate the transport properties of the system
Transmission spectra for various concentrations of boron doped graphene p-n junctions
are generated in this Chapter and various coefficients such as Seebeck Peltier and
Conductance are calculated
52
45 Calculating Transport coefficients
The linear response transport coefficient of an applied voltage difference or temperature
difference between the two electrodes is given by
Conductance
| dT 0
e
dI
dUG
(414)
Peltier coefficient
| d 0
Q
I
I
(415)
Seebeck coefficient
| 0
dUS I
dT T
(416)
These linear response coefficients are calculated by the Transport Coefficients To
perform these calculations the ATK uses the Electron Transmission Spectrum
53
CHAPTER 5
RESULTS AND DISCUSSION
51 Band Structure Analysis
The electronic bandstructure of GNR both doped and undoped are discussed in this
chapter
The armchair configuration of Pristine GNR (PGNR) has a band structure that is
dependent on its width This is explained by the fact that the sheet itself acts like a
potential well where the electrons are confined to form standing waves along Cr the
rolling vector albeit with slightly different boundary conditions (Cr = ma1 + na2
where m and n are integers and a1 and a2 are the unit cell vectors of graphene lattice) In
a GNR the two nodal points of the standing wave must be at the ribbon edge while in a
Single wall nanotube (SWNT) they can be anywhere ie a circumferential periodic
boundary condition
(a) (b)
Figure 51 Bandstructure of AGNR widths (a) 4 atoms (b) 5 atoms
54
(a) (b)
Figure 52 Bandstructure of AGNR widths (a) 6 atoms (b) 7 atoms
(a) (b)
Figure 53 Bandstructure of AGNR widths (a) 8 atoms (b) 9 atoms
55
(a) (b)
Figure 54 Bandstructure of AGNR widths (a) 10 atoms (b) 11 atoms
Figure 55 Bandstructure of AGNR with a width of 12 atoms
Figure 56 Variation in band gaps as the width (number of atoms) varies
0
05
1
15
2
25
0 2 4 6 8 10 12 14
Wdith vs Band Structure
eV
56
The band structure of 12 Atom AGNR is close to that of Ge (0626 eV) The
actual width of this nanoribbon is about 25 nm 12 AGNR has been fabricated
successfully and doped with various dopants Hence the 12 Atom AGNR has been chosen
to study the transport properties
A junction is created using ZGNR and AGNR To maintain the consistency in the
device analysis it is imperative that the band structure of ZGNR is also calculated From
the simulation it is evident that ZGNR-AGNR-ZGNR junction configuration displays the
Metal ndashSemiconductor-Metal configuration that is addressed in this work The Fermi
Level in all the Z-GNR nanoribbons of widths 4-12 lies within the conduction band
Figure 57 Band structure of ZGNR width (a) 4 atoms (b) 6 atoms
57
(a) (b)
Figure 58 Band structure of ZGNR width (a) 8 atoms and (b) 10 atoms
Figure 59 Band structure of ZGNR with a width of 12 atoms
In order to create viable junction that would show transistor properties doping of
the semiconductor part is necessary The 12 atom AGNR is doped with boron (p-type)
and nitrogen (n-type) - (Figure 510a) 4 N doped (Figure 510b) 4 B In both cases
the impurities lie on the edge of the atoms For 2 nitrogen doped GNR with the
58
impurities lying in the center of the ribbon the Fermi level is found to be in the
conduction band as shown in (Figure 510c) (Figure 510d) shows the position of N with
respect to the edge A very clear departure from the expected (the valence band extending
above Fermi level) is shown in (Figure 510a)
Figure 510 Band structures of Doped AGNR (a) 4 N Doped (b) 4 B Doped (c) 2
N Doped (d) position of Nitrogen from (c)
(a) (b)
(c) (d)
59
52 I-V Characteristics of GNR junction
In pristine graphene the chirality determines the conductivity as seen from the I-V curves
for various widths At certain widths the semiconducting properties are more
pronounced These widths determine the wavelengths of the standing waves which in
turn determine the sub-band locations in the E-k plot When the biasing potential
exceeds 012V the I-V curve shows linearity In case of the 8-atom wide PGNR the
band gap is about 03 eV and it is evident from the I-V plot that the On-State is + 033 V
The band gap of 10-atom and the 4-atom wide PGNR is large enough to show
semiconducting properties
Figure 511 Current Vs Voltage graph for varying graphene width showing
conductivity
-30000
-20000
-10000
0
10000
20000
30000
-3 -2 -1 0 1 2 3
Cu
rre
nt
(nA
)
Voltage (V) (bias)
Current (nA) Vs Voltage for varying graphene width
W=10
W=8
W=6
W=4
60
The ZAZ GNR Configurations show the properties of a semiconductor junction The 12
atom ZAZ structure is studied for its I-V characteristics In this Chapter undoped B-
doped N-Doped B and N Doped (P-N Junction) ZAZ junctions are simulated
Figure 512 ZAZ GNR junction device
61
The boron doped ZAZ junction I-V characteristics are shown below (Figure 513)
The impurity concentration is 2 and 4 Various device configurations are studied
Figure 513 I-V curve of Boron Doped ZAZ junction
-25000
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
25000
-205 -155 -105 -055 -005 045 095 145 195
Cu
rre
nt
(nA
)
VBias
2B_1G_R 2B_0G_R
4B_0G_L 4B_0G_C
4B_0G_R 4B_1G_L
4B_1G_C 4B_1G_R
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
-2 -1 0 1 2
Cu
ren
t(n
A)
VBias
4 B doped GNR Jn
62
Figure 514 I-V curve of Nitrogen Doped ZAZ
-25000
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
-2 -15 -1 -05 0 05 1 15 2
Cu
rre
nt(
nA
)
VBias
I-V Curve as function of Dopant location
2N_0G_L2N_0G_C2N_0G_R2N_1G2N_1G_C2N_1G_R
-15000
-10000
-5000
0
5000
10000
15000
-2 -1 0 1 2
Cu
rre
nt(
nA
)
VBias
2N_0G_C
2N_1G_C
63
Figure 513 and Figure 514 show the I-V characteristics of the GNR junction doped with
2 boron and nitrogen respectively The location of N and B is at the central region of
the edge of the GNR Both B doped and N doped GNR Junctions show significant
Negative Differential Resistance (NDR) This is more pronounced in case of nitrogen
doping Another interesting observation is increasing ohmic nature with the change in
location of the dopants Nitrogen doped device configuration exhibits a pronounced
semiconductor behavior and the NDR effect is observed to be minimal
53 Thermoelectric Properties
In this study the thermoelectric properties were simulated for the GNR Junctions that
displayed high NDR effect The variation in the Peltier coefficient with temperature is
shown as function of doping
When the concentration of nitrogen increases the dimensionless Figure of Merit
ZT seems to decrease considerably This is mostly explained by the decrease in both
conductivity and mobility of the electrons
ZT = S2σTk (51)
where S is the Seebeck coefficient σ is the electrical conductivity T is the
absolute temperature and k is the thermal conductivity
64
Figure 515 Variation of Peltier coefficient with temperature as function of
doping
Figure 515 shows the maximum Peltier coefficient for 2 boron This is
explained by the scattering by boron and the associated smallest mean free path
0
0001
0002
0003
0004
0005
0006
0007
0008
0009
001
250 270 290 310 330 350 370 390 410
ZT
T (K)
2B
4B
Undoped
2N
4N
65
CHAPTER 6
CONCLUSIONS
Graphene ZAZ junctions exhibit varying properties depending on the various structural
configurations In this thesis it was found that the transport properties of graphene
depend on their width the edge of GNR doping concentration and the type of dopant
used The calculations of the band structure contributed towards the determination of the
minimum length of GNR required for studying the transport properties The minimum
length had a band gap equivalent to that of germanium and hence the importance of the
width being 12 atoms wide This band gap indicated fluctuating changes when doped
with elements such as B and N The viable junction showing transistor properties was
hence created by doping the semiconductor part of ZAZ By doping the I-V
characteristics were studied which showed significant NDR which was more pronounced
in the case of nitrogen Also the changing positions of the dopants contributed towards
the I-V curve to be more ohmic The edge doping caused minimum NDR and
semiconductor behavior as compared to central doping Lastly the thermoelectric
properties were studied - the increasing concentration of N causes the Figure of Merit to
decline due to the decrease in conductivity as well as mobility of electrons
66
REFERENCES
1 Wikianswers What makes carbon unique
httpwikianswerscomQWhat_makes_carbon_so_unique (22 November)
2 Kopeliovich D D Graphite
httpwwwsubstechcomdokuwikidokuphpid=graphite (1128)
3 Barbier M Transport properties of nanostructures and superlattices on single layer and
bilayer graphene University Antwerpen Antwerpen 2012
4 Shylau A Electron transport interaction and spin in graphene and graphene
nanoribbons Linkoping Norrkoping 2012
5 HassJ R F T Li X Li Z Zong W A de Heer P N First E H Conrad C
AJeffrey and C Berger Applied Physics Letters 2006 89 (14) 143
6 Jones A Mechanical Exfoliation to Make Graphene and Visulization
httpcarbonchemwisceduFilesMechanicalExfoliationpdf (18 October)
7 Anteroinen J Structural and Electrical Characteristics of Graphene Field Effect
Transistors AALRO school of Electrical Engineering AALTO 2011
8 Novoselov K S A K G S V MorozovD JiangY Zhang S V Dubonos I V
Grigorieva A A Firsov Science 2004 306 (22)
9 Kosynkin D A L H A Sinitskii J R Lomeda A Dimiev K B Price and J M
Tour Nature 458 876
10 Yi Z Luyao Zhang Accounts of chemical research 46 (10) 2339
11 Eizenberg M B JM 1979 82 236
12 Yu Q K L J Siriponglert S Li H Chen Y P Pei S S Applied Physcis
Letters 2008 93 (113103)
13 Li X C W An J Kim S Nah J Yang D Piner R Velamakanni A Jung I
TutucE Banerjee S K Colombo L Ruoff R S Science 2009 324 1314
14 Schaefer H E Nanoscience Springer Berlin 2010
15 Levente Tapasztoacute G D Philippe Lambin amp Laacuteszloacute P Biroacute Nature Nanotechnology
2008 3 401
67
REFERENCES
16 Dacheng Wei Y L Advance Materials 2010 22 (30) 3241
17 Wei Yao K L Y GYGao Elsevier Solid State Communications 2013 153 52
18 Dacheng Wei Dagger Yunqi Liudagger Yu Wangdagger Hongliang ZhangdaggerDagger Liping HuangdaggerDagger
Yudagger a G NanoLetters 2009 9 (5) 1758
19 Nakada K M F G Dresselhaus and M S Dresselhaus PhysRevB 1996 54
(9858)
20 Son Y W C M L a L S G PhysRevLett 2006 97 (216803)
21 Raza H Graphene Nanoelectronics Springer 2012
22 Ryan W J Electronic Transport in Graphene p-n junctions Short Noise and
Nanoribbons Harvard University 2009
23 Fangping OuYang J X Rui Guo Hua Zhang and Hui Xu Nanotechnology 2009
20 6
24 Guo J Carbon nanotube electronicsModeling physics and applications Purdue
University West Lafayette IN 2005
25 Motta C S S-P MITrioni cond-matmes-hall 2012 7
26 B P Growing Graphene via Chemical Vapor Deposition Ponoma College Ponoma
2011
27 ZurichE Transport properties of three-terminal graphene devices University of
Science and Technology Norway 2008
28 Uichiro MIntroduction to the electron theory of metals
29 Robert Laughlin H S Additional background material on the Nobel Prize in Physics
1998 (410)
30 MarkGoerbig Quantum Hall Effects (11152013)
68
REFERENCES
31 Zurich E Transport properties of three-terminal graphene devices Norwegian
University of Science and Technology Norway 2008
32 Deepak R Klein Tunneling University og Tennessee Space Institute Tennessee
2011
33 Williams JR L D CMMarcus Quantum Hall Effect in a Gate-Controlled p-n
Junction in Graphene (1122013)
34 Avadhanulu MN P G K A Textbook of Engineering Physcis for BE BSc (Engg)
SChand New Delhi 1992
35 Andriotis A Applied Physics Letters 2007 91 (152105)
36 Qimin Yan B H dagger Jie Yudagger Fawei Zhengdagger Ji ZangDagger Jian Wudagger Bing-Lin Gu F
L Dagger and Wenhui Duandagger NanoLetters 2007 7 (6) 1473
37 Soler J M E A J D Gale A Garciacutea J Junquera P Ordejoacuten and D Saacutenchez-
Portal J Phys Condens Matter 2002 14 2745
BIOGRAPHICAL SKETCH
Author Natasha Parikh
Degree Master of Science
Date January 2014
Undergraduate and Graduate Education
bull Master of Science in Materials Science and EngineeringNew Jersey Institute of Technology Newark NJ 2014
bull Bachelor of Arts in Physics and Biological SciencesRutgers the State University of New Jersey New Brunswick NJ 2012
Major Materials Science and Engineering
iv
v
ACKNOWLEDGMENTS
I would like to express my gratitude to my supervisor Dr NM Ravindra for the useful
comments remarks and engagement throughout the learning process of this Mastersrsquo
thesis Furthermore I would like to thank Vijay Kasi Somayajula for introducing me to
the topic as well for the support I thank Dr Tao Zhou Dr Ken Ahn and Dr Halina
Opyrchal for serving on my thesis Committee I would like to thank my loved ones who
have supported me throughout the entire process both by keeping me harmonious and
helping me in putting pieces together
vi
TABLE OF CONTENTS
Chapter
Page
1 INTRODUCTIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
1
11 Graphene The New Carbonhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
1
12 Graphene Synthesishelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
3
121 Synthesis of Graphene on Nickel (Ni)helliphelliphelliphelliphelliphelliphelliphellip
5
122 Synthesis of Graphene on Copper (Cu)helliphelliphelliphelliphelliphelliphelliphellip
8
123 Transfer of Graphene Filmshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
8
124 Synthesis of Graphene Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
9
125 Doping in Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
10
126 Nitrogen (N) Doped Graphene Synthesis (Substitutional)hellip
12
13 Structure of Graphene Nanoribbon (GNR)helliphelliphelliphelliphelliphelliphelliphelliphelliphellip
13
14 Overview of Graphene Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
15
2 RESEARCH BACKGROUNDhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
21 Bandstructure of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
22 Transport Characteristics of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
20
23 Drude Theoryhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
22
24 Quantum Hall Effect (QHE)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
24
25 Resistivity and Resistancehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
27
26 Klein Tunnelinghelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
28
27 Quantum Hall Effect in Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
31
28 Thermoelectric Effecthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 34
vii
TABLE OF CONTENTS
(Continued)
Chapter Page
281 Seebeck Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
34
282 Peltier Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
36
29 Early Research ndash ab initio Studyhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
37
3 COMPUTATIONAL DETAILShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
31 Introductionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
311 Extended Huckel Theory helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
312 Introduction to NEGFhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
41
313 Electrostaticshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
42
314 Non-Equilibrium Greenrsquos Functionhelliphelliphelliphelliphelliphelliphelliphelliphellip
44
4 ATOMISTIX TOOLKIT DETAILShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
41 Introductionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
42 Device Structurehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
43 Transmission Spectrum Calculationhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
50
44 Calculating the Currenthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
51
45 Calculating the Transport Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
52
5 RESULTS AND DISCUSSIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
53
51 Band Structure Analysis helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
53
52 I-V Characteristics of GNR Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
59
53 Thermoelectric Propertieshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
63
6 CONCLUSIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 65
REFERENCEShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
66
viii
LIST OF FIGURES
Figure Page
11 (a) Chemical representation of Carbon (b) Graphite ore (c) Structure of
Graphite and a single layer Graphenhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
2
12 An optical image of Graphene flake obtained by exfoliation of
graphitehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
3
13 (a) Graphene formation on Nickel (b) Graphene atoms on Ni (111)
lattice (c)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
7
14 (a) SEM image of graphene on copper foil (b) High-resolution SEM
image of graphene on Cuhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
8
15 (a) Transfer process (b) Wafer-scale synthesis of graphene (c) Graphene
films transferred onto glass wafer (d) SiSiO2 with device patterned (e)
PET filmhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
9
16 (a) High-magnification image of the annealed sample showing that well-
defined zigzag armchair and zigzag-zigzag edges are formed (b) ) STM
image of an 8 nm wide bent junction connecting an armchair and a
zigzag graphene nanoribbon which was carved by STM
tipshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
10
17 Band structure of graphene before and after doping The image shows
shift towards the Fermi levelhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
11
18 Low resolution TEM image of N-doped graphene Background is the
lacey carbon TEM grid graphene sheet is crumpled with many
rippleshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
13
19 Zigzag and Armchair orientation of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphellip 13
110 Bandstructure of ZGNRhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 14
111 Bandstructure of AGNRhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 15
21 Left Real space Graphene lattice with basis vectors and Right
The first Brillouin zone of Graphene in reciprocal space with basis
vectors and K and Krsquo are responsible for massless transport at low
energyhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
ix
LIST OF FIGURES
(Continued)
Figure Page
22 Bandstructure of a graphene sheet showing a band gap of 0eVhelliphelliphellip 18
23 Band structure of Graphene calculated with the tight-binding modelhellip 19
24 The energy dispersion around the K pointhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 22
25 Electrons colliding with stationary ionshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 23
26 (a) 2D electrons in a perpendicular magnetic field Logitudinal resistance
measured across C5 and C6 Transverse resistance measured across C3
and C5 (b) Classical Hall resistance as a function on the magnetic field
25
27 Klein tunneling through an npn barrierhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 29
28 Electron trajectory considering the linear electrostatic potential U(x) = Fx 30
29 Electron like and hole like trajectories at same Ehelliphelliphelliphelliphelliphelliphelliphelliphellip 30
210 Quantum Hall effect in graphene 22
The Hall conductivity σxy and the
longitudinal resistivity of monolayer graphene as a function of carrier
density at B = 14T and T= 4K This shows half-integer QHE with chiral
index J= 1helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
32
211 (a) LL for Graphene bilayer (b) Schematics of Hall conductivity as a
function of nn0 for bilayer Graphene (solid line) and monolayer
Graphene (dotted line) (c) LL for monolayer Graphenehelliphelliphelliphelliphelliphelliphellip
33
212 Seebeck Effecthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 35
213 Transmission functions in units of (2e2h) for AZA structureshelliphelliphelliphellip 37
214 I-V curve for a 591nm long channel (Vbias=20mV)helliphelliphelliphelliphelliphelliphelliphellip 38
31 NEGF systemhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 42
41 Geometry of device configuration with two electrodeshelliphelliphelliphelliphelliphelliphellip 48
42 The electron distribution in a device configuration which illustrates a left
moving scattering state with origin in right electrodehelliphelliphelliphelliphelliphelliphelliphellip
48
x
LIST OF FIGURES
(Continued)
Figure Page
51 Band structure of AGNR widths (a) 4 atoms (b) 5 atomshelliphelliphelliphelliphelliphellip
53
52 Band structures of AGNR widths (a) 6 atoms (b) 7 atomshelliphelliphelliphelliphelliphellip 54
53 Band structure of AGNR widths (a) 8 atoms (b) 9 atomshelliphelliphelliphelliphelliphelliphellip 54
54 Band structures of AGNR widths (a) 10 atoms (b) 11 atomshelliphelliphelliphelliphellip 55
55 Band structure of AGNR with a width of 12 atomshelliphelliphelliphelliphelliphelliphelliphelliphellip 55
56 Variation in band gaps as the width (number of atoms) varieshelliphelliphelliphellip 55
57 Band structure of ZGNR width (a) 4 atoms (b) 6 atomshelliphelliphelliphelliphelliphelliphellip 56
58 Band structure of ZGNR width (a) 8atoms and (b) 10 atoms 57
59 Band structure of ZGNR with a width 12 atomshelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 57
510 Band structures of Doped AGNR (a) 4 N Doped (b) 4 B Doped (c)
2 N Doped (d) position of Nitrogen from (c)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
58
511 Current Vs Voltage graph for varying graphene width showing
conductivityhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
59
512 ZAZ GNR junction devicehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 60
513 I-V curve of Boron Doped ZAZ junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 61
514 I-V curve of Nitrogen Doped ZAZhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 62
515 Variation of Peltier effect coefficient with temperature for various doping 64
1
CHAPTER 1
INTRODUCTION
11 Graphene The New Carbon
Carbon (chemical symbol C atomic mass 1207amu) (Figure 11a) is a widely distributed
element in nature It is found abundantly in the sun stars comets and the atmospheres of
the planet Carbon can form up to four bonds it can bond with itself endlessly and with
most other elements in many different shapes making it a significant part of the
construction for many kinds of complex molecules1
Two allotropes of carbon are commonly used diamond and graphite (Figure
11b) The bonding structures of diamond and graphite contribute to the properties
individually In diamond all the p-orbitals are used forming a sp3
bonding whereas in
graphite only two orbitals are occupied allowing the unpaired bond for the transport of
electrons Each carbon atom in graphene possesses sp2 hybridization ie each carbon
atom is connected to three other carbon atoms via covalent bonds with a bond length of
142Å and an angle of 120deg between each bonded pair This makes graphite a better
conductor than diamond Graphite consists of many layers of 2D carbon lattices (Figure
11c) stacked on top of each other and held via Van der Waals forces A single layer of
graphite where carbon atoms are arranged in a honeycomb lattice is known as graphene
(Figure 11c)
2
Figure 11 (a) Chemical representation of Carbon (b) Graphite ore (c) Structure of
Graphite and a single layer Graphene2
Theoretical work on graphene was done specifically to study the other allotropes
The first study was done by Wallace in 1947 who calculated the band structure of
graphene3 Further the peculiar Landau levels were known by McClure in 1957 and the
relativistic Hofstadter butterfly by Ramal in 19853 Later in 1991 the invention of carbon
nanotubes by Iijima boosted the theoretical research on graphene3 Prior to the invention
of carbon nanotubes there were a few experimental papers on graphene growth via
various methods like intercalation of graphite (Shioyama 2001) free standing (Boehm
1962) epitaxial as well as graphene grown on metals (Bommel 1975 Land 1992 Itoh
1991)3 With all the various discoveries the electronic properties of graphene were not
studied until 2004 when Berger and Novoselov were able to access the electronic
properties with contact of graphene flakes3 (Figure 12)
3
Figure 12 An optical image of Graphene flake obtained by exfoliation of graphite3
The specific lattice structure of graphene possesses a number of unique electronic
properties making it an interesting material for theorists experimentalists and engineers
Utilization of graphene as a fundamental block of electronic devices requires
development of new theoretical methods for understanding the current propagations in
graphene constriction4
12 Graphene Synthesis
The discovery of graphene by mechanical exfoliation called the lsquoScotch tape methodrsquo led
to serious attempts towards the production of top quality graphene5 Graphene was first
exfoliated mechanically from graphite in 20046 The importance of high quality graphene
cannot be emphasized enough however electron transport has shown that defects play an
important role in hindering the transport properties of electrons (holes)7 The two
synthesizing methods for the large scale manufacture of graphene are chemical vapor
deposition (CVD) and silicon carbide (SiC) desorption method
4
Graphene can be synthesized by sublimation of silicon from SiC at high
temperature (1200degC) in high vacuum5 The major advantage of this method is that the
SiC provides an insulating substrate and no transfer of the graphene layer is needed Yet
the disadvantage of this method outweighs its advantages the high temperature is cost-
ineffective making it unsuitable for large scale manufacturing8 Also the crystal growth
face alters the properties of graphene Graphene grown on Si-terminated face has poor
homogeneity and is subjected to unintentional doping7 Conversely graphene grown on
C-terminated SiC has higher mobility and is often called lsquoturbostaticrsquo due to the
rotational disorder7
Unlike the SiC method the graphene produced via CVD method needs to be
transferred to a substrate making it difficult to maintain the quality of graphene Yet
CVD synthesized graphene has a larger grain size7 More research is being done on
various methods for synthesis of graphene The methods include direct chemical
synthesis ion implantation crystal sonification and lastly unzipping carbon nanotubes to
form graphene sheets9
Graphene and few-layer graphene have been grown by CVD from carbon
containing gases on catalytic metal surfaces andby surface segregation of C dissolved in
the bulk of such metals7 Growing graphene with CVD is a very attractive solution since
it is compatible with the existing semiconductor industry9 Graphene has been grown via
CVD process on metal substrates such as Nickel (Ni) and Copper (Cu)
5
121 Synthesis of Graphene on Nickel (Ni)
Polycrystalline Ni films are annealed in ArH2 atmosphere at 900-1000degC to increase
grain size and are then exposed to H2CH4 gas mixture10
In this step the hydrocarbon
decomposes and dissolves in Ni to form a solid solution Lastly the samples are cooled in
argon gas Ni has high carbon solubility at elevated temperatures and the solubility
decreases as temperature is reduced During the cooling process the carbon atoms diffuse
out from the Ni-C solid solution and precipitate on the Ni surface to form graphene films
(Figure 13a) Since Ni (111) has a lattice similar to the densely packed hexagonal lattice
of graphene (Figure 13b) they also have similar lattice constants and hence Ni surface
serves as an excellent lattice matched substrate for graphene growth11
The growth of graphene on Ni is based on carbon segregation and precipitation
process different segregation behavior is produced by different cooling rates which
affect the thickness and quality of graphene films12
Medium cooling rates lead to optimal
carbon segregation and produce few layers12
Graphene films grown on Ni are usually
continuous with monolayer and few layer regions Annealing of Ni substrates at elevated
temperatures in hydrogen atmosphere not only increases the single-crystalline Ni grain
size but also eliminates certain impurities in Ni thereby improving the graphene quality
Furthermore the graphene thickness can also be affected due to the amount of carbon
dissolved in the Ni films during the growth time
After synthesis the graphene can be transferred to other insulator substrates for
further characterization and applications Figure 13c shows the selected area electron
diffraction pattern of graphene film along the [001] direction which confirms the
graphene lattice structure shown After transfer to insulator substrates the geometry can
6
be retained as shown in Figure 13d Under optimal growth parameters graphene growth
is only limited by the Ni catalyst Lastly Figures 13e and 13f show the wafer-scale
graphene synthesis and transfer of graphene to a flexible transparent substrate
respectively
Though polycrystalline Ni is a good substrate the percentage and size of
graphene monolayer are still limited Researchers have hence tried other metal substrates
for graphene synthesis
7
Figure 13 (a) Graphene formation on Nickel (b) Graphene atoms on Ni (111) lattice
(c) Low magnification TEM image of graphene edges (d) Optical image of graphene
transferred from the Ni surface to SiO2Si substrate (e) Full-wafer scale deposition of
graphene layers on polycrystalline Ni (f) Transparent and flexible graphene films on
PDMS substrate10
8
122 Synthesis of Graphene on Copper (Cu)
Graphene films are grown on 25microm thick Cu foils in a hot wall furnace13
The Cu foil is
first annealed in hydrogen atmosphere at 1000degC and a mixture of H2CH4 is introduced
into the system to initiate graphene growth After a continuous graphene layer is formed
on the Cu foil the system is cooled to room temperature Figure 14a shows an SEM
image of graphene on Cu substrate indicating the Cu grains with contrast The Cu
surface steps are formed during thermal annealing and the darker flakes indicate multiple-
layer graphene (Figure 14b)10
The graphene wrinkles in Figure 14(b) originate from
different thermal expansion coefficient of graphene and Cu They go across the Cu grain
boundaries indicating that the graphene film is continuous
Figure 14 (a) SEM image of graphene on copper foil (b) High-resolution SEM image of
graphene on Cu10
123 Transfer of Graphene films
In order to facilitate the applications of graphene for electronic applications we need to
separate the graphene from the catalytic metal substrate Figure 15a shows the transfer
process of graphene Graphene is first coated with a thin layer of polymethyl
methacrylate (PMMA) and baked at 120degC to evaporate the solvent10
The metal layer is
then removed by Ni or Cu etchant leaving behind the PMMA graphene film The film is
then cleaned by deionized water and then transferred onto the target substrate After the
9
evaporation of water vapor the PMMA is removed by acetone leaving graphene film on
top of the target substrate Figure 15b shows a graphene wafer transferred from the
substrate onto glass and polyethylene terephthalate (PET) films
Figure 15 (a) Transfer process (b) Wafer-scale synthesis of graphene (c) Graphene
films transferred onto glass wafer (d) SiSiO2 with device patterned (e) PET film10
124 Synthesis of Graphene Junction
Graphene junctions with smooth armchair and zigzag edges are difficult to produce by
conventional methods such as mechanical exfoliation chemical exfoliation or lithography
etching14
The conventional methods can only produce rough edges Recently
Dresselhaus reported an edge reconstruction of graphene by Joule heating in a TEM-STM
10
(Figure16b) system15
An individual nanoribbon sample is attached to the sample holder
at one end and to the STM tip at the other end these ends also serve as the two
electrodes The structural transformation in the growth of graphene from armchair to zig-
zag is mainly attributed to the vaporization of carbon edges that reconstruct at high
temperatures in which resistive Joule heating and preferred current flow play an
important role This means that by controlling the flow of current a perfectly smooth
edged ribbon can be synthesized making graphene-based electronics possible16
Figure 16 (a) High-magnification image of the annealed sample showing that well-
defined zigzag armchair and zigzag-zigzag edges are formed (b) STM image of an 8 nm
wide bent junction connecting an armchair and a zigzag graphene nanoribbon which was
carved by STM tips14
125 Doping in Graphene
The doping of graphene can be roughly classified into two categories - electrical and
chemical Electrical doping involves changing gate voltages of graphene devices and
chemical doping uses chemical routes such as substitutional or interstitial This thesis
discusses chemical doping and the importance of doping sites by changing the dopant
Chemical doping is a common approach to tailor the electronic properties of
11
semiconductors Doping of graphene can cause its electronic properties to alter leading to
a metal-semiconductor transition The two means of doping graphene are interstitial and
substitutional In interstitial doping the dopant atoms or molecules are introduced as
adatoms or admolecules on the surface of graphene whereas in substitutional doping the
dopant atoms are replaced in the carbon lattice forming a bond in the lattice of
graphene16
Doping graphene results in the formation of n or p-type semiconductors
depending on the kind of dopant If the dopant is an electron donor it causes the Fermi
level to shift up resulting in n-type behavior of graphene Furthermore if the dopant is an
electron acceptor it causes the Fermi level to shift down resulting in a p-type behavior of
graphene (Figure 17)16
Figure 17 Band structure of graphene before and after doping The image shows shift
towards the Fermi level16
Graphene nanoribbons (GNR) can be made into a p- and n- type semiconductor
by doping with boron (B) and nitrogen (N) respectively In theory GNR p-n junction is
formed by doping GNR with B and N in different regions However experimentally
doping graphene with both these elements is very difficult due to the dopants reacting
with each other17
Hence most experimental studies use GNR doped by only one
12
element N-doped graphene was synthesized by Wei et al Wang and B-doped Graphene
was realized by Endo17
Many researchers have demonstrated interstitial doping of graphene by gas metal
and organic molecules16
The various gases and metals used are NO2 NH3 An-CH3 Na-
NH2 F4-TCNQ TPa TCNE and others16
Doping in graphene is hence possible by
electrons or holes in high concentration without deterioration of its mobility Interstitial
doping is highly sensitive due to most of the conducting channel being exposed to surface
absorbates and hence can be used in molecule detection
In substitutional doping the dopant atoms are included in the graphene lattice and
thus chemically bonded Substitutional doping is done via the CVD method using a
carbon and dopant source Substitutional doping opens up many applications in device
engineering making graphene a very good candidate as a semiconductor This study
involves the study of transport properties of graphene doped by substitution
126 Nitrogen (N) Doped Graphene Synthesis (Substitutional)
N-Doped graphene is prepared via a CVD process using a 25microm thick Cu film on a Si
substrate The substrate is placed in a quartz tube with the flow of hydrogen (20sccm) and
argon (100 sccm)18
When the center of the furnace reaches 800degC 60 sccm of CH4 and
60 sccm of NH3 is introduced into the flow as C source and N source respectively The
substrate is then moved to high temperature and after 10 min growth the sample is
cooled to room temperature under H2 ambient Figure 1 8 shows the growth of N-doped
graphene18
13
Figure 18 Low resolution TEM image of N-doped graphene Background is the lacey
carbon TEM grid graphene sheet is crumpled with many ripples18
13 Structure of Graphene Nanoribbon (GNR)
Graphene Nanoribbons (GNR) are strips of graphene with very thin width of lt50nm
GNRs can be terminated in three separate ways called zig-zag (0 n) armchair (m 0) and
chiral (m n) (Figure19) and this termination along the width of the ribbon dictates the
size of the band gap19
Figure 19 Zigzag and Armchair orientation of Graphene5
Due to their various edge structures GNRs exhibit different electronic properties
ranging from normal semiconductors to spin-polarized half metals which open the
possibility of GNRs as electronic devices19
14
Within a tight binding approach (AGNRs) could be metallic or semiconducting
depending on their ribbon width but all zigzag graphene nanoribbons (ZGNRs) are
metallic with a high density of electronic states at the edges Hence ZGNRs exhibit
characteristic edge effects which are not present in AGNRs These edge effects in
ZGNR create a flat band close to the Fermi level making the ZGNR edges more
reactive19
First-principles calculations show that the GNRs possess a non-zero direct
band gaps These gaps are small for ZGNR (Figure 110) caused due to spin ordering
effects at the edges For AGNRs the band gap arises from quantum confinement (Figure
111) effect that has larger magnitudes than ZGNR20
Figure 110 Band structure of ZGNR
15
Figure 111 Band structure of AGNR
For GNRs the band gap decreases as the ribbon width increases and in order to
create a semiconductor with a desirable band gap the nanoribbon width should be
adjusted accordingly This property of adjusting the band gap makes graphene an
excellent candidate for transistor switching By applying an electric field GNR can be
altered from an insulator to a conductor GNRs exhibit very intriguing properties and
have become one of the promising candidates for electronic applications
14 Overview of Graphene Junction
The invention of p-n junctions date back to 1940s which later resulted in the invention of
junction transistors One of the key technological reasons for success of the p-n junction
is mainly due to its ability to locally modulate the energy band gaps via an applied bias21
A graphene p-n junction is created via single layer of graphene in which the
carrier type and density in two adjacent regions are controlled by electrostatic gating8
For materials with a band gap the electric field can either switch lsquooffrsquo the current or
rectify it (p-n diode)22
Being a ldquogaplessrdquo material the off state is not achievable in
16
graphene In order to achieve an off state the gap can be created by doping graphene with
various elements (Group III or Group V) Doping allows p-n junctions to be
reconfigurable using a gate voltage to distinguish between graphene p- n regions within a
single sheet Many researchers have studied the electronic as well as transport properties
of doped graphene junctions
In 2009 Fangping OuYang studied the transport properties of T-shaped graphene
junctions using the ATK software and showed that the conductance depends on
geometric structures which can be controlled by selective doping23
Wei Yao in 2013
studied the transport properties in graphene p-n junctions and showed that the
rectification effect depends on boron doping density and position17
The study of transport properties in graphene p-n junctions is a recent
advancement The thesis discusses transport properties including the current-voltage (I-
V) characteristics of doped graphene junctions Moreover the software used is similar to
the software in use by current researchers since they have produced viable data using
ATK
17
CHAPTER 2
RESEARCH BACKGROUND
21 Band Structure of Graphene
The unique electronic properties of graphene were first predicted in 1946 Figure 21
shows a top view of the hexagonal arrangement of carbon atoms in real space as well as
the first Brillouin zone in reciprocal space
Figure 21 Left Real space graphene lattice with basis vectors and Right The
first Brillouin zone of graphene in reciprocal space with basis vectors and
K and
Krsquo are responsible for massless transport at low energy24
The real space basis vectors are radic
and
radic
The reciprocal space basis vectors are 1 2
0 0
4 1 3 4 1 3( )and ( )2 2 2 23 3
b x y b x ya a
where the magnitude of the basis vectors is |a0| = radic acc The distance between nearest
neighbor carbon atoms is acc=0142nm
18
The band structure can be calculated by solving the eigenvalues using the
dispersion relation E( )
1 2 3( ) 3 2cos 2cos 2cosE k t k a k a k a (21)
Transport properties of solids are closely related to the energy dispersion
relations E ( ) in the material and in particular to the behavior of E ( ) near the Fermi
level Graphene is a zero gap semimetal whose specific linear electronic band dispersion
near the Brillouin zone corners (Dirac points) gives rise to electrons and holes that
propagate as massless Fermions25
The valence and conduction bands do not overlap in
graphene they touch at the Fermi Level (Figure 22)
Figure 22 Band structure of a graphene sheet showing a band gap of 0eV
The low energy properties of graphene can be well described by making a linear
expansion of the band structure around the K and Krsquo This energy can be written as
19
E(k) = plusmnħvF|k (22)
where vF is the Fermi velocity of 1106ms given by
1F
Ev
k
ħ (23)
Figure 23 Band structure of graphene calculated with the tight-binding model
22
The Fermi surface of graphene consists of double cones with Fermi energy at the
intersection of these cones (Figure 23) The slope of the band is zero and hence the
effective mass of electrons in that region is zero which leads to an entirely new transport
mechanism in graphene26
20
22 Transport Characteristics of Graphene
Transport process usually involves a flow of charge or energy or both The flow is mainly
due to external perturbations such as electric field and temperature gradient The
relationship between forces and flow usually defines various transport coefficients that
are the characteristics of electrons and phonons in the material All modern electronics
are based on the ability to control the electronic properties of a material by applying
external voltage This is done by an electric field effect where the gate voltage changes
the carrier concentration of the material and consequently its conductivity The electric
field effect in graphene was reported by Novoselov in 2004 and is used in transport
measurements8
The electron-phonon interaction in graphene plays an important role in
understanding the photoemission spectra observed in graphene The electric field effect is
an alternative method for changing the charge carrier density in low dimensional systems
The electric field effect in graphene which was first reported by Novoselov et al in
2004 is widely used as a characterization tool in transport measurements25
The transport characteristics of the material are directly related to the
bandstructure of graphene The carriers in graphene lattice are free to move in two
dimensions In the carrier transport of graphene the carriers ndash electrons and holes ndash close
to the Dirac points are of importance The transport is described by a two component
wave function (Equation 24) which obeys the 2D Dirac-like equation for massless
particles27
21
-ivFσ nablaψ(r) = Eψ(r)
(24)
where σ is the 2D Pauli spin matrix In the continuum limit the above (Equation
24) corresponds to the effective low energy Dirac Hamiltonian (Equation 25)
0( )
0
x y
F F
x y
iH k k
i
k kv v
k k
(25)
The electronic band structure of the energy (E) versus wave vector (k) relation for
graphene is given by Equation 24
The two component wave function resembles the spin or wave function of
quantum electro dynamics (QED)27
Corresponding to the spin of particles in QED the
charge carriers of graphene can be attributed with a pseudospin σ The pseudospin is the
direct result of two different carbon sublattices corresponding to the bonding and
antibonding combinations27
22
Figure 24 The energy dispersion around the K point27
In Figure 24 the red and blue lines correspond to the antibonding and bonding
states respectively The pseudospin can have two values either in the direction of or
against the momentum It can be seen that the electrons with energy E travelling in the
positive direction originates from the same branch as a hole with energy ndashE travelling in
the negative direction giving it the same pseudospin This results in suppressed
backscattering and Klein tunneling The back scattering process requires the pseudospin
to flip which is possible in the presence of short range scatters that act differently on sub
lattices27
23 Drude Theory
The classical theory of metallic conductivity was presented by Drude in 1900 and was
elaborated by Lorentz in 190528
Drude treated the free electrons as classical ideal gas
meaning the electrons collide with stationary ions and not each other
23
Figure 25 Electrons colliding with stationary ions28
The Drude theory applied the kinetic theory of gases to a metal considered as a gas of
electrons The basic assumptions made by the Drude theory are28
When metallic elements are brought together to form a solid then the valence
electrons become freely moving through the metal whereas the ions remain intact
as nearly immobile positive particles
Between collisions the electrons move freely ie there is neither electron-
electron interaction nor electron-ion interaction
The scattering mechanism leads to instantaneous collisions of the electron with
the scatterers
The collisions are characterized by a relaxation time τ
The electrons achieve thermal equilibrium only through collisions the velocity
after a collision is randomly directed the speed is as appropriate to the
temperature
With the relaxation time Drude obtained the electrical conductivity expression
where n is the number of electrons per unit volume
σ = ne2τm
(25)
He also calculated the thermal conductivity and successfully provided the
theoretical basis for Wiedemann-Frantz law already established in 1853 which states that
24
the ratio of electrical and thermal conductivity of any metals is a universal constant at any
given temperature28
The Drude theory gives results which are qualitatively correct outside of the
quantum Hall regime28
In the Drude theory of the electrical conductivity of a metal an
electron is accelerated by the electric field for an average time τ before being scattered
by impurities lattice imperfections and phonons to a state which has zero average
velocity The average drift velocity of the electron is
d
eE mv (26)
It is assumed that all electrons drift together and hence the current density
j = -ne (27)
This Drude theory works well for fields below ~ 01T At stronger fields the Hall
resistivity becomes nearly constant over finite intervals of magnetic fields28
The QHE
reflects both novel disorder physics as well as novel interaction physics in the quantum
Hall regime
24 Quantum Hall Effect (QHE)
The discovery of QHE is a remarkable achievement in condensed matter physics The
Hall Effect was discovered by Edwin Hall in 187929
However the precise quantization
of the Hall conductance in units of e2h was not recognized until February 1980 Five
years later in 1985 Klaus von Klitzing was awarded the Nobel Prize in Physics for the
discovery of QHE29
The quantum Hall effect occurs in two-dimensional electron systems in the limit
of strong perpendicular magnetic field that stems from electronic transport
25
measurements where one drives a current I through the sample and where one measures
both the longitudinal and transverse resistance (Hall resistance) A longitudinal resistance
is a resistance measured between two contacts that may be connected by a line which
does not connect C1 and C430
Transverse resistance is measured between two contacts
connected by an imaginary line connecting C1 and C4 (Figure 26a)
Figure 26 (a) 2D electrons in a perpendicular magnetic field Logitudinal resistance
measured across C5 and C6 Transverse resistance measured across C3 and C5
(b) Classical Hall resistance as a function on the magnetic field30
Due to the existence of quantum Hall effect it is natural to expect that there exists
a classical Hall Effect Hall showed that the transverse resistance of a thin metallic plate
varies linearly with the strength B of the perpendicular magnetic field (Figure 26 b)
RH = Bqnel (28)
More quantitatively the classical Hall Effect can be understood within the Drude
model for diffusive transport in a metal Within this model one considers independent
26
charge carriers of momentum p described by the equation of motion
( )
b
dp p pe E B
dt m (29)
where E and B are the electric and magnetic field respectively The macroscopic
transport characteristics ie resistivity of the system are obtained from the static
solution of the equation of motion dpdt = 0 and one finds for 2D electrons with p =
(pxpy)
x
x yb
y
y xb
eBe
eBe
ppE
m
ppE
m
(210)
In the above expression characteristic frequency is visible as
C
b
eB
m (211)
This is known as cyclotron frequency as it characterizes the cyclotron motion of a
charged particle in a magnetic field30
With the Drude theory the conductivity can be
written as
j = -enelpmb (212)
and the mobility can be given as
micro = eτmb (213)
The transport properties in the limit of ωCτ-gt infin are entirely governed in the presence of
27
a magnetic field by the off-diagonal ie transverse components of
conductivityresistivity
The theory of quantum Hall effect subjects all physical properties of 2D electron
system in the limit where the magnetic field is strong so that the mixing of Landau levels
by disorder or electron-electron interaction is considered to be a weak perturbation30
This is known as the quantum Hall regime The ratios between the energy scales
corresponding to the two interactions are important The limit where disorder potential is
much stronger is referred to as integer quantum hall regime whereas the limit where the
interaction potential is much stronger is referred to as fractional quantum Hall regime
25 Resistivity and Resistance
The electronic transport in the framework of the Drude theory allows for the calculation
of conductivity or resistivity of a classical diffusive 2D electrons in a magnetic field30
The conductivity and conductance are related to one another but they depend on the
geometry of the conductor-the resistance R and hence the resistivity is given by
R = (LA)ρ (214)
where L is the length of the conductor and A is the cross section
For a d-dimensional conductor the cross section scales as Ld-1
such that the
scaling relation between the resistance and the resistivity is
R~ ρL2-d
(215)
From the dimension point of view resistance and resistivity are the same in 2D and the
resistance is scale-invariant Further the resistance of a 2D conductor depends in
general on the so-called aspect ratio LW via some factor f (LW)30
However for
transverse Hall resistance it is the length of the conductor that plays the role of cross
28
section such that the Hall resistivity and the Hall resistance truly coincide ie f=1 The
Quantum Hall effect is highly insensitive to the particular geometric properties of the
sample used in transport measurements Recently quantum Hall physics experienced the
discovery of ldquorelativisticrdquo quantum Hall effect in graphene The electrons in graphene
behave as if they were relativistic massless particles contributing to a very interesting
field of research30
26 Klein Tunneling
Klein tunneling in which relativistic particles penetrate through a potential barrier
without the exponential damping that is characteristic for nonrelativistic quantum
tunneling has never been observed for elementary particles The tunneling allows
transmission of a particle through a potential barrier higher than its kinetic energy
violating the principle of classical mechanics30
On the quantum scale the objects exhibit
wave-like characteristics in which the quanta move against a potential hill described by
their wave function This wave function represents the probability amplitude of finding
the object in a particular location The transmission of the object through the potential hill
is termed as tunneling When EltV then the ψ(x) over V is returned by ψrsquo(x) In quantum
mechanics an electron tunnels from the conduction into the valence band Such a
tunneling from an electron-like to hole-like state is called as Klein Tunneling in which the
electron avoids backscattering
In Figure 27 it is shown that an electron hitting a potential barrier is reflected
with 100 certainty In non-relativistic quantum mechanics the electrons can tunnel
through the barrier but the probability of tunneling exponentially decays with increasing
29
height and width of the barrier However in relativistic quantum mechanics the barrier
gets transparent even in the limit of infinite barrier height (Klein paradox)31
Figure 27 Klein tunneling through an npn barrier30
The Klein paradox in graphene can be understood in terms of electrons and holes
In graphene the massless carriers behave differently than ordinary carriers (with mass) in
the presence of an electric field A barrier which is repulsive for electrons will be
attractive for holes Since there are hole states inside the barrier with the same energy as
the electrons outside an electron arriving at the barrier can tunnel through it as a hole
before leaving again as an electron Klein tunneling for transport in graphene is that the
charge carriers cannot be confined by potential barriers The Klein tunneling effect has
been experimentally observed by Ando in 1998 in which the absence of backscattering
(Figure 28) is responsible for high conductivity in carbon nanotubes
30
Figure 28 Electron trajectory considering the linear electrostatic potential U(x) = Fx30
The electron is able to propagate through an infinitely high potential barrier since
it makes a transition from the conduction band to valence band In this transition from
conduction band to valence band its dynamics changes from electron-like to hole-like
The equation of motion is thus given by
2
2 2 2| | ( )
pdr E
dt E Up
p E U
v
v
at energy E (216)
This shows that in the conduction band (UltE) and in the valence band (UgtE)
In Klein tunneling the pairs of electron-like and hole-like trajectories at the same E and
py have turning points at dmin given by dmin=2v|py|F (Figure 29)
Figure 29 Electron like and hole like trajectories at same E21
31
The tunneling probability exponential dependence on dmin
2
min| |
( ) exp( ) exp( )2
y y
y
vT
F
p pdp
(217)
The applications of the Klein tunneling include Atomic clock Scanning tunneling
Microscope Tunnel diode Tunneling transistor and many more32
Since graphene
exhibits Klein tunneling it can be very useful to study the transport properties in
graphene and use it in such applications
27 Quantum Hall Effect in a Graphene
A monolayer graphene shows half-integer quantum Hall effects where the Hall
resistance is quantized at values of
2
1
xyh v eR
(218)
around filling factors
14( 1 2)Nv
(219)
where N is an integer e is the electron charge h is the Planckrsquos constant and the
factor 4 is due to spin and valley degeneracy QHE in graphene can be observed at room
temperature which is a very intriguing property (Figure 210) Graphene reveals
significant differences with respect to conventional 2D electron systems The Landau
quantization yields energy levels that disperse differently in graphene as well as
particular zero-energy level that is only half filled at the charge neutrality point (v=o)
32
Figure 210 Quantum Hall effect in graphene22
The Hall conductivity σxy and the
longitudinal resistivity of monolayer graphene as a function of carrier density at B = 14T
and T= 4K This shows half-integer QHE with chiral index J= 1
The QHE in graphene is not entirely similar to regular QHE since the charge
carriers in graphene are Dirac Fermions The charge carriers governed by
electrodynamics is given by (Equation 220) which does not apply for graphene and a
QED quantization of graphene electronic band structure is used
En = (n+12)ħω (220)
33
In the presence of magnetic field the nature of the Dirac Fermions in graphene
results in unevenly spaced Landau levels (LL) containing a distinctive LL at the electron-
hole degenerating a zero energy given by
2MG
MGFehn B
n vE (221)
The LL levels at high magnetic fields in MG are shown in Figure 211
Figure 211 (a) LL for Graphene bilayer (b) Schematics of Hall conductivity as a
function of nn0 for bilayer Graphene (solid line) and monolayer Graphene (dotted line)
(c) LL for monolayer Graphene33
It is found that the Hall resistance of a two dimensional electron system has
plateaus as a function of the number of electrons at low temperatures and strong magnetic
fields32
At large B the Dirac-like energy spectrum of graphene gives rise to a
characteristic series of QH plateaus in conductance reflecting the presence of a zero-
energy Landau level that include only odd multiples of 2e2h for uniform carrier density
in the sheet These plateaus of QH edge states at the edge of the sheet circulating in a
34
direction are determined by the direction of B and the carrier type33
This is why QHE in
graphene is known as Half-Integer Quantum Hall Effect
28 Thermoelectric Effect
Thermoelectricity refers to a class of phenomena in which a temperature difference
creates an electric potential or an electric potential creates a temperature difference The
principle of thermoelectric effect has been known for over 100 years Recently the
practical applications of thermoelectric effect have become more viable34
Thermoelectric effect is the direct conversion of temperature differences to
electric voltage and vice versa Joule heating is the heat generated whenever a voltage is
applied across a resistive material The Peltier-Seebeck effect is reversible whereas Joule
heating is not This effect can be used to generate electricity to measure temperature to
cool objects or to heat them Since the direction of heating and cooling is determined by
the sign of the applied voltage thermoelectric devices make very convenient temperature
controllers
281 Seebeck Coefficient
Thomas Johann Seebeck discovered that an emf appears in a circuit composed of two
dissimilar metals when the junction between the metals is held at different
temperatures34
The thermoelectric emf causes a continuous current in the circuit when a
complete loop is formed and the current is known as thermoelectric current This is
known as the Seebeck effect
35
Figure 212 Seebeck Effect34
As long as the two junctions are at different temperatures the thermoelectric emf
exists and the current will keep flowing between the hot and cold junction that are at
different temperatures The Seebeck effect is the conversion of temperature difference
directly into electricity The voltage developed in the circuit shown in Figure 212 is
proportional to the difference in temperature between the two junctions and is given by
V = α (T2-T1) (222)
This Seebeck effect is observed not only in metals but also in semiconductors
Here α is known as the Seebeck coefficient α measures the magnitude of an induced
thermoelectric voltage in response to the temperature difference across the material If the
temperature difference ∆T between the two ends of a material is small then the Seebeck
coefficient of a material is written by
α = ∆V∆T (223)
36
This can be expressed in terms of electric field as
α E∆T (224)
The units of Seebeck coefficient is given as VK The higher the Seebeck coefficient
value the better it is since it will create a very large voltage that can be used to provide
power
282 Peltier Coefficient
Peltier effect is the inverse of Seebeck effect involving a junction phenomenon There is
heat absorption or generation at the junctions depending on the direction of current flow
Heat generated by current flowing in one direction is absorbed if the current is reversed
The heat absorbed per second at a junction carrying current I is given by
Heat absorbed in t sec = πabIt (225)
Here πab is the Peltier coefficient and given by HIt Thus Peltier coefficient is
numerically equal to the applied potential difference expressed in Volts
Overall by studying the flow of electrons the values of Seebeck
coefficient and Peltier co-efficient can be estimated These values determine the various
applications of the materials In this thesis the Peltier and Seebeck coefficient of the
graphene junction and the new applications are discussed
37
29 Early Research ndash ab intio studies
In 2007 Androitis studied that the conducting properties of graphene nanoribbons and
junctions are strongly dependent on their size and geometric features35
He concluded that
there is no conductance for small AZA or ZAZ ribbons (Figure 213)
Figure 213 Transmission functions in units of (2e
2h) for AZA structures
35
Figure 213 shows that T (E) exhibits a negligible peak [T (E) = 001 in units of
2e2h] at E= -225 and 250eV However it was noted that when the width of the arm type
was increased T (E) at -225 and 250eV was 02035
Later in 2007 Qimin Yan used first principles methods to investigate the Current-
Voltage characteristics of GNR Transistors and the effect of edge doping He showed that
GNR field effect transistors can achieve high performance levels with ONOFF ratios on
the order of 103-10
436
Figure 214 is an I-V curve of AZA GNR-FET connected via
armchair metallic leads36
38
Figure 214 I-V curve for a 591nm long channel (Vbias=20mV)
36
In 2009 Fangping OuYang demonstrated the intrinsic transport properties and
effective B or N doping of the junctions by using first-principles quantum transport
simulations He concluded that the I-V characteristics of pure-carbon T-shaped junctions
exhibit metallic behavior and the current in the junction strongly depends on the height
of the stem23
He reported that the conductance of the devices depends on the geometric
structures which can be controlled by selective doping
In 2012 Wei Yao used the first principle calculations based on Density
Functional Theory (DFT) and Non-equilibrium Greens Function (NEGF) to study the
electronic as well as the transport properties of B-doped 6-GNR p-n junction His results
showed that the boron doping interval can influence the rectification effect at low bias
and also exhibit Negative Differential Resistance (NDR) phenomena at high positive
bias
39
CHAPTER 3
COMPUTATIONAL DETAILS
31 Introduction
The physical chemical electrical electronic and optical properties of a solid are
determined by their quantized electronic states The quantum states in low-dimensional
systems are produced due to the confinement of the carrier charges in one or two
dimensions Graphene is a conductor electrons are able to flow through graphene more
easily than through even copper The electrons can travel through the sheet of graphene
like mass-less particles as fast as just one hundredth that of the speed of light The ways
in which electrons behave in graphene make it very helpful to study their fundamental
physical properties Graphenersquos near perfect crystal lattice provides a very clean system
to experiment By restricting the electrons to only two dimensions they exhibit some
interesting properties such as the anomalous quantum Hall effect and Klein tunneling
In this chapter two theoretical concepts used for calculating the electronic structure
and the transport properties for graphene are described These include the Extended
Huckel Theory and Non-Equilibrium Greenrsquos Function (NEGF) method
311 Extended Huckel Theory
Erich Huumlckel was born in Germany on August 9th
1896 He studied mathematics and
physics in Berlin He is best known for his work in the field of chemistry and physics for
two contributions (1) Debye- Huumlckel theory of electrolytic solutions (2) Huumlckel
method of approximate molecular orbital calculations on electron systems In 1930 he
published his findings on systems in 1931 he generalized and expanded the system
40
theory to explain benzene Due to his poor communication skills his findings went
unrecognized for over 20 years It was in 1951 that his 4n + 2 rule was finally clarified by
Doering to show if C=C bonds would show aromaticity Huumlckel died on February 16th
1980 with very little worldwide recognition for his contributions to chemistry Today
chemistry students recognize his name and his contributions to the field are quite
substantial
One of the first semi-empirical methods to be developed was Huumlckel Molecular
Orbital Theory (HMO) HMO was developed to describe molecules containing
conjugated double bonds HMO considered only electrons in pi orbitals and ignored all
other electrons in a molecule The Extended Huumlckel Molecular Orbital Method (EH) was
developed out of the need to consider all valence electrons in a molecular orbital
calculation
By considering all the valence electrons chemists could determine molecular
structure compute energy barriers for bond rotations and determine energies and
structures of transition states for reactions By considering only the valence electrons the
computed energies could be used to choose between proposed transition states to clarify
reaction mechanisms The total valence electron wavefunction is described as a product
of the one-electron wave functions
1 2 3(1) (2) (3) ( )valence j n (31)
where n is the number of electrons and j identifies the molecular orbital Each
molecular orbital is written as a linear combination of atomic orbitals (LCAO)
1 12
N
j jr rrc j N
(32)
41
The energy of the jth
molecular orbital is given by a one-electron Schroumldinger
equation using an effective one electron Hamiltonian heff which expresses the interaction
of an electron with the rest of the molecule
eff j j jh (33)
This is the energy eigenvalue of jth
molecular orbital corresponding to the Eigen
function j The advantage of using this method is that the exact form of heff is not
required The total energy of the molecule is the sum of the single electron energies
j jj
E n (34)
where nj is the number of electrons in orbital j
In order to use the Extended Huckel method a set of calculation parameters and
approximations must be followed These parameters include the Basis set K-point and
the Brillouin Zone and lastly the Mesh cut-off
312 Introduction to NEGF
The Greenrsquos function is a function of two space-time coordinates From the knowledge of
this function one can calculate time-dependent expectation values such as currents and
densities electron addition and removal energies and the total energy of the system In
the absence of external fields the non-equilibrium Green function method reduces to the
equilibrium Green functions NEGF can be applied to both extended and finite systems
The generic system of NEGF consists of the electron dynamics of the channel described
by the Hamiltonian This channel consists of two contact reservoirs with respective
chemical potential μR and μL The NEGF assumes ballistic transport neglecting self-
42
energy from scattering The system is insulated from gate contacts whose effects are
realized via a 3D Poisson solver which solves for the potential at a given point in real
space based on electron density
22 ( ) [ ( ) ( )]D
qr N r n r
(35)
Figure 31 NEGF system
The system is easily expandable to systems with several contacts or gate
configurations by adding additional self-energy matrices to NEGF or additional sources
to the Poisson solver
313 Electrostatics
Electrostatic potential is created every time in the presence of a charge density due to an
induced electric field The Poissonrsquos equation correlates the electrostatic potential to
charge density as given in Equation 36
43
2( ( ) ( ) ( ) ( ))( )
( )( ) ( )
ADq p r n r r N rr
rr r
N
(36)
where ɛ(r) is the dielectric permittivity of the material ρ(r) n(r) ND(r) and NA(r) are the
hole electron donor and acceptor concentrations of the system respectively
Two types of boundary conditions are usually applied to the Poissonrsquos equation
Dirichlet boundary conditions
Φ (0) = F0 and Φ (L) = FL
von Neumann boundary conditions
00
( )
x
d x
dxB
and
( )L
x L
d x
dxB
For the transport problems with open boundary conditions the von Neumann
boundary conditions are used assuming that the potential vanishes at the boundary ie
B0=BL=0
The Poissonrsquos equation can hence be discretized on a grid as
2 ( )( )
( )
rx
r
= M (37)
where M is the matrix Φ and ρ are vectors containing the discretized values of
the electrostatic potential Φ and charge density ρ respectively
44
The Schroumldinger and Poisson equations are coupled since V(x) = -qΦ(x) is used
for the Schroumldinger to compute ρ(x) This self-consistent loop stops when the
convergence is reached
( )r
V(x) = -qΦ(x)
314 Non-Equilibrium Greenrsquos Function
Greenrsquos functions are a mathematical construction that are used to solve differential
equations subject to specific initial or boundary conditions They are named after the
British mathematician George Green The 1-D equation of L( )f( )=S( ) can be defined
by the Greenrsquos Function as given below
( ) ( ) ( )G x x f x x x (38)
The general Greenrsquos function is given by
( ) ( ) ( )f x dx G x x S x (39)
Applying the operator L( ) to the solution f( ) satisfies the original differential
equation The Greenrsquos Function G( ) is the propagator which propagates the influence
of a perturbation S( ) originally situated at the point to the point at which the
function f( ) is evaluated
The Greenrsquos Function G( ) can also be a correlation function If the points
and are strongly (weakly) correlated then S( ) will greatly (poorly) affect f( )
Poisson equation
2 ( )( )
( )
rr
r
Schroumldinger equation
2
2
( ( ) ) ( )
( )2
( ) | ( ) |
E H r E r S
H V rm
r dE E r
Figure 32 Self-consistent loop
45
The Schroumldinger equation with open boundaries can be written as
( )E H S (310)
Considering a 1-D and homogenous system ranging from =0 to L assuming
that Σ=0 and the form of equations is same before and after discretization then
22
2 0( ) ( ) ( )
2E x S x
m
dV
dx
(311)
The Greenrsquos function can hence be computed corresponding to the Schroumldinger
equation
22
2 0( ) ( ) ( )
2E G x x x x
m
dV
dx
(312)
Due to the delta-function at = a discontinuity is observed and hence the
Greens function is evaluated at boundary conditions
0
2
exp( ( )) x x 2 ( )( )
exp( ik(x x)) x x
ik x x m E VG x x k
A
A
(313)
By integrating the Schroumldinger equation twice and setting the lower and upper
integration boundaries to = -δ and = +δ the Greenrsquos Functions can be written as
2
( ) ( ) 0
( ) ( ) 2
x x x x
G x x G x x
dG x x dG x x m
dx dx
(314)
46
The coefficient A+ and A
- become
ik
mA A
(315)
The Greenrsquos Function takes a final form known as Retarded Greenrsquos Function and
is written as
( ) exp( | |)G x x i ik x xk
m (316)
And the wave function is
( ) ( ) ( )x dx G x x S x (317)
Retarded Greenrsquos Function propagates the wave functions generated by a source
or perturbation S from its origin at to any point
The retarded Greenrsquos Function as discretized Schroumldinger equation is written as
( )R RE H G I (318)
The wave function Φ can be calculated from the retarded Greenrsquos function and the
source vector as
Φ = GR∙S (319)
Overall in this section the Greenrsquos function approach in calculating the electron
dynamics is reviewed We defined the self-energy of each part of the system spectral
function and the probability current density the electric current is derived explicitly using
Non Equilibrium Greenrsquos function We will use this formalism to calculate the tunneling
phenomena in coupled quantum dots isolated or otherwise
47
CHAPTER 4
ATOMISTIX TOOLKIT DETAILS
41 Introduction
Virtual NanoLab (VNL) is a graphical user interface (GUI) that provides a group of
modeling tools the function of these tools involves the set-up investigation and the
study of nanoscale structures The quantum mechanical equations are solved by the
software by using the advanced software architecture and numerical methods to
implement ab initio calculations VNL simulates the electronic structure and calculates
the transport properties based on the two systems mentioned earlier NEGF and Extended
Huckel ATK is the main engine for computing the scripts and hence all the calculations
performed in VNL are done by ATK VNL is a user friendly software as it not only
allows creating a script but also helps to set up a virtual experiment
This thesis involves the use of VNL in order to study the effect of the width and
different orientations of the doped atoms Since the software allows for virtual
experiments it makes it much easier to study the I-V characteristics based on the change
in position of atoms
42 Device Structure
In this thesis AZA GNR p-n junction with boron doping (location) was created using the
ATK software which is based on NEGF and DFT Further the thesis discusses the
transport properties and the I-V curve of such junction
The input format of ATK is NanoLanguage which is an extension to Python
scripting language ATK uses the NEGF system for formalism of simulating device
48
Figure 41 Geometry of device configuration with two electrodes
37
The system is divided into three parts left central and right The implementation
relies on the screening approximation which assumes that the properties of the left and
right regions can be decribed by solving a bulk problem for fully periodic electrode cell37
This screening approximation is fulfilled when the electrode regions can be described by
an equilibrium electron distribution
Figure 42 The electron distribution in a device configuration which illustrates a left
moving scattering state with origin in right electrode37
The system assumes that in steady state the electron density of the central region
is constant in time and hence the electron density is calculated independently from each
electrode The electron density is given by the occupied eigenstates of the system
n(r) = nL(r) + n
R(r) (41)
49
The left and right densities are calculated by summing up the occupied scattering
states
nL(r) = sum
(42)
nR(r) = sum
(43)
The scattering states are usually calculated by first calculating the Bloch states in
the electrodes and then solving the Schroumldinger equation of the central region using the
Bloch state as matching boundary Instead of using the scattering states the ATK
software uses the NEGF method to calculate the non-equilibrium electron density
The electron density is given in terms of electron density matrix
D = DL + D
R (44)
The left density matrix is given by NEGF theory
DL = int
(45)
where
ρL(ɛ) =
(46)
ρL(ɛ) = is the special density matrix
Also if there is a non-equilibrium electron distribution in the central region then
the electron distribution in electrode is given by the Fermi function f with an electron
temperature TL
G(ɛ) =
(47)
G = retarded Green function
δ+ is an infinitesimal positive number and S H overlap the Hamiltonian matrices
L =
sum sum
(48)
50
L
is the broadening function of the left electrode given in terms of left electrode
self -energysum
43 Transmission Spectrum Calculations
Once the self-consistent non-equilibrium density matrix has been obtained the various
transport properties of the system can be calculated One of the most important properties
is the transmission spectrum from which the current and differential conductance can be
obtained
The transmission coefficient in ATK is obtained by the retarded Greens function
T(ɛ) = G(ɛ)ΓL(ɛ)G
ϯ(ɛ)Γ
R(ɛ) (49)
The transmission amplitude of individual scattering states may be obtained
through the Transmission Eigenvalues The ldquoTransmission Eigenvaluesrdquo is an analysis
which finds the eigenvalues of the transmission matrix
The transmission matrix at energy E and k-point is given by
Tnm(Ek) = sum (410)
where
= transmission amplitude from Bloch state ψn(k)
The transmission coefficient is given by the trace of transmission matrix
T(Ek) = sum (411)
Keeping in mind all quantities depend on the quantum numbers parametrically
Transmission eigenvalues sum up to the transmission coefficient
T = sum (412)
51
44 Calculating the Current
Current is calculated from the transmission coefficient using
I( ) ( )R L
L RL R
R LB B
eE f f dE
h
E EV V T T T
k kT T
(413)
where f is the Fermi function TRL is the electron temperature of the right or left
electrode and Tσ(E) is the transmission coefficient for the spin component σ
The chemical potentials of the left and right electrode given by
L
F R LR L
eVE
are defined relative to the Fermi level of the left electrode These chemical potential are
related to the applied bias and hencebiasR L
eV therefore bias L RV V V
The transmission spectrum itself is usually rather insensitive to temperature and is
used in self-consistent calculations but often depends strongly on the electrode voltages
Thus for an accurate estimate of the current the transmission spectrum should be
calculated self-consistently for each desired bias
ATK uses very precise method to calculate the transport properties of the system
Transmission spectra for various concentrations of boron doped graphene p-n junctions
are generated in this Chapter and various coefficients such as Seebeck Peltier and
Conductance are calculated
52
45 Calculating Transport coefficients
The linear response transport coefficient of an applied voltage difference or temperature
difference between the two electrodes is given by
Conductance
| dT 0
e
dI
dUG
(414)
Peltier coefficient
| d 0
Q
I
I
(415)
Seebeck coefficient
| 0
dUS I
dT T
(416)
These linear response coefficients are calculated by the Transport Coefficients To
perform these calculations the ATK uses the Electron Transmission Spectrum
53
CHAPTER 5
RESULTS AND DISCUSSION
51 Band Structure Analysis
The electronic bandstructure of GNR both doped and undoped are discussed in this
chapter
The armchair configuration of Pristine GNR (PGNR) has a band structure that is
dependent on its width This is explained by the fact that the sheet itself acts like a
potential well where the electrons are confined to form standing waves along Cr the
rolling vector albeit with slightly different boundary conditions (Cr = ma1 + na2
where m and n are integers and a1 and a2 are the unit cell vectors of graphene lattice) In
a GNR the two nodal points of the standing wave must be at the ribbon edge while in a
Single wall nanotube (SWNT) they can be anywhere ie a circumferential periodic
boundary condition
(a) (b)
Figure 51 Bandstructure of AGNR widths (a) 4 atoms (b) 5 atoms
54
(a) (b)
Figure 52 Bandstructure of AGNR widths (a) 6 atoms (b) 7 atoms
(a) (b)
Figure 53 Bandstructure of AGNR widths (a) 8 atoms (b) 9 atoms
55
(a) (b)
Figure 54 Bandstructure of AGNR widths (a) 10 atoms (b) 11 atoms
Figure 55 Bandstructure of AGNR with a width of 12 atoms
Figure 56 Variation in band gaps as the width (number of atoms) varies
0
05
1
15
2
25
0 2 4 6 8 10 12 14
Wdith vs Band Structure
eV
56
The band structure of 12 Atom AGNR is close to that of Ge (0626 eV) The
actual width of this nanoribbon is about 25 nm 12 AGNR has been fabricated
successfully and doped with various dopants Hence the 12 Atom AGNR has been chosen
to study the transport properties
A junction is created using ZGNR and AGNR To maintain the consistency in the
device analysis it is imperative that the band structure of ZGNR is also calculated From
the simulation it is evident that ZGNR-AGNR-ZGNR junction configuration displays the
Metal ndashSemiconductor-Metal configuration that is addressed in this work The Fermi
Level in all the Z-GNR nanoribbons of widths 4-12 lies within the conduction band
Figure 57 Band structure of ZGNR width (a) 4 atoms (b) 6 atoms
57
(a) (b)
Figure 58 Band structure of ZGNR width (a) 8 atoms and (b) 10 atoms
Figure 59 Band structure of ZGNR with a width of 12 atoms
In order to create viable junction that would show transistor properties doping of
the semiconductor part is necessary The 12 atom AGNR is doped with boron (p-type)
and nitrogen (n-type) - (Figure 510a) 4 N doped (Figure 510b) 4 B In both cases
the impurities lie on the edge of the atoms For 2 nitrogen doped GNR with the
58
impurities lying in the center of the ribbon the Fermi level is found to be in the
conduction band as shown in (Figure 510c) (Figure 510d) shows the position of N with
respect to the edge A very clear departure from the expected (the valence band extending
above Fermi level) is shown in (Figure 510a)
Figure 510 Band structures of Doped AGNR (a) 4 N Doped (b) 4 B Doped (c) 2
N Doped (d) position of Nitrogen from (c)
(a) (b)
(c) (d)
59
52 I-V Characteristics of GNR junction
In pristine graphene the chirality determines the conductivity as seen from the I-V curves
for various widths At certain widths the semiconducting properties are more
pronounced These widths determine the wavelengths of the standing waves which in
turn determine the sub-band locations in the E-k plot When the biasing potential
exceeds 012V the I-V curve shows linearity In case of the 8-atom wide PGNR the
band gap is about 03 eV and it is evident from the I-V plot that the On-State is + 033 V
The band gap of 10-atom and the 4-atom wide PGNR is large enough to show
semiconducting properties
Figure 511 Current Vs Voltage graph for varying graphene width showing
conductivity
-30000
-20000
-10000
0
10000
20000
30000
-3 -2 -1 0 1 2 3
Cu
rre
nt
(nA
)
Voltage (V) (bias)
Current (nA) Vs Voltage for varying graphene width
W=10
W=8
W=6
W=4
60
The ZAZ GNR Configurations show the properties of a semiconductor junction The 12
atom ZAZ structure is studied for its I-V characteristics In this Chapter undoped B-
doped N-Doped B and N Doped (P-N Junction) ZAZ junctions are simulated
Figure 512 ZAZ GNR junction device
61
The boron doped ZAZ junction I-V characteristics are shown below (Figure 513)
The impurity concentration is 2 and 4 Various device configurations are studied
Figure 513 I-V curve of Boron Doped ZAZ junction
-25000
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
25000
-205 -155 -105 -055 -005 045 095 145 195
Cu
rre
nt
(nA
)
VBias
2B_1G_R 2B_0G_R
4B_0G_L 4B_0G_C
4B_0G_R 4B_1G_L
4B_1G_C 4B_1G_R
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
-2 -1 0 1 2
Cu
ren
t(n
A)
VBias
4 B doped GNR Jn
62
Figure 514 I-V curve of Nitrogen Doped ZAZ
-25000
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
-2 -15 -1 -05 0 05 1 15 2
Cu
rre
nt(
nA
)
VBias
I-V Curve as function of Dopant location
2N_0G_L2N_0G_C2N_0G_R2N_1G2N_1G_C2N_1G_R
-15000
-10000
-5000
0
5000
10000
15000
-2 -1 0 1 2
Cu
rre
nt(
nA
)
VBias
2N_0G_C
2N_1G_C
63
Figure 513 and Figure 514 show the I-V characteristics of the GNR junction doped with
2 boron and nitrogen respectively The location of N and B is at the central region of
the edge of the GNR Both B doped and N doped GNR Junctions show significant
Negative Differential Resistance (NDR) This is more pronounced in case of nitrogen
doping Another interesting observation is increasing ohmic nature with the change in
location of the dopants Nitrogen doped device configuration exhibits a pronounced
semiconductor behavior and the NDR effect is observed to be minimal
53 Thermoelectric Properties
In this study the thermoelectric properties were simulated for the GNR Junctions that
displayed high NDR effect The variation in the Peltier coefficient with temperature is
shown as function of doping
When the concentration of nitrogen increases the dimensionless Figure of Merit
ZT seems to decrease considerably This is mostly explained by the decrease in both
conductivity and mobility of the electrons
ZT = S2σTk (51)
where S is the Seebeck coefficient σ is the electrical conductivity T is the
absolute temperature and k is the thermal conductivity
64
Figure 515 Variation of Peltier coefficient with temperature as function of
doping
Figure 515 shows the maximum Peltier coefficient for 2 boron This is
explained by the scattering by boron and the associated smallest mean free path
0
0001
0002
0003
0004
0005
0006
0007
0008
0009
001
250 270 290 310 330 350 370 390 410
ZT
T (K)
2B
4B
Undoped
2N
4N
65
CHAPTER 6
CONCLUSIONS
Graphene ZAZ junctions exhibit varying properties depending on the various structural
configurations In this thesis it was found that the transport properties of graphene
depend on their width the edge of GNR doping concentration and the type of dopant
used The calculations of the band structure contributed towards the determination of the
minimum length of GNR required for studying the transport properties The minimum
length had a band gap equivalent to that of germanium and hence the importance of the
width being 12 atoms wide This band gap indicated fluctuating changes when doped
with elements such as B and N The viable junction showing transistor properties was
hence created by doping the semiconductor part of ZAZ By doping the I-V
characteristics were studied which showed significant NDR which was more pronounced
in the case of nitrogen Also the changing positions of the dopants contributed towards
the I-V curve to be more ohmic The edge doping caused minimum NDR and
semiconductor behavior as compared to central doping Lastly the thermoelectric
properties were studied - the increasing concentration of N causes the Figure of Merit to
decline due to the decrease in conductivity as well as mobility of electrons
66
REFERENCES
1 Wikianswers What makes carbon unique
httpwikianswerscomQWhat_makes_carbon_so_unique (22 November)
2 Kopeliovich D D Graphite
httpwwwsubstechcomdokuwikidokuphpid=graphite (1128)
3 Barbier M Transport properties of nanostructures and superlattices on single layer and
bilayer graphene University Antwerpen Antwerpen 2012
4 Shylau A Electron transport interaction and spin in graphene and graphene
nanoribbons Linkoping Norrkoping 2012
5 HassJ R F T Li X Li Z Zong W A de Heer P N First E H Conrad C
AJeffrey and C Berger Applied Physics Letters 2006 89 (14) 143
6 Jones A Mechanical Exfoliation to Make Graphene and Visulization
httpcarbonchemwisceduFilesMechanicalExfoliationpdf (18 October)
7 Anteroinen J Structural and Electrical Characteristics of Graphene Field Effect
Transistors AALRO school of Electrical Engineering AALTO 2011
8 Novoselov K S A K G S V MorozovD JiangY Zhang S V Dubonos I V
Grigorieva A A Firsov Science 2004 306 (22)
9 Kosynkin D A L H A Sinitskii J R Lomeda A Dimiev K B Price and J M
Tour Nature 458 876
10 Yi Z Luyao Zhang Accounts of chemical research 46 (10) 2339
11 Eizenberg M B JM 1979 82 236
12 Yu Q K L J Siriponglert S Li H Chen Y P Pei S S Applied Physcis
Letters 2008 93 (113103)
13 Li X C W An J Kim S Nah J Yang D Piner R Velamakanni A Jung I
TutucE Banerjee S K Colombo L Ruoff R S Science 2009 324 1314
14 Schaefer H E Nanoscience Springer Berlin 2010
15 Levente Tapasztoacute G D Philippe Lambin amp Laacuteszloacute P Biroacute Nature Nanotechnology
2008 3 401
67
REFERENCES
16 Dacheng Wei Y L Advance Materials 2010 22 (30) 3241
17 Wei Yao K L Y GYGao Elsevier Solid State Communications 2013 153 52
18 Dacheng Wei Dagger Yunqi Liudagger Yu Wangdagger Hongliang ZhangdaggerDagger Liping HuangdaggerDagger
Yudagger a G NanoLetters 2009 9 (5) 1758
19 Nakada K M F G Dresselhaus and M S Dresselhaus PhysRevB 1996 54
(9858)
20 Son Y W C M L a L S G PhysRevLett 2006 97 (216803)
21 Raza H Graphene Nanoelectronics Springer 2012
22 Ryan W J Electronic Transport in Graphene p-n junctions Short Noise and
Nanoribbons Harvard University 2009
23 Fangping OuYang J X Rui Guo Hua Zhang and Hui Xu Nanotechnology 2009
20 6
24 Guo J Carbon nanotube electronicsModeling physics and applications Purdue
University West Lafayette IN 2005
25 Motta C S S-P MITrioni cond-matmes-hall 2012 7
26 B P Growing Graphene via Chemical Vapor Deposition Ponoma College Ponoma
2011
27 ZurichE Transport properties of three-terminal graphene devices University of
Science and Technology Norway 2008
28 Uichiro MIntroduction to the electron theory of metals
29 Robert Laughlin H S Additional background material on the Nobel Prize in Physics
1998 (410)
30 MarkGoerbig Quantum Hall Effects (11152013)
68
REFERENCES
31 Zurich E Transport properties of three-terminal graphene devices Norwegian
University of Science and Technology Norway 2008
32 Deepak R Klein Tunneling University og Tennessee Space Institute Tennessee
2011
33 Williams JR L D CMMarcus Quantum Hall Effect in a Gate-Controlled p-n
Junction in Graphene (1122013)
34 Avadhanulu MN P G K A Textbook of Engineering Physcis for BE BSc (Engg)
SChand New Delhi 1992
35 Andriotis A Applied Physics Letters 2007 91 (152105)
36 Qimin Yan B H dagger Jie Yudagger Fawei Zhengdagger Ji ZangDagger Jian Wudagger Bing-Lin Gu F
L Dagger and Wenhui Duandagger NanoLetters 2007 7 (6) 1473
37 Soler J M E A J D Gale A Garciacutea J Junquera P Ordejoacuten and D Saacutenchez-
Portal J Phys Condens Matter 2002 14 2745
v
ACKNOWLEDGMENTS
I would like to express my gratitude to my supervisor Dr NM Ravindra for the useful
comments remarks and engagement throughout the learning process of this Mastersrsquo
thesis Furthermore I would like to thank Vijay Kasi Somayajula for introducing me to
the topic as well for the support I thank Dr Tao Zhou Dr Ken Ahn and Dr Halina
Opyrchal for serving on my thesis Committee I would like to thank my loved ones who
have supported me throughout the entire process both by keeping me harmonious and
helping me in putting pieces together
vi
TABLE OF CONTENTS
Chapter
Page
1 INTRODUCTIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
1
11 Graphene The New Carbonhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
1
12 Graphene Synthesishelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
3
121 Synthesis of Graphene on Nickel (Ni)helliphelliphelliphelliphelliphelliphelliphellip
5
122 Synthesis of Graphene on Copper (Cu)helliphelliphelliphelliphelliphelliphelliphellip
8
123 Transfer of Graphene Filmshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
8
124 Synthesis of Graphene Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
9
125 Doping in Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
10
126 Nitrogen (N) Doped Graphene Synthesis (Substitutional)hellip
12
13 Structure of Graphene Nanoribbon (GNR)helliphelliphelliphelliphelliphelliphelliphelliphelliphellip
13
14 Overview of Graphene Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
15
2 RESEARCH BACKGROUNDhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
21 Bandstructure of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
22 Transport Characteristics of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
20
23 Drude Theoryhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
22
24 Quantum Hall Effect (QHE)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
24
25 Resistivity and Resistancehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
27
26 Klein Tunnelinghelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
28
27 Quantum Hall Effect in Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
31
28 Thermoelectric Effecthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 34
vii
TABLE OF CONTENTS
(Continued)
Chapter Page
281 Seebeck Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
34
282 Peltier Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
36
29 Early Research ndash ab initio Studyhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
37
3 COMPUTATIONAL DETAILShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
31 Introductionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
311 Extended Huckel Theory helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
312 Introduction to NEGFhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
41
313 Electrostaticshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
42
314 Non-Equilibrium Greenrsquos Functionhelliphelliphelliphelliphelliphelliphelliphelliphellip
44
4 ATOMISTIX TOOLKIT DETAILShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
41 Introductionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
42 Device Structurehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
43 Transmission Spectrum Calculationhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
50
44 Calculating the Currenthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
51
45 Calculating the Transport Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
52
5 RESULTS AND DISCUSSIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
53
51 Band Structure Analysis helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
53
52 I-V Characteristics of GNR Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
59
53 Thermoelectric Propertieshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
63
6 CONCLUSIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 65
REFERENCEShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
66
viii
LIST OF FIGURES
Figure Page
11 (a) Chemical representation of Carbon (b) Graphite ore (c) Structure of
Graphite and a single layer Graphenhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
2
12 An optical image of Graphene flake obtained by exfoliation of
graphitehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
3
13 (a) Graphene formation on Nickel (b) Graphene atoms on Ni (111)
lattice (c)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
7
14 (a) SEM image of graphene on copper foil (b) High-resolution SEM
image of graphene on Cuhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
8
15 (a) Transfer process (b) Wafer-scale synthesis of graphene (c) Graphene
films transferred onto glass wafer (d) SiSiO2 with device patterned (e)
PET filmhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
9
16 (a) High-magnification image of the annealed sample showing that well-
defined zigzag armchair and zigzag-zigzag edges are formed (b) ) STM
image of an 8 nm wide bent junction connecting an armchair and a
zigzag graphene nanoribbon which was carved by STM
tipshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
10
17 Band structure of graphene before and after doping The image shows
shift towards the Fermi levelhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
11
18 Low resolution TEM image of N-doped graphene Background is the
lacey carbon TEM grid graphene sheet is crumpled with many
rippleshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
13
19 Zigzag and Armchair orientation of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphellip 13
110 Bandstructure of ZGNRhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 14
111 Bandstructure of AGNRhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 15
21 Left Real space Graphene lattice with basis vectors and Right
The first Brillouin zone of Graphene in reciprocal space with basis
vectors and K and Krsquo are responsible for massless transport at low
energyhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
ix
LIST OF FIGURES
(Continued)
Figure Page
22 Bandstructure of a graphene sheet showing a band gap of 0eVhelliphelliphellip 18
23 Band structure of Graphene calculated with the tight-binding modelhellip 19
24 The energy dispersion around the K pointhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 22
25 Electrons colliding with stationary ionshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 23
26 (a) 2D electrons in a perpendicular magnetic field Logitudinal resistance
measured across C5 and C6 Transverse resistance measured across C3
and C5 (b) Classical Hall resistance as a function on the magnetic field
25
27 Klein tunneling through an npn barrierhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 29
28 Electron trajectory considering the linear electrostatic potential U(x) = Fx 30
29 Electron like and hole like trajectories at same Ehelliphelliphelliphelliphelliphelliphelliphelliphellip 30
210 Quantum Hall effect in graphene 22
The Hall conductivity σxy and the
longitudinal resistivity of monolayer graphene as a function of carrier
density at B = 14T and T= 4K This shows half-integer QHE with chiral
index J= 1helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
32
211 (a) LL for Graphene bilayer (b) Schematics of Hall conductivity as a
function of nn0 for bilayer Graphene (solid line) and monolayer
Graphene (dotted line) (c) LL for monolayer Graphenehelliphelliphelliphelliphelliphelliphellip
33
212 Seebeck Effecthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 35
213 Transmission functions in units of (2e2h) for AZA structureshelliphelliphelliphellip 37
214 I-V curve for a 591nm long channel (Vbias=20mV)helliphelliphelliphelliphelliphelliphelliphellip 38
31 NEGF systemhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 42
41 Geometry of device configuration with two electrodeshelliphelliphelliphelliphelliphelliphellip 48
42 The electron distribution in a device configuration which illustrates a left
moving scattering state with origin in right electrodehelliphelliphelliphelliphelliphelliphelliphellip
48
x
LIST OF FIGURES
(Continued)
Figure Page
51 Band structure of AGNR widths (a) 4 atoms (b) 5 atomshelliphelliphelliphelliphelliphellip
53
52 Band structures of AGNR widths (a) 6 atoms (b) 7 atomshelliphelliphelliphelliphelliphellip 54
53 Band structure of AGNR widths (a) 8 atoms (b) 9 atomshelliphelliphelliphelliphelliphelliphellip 54
54 Band structures of AGNR widths (a) 10 atoms (b) 11 atomshelliphelliphelliphelliphellip 55
55 Band structure of AGNR with a width of 12 atomshelliphelliphelliphelliphelliphelliphelliphelliphellip 55
56 Variation in band gaps as the width (number of atoms) varieshelliphelliphelliphellip 55
57 Band structure of ZGNR width (a) 4 atoms (b) 6 atomshelliphelliphelliphelliphelliphelliphellip 56
58 Band structure of ZGNR width (a) 8atoms and (b) 10 atoms 57
59 Band structure of ZGNR with a width 12 atomshelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 57
510 Band structures of Doped AGNR (a) 4 N Doped (b) 4 B Doped (c)
2 N Doped (d) position of Nitrogen from (c)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
58
511 Current Vs Voltage graph for varying graphene width showing
conductivityhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
59
512 ZAZ GNR junction devicehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 60
513 I-V curve of Boron Doped ZAZ junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 61
514 I-V curve of Nitrogen Doped ZAZhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 62
515 Variation of Peltier effect coefficient with temperature for various doping 64
1
CHAPTER 1
INTRODUCTION
11 Graphene The New Carbon
Carbon (chemical symbol C atomic mass 1207amu) (Figure 11a) is a widely distributed
element in nature It is found abundantly in the sun stars comets and the atmospheres of
the planet Carbon can form up to four bonds it can bond with itself endlessly and with
most other elements in many different shapes making it a significant part of the
construction for many kinds of complex molecules1
Two allotropes of carbon are commonly used diamond and graphite (Figure
11b) The bonding structures of diamond and graphite contribute to the properties
individually In diamond all the p-orbitals are used forming a sp3
bonding whereas in
graphite only two orbitals are occupied allowing the unpaired bond for the transport of
electrons Each carbon atom in graphene possesses sp2 hybridization ie each carbon
atom is connected to three other carbon atoms via covalent bonds with a bond length of
142Å and an angle of 120deg between each bonded pair This makes graphite a better
conductor than diamond Graphite consists of many layers of 2D carbon lattices (Figure
11c) stacked on top of each other and held via Van der Waals forces A single layer of
graphite where carbon atoms are arranged in a honeycomb lattice is known as graphene
(Figure 11c)
2
Figure 11 (a) Chemical representation of Carbon (b) Graphite ore (c) Structure of
Graphite and a single layer Graphene2
Theoretical work on graphene was done specifically to study the other allotropes
The first study was done by Wallace in 1947 who calculated the band structure of
graphene3 Further the peculiar Landau levels were known by McClure in 1957 and the
relativistic Hofstadter butterfly by Ramal in 19853 Later in 1991 the invention of carbon
nanotubes by Iijima boosted the theoretical research on graphene3 Prior to the invention
of carbon nanotubes there were a few experimental papers on graphene growth via
various methods like intercalation of graphite (Shioyama 2001) free standing (Boehm
1962) epitaxial as well as graphene grown on metals (Bommel 1975 Land 1992 Itoh
1991)3 With all the various discoveries the electronic properties of graphene were not
studied until 2004 when Berger and Novoselov were able to access the electronic
properties with contact of graphene flakes3 (Figure 12)
3
Figure 12 An optical image of Graphene flake obtained by exfoliation of graphite3
The specific lattice structure of graphene possesses a number of unique electronic
properties making it an interesting material for theorists experimentalists and engineers
Utilization of graphene as a fundamental block of electronic devices requires
development of new theoretical methods for understanding the current propagations in
graphene constriction4
12 Graphene Synthesis
The discovery of graphene by mechanical exfoliation called the lsquoScotch tape methodrsquo led
to serious attempts towards the production of top quality graphene5 Graphene was first
exfoliated mechanically from graphite in 20046 The importance of high quality graphene
cannot be emphasized enough however electron transport has shown that defects play an
important role in hindering the transport properties of electrons (holes)7 The two
synthesizing methods for the large scale manufacture of graphene are chemical vapor
deposition (CVD) and silicon carbide (SiC) desorption method
4
Graphene can be synthesized by sublimation of silicon from SiC at high
temperature (1200degC) in high vacuum5 The major advantage of this method is that the
SiC provides an insulating substrate and no transfer of the graphene layer is needed Yet
the disadvantage of this method outweighs its advantages the high temperature is cost-
ineffective making it unsuitable for large scale manufacturing8 Also the crystal growth
face alters the properties of graphene Graphene grown on Si-terminated face has poor
homogeneity and is subjected to unintentional doping7 Conversely graphene grown on
C-terminated SiC has higher mobility and is often called lsquoturbostaticrsquo due to the
rotational disorder7
Unlike the SiC method the graphene produced via CVD method needs to be
transferred to a substrate making it difficult to maintain the quality of graphene Yet
CVD synthesized graphene has a larger grain size7 More research is being done on
various methods for synthesis of graphene The methods include direct chemical
synthesis ion implantation crystal sonification and lastly unzipping carbon nanotubes to
form graphene sheets9
Graphene and few-layer graphene have been grown by CVD from carbon
containing gases on catalytic metal surfaces andby surface segregation of C dissolved in
the bulk of such metals7 Growing graphene with CVD is a very attractive solution since
it is compatible with the existing semiconductor industry9 Graphene has been grown via
CVD process on metal substrates such as Nickel (Ni) and Copper (Cu)
5
121 Synthesis of Graphene on Nickel (Ni)
Polycrystalline Ni films are annealed in ArH2 atmosphere at 900-1000degC to increase
grain size and are then exposed to H2CH4 gas mixture10
In this step the hydrocarbon
decomposes and dissolves in Ni to form a solid solution Lastly the samples are cooled in
argon gas Ni has high carbon solubility at elevated temperatures and the solubility
decreases as temperature is reduced During the cooling process the carbon atoms diffuse
out from the Ni-C solid solution and precipitate on the Ni surface to form graphene films
(Figure 13a) Since Ni (111) has a lattice similar to the densely packed hexagonal lattice
of graphene (Figure 13b) they also have similar lattice constants and hence Ni surface
serves as an excellent lattice matched substrate for graphene growth11
The growth of graphene on Ni is based on carbon segregation and precipitation
process different segregation behavior is produced by different cooling rates which
affect the thickness and quality of graphene films12
Medium cooling rates lead to optimal
carbon segregation and produce few layers12
Graphene films grown on Ni are usually
continuous with monolayer and few layer regions Annealing of Ni substrates at elevated
temperatures in hydrogen atmosphere not only increases the single-crystalline Ni grain
size but also eliminates certain impurities in Ni thereby improving the graphene quality
Furthermore the graphene thickness can also be affected due to the amount of carbon
dissolved in the Ni films during the growth time
After synthesis the graphene can be transferred to other insulator substrates for
further characterization and applications Figure 13c shows the selected area electron
diffraction pattern of graphene film along the [001] direction which confirms the
graphene lattice structure shown After transfer to insulator substrates the geometry can
6
be retained as shown in Figure 13d Under optimal growth parameters graphene growth
is only limited by the Ni catalyst Lastly Figures 13e and 13f show the wafer-scale
graphene synthesis and transfer of graphene to a flexible transparent substrate
respectively
Though polycrystalline Ni is a good substrate the percentage and size of
graphene monolayer are still limited Researchers have hence tried other metal substrates
for graphene synthesis
7
Figure 13 (a) Graphene formation on Nickel (b) Graphene atoms on Ni (111) lattice
(c) Low magnification TEM image of graphene edges (d) Optical image of graphene
transferred from the Ni surface to SiO2Si substrate (e) Full-wafer scale deposition of
graphene layers on polycrystalline Ni (f) Transparent and flexible graphene films on
PDMS substrate10
8
122 Synthesis of Graphene on Copper (Cu)
Graphene films are grown on 25microm thick Cu foils in a hot wall furnace13
The Cu foil is
first annealed in hydrogen atmosphere at 1000degC and a mixture of H2CH4 is introduced
into the system to initiate graphene growth After a continuous graphene layer is formed
on the Cu foil the system is cooled to room temperature Figure 14a shows an SEM
image of graphene on Cu substrate indicating the Cu grains with contrast The Cu
surface steps are formed during thermal annealing and the darker flakes indicate multiple-
layer graphene (Figure 14b)10
The graphene wrinkles in Figure 14(b) originate from
different thermal expansion coefficient of graphene and Cu They go across the Cu grain
boundaries indicating that the graphene film is continuous
Figure 14 (a) SEM image of graphene on copper foil (b) High-resolution SEM image of
graphene on Cu10
123 Transfer of Graphene films
In order to facilitate the applications of graphene for electronic applications we need to
separate the graphene from the catalytic metal substrate Figure 15a shows the transfer
process of graphene Graphene is first coated with a thin layer of polymethyl
methacrylate (PMMA) and baked at 120degC to evaporate the solvent10
The metal layer is
then removed by Ni or Cu etchant leaving behind the PMMA graphene film The film is
then cleaned by deionized water and then transferred onto the target substrate After the
9
evaporation of water vapor the PMMA is removed by acetone leaving graphene film on
top of the target substrate Figure 15b shows a graphene wafer transferred from the
substrate onto glass and polyethylene terephthalate (PET) films
Figure 15 (a) Transfer process (b) Wafer-scale synthesis of graphene (c) Graphene
films transferred onto glass wafer (d) SiSiO2 with device patterned (e) PET film10
124 Synthesis of Graphene Junction
Graphene junctions with smooth armchair and zigzag edges are difficult to produce by
conventional methods such as mechanical exfoliation chemical exfoliation or lithography
etching14
The conventional methods can only produce rough edges Recently
Dresselhaus reported an edge reconstruction of graphene by Joule heating in a TEM-STM
10
(Figure16b) system15
An individual nanoribbon sample is attached to the sample holder
at one end and to the STM tip at the other end these ends also serve as the two
electrodes The structural transformation in the growth of graphene from armchair to zig-
zag is mainly attributed to the vaporization of carbon edges that reconstruct at high
temperatures in which resistive Joule heating and preferred current flow play an
important role This means that by controlling the flow of current a perfectly smooth
edged ribbon can be synthesized making graphene-based electronics possible16
Figure 16 (a) High-magnification image of the annealed sample showing that well-
defined zigzag armchair and zigzag-zigzag edges are formed (b) STM image of an 8 nm
wide bent junction connecting an armchair and a zigzag graphene nanoribbon which was
carved by STM tips14
125 Doping in Graphene
The doping of graphene can be roughly classified into two categories - electrical and
chemical Electrical doping involves changing gate voltages of graphene devices and
chemical doping uses chemical routes such as substitutional or interstitial This thesis
discusses chemical doping and the importance of doping sites by changing the dopant
Chemical doping is a common approach to tailor the electronic properties of
11
semiconductors Doping of graphene can cause its electronic properties to alter leading to
a metal-semiconductor transition The two means of doping graphene are interstitial and
substitutional In interstitial doping the dopant atoms or molecules are introduced as
adatoms or admolecules on the surface of graphene whereas in substitutional doping the
dopant atoms are replaced in the carbon lattice forming a bond in the lattice of
graphene16
Doping graphene results in the formation of n or p-type semiconductors
depending on the kind of dopant If the dopant is an electron donor it causes the Fermi
level to shift up resulting in n-type behavior of graphene Furthermore if the dopant is an
electron acceptor it causes the Fermi level to shift down resulting in a p-type behavior of
graphene (Figure 17)16
Figure 17 Band structure of graphene before and after doping The image shows shift
towards the Fermi level16
Graphene nanoribbons (GNR) can be made into a p- and n- type semiconductor
by doping with boron (B) and nitrogen (N) respectively In theory GNR p-n junction is
formed by doping GNR with B and N in different regions However experimentally
doping graphene with both these elements is very difficult due to the dopants reacting
with each other17
Hence most experimental studies use GNR doped by only one
12
element N-doped graphene was synthesized by Wei et al Wang and B-doped Graphene
was realized by Endo17
Many researchers have demonstrated interstitial doping of graphene by gas metal
and organic molecules16
The various gases and metals used are NO2 NH3 An-CH3 Na-
NH2 F4-TCNQ TPa TCNE and others16
Doping in graphene is hence possible by
electrons or holes in high concentration without deterioration of its mobility Interstitial
doping is highly sensitive due to most of the conducting channel being exposed to surface
absorbates and hence can be used in molecule detection
In substitutional doping the dopant atoms are included in the graphene lattice and
thus chemically bonded Substitutional doping is done via the CVD method using a
carbon and dopant source Substitutional doping opens up many applications in device
engineering making graphene a very good candidate as a semiconductor This study
involves the study of transport properties of graphene doped by substitution
126 Nitrogen (N) Doped Graphene Synthesis (Substitutional)
N-Doped graphene is prepared via a CVD process using a 25microm thick Cu film on a Si
substrate The substrate is placed in a quartz tube with the flow of hydrogen (20sccm) and
argon (100 sccm)18
When the center of the furnace reaches 800degC 60 sccm of CH4 and
60 sccm of NH3 is introduced into the flow as C source and N source respectively The
substrate is then moved to high temperature and after 10 min growth the sample is
cooled to room temperature under H2 ambient Figure 1 8 shows the growth of N-doped
graphene18
13
Figure 18 Low resolution TEM image of N-doped graphene Background is the lacey
carbon TEM grid graphene sheet is crumpled with many ripples18
13 Structure of Graphene Nanoribbon (GNR)
Graphene Nanoribbons (GNR) are strips of graphene with very thin width of lt50nm
GNRs can be terminated in three separate ways called zig-zag (0 n) armchair (m 0) and
chiral (m n) (Figure19) and this termination along the width of the ribbon dictates the
size of the band gap19
Figure 19 Zigzag and Armchair orientation of Graphene5
Due to their various edge structures GNRs exhibit different electronic properties
ranging from normal semiconductors to spin-polarized half metals which open the
possibility of GNRs as electronic devices19
14
Within a tight binding approach (AGNRs) could be metallic or semiconducting
depending on their ribbon width but all zigzag graphene nanoribbons (ZGNRs) are
metallic with a high density of electronic states at the edges Hence ZGNRs exhibit
characteristic edge effects which are not present in AGNRs These edge effects in
ZGNR create a flat band close to the Fermi level making the ZGNR edges more
reactive19
First-principles calculations show that the GNRs possess a non-zero direct
band gaps These gaps are small for ZGNR (Figure 110) caused due to spin ordering
effects at the edges For AGNRs the band gap arises from quantum confinement (Figure
111) effect that has larger magnitudes than ZGNR20
Figure 110 Band structure of ZGNR
15
Figure 111 Band structure of AGNR
For GNRs the band gap decreases as the ribbon width increases and in order to
create a semiconductor with a desirable band gap the nanoribbon width should be
adjusted accordingly This property of adjusting the band gap makes graphene an
excellent candidate for transistor switching By applying an electric field GNR can be
altered from an insulator to a conductor GNRs exhibit very intriguing properties and
have become one of the promising candidates for electronic applications
14 Overview of Graphene Junction
The invention of p-n junctions date back to 1940s which later resulted in the invention of
junction transistors One of the key technological reasons for success of the p-n junction
is mainly due to its ability to locally modulate the energy band gaps via an applied bias21
A graphene p-n junction is created via single layer of graphene in which the
carrier type and density in two adjacent regions are controlled by electrostatic gating8
For materials with a band gap the electric field can either switch lsquooffrsquo the current or
rectify it (p-n diode)22
Being a ldquogaplessrdquo material the off state is not achievable in
16
graphene In order to achieve an off state the gap can be created by doping graphene with
various elements (Group III or Group V) Doping allows p-n junctions to be
reconfigurable using a gate voltage to distinguish between graphene p- n regions within a
single sheet Many researchers have studied the electronic as well as transport properties
of doped graphene junctions
In 2009 Fangping OuYang studied the transport properties of T-shaped graphene
junctions using the ATK software and showed that the conductance depends on
geometric structures which can be controlled by selective doping23
Wei Yao in 2013
studied the transport properties in graphene p-n junctions and showed that the
rectification effect depends on boron doping density and position17
The study of transport properties in graphene p-n junctions is a recent
advancement The thesis discusses transport properties including the current-voltage (I-
V) characteristics of doped graphene junctions Moreover the software used is similar to
the software in use by current researchers since they have produced viable data using
ATK
17
CHAPTER 2
RESEARCH BACKGROUND
21 Band Structure of Graphene
The unique electronic properties of graphene were first predicted in 1946 Figure 21
shows a top view of the hexagonal arrangement of carbon atoms in real space as well as
the first Brillouin zone in reciprocal space
Figure 21 Left Real space graphene lattice with basis vectors and Right The
first Brillouin zone of graphene in reciprocal space with basis vectors and
K and
Krsquo are responsible for massless transport at low energy24
The real space basis vectors are radic
and
radic
The reciprocal space basis vectors are 1 2
0 0
4 1 3 4 1 3( )and ( )2 2 2 23 3
b x y b x ya a
where the magnitude of the basis vectors is |a0| = radic acc The distance between nearest
neighbor carbon atoms is acc=0142nm
18
The band structure can be calculated by solving the eigenvalues using the
dispersion relation E( )
1 2 3( ) 3 2cos 2cos 2cosE k t k a k a k a (21)
Transport properties of solids are closely related to the energy dispersion
relations E ( ) in the material and in particular to the behavior of E ( ) near the Fermi
level Graphene is a zero gap semimetal whose specific linear electronic band dispersion
near the Brillouin zone corners (Dirac points) gives rise to electrons and holes that
propagate as massless Fermions25
The valence and conduction bands do not overlap in
graphene they touch at the Fermi Level (Figure 22)
Figure 22 Band structure of a graphene sheet showing a band gap of 0eV
The low energy properties of graphene can be well described by making a linear
expansion of the band structure around the K and Krsquo This energy can be written as
19
E(k) = plusmnħvF|k (22)
where vF is the Fermi velocity of 1106ms given by
1F
Ev
k
ħ (23)
Figure 23 Band structure of graphene calculated with the tight-binding model
22
The Fermi surface of graphene consists of double cones with Fermi energy at the
intersection of these cones (Figure 23) The slope of the band is zero and hence the
effective mass of electrons in that region is zero which leads to an entirely new transport
mechanism in graphene26
20
22 Transport Characteristics of Graphene
Transport process usually involves a flow of charge or energy or both The flow is mainly
due to external perturbations such as electric field and temperature gradient The
relationship between forces and flow usually defines various transport coefficients that
are the characteristics of electrons and phonons in the material All modern electronics
are based on the ability to control the electronic properties of a material by applying
external voltage This is done by an electric field effect where the gate voltage changes
the carrier concentration of the material and consequently its conductivity The electric
field effect in graphene was reported by Novoselov in 2004 and is used in transport
measurements8
The electron-phonon interaction in graphene plays an important role in
understanding the photoemission spectra observed in graphene The electric field effect is
an alternative method for changing the charge carrier density in low dimensional systems
The electric field effect in graphene which was first reported by Novoselov et al in
2004 is widely used as a characterization tool in transport measurements25
The transport characteristics of the material are directly related to the
bandstructure of graphene The carriers in graphene lattice are free to move in two
dimensions In the carrier transport of graphene the carriers ndash electrons and holes ndash close
to the Dirac points are of importance The transport is described by a two component
wave function (Equation 24) which obeys the 2D Dirac-like equation for massless
particles27
21
-ivFσ nablaψ(r) = Eψ(r)
(24)
where σ is the 2D Pauli spin matrix In the continuum limit the above (Equation
24) corresponds to the effective low energy Dirac Hamiltonian (Equation 25)
0( )
0
x y
F F
x y
iH k k
i
k kv v
k k
(25)
The electronic band structure of the energy (E) versus wave vector (k) relation for
graphene is given by Equation 24
The two component wave function resembles the spin or wave function of
quantum electro dynamics (QED)27
Corresponding to the spin of particles in QED the
charge carriers of graphene can be attributed with a pseudospin σ The pseudospin is the
direct result of two different carbon sublattices corresponding to the bonding and
antibonding combinations27
22
Figure 24 The energy dispersion around the K point27
In Figure 24 the red and blue lines correspond to the antibonding and bonding
states respectively The pseudospin can have two values either in the direction of or
against the momentum It can be seen that the electrons with energy E travelling in the
positive direction originates from the same branch as a hole with energy ndashE travelling in
the negative direction giving it the same pseudospin This results in suppressed
backscattering and Klein tunneling The back scattering process requires the pseudospin
to flip which is possible in the presence of short range scatters that act differently on sub
lattices27
23 Drude Theory
The classical theory of metallic conductivity was presented by Drude in 1900 and was
elaborated by Lorentz in 190528
Drude treated the free electrons as classical ideal gas
meaning the electrons collide with stationary ions and not each other
23
Figure 25 Electrons colliding with stationary ions28
The Drude theory applied the kinetic theory of gases to a metal considered as a gas of
electrons The basic assumptions made by the Drude theory are28
When metallic elements are brought together to form a solid then the valence
electrons become freely moving through the metal whereas the ions remain intact
as nearly immobile positive particles
Between collisions the electrons move freely ie there is neither electron-
electron interaction nor electron-ion interaction
The scattering mechanism leads to instantaneous collisions of the electron with
the scatterers
The collisions are characterized by a relaxation time τ
The electrons achieve thermal equilibrium only through collisions the velocity
after a collision is randomly directed the speed is as appropriate to the
temperature
With the relaxation time Drude obtained the electrical conductivity expression
where n is the number of electrons per unit volume
σ = ne2τm
(25)
He also calculated the thermal conductivity and successfully provided the
theoretical basis for Wiedemann-Frantz law already established in 1853 which states that
24
the ratio of electrical and thermal conductivity of any metals is a universal constant at any
given temperature28
The Drude theory gives results which are qualitatively correct outside of the
quantum Hall regime28
In the Drude theory of the electrical conductivity of a metal an
electron is accelerated by the electric field for an average time τ before being scattered
by impurities lattice imperfections and phonons to a state which has zero average
velocity The average drift velocity of the electron is
d
eE mv (26)
It is assumed that all electrons drift together and hence the current density
j = -ne (27)
This Drude theory works well for fields below ~ 01T At stronger fields the Hall
resistivity becomes nearly constant over finite intervals of magnetic fields28
The QHE
reflects both novel disorder physics as well as novel interaction physics in the quantum
Hall regime
24 Quantum Hall Effect (QHE)
The discovery of QHE is a remarkable achievement in condensed matter physics The
Hall Effect was discovered by Edwin Hall in 187929
However the precise quantization
of the Hall conductance in units of e2h was not recognized until February 1980 Five
years later in 1985 Klaus von Klitzing was awarded the Nobel Prize in Physics for the
discovery of QHE29
The quantum Hall effect occurs in two-dimensional electron systems in the limit
of strong perpendicular magnetic field that stems from electronic transport
25
measurements where one drives a current I through the sample and where one measures
both the longitudinal and transverse resistance (Hall resistance) A longitudinal resistance
is a resistance measured between two contacts that may be connected by a line which
does not connect C1 and C430
Transverse resistance is measured between two contacts
connected by an imaginary line connecting C1 and C4 (Figure 26a)
Figure 26 (a) 2D electrons in a perpendicular magnetic field Logitudinal resistance
measured across C5 and C6 Transverse resistance measured across C3 and C5
(b) Classical Hall resistance as a function on the magnetic field30
Due to the existence of quantum Hall effect it is natural to expect that there exists
a classical Hall Effect Hall showed that the transverse resistance of a thin metallic plate
varies linearly with the strength B of the perpendicular magnetic field (Figure 26 b)
RH = Bqnel (28)
More quantitatively the classical Hall Effect can be understood within the Drude
model for diffusive transport in a metal Within this model one considers independent
26
charge carriers of momentum p described by the equation of motion
( )
b
dp p pe E B
dt m (29)
where E and B are the electric and magnetic field respectively The macroscopic
transport characteristics ie resistivity of the system are obtained from the static
solution of the equation of motion dpdt = 0 and one finds for 2D electrons with p =
(pxpy)
x
x yb
y
y xb
eBe
eBe
ppE
m
ppE
m
(210)
In the above expression characteristic frequency is visible as
C
b
eB
m (211)
This is known as cyclotron frequency as it characterizes the cyclotron motion of a
charged particle in a magnetic field30
With the Drude theory the conductivity can be
written as
j = -enelpmb (212)
and the mobility can be given as
micro = eτmb (213)
The transport properties in the limit of ωCτ-gt infin are entirely governed in the presence of
27
a magnetic field by the off-diagonal ie transverse components of
conductivityresistivity
The theory of quantum Hall effect subjects all physical properties of 2D electron
system in the limit where the magnetic field is strong so that the mixing of Landau levels
by disorder or electron-electron interaction is considered to be a weak perturbation30
This is known as the quantum Hall regime The ratios between the energy scales
corresponding to the two interactions are important The limit where disorder potential is
much stronger is referred to as integer quantum hall regime whereas the limit where the
interaction potential is much stronger is referred to as fractional quantum Hall regime
25 Resistivity and Resistance
The electronic transport in the framework of the Drude theory allows for the calculation
of conductivity or resistivity of a classical diffusive 2D electrons in a magnetic field30
The conductivity and conductance are related to one another but they depend on the
geometry of the conductor-the resistance R and hence the resistivity is given by
R = (LA)ρ (214)
where L is the length of the conductor and A is the cross section
For a d-dimensional conductor the cross section scales as Ld-1
such that the
scaling relation between the resistance and the resistivity is
R~ ρL2-d
(215)
From the dimension point of view resistance and resistivity are the same in 2D and the
resistance is scale-invariant Further the resistance of a 2D conductor depends in
general on the so-called aspect ratio LW via some factor f (LW)30
However for
transverse Hall resistance it is the length of the conductor that plays the role of cross
28
section such that the Hall resistivity and the Hall resistance truly coincide ie f=1 The
Quantum Hall effect is highly insensitive to the particular geometric properties of the
sample used in transport measurements Recently quantum Hall physics experienced the
discovery of ldquorelativisticrdquo quantum Hall effect in graphene The electrons in graphene
behave as if they were relativistic massless particles contributing to a very interesting
field of research30
26 Klein Tunneling
Klein tunneling in which relativistic particles penetrate through a potential barrier
without the exponential damping that is characteristic for nonrelativistic quantum
tunneling has never been observed for elementary particles The tunneling allows
transmission of a particle through a potential barrier higher than its kinetic energy
violating the principle of classical mechanics30
On the quantum scale the objects exhibit
wave-like characteristics in which the quanta move against a potential hill described by
their wave function This wave function represents the probability amplitude of finding
the object in a particular location The transmission of the object through the potential hill
is termed as tunneling When EltV then the ψ(x) over V is returned by ψrsquo(x) In quantum
mechanics an electron tunnels from the conduction into the valence band Such a
tunneling from an electron-like to hole-like state is called as Klein Tunneling in which the
electron avoids backscattering
In Figure 27 it is shown that an electron hitting a potential barrier is reflected
with 100 certainty In non-relativistic quantum mechanics the electrons can tunnel
through the barrier but the probability of tunneling exponentially decays with increasing
29
height and width of the barrier However in relativistic quantum mechanics the barrier
gets transparent even in the limit of infinite barrier height (Klein paradox)31
Figure 27 Klein tunneling through an npn barrier30
The Klein paradox in graphene can be understood in terms of electrons and holes
In graphene the massless carriers behave differently than ordinary carriers (with mass) in
the presence of an electric field A barrier which is repulsive for electrons will be
attractive for holes Since there are hole states inside the barrier with the same energy as
the electrons outside an electron arriving at the barrier can tunnel through it as a hole
before leaving again as an electron Klein tunneling for transport in graphene is that the
charge carriers cannot be confined by potential barriers The Klein tunneling effect has
been experimentally observed by Ando in 1998 in which the absence of backscattering
(Figure 28) is responsible for high conductivity in carbon nanotubes
30
Figure 28 Electron trajectory considering the linear electrostatic potential U(x) = Fx30
The electron is able to propagate through an infinitely high potential barrier since
it makes a transition from the conduction band to valence band In this transition from
conduction band to valence band its dynamics changes from electron-like to hole-like
The equation of motion is thus given by
2
2 2 2| | ( )
pdr E
dt E Up
p E U
v
v
at energy E (216)
This shows that in the conduction band (UltE) and in the valence band (UgtE)
In Klein tunneling the pairs of electron-like and hole-like trajectories at the same E and
py have turning points at dmin given by dmin=2v|py|F (Figure 29)
Figure 29 Electron like and hole like trajectories at same E21
31
The tunneling probability exponential dependence on dmin
2
min| |
( ) exp( ) exp( )2
y y
y
vT
F
p pdp
(217)
The applications of the Klein tunneling include Atomic clock Scanning tunneling
Microscope Tunnel diode Tunneling transistor and many more32
Since graphene
exhibits Klein tunneling it can be very useful to study the transport properties in
graphene and use it in such applications
27 Quantum Hall Effect in a Graphene
A monolayer graphene shows half-integer quantum Hall effects where the Hall
resistance is quantized at values of
2
1
xyh v eR
(218)
around filling factors
14( 1 2)Nv
(219)
where N is an integer e is the electron charge h is the Planckrsquos constant and the
factor 4 is due to spin and valley degeneracy QHE in graphene can be observed at room
temperature which is a very intriguing property (Figure 210) Graphene reveals
significant differences with respect to conventional 2D electron systems The Landau
quantization yields energy levels that disperse differently in graphene as well as
particular zero-energy level that is only half filled at the charge neutrality point (v=o)
32
Figure 210 Quantum Hall effect in graphene22
The Hall conductivity σxy and the
longitudinal resistivity of monolayer graphene as a function of carrier density at B = 14T
and T= 4K This shows half-integer QHE with chiral index J= 1
The QHE in graphene is not entirely similar to regular QHE since the charge
carriers in graphene are Dirac Fermions The charge carriers governed by
electrodynamics is given by (Equation 220) which does not apply for graphene and a
QED quantization of graphene electronic band structure is used
En = (n+12)ħω (220)
33
In the presence of magnetic field the nature of the Dirac Fermions in graphene
results in unevenly spaced Landau levels (LL) containing a distinctive LL at the electron-
hole degenerating a zero energy given by
2MG
MGFehn B
n vE (221)
The LL levels at high magnetic fields in MG are shown in Figure 211
Figure 211 (a) LL for Graphene bilayer (b) Schematics of Hall conductivity as a
function of nn0 for bilayer Graphene (solid line) and monolayer Graphene (dotted line)
(c) LL for monolayer Graphene33
It is found that the Hall resistance of a two dimensional electron system has
plateaus as a function of the number of electrons at low temperatures and strong magnetic
fields32
At large B the Dirac-like energy spectrum of graphene gives rise to a
characteristic series of QH plateaus in conductance reflecting the presence of a zero-
energy Landau level that include only odd multiples of 2e2h for uniform carrier density
in the sheet These plateaus of QH edge states at the edge of the sheet circulating in a
34
direction are determined by the direction of B and the carrier type33
This is why QHE in
graphene is known as Half-Integer Quantum Hall Effect
28 Thermoelectric Effect
Thermoelectricity refers to a class of phenomena in which a temperature difference
creates an electric potential or an electric potential creates a temperature difference The
principle of thermoelectric effect has been known for over 100 years Recently the
practical applications of thermoelectric effect have become more viable34
Thermoelectric effect is the direct conversion of temperature differences to
electric voltage and vice versa Joule heating is the heat generated whenever a voltage is
applied across a resistive material The Peltier-Seebeck effect is reversible whereas Joule
heating is not This effect can be used to generate electricity to measure temperature to
cool objects or to heat them Since the direction of heating and cooling is determined by
the sign of the applied voltage thermoelectric devices make very convenient temperature
controllers
281 Seebeck Coefficient
Thomas Johann Seebeck discovered that an emf appears in a circuit composed of two
dissimilar metals when the junction between the metals is held at different
temperatures34
The thermoelectric emf causes a continuous current in the circuit when a
complete loop is formed and the current is known as thermoelectric current This is
known as the Seebeck effect
35
Figure 212 Seebeck Effect34
As long as the two junctions are at different temperatures the thermoelectric emf
exists and the current will keep flowing between the hot and cold junction that are at
different temperatures The Seebeck effect is the conversion of temperature difference
directly into electricity The voltage developed in the circuit shown in Figure 212 is
proportional to the difference in temperature between the two junctions and is given by
V = α (T2-T1) (222)
This Seebeck effect is observed not only in metals but also in semiconductors
Here α is known as the Seebeck coefficient α measures the magnitude of an induced
thermoelectric voltage in response to the temperature difference across the material If the
temperature difference ∆T between the two ends of a material is small then the Seebeck
coefficient of a material is written by
α = ∆V∆T (223)
36
This can be expressed in terms of electric field as
α E∆T (224)
The units of Seebeck coefficient is given as VK The higher the Seebeck coefficient
value the better it is since it will create a very large voltage that can be used to provide
power
282 Peltier Coefficient
Peltier effect is the inverse of Seebeck effect involving a junction phenomenon There is
heat absorption or generation at the junctions depending on the direction of current flow
Heat generated by current flowing in one direction is absorbed if the current is reversed
The heat absorbed per second at a junction carrying current I is given by
Heat absorbed in t sec = πabIt (225)
Here πab is the Peltier coefficient and given by HIt Thus Peltier coefficient is
numerically equal to the applied potential difference expressed in Volts
Overall by studying the flow of electrons the values of Seebeck
coefficient and Peltier co-efficient can be estimated These values determine the various
applications of the materials In this thesis the Peltier and Seebeck coefficient of the
graphene junction and the new applications are discussed
37
29 Early Research ndash ab intio studies
In 2007 Androitis studied that the conducting properties of graphene nanoribbons and
junctions are strongly dependent on their size and geometric features35
He concluded that
there is no conductance for small AZA or ZAZ ribbons (Figure 213)
Figure 213 Transmission functions in units of (2e
2h) for AZA structures
35
Figure 213 shows that T (E) exhibits a negligible peak [T (E) = 001 in units of
2e2h] at E= -225 and 250eV However it was noted that when the width of the arm type
was increased T (E) at -225 and 250eV was 02035
Later in 2007 Qimin Yan used first principles methods to investigate the Current-
Voltage characteristics of GNR Transistors and the effect of edge doping He showed that
GNR field effect transistors can achieve high performance levels with ONOFF ratios on
the order of 103-10
436
Figure 214 is an I-V curve of AZA GNR-FET connected via
armchair metallic leads36
38
Figure 214 I-V curve for a 591nm long channel (Vbias=20mV)
36
In 2009 Fangping OuYang demonstrated the intrinsic transport properties and
effective B or N doping of the junctions by using first-principles quantum transport
simulations He concluded that the I-V characteristics of pure-carbon T-shaped junctions
exhibit metallic behavior and the current in the junction strongly depends on the height
of the stem23
He reported that the conductance of the devices depends on the geometric
structures which can be controlled by selective doping
In 2012 Wei Yao used the first principle calculations based on Density
Functional Theory (DFT) and Non-equilibrium Greens Function (NEGF) to study the
electronic as well as the transport properties of B-doped 6-GNR p-n junction His results
showed that the boron doping interval can influence the rectification effect at low bias
and also exhibit Negative Differential Resistance (NDR) phenomena at high positive
bias
39
CHAPTER 3
COMPUTATIONAL DETAILS
31 Introduction
The physical chemical electrical electronic and optical properties of a solid are
determined by their quantized electronic states The quantum states in low-dimensional
systems are produced due to the confinement of the carrier charges in one or two
dimensions Graphene is a conductor electrons are able to flow through graphene more
easily than through even copper The electrons can travel through the sheet of graphene
like mass-less particles as fast as just one hundredth that of the speed of light The ways
in which electrons behave in graphene make it very helpful to study their fundamental
physical properties Graphenersquos near perfect crystal lattice provides a very clean system
to experiment By restricting the electrons to only two dimensions they exhibit some
interesting properties such as the anomalous quantum Hall effect and Klein tunneling
In this chapter two theoretical concepts used for calculating the electronic structure
and the transport properties for graphene are described These include the Extended
Huckel Theory and Non-Equilibrium Greenrsquos Function (NEGF) method
311 Extended Huckel Theory
Erich Huumlckel was born in Germany on August 9th
1896 He studied mathematics and
physics in Berlin He is best known for his work in the field of chemistry and physics for
two contributions (1) Debye- Huumlckel theory of electrolytic solutions (2) Huumlckel
method of approximate molecular orbital calculations on electron systems In 1930 he
published his findings on systems in 1931 he generalized and expanded the system
40
theory to explain benzene Due to his poor communication skills his findings went
unrecognized for over 20 years It was in 1951 that his 4n + 2 rule was finally clarified by
Doering to show if C=C bonds would show aromaticity Huumlckel died on February 16th
1980 with very little worldwide recognition for his contributions to chemistry Today
chemistry students recognize his name and his contributions to the field are quite
substantial
One of the first semi-empirical methods to be developed was Huumlckel Molecular
Orbital Theory (HMO) HMO was developed to describe molecules containing
conjugated double bonds HMO considered only electrons in pi orbitals and ignored all
other electrons in a molecule The Extended Huumlckel Molecular Orbital Method (EH) was
developed out of the need to consider all valence electrons in a molecular orbital
calculation
By considering all the valence electrons chemists could determine molecular
structure compute energy barriers for bond rotations and determine energies and
structures of transition states for reactions By considering only the valence electrons the
computed energies could be used to choose between proposed transition states to clarify
reaction mechanisms The total valence electron wavefunction is described as a product
of the one-electron wave functions
1 2 3(1) (2) (3) ( )valence j n (31)
where n is the number of electrons and j identifies the molecular orbital Each
molecular orbital is written as a linear combination of atomic orbitals (LCAO)
1 12
N
j jr rrc j N
(32)
41
The energy of the jth
molecular orbital is given by a one-electron Schroumldinger
equation using an effective one electron Hamiltonian heff which expresses the interaction
of an electron with the rest of the molecule
eff j j jh (33)
This is the energy eigenvalue of jth
molecular orbital corresponding to the Eigen
function j The advantage of using this method is that the exact form of heff is not
required The total energy of the molecule is the sum of the single electron energies
j jj
E n (34)
where nj is the number of electrons in orbital j
In order to use the Extended Huckel method a set of calculation parameters and
approximations must be followed These parameters include the Basis set K-point and
the Brillouin Zone and lastly the Mesh cut-off
312 Introduction to NEGF
The Greenrsquos function is a function of two space-time coordinates From the knowledge of
this function one can calculate time-dependent expectation values such as currents and
densities electron addition and removal energies and the total energy of the system In
the absence of external fields the non-equilibrium Green function method reduces to the
equilibrium Green functions NEGF can be applied to both extended and finite systems
The generic system of NEGF consists of the electron dynamics of the channel described
by the Hamiltonian This channel consists of two contact reservoirs with respective
chemical potential μR and μL The NEGF assumes ballistic transport neglecting self-
42
energy from scattering The system is insulated from gate contacts whose effects are
realized via a 3D Poisson solver which solves for the potential at a given point in real
space based on electron density
22 ( ) [ ( ) ( )]D
qr N r n r
(35)
Figure 31 NEGF system
The system is easily expandable to systems with several contacts or gate
configurations by adding additional self-energy matrices to NEGF or additional sources
to the Poisson solver
313 Electrostatics
Electrostatic potential is created every time in the presence of a charge density due to an
induced electric field The Poissonrsquos equation correlates the electrostatic potential to
charge density as given in Equation 36
43
2( ( ) ( ) ( ) ( ))( )
( )( ) ( )
ADq p r n r r N rr
rr r
N
(36)
where ɛ(r) is the dielectric permittivity of the material ρ(r) n(r) ND(r) and NA(r) are the
hole electron donor and acceptor concentrations of the system respectively
Two types of boundary conditions are usually applied to the Poissonrsquos equation
Dirichlet boundary conditions
Φ (0) = F0 and Φ (L) = FL
von Neumann boundary conditions
00
( )
x
d x
dxB
and
( )L
x L
d x
dxB
For the transport problems with open boundary conditions the von Neumann
boundary conditions are used assuming that the potential vanishes at the boundary ie
B0=BL=0
The Poissonrsquos equation can hence be discretized on a grid as
2 ( )( )
( )
rx
r
= M (37)
where M is the matrix Φ and ρ are vectors containing the discretized values of
the electrostatic potential Φ and charge density ρ respectively
44
The Schroumldinger and Poisson equations are coupled since V(x) = -qΦ(x) is used
for the Schroumldinger to compute ρ(x) This self-consistent loop stops when the
convergence is reached
( )r
V(x) = -qΦ(x)
314 Non-Equilibrium Greenrsquos Function
Greenrsquos functions are a mathematical construction that are used to solve differential
equations subject to specific initial or boundary conditions They are named after the
British mathematician George Green The 1-D equation of L( )f( )=S( ) can be defined
by the Greenrsquos Function as given below
( ) ( ) ( )G x x f x x x (38)
The general Greenrsquos function is given by
( ) ( ) ( )f x dx G x x S x (39)
Applying the operator L( ) to the solution f( ) satisfies the original differential
equation The Greenrsquos Function G( ) is the propagator which propagates the influence
of a perturbation S( ) originally situated at the point to the point at which the
function f( ) is evaluated
The Greenrsquos Function G( ) can also be a correlation function If the points
and are strongly (weakly) correlated then S( ) will greatly (poorly) affect f( )
Poisson equation
2 ( )( )
( )
rr
r
Schroumldinger equation
2
2
( ( ) ) ( )
( )2
( ) | ( ) |
E H r E r S
H V rm
r dE E r
Figure 32 Self-consistent loop
45
The Schroumldinger equation with open boundaries can be written as
( )E H S (310)
Considering a 1-D and homogenous system ranging from =0 to L assuming
that Σ=0 and the form of equations is same before and after discretization then
22
2 0( ) ( ) ( )
2E x S x
m
dV
dx
(311)
The Greenrsquos function can hence be computed corresponding to the Schroumldinger
equation
22
2 0( ) ( ) ( )
2E G x x x x
m
dV
dx
(312)
Due to the delta-function at = a discontinuity is observed and hence the
Greens function is evaluated at boundary conditions
0
2
exp( ( )) x x 2 ( )( )
exp( ik(x x)) x x
ik x x m E VG x x k
A
A
(313)
By integrating the Schroumldinger equation twice and setting the lower and upper
integration boundaries to = -δ and = +δ the Greenrsquos Functions can be written as
2
( ) ( ) 0
( ) ( ) 2
x x x x
G x x G x x
dG x x dG x x m
dx dx
(314)
46
The coefficient A+ and A
- become
ik
mA A
(315)
The Greenrsquos Function takes a final form known as Retarded Greenrsquos Function and
is written as
( ) exp( | |)G x x i ik x xk
m (316)
And the wave function is
( ) ( ) ( )x dx G x x S x (317)
Retarded Greenrsquos Function propagates the wave functions generated by a source
or perturbation S from its origin at to any point
The retarded Greenrsquos Function as discretized Schroumldinger equation is written as
( )R RE H G I (318)
The wave function Φ can be calculated from the retarded Greenrsquos function and the
source vector as
Φ = GR∙S (319)
Overall in this section the Greenrsquos function approach in calculating the electron
dynamics is reviewed We defined the self-energy of each part of the system spectral
function and the probability current density the electric current is derived explicitly using
Non Equilibrium Greenrsquos function We will use this formalism to calculate the tunneling
phenomena in coupled quantum dots isolated or otherwise
47
CHAPTER 4
ATOMISTIX TOOLKIT DETAILS
41 Introduction
Virtual NanoLab (VNL) is a graphical user interface (GUI) that provides a group of
modeling tools the function of these tools involves the set-up investigation and the
study of nanoscale structures The quantum mechanical equations are solved by the
software by using the advanced software architecture and numerical methods to
implement ab initio calculations VNL simulates the electronic structure and calculates
the transport properties based on the two systems mentioned earlier NEGF and Extended
Huckel ATK is the main engine for computing the scripts and hence all the calculations
performed in VNL are done by ATK VNL is a user friendly software as it not only
allows creating a script but also helps to set up a virtual experiment
This thesis involves the use of VNL in order to study the effect of the width and
different orientations of the doped atoms Since the software allows for virtual
experiments it makes it much easier to study the I-V characteristics based on the change
in position of atoms
42 Device Structure
In this thesis AZA GNR p-n junction with boron doping (location) was created using the
ATK software which is based on NEGF and DFT Further the thesis discusses the
transport properties and the I-V curve of such junction
The input format of ATK is NanoLanguage which is an extension to Python
scripting language ATK uses the NEGF system for formalism of simulating device
48
Figure 41 Geometry of device configuration with two electrodes
37
The system is divided into three parts left central and right The implementation
relies on the screening approximation which assumes that the properties of the left and
right regions can be decribed by solving a bulk problem for fully periodic electrode cell37
This screening approximation is fulfilled when the electrode regions can be described by
an equilibrium electron distribution
Figure 42 The electron distribution in a device configuration which illustrates a left
moving scattering state with origin in right electrode37
The system assumes that in steady state the electron density of the central region
is constant in time and hence the electron density is calculated independently from each
electrode The electron density is given by the occupied eigenstates of the system
n(r) = nL(r) + n
R(r) (41)
49
The left and right densities are calculated by summing up the occupied scattering
states
nL(r) = sum
(42)
nR(r) = sum
(43)
The scattering states are usually calculated by first calculating the Bloch states in
the electrodes and then solving the Schroumldinger equation of the central region using the
Bloch state as matching boundary Instead of using the scattering states the ATK
software uses the NEGF method to calculate the non-equilibrium electron density
The electron density is given in terms of electron density matrix
D = DL + D
R (44)
The left density matrix is given by NEGF theory
DL = int
(45)
where
ρL(ɛ) =
(46)
ρL(ɛ) = is the special density matrix
Also if there is a non-equilibrium electron distribution in the central region then
the electron distribution in electrode is given by the Fermi function f with an electron
temperature TL
G(ɛ) =
(47)
G = retarded Green function
δ+ is an infinitesimal positive number and S H overlap the Hamiltonian matrices
L =
sum sum
(48)
50
L
is the broadening function of the left electrode given in terms of left electrode
self -energysum
43 Transmission Spectrum Calculations
Once the self-consistent non-equilibrium density matrix has been obtained the various
transport properties of the system can be calculated One of the most important properties
is the transmission spectrum from which the current and differential conductance can be
obtained
The transmission coefficient in ATK is obtained by the retarded Greens function
T(ɛ) = G(ɛ)ΓL(ɛ)G
ϯ(ɛ)Γ
R(ɛ) (49)
The transmission amplitude of individual scattering states may be obtained
through the Transmission Eigenvalues The ldquoTransmission Eigenvaluesrdquo is an analysis
which finds the eigenvalues of the transmission matrix
The transmission matrix at energy E and k-point is given by
Tnm(Ek) = sum (410)
where
= transmission amplitude from Bloch state ψn(k)
The transmission coefficient is given by the trace of transmission matrix
T(Ek) = sum (411)
Keeping in mind all quantities depend on the quantum numbers parametrically
Transmission eigenvalues sum up to the transmission coefficient
T = sum (412)
51
44 Calculating the Current
Current is calculated from the transmission coefficient using
I( ) ( )R L
L RL R
R LB B
eE f f dE
h
E EV V T T T
k kT T
(413)
where f is the Fermi function TRL is the electron temperature of the right or left
electrode and Tσ(E) is the transmission coefficient for the spin component σ
The chemical potentials of the left and right electrode given by
L
F R LR L
eVE
are defined relative to the Fermi level of the left electrode These chemical potential are
related to the applied bias and hencebiasR L
eV therefore bias L RV V V
The transmission spectrum itself is usually rather insensitive to temperature and is
used in self-consistent calculations but often depends strongly on the electrode voltages
Thus for an accurate estimate of the current the transmission spectrum should be
calculated self-consistently for each desired bias
ATK uses very precise method to calculate the transport properties of the system
Transmission spectra for various concentrations of boron doped graphene p-n junctions
are generated in this Chapter and various coefficients such as Seebeck Peltier and
Conductance are calculated
52
45 Calculating Transport coefficients
The linear response transport coefficient of an applied voltage difference or temperature
difference between the two electrodes is given by
Conductance
| dT 0
e
dI
dUG
(414)
Peltier coefficient
| d 0
Q
I
I
(415)
Seebeck coefficient
| 0
dUS I
dT T
(416)
These linear response coefficients are calculated by the Transport Coefficients To
perform these calculations the ATK uses the Electron Transmission Spectrum
53
CHAPTER 5
RESULTS AND DISCUSSION
51 Band Structure Analysis
The electronic bandstructure of GNR both doped and undoped are discussed in this
chapter
The armchair configuration of Pristine GNR (PGNR) has a band structure that is
dependent on its width This is explained by the fact that the sheet itself acts like a
potential well where the electrons are confined to form standing waves along Cr the
rolling vector albeit with slightly different boundary conditions (Cr = ma1 + na2
where m and n are integers and a1 and a2 are the unit cell vectors of graphene lattice) In
a GNR the two nodal points of the standing wave must be at the ribbon edge while in a
Single wall nanotube (SWNT) they can be anywhere ie a circumferential periodic
boundary condition
(a) (b)
Figure 51 Bandstructure of AGNR widths (a) 4 atoms (b) 5 atoms
54
(a) (b)
Figure 52 Bandstructure of AGNR widths (a) 6 atoms (b) 7 atoms
(a) (b)
Figure 53 Bandstructure of AGNR widths (a) 8 atoms (b) 9 atoms
55
(a) (b)
Figure 54 Bandstructure of AGNR widths (a) 10 atoms (b) 11 atoms
Figure 55 Bandstructure of AGNR with a width of 12 atoms
Figure 56 Variation in band gaps as the width (number of atoms) varies
0
05
1
15
2
25
0 2 4 6 8 10 12 14
Wdith vs Band Structure
eV
56
The band structure of 12 Atom AGNR is close to that of Ge (0626 eV) The
actual width of this nanoribbon is about 25 nm 12 AGNR has been fabricated
successfully and doped with various dopants Hence the 12 Atom AGNR has been chosen
to study the transport properties
A junction is created using ZGNR and AGNR To maintain the consistency in the
device analysis it is imperative that the band structure of ZGNR is also calculated From
the simulation it is evident that ZGNR-AGNR-ZGNR junction configuration displays the
Metal ndashSemiconductor-Metal configuration that is addressed in this work The Fermi
Level in all the Z-GNR nanoribbons of widths 4-12 lies within the conduction band
Figure 57 Band structure of ZGNR width (a) 4 atoms (b) 6 atoms
57
(a) (b)
Figure 58 Band structure of ZGNR width (a) 8 atoms and (b) 10 atoms
Figure 59 Band structure of ZGNR with a width of 12 atoms
In order to create viable junction that would show transistor properties doping of
the semiconductor part is necessary The 12 atom AGNR is doped with boron (p-type)
and nitrogen (n-type) - (Figure 510a) 4 N doped (Figure 510b) 4 B In both cases
the impurities lie on the edge of the atoms For 2 nitrogen doped GNR with the
58
impurities lying in the center of the ribbon the Fermi level is found to be in the
conduction band as shown in (Figure 510c) (Figure 510d) shows the position of N with
respect to the edge A very clear departure from the expected (the valence band extending
above Fermi level) is shown in (Figure 510a)
Figure 510 Band structures of Doped AGNR (a) 4 N Doped (b) 4 B Doped (c) 2
N Doped (d) position of Nitrogen from (c)
(a) (b)
(c) (d)
59
52 I-V Characteristics of GNR junction
In pristine graphene the chirality determines the conductivity as seen from the I-V curves
for various widths At certain widths the semiconducting properties are more
pronounced These widths determine the wavelengths of the standing waves which in
turn determine the sub-band locations in the E-k plot When the biasing potential
exceeds 012V the I-V curve shows linearity In case of the 8-atom wide PGNR the
band gap is about 03 eV and it is evident from the I-V plot that the On-State is + 033 V
The band gap of 10-atom and the 4-atom wide PGNR is large enough to show
semiconducting properties
Figure 511 Current Vs Voltage graph for varying graphene width showing
conductivity
-30000
-20000
-10000
0
10000
20000
30000
-3 -2 -1 0 1 2 3
Cu
rre
nt
(nA
)
Voltage (V) (bias)
Current (nA) Vs Voltage for varying graphene width
W=10
W=8
W=6
W=4
60
The ZAZ GNR Configurations show the properties of a semiconductor junction The 12
atom ZAZ structure is studied for its I-V characteristics In this Chapter undoped B-
doped N-Doped B and N Doped (P-N Junction) ZAZ junctions are simulated
Figure 512 ZAZ GNR junction device
61
The boron doped ZAZ junction I-V characteristics are shown below (Figure 513)
The impurity concentration is 2 and 4 Various device configurations are studied
Figure 513 I-V curve of Boron Doped ZAZ junction
-25000
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
25000
-205 -155 -105 -055 -005 045 095 145 195
Cu
rre
nt
(nA
)
VBias
2B_1G_R 2B_0G_R
4B_0G_L 4B_0G_C
4B_0G_R 4B_1G_L
4B_1G_C 4B_1G_R
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
-2 -1 0 1 2
Cu
ren
t(n
A)
VBias
4 B doped GNR Jn
62
Figure 514 I-V curve of Nitrogen Doped ZAZ
-25000
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
-2 -15 -1 -05 0 05 1 15 2
Cu
rre
nt(
nA
)
VBias
I-V Curve as function of Dopant location
2N_0G_L2N_0G_C2N_0G_R2N_1G2N_1G_C2N_1G_R
-15000
-10000
-5000
0
5000
10000
15000
-2 -1 0 1 2
Cu
rre
nt(
nA
)
VBias
2N_0G_C
2N_1G_C
63
Figure 513 and Figure 514 show the I-V characteristics of the GNR junction doped with
2 boron and nitrogen respectively The location of N and B is at the central region of
the edge of the GNR Both B doped and N doped GNR Junctions show significant
Negative Differential Resistance (NDR) This is more pronounced in case of nitrogen
doping Another interesting observation is increasing ohmic nature with the change in
location of the dopants Nitrogen doped device configuration exhibits a pronounced
semiconductor behavior and the NDR effect is observed to be minimal
53 Thermoelectric Properties
In this study the thermoelectric properties were simulated for the GNR Junctions that
displayed high NDR effect The variation in the Peltier coefficient with temperature is
shown as function of doping
When the concentration of nitrogen increases the dimensionless Figure of Merit
ZT seems to decrease considerably This is mostly explained by the decrease in both
conductivity and mobility of the electrons
ZT = S2σTk (51)
where S is the Seebeck coefficient σ is the electrical conductivity T is the
absolute temperature and k is the thermal conductivity
64
Figure 515 Variation of Peltier coefficient with temperature as function of
doping
Figure 515 shows the maximum Peltier coefficient for 2 boron This is
explained by the scattering by boron and the associated smallest mean free path
0
0001
0002
0003
0004
0005
0006
0007
0008
0009
001
250 270 290 310 330 350 370 390 410
ZT
T (K)
2B
4B
Undoped
2N
4N
65
CHAPTER 6
CONCLUSIONS
Graphene ZAZ junctions exhibit varying properties depending on the various structural
configurations In this thesis it was found that the transport properties of graphene
depend on their width the edge of GNR doping concentration and the type of dopant
used The calculations of the band structure contributed towards the determination of the
minimum length of GNR required for studying the transport properties The minimum
length had a band gap equivalent to that of germanium and hence the importance of the
width being 12 atoms wide This band gap indicated fluctuating changes when doped
with elements such as B and N The viable junction showing transistor properties was
hence created by doping the semiconductor part of ZAZ By doping the I-V
characteristics were studied which showed significant NDR which was more pronounced
in the case of nitrogen Also the changing positions of the dopants contributed towards
the I-V curve to be more ohmic The edge doping caused minimum NDR and
semiconductor behavior as compared to central doping Lastly the thermoelectric
properties were studied - the increasing concentration of N causes the Figure of Merit to
decline due to the decrease in conductivity as well as mobility of electrons
66
REFERENCES
1 Wikianswers What makes carbon unique
httpwikianswerscomQWhat_makes_carbon_so_unique (22 November)
2 Kopeliovich D D Graphite
httpwwwsubstechcomdokuwikidokuphpid=graphite (1128)
3 Barbier M Transport properties of nanostructures and superlattices on single layer and
bilayer graphene University Antwerpen Antwerpen 2012
4 Shylau A Electron transport interaction and spin in graphene and graphene
nanoribbons Linkoping Norrkoping 2012
5 HassJ R F T Li X Li Z Zong W A de Heer P N First E H Conrad C
AJeffrey and C Berger Applied Physics Letters 2006 89 (14) 143
6 Jones A Mechanical Exfoliation to Make Graphene and Visulization
httpcarbonchemwisceduFilesMechanicalExfoliationpdf (18 October)
7 Anteroinen J Structural and Electrical Characteristics of Graphene Field Effect
Transistors AALRO school of Electrical Engineering AALTO 2011
8 Novoselov K S A K G S V MorozovD JiangY Zhang S V Dubonos I V
Grigorieva A A Firsov Science 2004 306 (22)
9 Kosynkin D A L H A Sinitskii J R Lomeda A Dimiev K B Price and J M
Tour Nature 458 876
10 Yi Z Luyao Zhang Accounts of chemical research 46 (10) 2339
11 Eizenberg M B JM 1979 82 236
12 Yu Q K L J Siriponglert S Li H Chen Y P Pei S S Applied Physcis
Letters 2008 93 (113103)
13 Li X C W An J Kim S Nah J Yang D Piner R Velamakanni A Jung I
TutucE Banerjee S K Colombo L Ruoff R S Science 2009 324 1314
14 Schaefer H E Nanoscience Springer Berlin 2010
15 Levente Tapasztoacute G D Philippe Lambin amp Laacuteszloacute P Biroacute Nature Nanotechnology
2008 3 401
67
REFERENCES
16 Dacheng Wei Y L Advance Materials 2010 22 (30) 3241
17 Wei Yao K L Y GYGao Elsevier Solid State Communications 2013 153 52
18 Dacheng Wei Dagger Yunqi Liudagger Yu Wangdagger Hongliang ZhangdaggerDagger Liping HuangdaggerDagger
Yudagger a G NanoLetters 2009 9 (5) 1758
19 Nakada K M F G Dresselhaus and M S Dresselhaus PhysRevB 1996 54
(9858)
20 Son Y W C M L a L S G PhysRevLett 2006 97 (216803)
21 Raza H Graphene Nanoelectronics Springer 2012
22 Ryan W J Electronic Transport in Graphene p-n junctions Short Noise and
Nanoribbons Harvard University 2009
23 Fangping OuYang J X Rui Guo Hua Zhang and Hui Xu Nanotechnology 2009
20 6
24 Guo J Carbon nanotube electronicsModeling physics and applications Purdue
University West Lafayette IN 2005
25 Motta C S S-P MITrioni cond-matmes-hall 2012 7
26 B P Growing Graphene via Chemical Vapor Deposition Ponoma College Ponoma
2011
27 ZurichE Transport properties of three-terminal graphene devices University of
Science and Technology Norway 2008
28 Uichiro MIntroduction to the electron theory of metals
29 Robert Laughlin H S Additional background material on the Nobel Prize in Physics
1998 (410)
30 MarkGoerbig Quantum Hall Effects (11152013)
68
REFERENCES
31 Zurich E Transport properties of three-terminal graphene devices Norwegian
University of Science and Technology Norway 2008
32 Deepak R Klein Tunneling University og Tennessee Space Institute Tennessee
2011
33 Williams JR L D CMMarcus Quantum Hall Effect in a Gate-Controlled p-n
Junction in Graphene (1122013)
34 Avadhanulu MN P G K A Textbook of Engineering Physcis for BE BSc (Engg)
SChand New Delhi 1992
35 Andriotis A Applied Physics Letters 2007 91 (152105)
36 Qimin Yan B H dagger Jie Yudagger Fawei Zhengdagger Ji ZangDagger Jian Wudagger Bing-Lin Gu F
L Dagger and Wenhui Duandagger NanoLetters 2007 7 (6) 1473
37 Soler J M E A J D Gale A Garciacutea J Junquera P Ordejoacuten and D Saacutenchez-
Portal J Phys Condens Matter 2002 14 2745
vi
TABLE OF CONTENTS
Chapter
Page
1 INTRODUCTIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
1
11 Graphene The New Carbonhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
1
12 Graphene Synthesishelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
3
121 Synthesis of Graphene on Nickel (Ni)helliphelliphelliphelliphelliphelliphelliphellip
5
122 Synthesis of Graphene on Copper (Cu)helliphelliphelliphelliphelliphelliphelliphellip
8
123 Transfer of Graphene Filmshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
8
124 Synthesis of Graphene Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
9
125 Doping in Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
10
126 Nitrogen (N) Doped Graphene Synthesis (Substitutional)hellip
12
13 Structure of Graphene Nanoribbon (GNR)helliphelliphelliphelliphelliphelliphelliphelliphelliphellip
13
14 Overview of Graphene Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
15
2 RESEARCH BACKGROUNDhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
21 Bandstructure of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
22 Transport Characteristics of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
20
23 Drude Theoryhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
22
24 Quantum Hall Effect (QHE)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
24
25 Resistivity and Resistancehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
27
26 Klein Tunnelinghelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
28
27 Quantum Hall Effect in Graphenehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
31
28 Thermoelectric Effecthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 34
vii
TABLE OF CONTENTS
(Continued)
Chapter Page
281 Seebeck Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
34
282 Peltier Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
36
29 Early Research ndash ab initio Studyhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
37
3 COMPUTATIONAL DETAILShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
31 Introductionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
311 Extended Huckel Theory helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
312 Introduction to NEGFhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
41
313 Electrostaticshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
42
314 Non-Equilibrium Greenrsquos Functionhelliphelliphelliphelliphelliphelliphelliphelliphellip
44
4 ATOMISTIX TOOLKIT DETAILShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
41 Introductionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
42 Device Structurehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
43 Transmission Spectrum Calculationhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
50
44 Calculating the Currenthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
51
45 Calculating the Transport Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
52
5 RESULTS AND DISCUSSIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
53
51 Band Structure Analysis helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
53
52 I-V Characteristics of GNR Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
59
53 Thermoelectric Propertieshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
63
6 CONCLUSIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 65
REFERENCEShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
66
viii
LIST OF FIGURES
Figure Page
11 (a) Chemical representation of Carbon (b) Graphite ore (c) Structure of
Graphite and a single layer Graphenhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
2
12 An optical image of Graphene flake obtained by exfoliation of
graphitehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
3
13 (a) Graphene formation on Nickel (b) Graphene atoms on Ni (111)
lattice (c)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
7
14 (a) SEM image of graphene on copper foil (b) High-resolution SEM
image of graphene on Cuhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
8
15 (a) Transfer process (b) Wafer-scale synthesis of graphene (c) Graphene
films transferred onto glass wafer (d) SiSiO2 with device patterned (e)
PET filmhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
9
16 (a) High-magnification image of the annealed sample showing that well-
defined zigzag armchair and zigzag-zigzag edges are formed (b) ) STM
image of an 8 nm wide bent junction connecting an armchair and a
zigzag graphene nanoribbon which was carved by STM
tipshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
10
17 Band structure of graphene before and after doping The image shows
shift towards the Fermi levelhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
11
18 Low resolution TEM image of N-doped graphene Background is the
lacey carbon TEM grid graphene sheet is crumpled with many
rippleshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
13
19 Zigzag and Armchair orientation of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphellip 13
110 Bandstructure of ZGNRhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 14
111 Bandstructure of AGNRhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 15
21 Left Real space Graphene lattice with basis vectors and Right
The first Brillouin zone of Graphene in reciprocal space with basis
vectors and K and Krsquo are responsible for massless transport at low
energyhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
ix
LIST OF FIGURES
(Continued)
Figure Page
22 Bandstructure of a graphene sheet showing a band gap of 0eVhelliphelliphellip 18
23 Band structure of Graphene calculated with the tight-binding modelhellip 19
24 The energy dispersion around the K pointhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 22
25 Electrons colliding with stationary ionshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 23
26 (a) 2D electrons in a perpendicular magnetic field Logitudinal resistance
measured across C5 and C6 Transverse resistance measured across C3
and C5 (b) Classical Hall resistance as a function on the magnetic field
25
27 Klein tunneling through an npn barrierhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 29
28 Electron trajectory considering the linear electrostatic potential U(x) = Fx 30
29 Electron like and hole like trajectories at same Ehelliphelliphelliphelliphelliphelliphelliphelliphellip 30
210 Quantum Hall effect in graphene 22
The Hall conductivity σxy and the
longitudinal resistivity of monolayer graphene as a function of carrier
density at B = 14T and T= 4K This shows half-integer QHE with chiral
index J= 1helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
32
211 (a) LL for Graphene bilayer (b) Schematics of Hall conductivity as a
function of nn0 for bilayer Graphene (solid line) and monolayer
Graphene (dotted line) (c) LL for monolayer Graphenehelliphelliphelliphelliphelliphelliphellip
33
212 Seebeck Effecthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 35
213 Transmission functions in units of (2e2h) for AZA structureshelliphelliphelliphellip 37
214 I-V curve for a 591nm long channel (Vbias=20mV)helliphelliphelliphelliphelliphelliphelliphellip 38
31 NEGF systemhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 42
41 Geometry of device configuration with two electrodeshelliphelliphelliphelliphelliphelliphellip 48
42 The electron distribution in a device configuration which illustrates a left
moving scattering state with origin in right electrodehelliphelliphelliphelliphelliphelliphelliphellip
48
x
LIST OF FIGURES
(Continued)
Figure Page
51 Band structure of AGNR widths (a) 4 atoms (b) 5 atomshelliphelliphelliphelliphelliphellip
53
52 Band structures of AGNR widths (a) 6 atoms (b) 7 atomshelliphelliphelliphelliphelliphellip 54
53 Band structure of AGNR widths (a) 8 atoms (b) 9 atomshelliphelliphelliphelliphelliphelliphellip 54
54 Band structures of AGNR widths (a) 10 atoms (b) 11 atomshelliphelliphelliphelliphellip 55
55 Band structure of AGNR with a width of 12 atomshelliphelliphelliphelliphelliphelliphelliphelliphellip 55
56 Variation in band gaps as the width (number of atoms) varieshelliphelliphelliphellip 55
57 Band structure of ZGNR width (a) 4 atoms (b) 6 atomshelliphelliphelliphelliphelliphelliphellip 56
58 Band structure of ZGNR width (a) 8atoms and (b) 10 atoms 57
59 Band structure of ZGNR with a width 12 atomshelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 57
510 Band structures of Doped AGNR (a) 4 N Doped (b) 4 B Doped (c)
2 N Doped (d) position of Nitrogen from (c)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
58
511 Current Vs Voltage graph for varying graphene width showing
conductivityhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
59
512 ZAZ GNR junction devicehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 60
513 I-V curve of Boron Doped ZAZ junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 61
514 I-V curve of Nitrogen Doped ZAZhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 62
515 Variation of Peltier effect coefficient with temperature for various doping 64
1
CHAPTER 1
INTRODUCTION
11 Graphene The New Carbon
Carbon (chemical symbol C atomic mass 1207amu) (Figure 11a) is a widely distributed
element in nature It is found abundantly in the sun stars comets and the atmospheres of
the planet Carbon can form up to four bonds it can bond with itself endlessly and with
most other elements in many different shapes making it a significant part of the
construction for many kinds of complex molecules1
Two allotropes of carbon are commonly used diamond and graphite (Figure
11b) The bonding structures of diamond and graphite contribute to the properties
individually In diamond all the p-orbitals are used forming a sp3
bonding whereas in
graphite only two orbitals are occupied allowing the unpaired bond for the transport of
electrons Each carbon atom in graphene possesses sp2 hybridization ie each carbon
atom is connected to three other carbon atoms via covalent bonds with a bond length of
142Å and an angle of 120deg between each bonded pair This makes graphite a better
conductor than diamond Graphite consists of many layers of 2D carbon lattices (Figure
11c) stacked on top of each other and held via Van der Waals forces A single layer of
graphite where carbon atoms are arranged in a honeycomb lattice is known as graphene
(Figure 11c)
2
Figure 11 (a) Chemical representation of Carbon (b) Graphite ore (c) Structure of
Graphite and a single layer Graphene2
Theoretical work on graphene was done specifically to study the other allotropes
The first study was done by Wallace in 1947 who calculated the band structure of
graphene3 Further the peculiar Landau levels were known by McClure in 1957 and the
relativistic Hofstadter butterfly by Ramal in 19853 Later in 1991 the invention of carbon
nanotubes by Iijima boosted the theoretical research on graphene3 Prior to the invention
of carbon nanotubes there were a few experimental papers on graphene growth via
various methods like intercalation of graphite (Shioyama 2001) free standing (Boehm
1962) epitaxial as well as graphene grown on metals (Bommel 1975 Land 1992 Itoh
1991)3 With all the various discoveries the electronic properties of graphene were not
studied until 2004 when Berger and Novoselov were able to access the electronic
properties with contact of graphene flakes3 (Figure 12)
3
Figure 12 An optical image of Graphene flake obtained by exfoliation of graphite3
The specific lattice structure of graphene possesses a number of unique electronic
properties making it an interesting material for theorists experimentalists and engineers
Utilization of graphene as a fundamental block of electronic devices requires
development of new theoretical methods for understanding the current propagations in
graphene constriction4
12 Graphene Synthesis
The discovery of graphene by mechanical exfoliation called the lsquoScotch tape methodrsquo led
to serious attempts towards the production of top quality graphene5 Graphene was first
exfoliated mechanically from graphite in 20046 The importance of high quality graphene
cannot be emphasized enough however electron transport has shown that defects play an
important role in hindering the transport properties of electrons (holes)7 The two
synthesizing methods for the large scale manufacture of graphene are chemical vapor
deposition (CVD) and silicon carbide (SiC) desorption method
4
Graphene can be synthesized by sublimation of silicon from SiC at high
temperature (1200degC) in high vacuum5 The major advantage of this method is that the
SiC provides an insulating substrate and no transfer of the graphene layer is needed Yet
the disadvantage of this method outweighs its advantages the high temperature is cost-
ineffective making it unsuitable for large scale manufacturing8 Also the crystal growth
face alters the properties of graphene Graphene grown on Si-terminated face has poor
homogeneity and is subjected to unintentional doping7 Conversely graphene grown on
C-terminated SiC has higher mobility and is often called lsquoturbostaticrsquo due to the
rotational disorder7
Unlike the SiC method the graphene produced via CVD method needs to be
transferred to a substrate making it difficult to maintain the quality of graphene Yet
CVD synthesized graphene has a larger grain size7 More research is being done on
various methods for synthesis of graphene The methods include direct chemical
synthesis ion implantation crystal sonification and lastly unzipping carbon nanotubes to
form graphene sheets9
Graphene and few-layer graphene have been grown by CVD from carbon
containing gases on catalytic metal surfaces andby surface segregation of C dissolved in
the bulk of such metals7 Growing graphene with CVD is a very attractive solution since
it is compatible with the existing semiconductor industry9 Graphene has been grown via
CVD process on metal substrates such as Nickel (Ni) and Copper (Cu)
5
121 Synthesis of Graphene on Nickel (Ni)
Polycrystalline Ni films are annealed in ArH2 atmosphere at 900-1000degC to increase
grain size and are then exposed to H2CH4 gas mixture10
In this step the hydrocarbon
decomposes and dissolves in Ni to form a solid solution Lastly the samples are cooled in
argon gas Ni has high carbon solubility at elevated temperatures and the solubility
decreases as temperature is reduced During the cooling process the carbon atoms diffuse
out from the Ni-C solid solution and precipitate on the Ni surface to form graphene films
(Figure 13a) Since Ni (111) has a lattice similar to the densely packed hexagonal lattice
of graphene (Figure 13b) they also have similar lattice constants and hence Ni surface
serves as an excellent lattice matched substrate for graphene growth11
The growth of graphene on Ni is based on carbon segregation and precipitation
process different segregation behavior is produced by different cooling rates which
affect the thickness and quality of graphene films12
Medium cooling rates lead to optimal
carbon segregation and produce few layers12
Graphene films grown on Ni are usually
continuous with monolayer and few layer regions Annealing of Ni substrates at elevated
temperatures in hydrogen atmosphere not only increases the single-crystalline Ni grain
size but also eliminates certain impurities in Ni thereby improving the graphene quality
Furthermore the graphene thickness can also be affected due to the amount of carbon
dissolved in the Ni films during the growth time
After synthesis the graphene can be transferred to other insulator substrates for
further characterization and applications Figure 13c shows the selected area electron
diffraction pattern of graphene film along the [001] direction which confirms the
graphene lattice structure shown After transfer to insulator substrates the geometry can
6
be retained as shown in Figure 13d Under optimal growth parameters graphene growth
is only limited by the Ni catalyst Lastly Figures 13e and 13f show the wafer-scale
graphene synthesis and transfer of graphene to a flexible transparent substrate
respectively
Though polycrystalline Ni is a good substrate the percentage and size of
graphene monolayer are still limited Researchers have hence tried other metal substrates
for graphene synthesis
7
Figure 13 (a) Graphene formation on Nickel (b) Graphene atoms on Ni (111) lattice
(c) Low magnification TEM image of graphene edges (d) Optical image of graphene
transferred from the Ni surface to SiO2Si substrate (e) Full-wafer scale deposition of
graphene layers on polycrystalline Ni (f) Transparent and flexible graphene films on
PDMS substrate10
8
122 Synthesis of Graphene on Copper (Cu)
Graphene films are grown on 25microm thick Cu foils in a hot wall furnace13
The Cu foil is
first annealed in hydrogen atmosphere at 1000degC and a mixture of H2CH4 is introduced
into the system to initiate graphene growth After a continuous graphene layer is formed
on the Cu foil the system is cooled to room temperature Figure 14a shows an SEM
image of graphene on Cu substrate indicating the Cu grains with contrast The Cu
surface steps are formed during thermal annealing and the darker flakes indicate multiple-
layer graphene (Figure 14b)10
The graphene wrinkles in Figure 14(b) originate from
different thermal expansion coefficient of graphene and Cu They go across the Cu grain
boundaries indicating that the graphene film is continuous
Figure 14 (a) SEM image of graphene on copper foil (b) High-resolution SEM image of
graphene on Cu10
123 Transfer of Graphene films
In order to facilitate the applications of graphene for electronic applications we need to
separate the graphene from the catalytic metal substrate Figure 15a shows the transfer
process of graphene Graphene is first coated with a thin layer of polymethyl
methacrylate (PMMA) and baked at 120degC to evaporate the solvent10
The metal layer is
then removed by Ni or Cu etchant leaving behind the PMMA graphene film The film is
then cleaned by deionized water and then transferred onto the target substrate After the
9
evaporation of water vapor the PMMA is removed by acetone leaving graphene film on
top of the target substrate Figure 15b shows a graphene wafer transferred from the
substrate onto glass and polyethylene terephthalate (PET) films
Figure 15 (a) Transfer process (b) Wafer-scale synthesis of graphene (c) Graphene
films transferred onto glass wafer (d) SiSiO2 with device patterned (e) PET film10
124 Synthesis of Graphene Junction
Graphene junctions with smooth armchair and zigzag edges are difficult to produce by
conventional methods such as mechanical exfoliation chemical exfoliation or lithography
etching14
The conventional methods can only produce rough edges Recently
Dresselhaus reported an edge reconstruction of graphene by Joule heating in a TEM-STM
10
(Figure16b) system15
An individual nanoribbon sample is attached to the sample holder
at one end and to the STM tip at the other end these ends also serve as the two
electrodes The structural transformation in the growth of graphene from armchair to zig-
zag is mainly attributed to the vaporization of carbon edges that reconstruct at high
temperatures in which resistive Joule heating and preferred current flow play an
important role This means that by controlling the flow of current a perfectly smooth
edged ribbon can be synthesized making graphene-based electronics possible16
Figure 16 (a) High-magnification image of the annealed sample showing that well-
defined zigzag armchair and zigzag-zigzag edges are formed (b) STM image of an 8 nm
wide bent junction connecting an armchair and a zigzag graphene nanoribbon which was
carved by STM tips14
125 Doping in Graphene
The doping of graphene can be roughly classified into two categories - electrical and
chemical Electrical doping involves changing gate voltages of graphene devices and
chemical doping uses chemical routes such as substitutional or interstitial This thesis
discusses chemical doping and the importance of doping sites by changing the dopant
Chemical doping is a common approach to tailor the electronic properties of
11
semiconductors Doping of graphene can cause its electronic properties to alter leading to
a metal-semiconductor transition The two means of doping graphene are interstitial and
substitutional In interstitial doping the dopant atoms or molecules are introduced as
adatoms or admolecules on the surface of graphene whereas in substitutional doping the
dopant atoms are replaced in the carbon lattice forming a bond in the lattice of
graphene16
Doping graphene results in the formation of n or p-type semiconductors
depending on the kind of dopant If the dopant is an electron donor it causes the Fermi
level to shift up resulting in n-type behavior of graphene Furthermore if the dopant is an
electron acceptor it causes the Fermi level to shift down resulting in a p-type behavior of
graphene (Figure 17)16
Figure 17 Band structure of graphene before and after doping The image shows shift
towards the Fermi level16
Graphene nanoribbons (GNR) can be made into a p- and n- type semiconductor
by doping with boron (B) and nitrogen (N) respectively In theory GNR p-n junction is
formed by doping GNR with B and N in different regions However experimentally
doping graphene with both these elements is very difficult due to the dopants reacting
with each other17
Hence most experimental studies use GNR doped by only one
12
element N-doped graphene was synthesized by Wei et al Wang and B-doped Graphene
was realized by Endo17
Many researchers have demonstrated interstitial doping of graphene by gas metal
and organic molecules16
The various gases and metals used are NO2 NH3 An-CH3 Na-
NH2 F4-TCNQ TPa TCNE and others16
Doping in graphene is hence possible by
electrons or holes in high concentration without deterioration of its mobility Interstitial
doping is highly sensitive due to most of the conducting channel being exposed to surface
absorbates and hence can be used in molecule detection
In substitutional doping the dopant atoms are included in the graphene lattice and
thus chemically bonded Substitutional doping is done via the CVD method using a
carbon and dopant source Substitutional doping opens up many applications in device
engineering making graphene a very good candidate as a semiconductor This study
involves the study of transport properties of graphene doped by substitution
126 Nitrogen (N) Doped Graphene Synthesis (Substitutional)
N-Doped graphene is prepared via a CVD process using a 25microm thick Cu film on a Si
substrate The substrate is placed in a quartz tube with the flow of hydrogen (20sccm) and
argon (100 sccm)18
When the center of the furnace reaches 800degC 60 sccm of CH4 and
60 sccm of NH3 is introduced into the flow as C source and N source respectively The
substrate is then moved to high temperature and after 10 min growth the sample is
cooled to room temperature under H2 ambient Figure 1 8 shows the growth of N-doped
graphene18
13
Figure 18 Low resolution TEM image of N-doped graphene Background is the lacey
carbon TEM grid graphene sheet is crumpled with many ripples18
13 Structure of Graphene Nanoribbon (GNR)
Graphene Nanoribbons (GNR) are strips of graphene with very thin width of lt50nm
GNRs can be terminated in three separate ways called zig-zag (0 n) armchair (m 0) and
chiral (m n) (Figure19) and this termination along the width of the ribbon dictates the
size of the band gap19
Figure 19 Zigzag and Armchair orientation of Graphene5
Due to their various edge structures GNRs exhibit different electronic properties
ranging from normal semiconductors to spin-polarized half metals which open the
possibility of GNRs as electronic devices19
14
Within a tight binding approach (AGNRs) could be metallic or semiconducting
depending on their ribbon width but all zigzag graphene nanoribbons (ZGNRs) are
metallic with a high density of electronic states at the edges Hence ZGNRs exhibit
characteristic edge effects which are not present in AGNRs These edge effects in
ZGNR create a flat band close to the Fermi level making the ZGNR edges more
reactive19
First-principles calculations show that the GNRs possess a non-zero direct
band gaps These gaps are small for ZGNR (Figure 110) caused due to spin ordering
effects at the edges For AGNRs the band gap arises from quantum confinement (Figure
111) effect that has larger magnitudes than ZGNR20
Figure 110 Band structure of ZGNR
15
Figure 111 Band structure of AGNR
For GNRs the band gap decreases as the ribbon width increases and in order to
create a semiconductor with a desirable band gap the nanoribbon width should be
adjusted accordingly This property of adjusting the band gap makes graphene an
excellent candidate for transistor switching By applying an electric field GNR can be
altered from an insulator to a conductor GNRs exhibit very intriguing properties and
have become one of the promising candidates for electronic applications
14 Overview of Graphene Junction
The invention of p-n junctions date back to 1940s which later resulted in the invention of
junction transistors One of the key technological reasons for success of the p-n junction
is mainly due to its ability to locally modulate the energy band gaps via an applied bias21
A graphene p-n junction is created via single layer of graphene in which the
carrier type and density in two adjacent regions are controlled by electrostatic gating8
For materials with a band gap the electric field can either switch lsquooffrsquo the current or
rectify it (p-n diode)22
Being a ldquogaplessrdquo material the off state is not achievable in
16
graphene In order to achieve an off state the gap can be created by doping graphene with
various elements (Group III or Group V) Doping allows p-n junctions to be
reconfigurable using a gate voltage to distinguish between graphene p- n regions within a
single sheet Many researchers have studied the electronic as well as transport properties
of doped graphene junctions
In 2009 Fangping OuYang studied the transport properties of T-shaped graphene
junctions using the ATK software and showed that the conductance depends on
geometric structures which can be controlled by selective doping23
Wei Yao in 2013
studied the transport properties in graphene p-n junctions and showed that the
rectification effect depends on boron doping density and position17
The study of transport properties in graphene p-n junctions is a recent
advancement The thesis discusses transport properties including the current-voltage (I-
V) characteristics of doped graphene junctions Moreover the software used is similar to
the software in use by current researchers since they have produced viable data using
ATK
17
CHAPTER 2
RESEARCH BACKGROUND
21 Band Structure of Graphene
The unique electronic properties of graphene were first predicted in 1946 Figure 21
shows a top view of the hexagonal arrangement of carbon atoms in real space as well as
the first Brillouin zone in reciprocal space
Figure 21 Left Real space graphene lattice with basis vectors and Right The
first Brillouin zone of graphene in reciprocal space with basis vectors and
K and
Krsquo are responsible for massless transport at low energy24
The real space basis vectors are radic
and
radic
The reciprocal space basis vectors are 1 2
0 0
4 1 3 4 1 3( )and ( )2 2 2 23 3
b x y b x ya a
where the magnitude of the basis vectors is |a0| = radic acc The distance between nearest
neighbor carbon atoms is acc=0142nm
18
The band structure can be calculated by solving the eigenvalues using the
dispersion relation E( )
1 2 3( ) 3 2cos 2cos 2cosE k t k a k a k a (21)
Transport properties of solids are closely related to the energy dispersion
relations E ( ) in the material and in particular to the behavior of E ( ) near the Fermi
level Graphene is a zero gap semimetal whose specific linear electronic band dispersion
near the Brillouin zone corners (Dirac points) gives rise to electrons and holes that
propagate as massless Fermions25
The valence and conduction bands do not overlap in
graphene they touch at the Fermi Level (Figure 22)
Figure 22 Band structure of a graphene sheet showing a band gap of 0eV
The low energy properties of graphene can be well described by making a linear
expansion of the band structure around the K and Krsquo This energy can be written as
19
E(k) = plusmnħvF|k (22)
where vF is the Fermi velocity of 1106ms given by
1F
Ev
k
ħ (23)
Figure 23 Band structure of graphene calculated with the tight-binding model
22
The Fermi surface of graphene consists of double cones with Fermi energy at the
intersection of these cones (Figure 23) The slope of the band is zero and hence the
effective mass of electrons in that region is zero which leads to an entirely new transport
mechanism in graphene26
20
22 Transport Characteristics of Graphene
Transport process usually involves a flow of charge or energy or both The flow is mainly
due to external perturbations such as electric field and temperature gradient The
relationship between forces and flow usually defines various transport coefficients that
are the characteristics of electrons and phonons in the material All modern electronics
are based on the ability to control the electronic properties of a material by applying
external voltage This is done by an electric field effect where the gate voltage changes
the carrier concentration of the material and consequently its conductivity The electric
field effect in graphene was reported by Novoselov in 2004 and is used in transport
measurements8
The electron-phonon interaction in graphene plays an important role in
understanding the photoemission spectra observed in graphene The electric field effect is
an alternative method for changing the charge carrier density in low dimensional systems
The electric field effect in graphene which was first reported by Novoselov et al in
2004 is widely used as a characterization tool in transport measurements25
The transport characteristics of the material are directly related to the
bandstructure of graphene The carriers in graphene lattice are free to move in two
dimensions In the carrier transport of graphene the carriers ndash electrons and holes ndash close
to the Dirac points are of importance The transport is described by a two component
wave function (Equation 24) which obeys the 2D Dirac-like equation for massless
particles27
21
-ivFσ nablaψ(r) = Eψ(r)
(24)
where σ is the 2D Pauli spin matrix In the continuum limit the above (Equation
24) corresponds to the effective low energy Dirac Hamiltonian (Equation 25)
0( )
0
x y
F F
x y
iH k k
i
k kv v
k k
(25)
The electronic band structure of the energy (E) versus wave vector (k) relation for
graphene is given by Equation 24
The two component wave function resembles the spin or wave function of
quantum electro dynamics (QED)27
Corresponding to the spin of particles in QED the
charge carriers of graphene can be attributed with a pseudospin σ The pseudospin is the
direct result of two different carbon sublattices corresponding to the bonding and
antibonding combinations27
22
Figure 24 The energy dispersion around the K point27
In Figure 24 the red and blue lines correspond to the antibonding and bonding
states respectively The pseudospin can have two values either in the direction of or
against the momentum It can be seen that the electrons with energy E travelling in the
positive direction originates from the same branch as a hole with energy ndashE travelling in
the negative direction giving it the same pseudospin This results in suppressed
backscattering and Klein tunneling The back scattering process requires the pseudospin
to flip which is possible in the presence of short range scatters that act differently on sub
lattices27
23 Drude Theory
The classical theory of metallic conductivity was presented by Drude in 1900 and was
elaborated by Lorentz in 190528
Drude treated the free electrons as classical ideal gas
meaning the electrons collide with stationary ions and not each other
23
Figure 25 Electrons colliding with stationary ions28
The Drude theory applied the kinetic theory of gases to a metal considered as a gas of
electrons The basic assumptions made by the Drude theory are28
When metallic elements are brought together to form a solid then the valence
electrons become freely moving through the metal whereas the ions remain intact
as nearly immobile positive particles
Between collisions the electrons move freely ie there is neither electron-
electron interaction nor electron-ion interaction
The scattering mechanism leads to instantaneous collisions of the electron with
the scatterers
The collisions are characterized by a relaxation time τ
The electrons achieve thermal equilibrium only through collisions the velocity
after a collision is randomly directed the speed is as appropriate to the
temperature
With the relaxation time Drude obtained the electrical conductivity expression
where n is the number of electrons per unit volume
σ = ne2τm
(25)
He also calculated the thermal conductivity and successfully provided the
theoretical basis for Wiedemann-Frantz law already established in 1853 which states that
24
the ratio of electrical and thermal conductivity of any metals is a universal constant at any
given temperature28
The Drude theory gives results which are qualitatively correct outside of the
quantum Hall regime28
In the Drude theory of the electrical conductivity of a metal an
electron is accelerated by the electric field for an average time τ before being scattered
by impurities lattice imperfections and phonons to a state which has zero average
velocity The average drift velocity of the electron is
d
eE mv (26)
It is assumed that all electrons drift together and hence the current density
j = -ne (27)
This Drude theory works well for fields below ~ 01T At stronger fields the Hall
resistivity becomes nearly constant over finite intervals of magnetic fields28
The QHE
reflects both novel disorder physics as well as novel interaction physics in the quantum
Hall regime
24 Quantum Hall Effect (QHE)
The discovery of QHE is a remarkable achievement in condensed matter physics The
Hall Effect was discovered by Edwin Hall in 187929
However the precise quantization
of the Hall conductance in units of e2h was not recognized until February 1980 Five
years later in 1985 Klaus von Klitzing was awarded the Nobel Prize in Physics for the
discovery of QHE29
The quantum Hall effect occurs in two-dimensional electron systems in the limit
of strong perpendicular magnetic field that stems from electronic transport
25
measurements where one drives a current I through the sample and where one measures
both the longitudinal and transverse resistance (Hall resistance) A longitudinal resistance
is a resistance measured between two contacts that may be connected by a line which
does not connect C1 and C430
Transverse resistance is measured between two contacts
connected by an imaginary line connecting C1 and C4 (Figure 26a)
Figure 26 (a) 2D electrons in a perpendicular magnetic field Logitudinal resistance
measured across C5 and C6 Transverse resistance measured across C3 and C5
(b) Classical Hall resistance as a function on the magnetic field30
Due to the existence of quantum Hall effect it is natural to expect that there exists
a classical Hall Effect Hall showed that the transverse resistance of a thin metallic plate
varies linearly with the strength B of the perpendicular magnetic field (Figure 26 b)
RH = Bqnel (28)
More quantitatively the classical Hall Effect can be understood within the Drude
model for diffusive transport in a metal Within this model one considers independent
26
charge carriers of momentum p described by the equation of motion
( )
b
dp p pe E B
dt m (29)
where E and B are the electric and magnetic field respectively The macroscopic
transport characteristics ie resistivity of the system are obtained from the static
solution of the equation of motion dpdt = 0 and one finds for 2D electrons with p =
(pxpy)
x
x yb
y
y xb
eBe
eBe
ppE
m
ppE
m
(210)
In the above expression characteristic frequency is visible as
C
b
eB
m (211)
This is known as cyclotron frequency as it characterizes the cyclotron motion of a
charged particle in a magnetic field30
With the Drude theory the conductivity can be
written as
j = -enelpmb (212)
and the mobility can be given as
micro = eτmb (213)
The transport properties in the limit of ωCτ-gt infin are entirely governed in the presence of
27
a magnetic field by the off-diagonal ie transverse components of
conductivityresistivity
The theory of quantum Hall effect subjects all physical properties of 2D electron
system in the limit where the magnetic field is strong so that the mixing of Landau levels
by disorder or electron-electron interaction is considered to be a weak perturbation30
This is known as the quantum Hall regime The ratios between the energy scales
corresponding to the two interactions are important The limit where disorder potential is
much stronger is referred to as integer quantum hall regime whereas the limit where the
interaction potential is much stronger is referred to as fractional quantum Hall regime
25 Resistivity and Resistance
The electronic transport in the framework of the Drude theory allows for the calculation
of conductivity or resistivity of a classical diffusive 2D electrons in a magnetic field30
The conductivity and conductance are related to one another but they depend on the
geometry of the conductor-the resistance R and hence the resistivity is given by
R = (LA)ρ (214)
where L is the length of the conductor and A is the cross section
For a d-dimensional conductor the cross section scales as Ld-1
such that the
scaling relation between the resistance and the resistivity is
R~ ρL2-d
(215)
From the dimension point of view resistance and resistivity are the same in 2D and the
resistance is scale-invariant Further the resistance of a 2D conductor depends in
general on the so-called aspect ratio LW via some factor f (LW)30
However for
transverse Hall resistance it is the length of the conductor that plays the role of cross
28
section such that the Hall resistivity and the Hall resistance truly coincide ie f=1 The
Quantum Hall effect is highly insensitive to the particular geometric properties of the
sample used in transport measurements Recently quantum Hall physics experienced the
discovery of ldquorelativisticrdquo quantum Hall effect in graphene The electrons in graphene
behave as if they were relativistic massless particles contributing to a very interesting
field of research30
26 Klein Tunneling
Klein tunneling in which relativistic particles penetrate through a potential barrier
without the exponential damping that is characteristic for nonrelativistic quantum
tunneling has never been observed for elementary particles The tunneling allows
transmission of a particle through a potential barrier higher than its kinetic energy
violating the principle of classical mechanics30
On the quantum scale the objects exhibit
wave-like characteristics in which the quanta move against a potential hill described by
their wave function This wave function represents the probability amplitude of finding
the object in a particular location The transmission of the object through the potential hill
is termed as tunneling When EltV then the ψ(x) over V is returned by ψrsquo(x) In quantum
mechanics an electron tunnels from the conduction into the valence band Such a
tunneling from an electron-like to hole-like state is called as Klein Tunneling in which the
electron avoids backscattering
In Figure 27 it is shown that an electron hitting a potential barrier is reflected
with 100 certainty In non-relativistic quantum mechanics the electrons can tunnel
through the barrier but the probability of tunneling exponentially decays with increasing
29
height and width of the barrier However in relativistic quantum mechanics the barrier
gets transparent even in the limit of infinite barrier height (Klein paradox)31
Figure 27 Klein tunneling through an npn barrier30
The Klein paradox in graphene can be understood in terms of electrons and holes
In graphene the massless carriers behave differently than ordinary carriers (with mass) in
the presence of an electric field A barrier which is repulsive for electrons will be
attractive for holes Since there are hole states inside the barrier with the same energy as
the electrons outside an electron arriving at the barrier can tunnel through it as a hole
before leaving again as an electron Klein tunneling for transport in graphene is that the
charge carriers cannot be confined by potential barriers The Klein tunneling effect has
been experimentally observed by Ando in 1998 in which the absence of backscattering
(Figure 28) is responsible for high conductivity in carbon nanotubes
30
Figure 28 Electron trajectory considering the linear electrostatic potential U(x) = Fx30
The electron is able to propagate through an infinitely high potential barrier since
it makes a transition from the conduction band to valence band In this transition from
conduction band to valence band its dynamics changes from electron-like to hole-like
The equation of motion is thus given by
2
2 2 2| | ( )
pdr E
dt E Up
p E U
v
v
at energy E (216)
This shows that in the conduction band (UltE) and in the valence band (UgtE)
In Klein tunneling the pairs of electron-like and hole-like trajectories at the same E and
py have turning points at dmin given by dmin=2v|py|F (Figure 29)
Figure 29 Electron like and hole like trajectories at same E21
31
The tunneling probability exponential dependence on dmin
2
min| |
( ) exp( ) exp( )2
y y
y
vT
F
p pdp
(217)
The applications of the Klein tunneling include Atomic clock Scanning tunneling
Microscope Tunnel diode Tunneling transistor and many more32
Since graphene
exhibits Klein tunneling it can be very useful to study the transport properties in
graphene and use it in such applications
27 Quantum Hall Effect in a Graphene
A monolayer graphene shows half-integer quantum Hall effects where the Hall
resistance is quantized at values of
2
1
xyh v eR
(218)
around filling factors
14( 1 2)Nv
(219)
where N is an integer e is the electron charge h is the Planckrsquos constant and the
factor 4 is due to spin and valley degeneracy QHE in graphene can be observed at room
temperature which is a very intriguing property (Figure 210) Graphene reveals
significant differences with respect to conventional 2D electron systems The Landau
quantization yields energy levels that disperse differently in graphene as well as
particular zero-energy level that is only half filled at the charge neutrality point (v=o)
32
Figure 210 Quantum Hall effect in graphene22
The Hall conductivity σxy and the
longitudinal resistivity of monolayer graphene as a function of carrier density at B = 14T
and T= 4K This shows half-integer QHE with chiral index J= 1
The QHE in graphene is not entirely similar to regular QHE since the charge
carriers in graphene are Dirac Fermions The charge carriers governed by
electrodynamics is given by (Equation 220) which does not apply for graphene and a
QED quantization of graphene electronic band structure is used
En = (n+12)ħω (220)
33
In the presence of magnetic field the nature of the Dirac Fermions in graphene
results in unevenly spaced Landau levels (LL) containing a distinctive LL at the electron-
hole degenerating a zero energy given by
2MG
MGFehn B
n vE (221)
The LL levels at high magnetic fields in MG are shown in Figure 211
Figure 211 (a) LL for Graphene bilayer (b) Schematics of Hall conductivity as a
function of nn0 for bilayer Graphene (solid line) and monolayer Graphene (dotted line)
(c) LL for monolayer Graphene33
It is found that the Hall resistance of a two dimensional electron system has
plateaus as a function of the number of electrons at low temperatures and strong magnetic
fields32
At large B the Dirac-like energy spectrum of graphene gives rise to a
characteristic series of QH plateaus in conductance reflecting the presence of a zero-
energy Landau level that include only odd multiples of 2e2h for uniform carrier density
in the sheet These plateaus of QH edge states at the edge of the sheet circulating in a
34
direction are determined by the direction of B and the carrier type33
This is why QHE in
graphene is known as Half-Integer Quantum Hall Effect
28 Thermoelectric Effect
Thermoelectricity refers to a class of phenomena in which a temperature difference
creates an electric potential or an electric potential creates a temperature difference The
principle of thermoelectric effect has been known for over 100 years Recently the
practical applications of thermoelectric effect have become more viable34
Thermoelectric effect is the direct conversion of temperature differences to
electric voltage and vice versa Joule heating is the heat generated whenever a voltage is
applied across a resistive material The Peltier-Seebeck effect is reversible whereas Joule
heating is not This effect can be used to generate electricity to measure temperature to
cool objects or to heat them Since the direction of heating and cooling is determined by
the sign of the applied voltage thermoelectric devices make very convenient temperature
controllers
281 Seebeck Coefficient
Thomas Johann Seebeck discovered that an emf appears in a circuit composed of two
dissimilar metals when the junction between the metals is held at different
temperatures34
The thermoelectric emf causes a continuous current in the circuit when a
complete loop is formed and the current is known as thermoelectric current This is
known as the Seebeck effect
35
Figure 212 Seebeck Effect34
As long as the two junctions are at different temperatures the thermoelectric emf
exists and the current will keep flowing between the hot and cold junction that are at
different temperatures The Seebeck effect is the conversion of temperature difference
directly into electricity The voltage developed in the circuit shown in Figure 212 is
proportional to the difference in temperature between the two junctions and is given by
V = α (T2-T1) (222)
This Seebeck effect is observed not only in metals but also in semiconductors
Here α is known as the Seebeck coefficient α measures the magnitude of an induced
thermoelectric voltage in response to the temperature difference across the material If the
temperature difference ∆T between the two ends of a material is small then the Seebeck
coefficient of a material is written by
α = ∆V∆T (223)
36
This can be expressed in terms of electric field as
α E∆T (224)
The units of Seebeck coefficient is given as VK The higher the Seebeck coefficient
value the better it is since it will create a very large voltage that can be used to provide
power
282 Peltier Coefficient
Peltier effect is the inverse of Seebeck effect involving a junction phenomenon There is
heat absorption or generation at the junctions depending on the direction of current flow
Heat generated by current flowing in one direction is absorbed if the current is reversed
The heat absorbed per second at a junction carrying current I is given by
Heat absorbed in t sec = πabIt (225)
Here πab is the Peltier coefficient and given by HIt Thus Peltier coefficient is
numerically equal to the applied potential difference expressed in Volts
Overall by studying the flow of electrons the values of Seebeck
coefficient and Peltier co-efficient can be estimated These values determine the various
applications of the materials In this thesis the Peltier and Seebeck coefficient of the
graphene junction and the new applications are discussed
37
29 Early Research ndash ab intio studies
In 2007 Androitis studied that the conducting properties of graphene nanoribbons and
junctions are strongly dependent on their size and geometric features35
He concluded that
there is no conductance for small AZA or ZAZ ribbons (Figure 213)
Figure 213 Transmission functions in units of (2e
2h) for AZA structures
35
Figure 213 shows that T (E) exhibits a negligible peak [T (E) = 001 in units of
2e2h] at E= -225 and 250eV However it was noted that when the width of the arm type
was increased T (E) at -225 and 250eV was 02035
Later in 2007 Qimin Yan used first principles methods to investigate the Current-
Voltage characteristics of GNR Transistors and the effect of edge doping He showed that
GNR field effect transistors can achieve high performance levels with ONOFF ratios on
the order of 103-10
436
Figure 214 is an I-V curve of AZA GNR-FET connected via
armchair metallic leads36
38
Figure 214 I-V curve for a 591nm long channel (Vbias=20mV)
36
In 2009 Fangping OuYang demonstrated the intrinsic transport properties and
effective B or N doping of the junctions by using first-principles quantum transport
simulations He concluded that the I-V characteristics of pure-carbon T-shaped junctions
exhibit metallic behavior and the current in the junction strongly depends on the height
of the stem23
He reported that the conductance of the devices depends on the geometric
structures which can be controlled by selective doping
In 2012 Wei Yao used the first principle calculations based on Density
Functional Theory (DFT) and Non-equilibrium Greens Function (NEGF) to study the
electronic as well as the transport properties of B-doped 6-GNR p-n junction His results
showed that the boron doping interval can influence the rectification effect at low bias
and also exhibit Negative Differential Resistance (NDR) phenomena at high positive
bias
39
CHAPTER 3
COMPUTATIONAL DETAILS
31 Introduction
The physical chemical electrical electronic and optical properties of a solid are
determined by their quantized electronic states The quantum states in low-dimensional
systems are produced due to the confinement of the carrier charges in one or two
dimensions Graphene is a conductor electrons are able to flow through graphene more
easily than through even copper The electrons can travel through the sheet of graphene
like mass-less particles as fast as just one hundredth that of the speed of light The ways
in which electrons behave in graphene make it very helpful to study their fundamental
physical properties Graphenersquos near perfect crystal lattice provides a very clean system
to experiment By restricting the electrons to only two dimensions they exhibit some
interesting properties such as the anomalous quantum Hall effect and Klein tunneling
In this chapter two theoretical concepts used for calculating the electronic structure
and the transport properties for graphene are described These include the Extended
Huckel Theory and Non-Equilibrium Greenrsquos Function (NEGF) method
311 Extended Huckel Theory
Erich Huumlckel was born in Germany on August 9th
1896 He studied mathematics and
physics in Berlin He is best known for his work in the field of chemistry and physics for
two contributions (1) Debye- Huumlckel theory of electrolytic solutions (2) Huumlckel
method of approximate molecular orbital calculations on electron systems In 1930 he
published his findings on systems in 1931 he generalized and expanded the system
40
theory to explain benzene Due to his poor communication skills his findings went
unrecognized for over 20 years It was in 1951 that his 4n + 2 rule was finally clarified by
Doering to show if C=C bonds would show aromaticity Huumlckel died on February 16th
1980 with very little worldwide recognition for his contributions to chemistry Today
chemistry students recognize his name and his contributions to the field are quite
substantial
One of the first semi-empirical methods to be developed was Huumlckel Molecular
Orbital Theory (HMO) HMO was developed to describe molecules containing
conjugated double bonds HMO considered only electrons in pi orbitals and ignored all
other electrons in a molecule The Extended Huumlckel Molecular Orbital Method (EH) was
developed out of the need to consider all valence electrons in a molecular orbital
calculation
By considering all the valence electrons chemists could determine molecular
structure compute energy barriers for bond rotations and determine energies and
structures of transition states for reactions By considering only the valence electrons the
computed energies could be used to choose between proposed transition states to clarify
reaction mechanisms The total valence electron wavefunction is described as a product
of the one-electron wave functions
1 2 3(1) (2) (3) ( )valence j n (31)
where n is the number of electrons and j identifies the molecular orbital Each
molecular orbital is written as a linear combination of atomic orbitals (LCAO)
1 12
N
j jr rrc j N
(32)
41
The energy of the jth
molecular orbital is given by a one-electron Schroumldinger
equation using an effective one electron Hamiltonian heff which expresses the interaction
of an electron with the rest of the molecule
eff j j jh (33)
This is the energy eigenvalue of jth
molecular orbital corresponding to the Eigen
function j The advantage of using this method is that the exact form of heff is not
required The total energy of the molecule is the sum of the single electron energies
j jj
E n (34)
where nj is the number of electrons in orbital j
In order to use the Extended Huckel method a set of calculation parameters and
approximations must be followed These parameters include the Basis set K-point and
the Brillouin Zone and lastly the Mesh cut-off
312 Introduction to NEGF
The Greenrsquos function is a function of two space-time coordinates From the knowledge of
this function one can calculate time-dependent expectation values such as currents and
densities electron addition and removal energies and the total energy of the system In
the absence of external fields the non-equilibrium Green function method reduces to the
equilibrium Green functions NEGF can be applied to both extended and finite systems
The generic system of NEGF consists of the electron dynamics of the channel described
by the Hamiltonian This channel consists of two contact reservoirs with respective
chemical potential μR and μL The NEGF assumes ballistic transport neglecting self-
42
energy from scattering The system is insulated from gate contacts whose effects are
realized via a 3D Poisson solver which solves for the potential at a given point in real
space based on electron density
22 ( ) [ ( ) ( )]D
qr N r n r
(35)
Figure 31 NEGF system
The system is easily expandable to systems with several contacts or gate
configurations by adding additional self-energy matrices to NEGF or additional sources
to the Poisson solver
313 Electrostatics
Electrostatic potential is created every time in the presence of a charge density due to an
induced electric field The Poissonrsquos equation correlates the electrostatic potential to
charge density as given in Equation 36
43
2( ( ) ( ) ( ) ( ))( )
( )( ) ( )
ADq p r n r r N rr
rr r
N
(36)
where ɛ(r) is the dielectric permittivity of the material ρ(r) n(r) ND(r) and NA(r) are the
hole electron donor and acceptor concentrations of the system respectively
Two types of boundary conditions are usually applied to the Poissonrsquos equation
Dirichlet boundary conditions
Φ (0) = F0 and Φ (L) = FL
von Neumann boundary conditions
00
( )
x
d x
dxB
and
( )L
x L
d x
dxB
For the transport problems with open boundary conditions the von Neumann
boundary conditions are used assuming that the potential vanishes at the boundary ie
B0=BL=0
The Poissonrsquos equation can hence be discretized on a grid as
2 ( )( )
( )
rx
r
= M (37)
where M is the matrix Φ and ρ are vectors containing the discretized values of
the electrostatic potential Φ and charge density ρ respectively
44
The Schroumldinger and Poisson equations are coupled since V(x) = -qΦ(x) is used
for the Schroumldinger to compute ρ(x) This self-consistent loop stops when the
convergence is reached
( )r
V(x) = -qΦ(x)
314 Non-Equilibrium Greenrsquos Function
Greenrsquos functions are a mathematical construction that are used to solve differential
equations subject to specific initial or boundary conditions They are named after the
British mathematician George Green The 1-D equation of L( )f( )=S( ) can be defined
by the Greenrsquos Function as given below
( ) ( ) ( )G x x f x x x (38)
The general Greenrsquos function is given by
( ) ( ) ( )f x dx G x x S x (39)
Applying the operator L( ) to the solution f( ) satisfies the original differential
equation The Greenrsquos Function G( ) is the propagator which propagates the influence
of a perturbation S( ) originally situated at the point to the point at which the
function f( ) is evaluated
The Greenrsquos Function G( ) can also be a correlation function If the points
and are strongly (weakly) correlated then S( ) will greatly (poorly) affect f( )
Poisson equation
2 ( )( )
( )
rr
r
Schroumldinger equation
2
2
( ( ) ) ( )
( )2
( ) | ( ) |
E H r E r S
H V rm
r dE E r
Figure 32 Self-consistent loop
45
The Schroumldinger equation with open boundaries can be written as
( )E H S (310)
Considering a 1-D and homogenous system ranging from =0 to L assuming
that Σ=0 and the form of equations is same before and after discretization then
22
2 0( ) ( ) ( )
2E x S x
m
dV
dx
(311)
The Greenrsquos function can hence be computed corresponding to the Schroumldinger
equation
22
2 0( ) ( ) ( )
2E G x x x x
m
dV
dx
(312)
Due to the delta-function at = a discontinuity is observed and hence the
Greens function is evaluated at boundary conditions
0
2
exp( ( )) x x 2 ( )( )
exp( ik(x x)) x x
ik x x m E VG x x k
A
A
(313)
By integrating the Schroumldinger equation twice and setting the lower and upper
integration boundaries to = -δ and = +δ the Greenrsquos Functions can be written as
2
( ) ( ) 0
( ) ( ) 2
x x x x
G x x G x x
dG x x dG x x m
dx dx
(314)
46
The coefficient A+ and A
- become
ik
mA A
(315)
The Greenrsquos Function takes a final form known as Retarded Greenrsquos Function and
is written as
( ) exp( | |)G x x i ik x xk
m (316)
And the wave function is
( ) ( ) ( )x dx G x x S x (317)
Retarded Greenrsquos Function propagates the wave functions generated by a source
or perturbation S from its origin at to any point
The retarded Greenrsquos Function as discretized Schroumldinger equation is written as
( )R RE H G I (318)
The wave function Φ can be calculated from the retarded Greenrsquos function and the
source vector as
Φ = GR∙S (319)
Overall in this section the Greenrsquos function approach in calculating the electron
dynamics is reviewed We defined the self-energy of each part of the system spectral
function and the probability current density the electric current is derived explicitly using
Non Equilibrium Greenrsquos function We will use this formalism to calculate the tunneling
phenomena in coupled quantum dots isolated or otherwise
47
CHAPTER 4
ATOMISTIX TOOLKIT DETAILS
41 Introduction
Virtual NanoLab (VNL) is a graphical user interface (GUI) that provides a group of
modeling tools the function of these tools involves the set-up investigation and the
study of nanoscale structures The quantum mechanical equations are solved by the
software by using the advanced software architecture and numerical methods to
implement ab initio calculations VNL simulates the electronic structure and calculates
the transport properties based on the two systems mentioned earlier NEGF and Extended
Huckel ATK is the main engine for computing the scripts and hence all the calculations
performed in VNL are done by ATK VNL is a user friendly software as it not only
allows creating a script but also helps to set up a virtual experiment
This thesis involves the use of VNL in order to study the effect of the width and
different orientations of the doped atoms Since the software allows for virtual
experiments it makes it much easier to study the I-V characteristics based on the change
in position of atoms
42 Device Structure
In this thesis AZA GNR p-n junction with boron doping (location) was created using the
ATK software which is based on NEGF and DFT Further the thesis discusses the
transport properties and the I-V curve of such junction
The input format of ATK is NanoLanguage which is an extension to Python
scripting language ATK uses the NEGF system for formalism of simulating device
48
Figure 41 Geometry of device configuration with two electrodes
37
The system is divided into three parts left central and right The implementation
relies on the screening approximation which assumes that the properties of the left and
right regions can be decribed by solving a bulk problem for fully periodic electrode cell37
This screening approximation is fulfilled when the electrode regions can be described by
an equilibrium electron distribution
Figure 42 The electron distribution in a device configuration which illustrates a left
moving scattering state with origin in right electrode37
The system assumes that in steady state the electron density of the central region
is constant in time and hence the electron density is calculated independently from each
electrode The electron density is given by the occupied eigenstates of the system
n(r) = nL(r) + n
R(r) (41)
49
The left and right densities are calculated by summing up the occupied scattering
states
nL(r) = sum
(42)
nR(r) = sum
(43)
The scattering states are usually calculated by first calculating the Bloch states in
the electrodes and then solving the Schroumldinger equation of the central region using the
Bloch state as matching boundary Instead of using the scattering states the ATK
software uses the NEGF method to calculate the non-equilibrium electron density
The electron density is given in terms of electron density matrix
D = DL + D
R (44)
The left density matrix is given by NEGF theory
DL = int
(45)
where
ρL(ɛ) =
(46)
ρL(ɛ) = is the special density matrix
Also if there is a non-equilibrium electron distribution in the central region then
the electron distribution in electrode is given by the Fermi function f with an electron
temperature TL
G(ɛ) =
(47)
G = retarded Green function
δ+ is an infinitesimal positive number and S H overlap the Hamiltonian matrices
L =
sum sum
(48)
50
L
is the broadening function of the left electrode given in terms of left electrode
self -energysum
43 Transmission Spectrum Calculations
Once the self-consistent non-equilibrium density matrix has been obtained the various
transport properties of the system can be calculated One of the most important properties
is the transmission spectrum from which the current and differential conductance can be
obtained
The transmission coefficient in ATK is obtained by the retarded Greens function
T(ɛ) = G(ɛ)ΓL(ɛ)G
ϯ(ɛ)Γ
R(ɛ) (49)
The transmission amplitude of individual scattering states may be obtained
through the Transmission Eigenvalues The ldquoTransmission Eigenvaluesrdquo is an analysis
which finds the eigenvalues of the transmission matrix
The transmission matrix at energy E and k-point is given by
Tnm(Ek) = sum (410)
where
= transmission amplitude from Bloch state ψn(k)
The transmission coefficient is given by the trace of transmission matrix
T(Ek) = sum (411)
Keeping in mind all quantities depend on the quantum numbers parametrically
Transmission eigenvalues sum up to the transmission coefficient
T = sum (412)
51
44 Calculating the Current
Current is calculated from the transmission coefficient using
I( ) ( )R L
L RL R
R LB B
eE f f dE
h
E EV V T T T
k kT T
(413)
where f is the Fermi function TRL is the electron temperature of the right or left
electrode and Tσ(E) is the transmission coefficient for the spin component σ
The chemical potentials of the left and right electrode given by
L
F R LR L
eVE
are defined relative to the Fermi level of the left electrode These chemical potential are
related to the applied bias and hencebiasR L
eV therefore bias L RV V V
The transmission spectrum itself is usually rather insensitive to temperature and is
used in self-consistent calculations but often depends strongly on the electrode voltages
Thus for an accurate estimate of the current the transmission spectrum should be
calculated self-consistently for each desired bias
ATK uses very precise method to calculate the transport properties of the system
Transmission spectra for various concentrations of boron doped graphene p-n junctions
are generated in this Chapter and various coefficients such as Seebeck Peltier and
Conductance are calculated
52
45 Calculating Transport coefficients
The linear response transport coefficient of an applied voltage difference or temperature
difference between the two electrodes is given by
Conductance
| dT 0
e
dI
dUG
(414)
Peltier coefficient
| d 0
Q
I
I
(415)
Seebeck coefficient
| 0
dUS I
dT T
(416)
These linear response coefficients are calculated by the Transport Coefficients To
perform these calculations the ATK uses the Electron Transmission Spectrum
53
CHAPTER 5
RESULTS AND DISCUSSION
51 Band Structure Analysis
The electronic bandstructure of GNR both doped and undoped are discussed in this
chapter
The armchair configuration of Pristine GNR (PGNR) has a band structure that is
dependent on its width This is explained by the fact that the sheet itself acts like a
potential well where the electrons are confined to form standing waves along Cr the
rolling vector albeit with slightly different boundary conditions (Cr = ma1 + na2
where m and n are integers and a1 and a2 are the unit cell vectors of graphene lattice) In
a GNR the two nodal points of the standing wave must be at the ribbon edge while in a
Single wall nanotube (SWNT) they can be anywhere ie a circumferential periodic
boundary condition
(a) (b)
Figure 51 Bandstructure of AGNR widths (a) 4 atoms (b) 5 atoms
54
(a) (b)
Figure 52 Bandstructure of AGNR widths (a) 6 atoms (b) 7 atoms
(a) (b)
Figure 53 Bandstructure of AGNR widths (a) 8 atoms (b) 9 atoms
55
(a) (b)
Figure 54 Bandstructure of AGNR widths (a) 10 atoms (b) 11 atoms
Figure 55 Bandstructure of AGNR with a width of 12 atoms
Figure 56 Variation in band gaps as the width (number of atoms) varies
0
05
1
15
2
25
0 2 4 6 8 10 12 14
Wdith vs Band Structure
eV
56
The band structure of 12 Atom AGNR is close to that of Ge (0626 eV) The
actual width of this nanoribbon is about 25 nm 12 AGNR has been fabricated
successfully and doped with various dopants Hence the 12 Atom AGNR has been chosen
to study the transport properties
A junction is created using ZGNR and AGNR To maintain the consistency in the
device analysis it is imperative that the band structure of ZGNR is also calculated From
the simulation it is evident that ZGNR-AGNR-ZGNR junction configuration displays the
Metal ndashSemiconductor-Metal configuration that is addressed in this work The Fermi
Level in all the Z-GNR nanoribbons of widths 4-12 lies within the conduction band
Figure 57 Band structure of ZGNR width (a) 4 atoms (b) 6 atoms
57
(a) (b)
Figure 58 Band structure of ZGNR width (a) 8 atoms and (b) 10 atoms
Figure 59 Band structure of ZGNR with a width of 12 atoms
In order to create viable junction that would show transistor properties doping of
the semiconductor part is necessary The 12 atom AGNR is doped with boron (p-type)
and nitrogen (n-type) - (Figure 510a) 4 N doped (Figure 510b) 4 B In both cases
the impurities lie on the edge of the atoms For 2 nitrogen doped GNR with the
58
impurities lying in the center of the ribbon the Fermi level is found to be in the
conduction band as shown in (Figure 510c) (Figure 510d) shows the position of N with
respect to the edge A very clear departure from the expected (the valence band extending
above Fermi level) is shown in (Figure 510a)
Figure 510 Band structures of Doped AGNR (a) 4 N Doped (b) 4 B Doped (c) 2
N Doped (d) position of Nitrogen from (c)
(a) (b)
(c) (d)
59
52 I-V Characteristics of GNR junction
In pristine graphene the chirality determines the conductivity as seen from the I-V curves
for various widths At certain widths the semiconducting properties are more
pronounced These widths determine the wavelengths of the standing waves which in
turn determine the sub-band locations in the E-k plot When the biasing potential
exceeds 012V the I-V curve shows linearity In case of the 8-atom wide PGNR the
band gap is about 03 eV and it is evident from the I-V plot that the On-State is + 033 V
The band gap of 10-atom and the 4-atom wide PGNR is large enough to show
semiconducting properties
Figure 511 Current Vs Voltage graph for varying graphene width showing
conductivity
-30000
-20000
-10000
0
10000
20000
30000
-3 -2 -1 0 1 2 3
Cu
rre
nt
(nA
)
Voltage (V) (bias)
Current (nA) Vs Voltage for varying graphene width
W=10
W=8
W=6
W=4
60
The ZAZ GNR Configurations show the properties of a semiconductor junction The 12
atom ZAZ structure is studied for its I-V characteristics In this Chapter undoped B-
doped N-Doped B and N Doped (P-N Junction) ZAZ junctions are simulated
Figure 512 ZAZ GNR junction device
61
The boron doped ZAZ junction I-V characteristics are shown below (Figure 513)
The impurity concentration is 2 and 4 Various device configurations are studied
Figure 513 I-V curve of Boron Doped ZAZ junction
-25000
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
25000
-205 -155 -105 -055 -005 045 095 145 195
Cu
rre
nt
(nA
)
VBias
2B_1G_R 2B_0G_R
4B_0G_L 4B_0G_C
4B_0G_R 4B_1G_L
4B_1G_C 4B_1G_R
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
-2 -1 0 1 2
Cu
ren
t(n
A)
VBias
4 B doped GNR Jn
62
Figure 514 I-V curve of Nitrogen Doped ZAZ
-25000
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
-2 -15 -1 -05 0 05 1 15 2
Cu
rre
nt(
nA
)
VBias
I-V Curve as function of Dopant location
2N_0G_L2N_0G_C2N_0G_R2N_1G2N_1G_C2N_1G_R
-15000
-10000
-5000
0
5000
10000
15000
-2 -1 0 1 2
Cu
rre
nt(
nA
)
VBias
2N_0G_C
2N_1G_C
63
Figure 513 and Figure 514 show the I-V characteristics of the GNR junction doped with
2 boron and nitrogen respectively The location of N and B is at the central region of
the edge of the GNR Both B doped and N doped GNR Junctions show significant
Negative Differential Resistance (NDR) This is more pronounced in case of nitrogen
doping Another interesting observation is increasing ohmic nature with the change in
location of the dopants Nitrogen doped device configuration exhibits a pronounced
semiconductor behavior and the NDR effect is observed to be minimal
53 Thermoelectric Properties
In this study the thermoelectric properties were simulated for the GNR Junctions that
displayed high NDR effect The variation in the Peltier coefficient with temperature is
shown as function of doping
When the concentration of nitrogen increases the dimensionless Figure of Merit
ZT seems to decrease considerably This is mostly explained by the decrease in both
conductivity and mobility of the electrons
ZT = S2σTk (51)
where S is the Seebeck coefficient σ is the electrical conductivity T is the
absolute temperature and k is the thermal conductivity
64
Figure 515 Variation of Peltier coefficient with temperature as function of
doping
Figure 515 shows the maximum Peltier coefficient for 2 boron This is
explained by the scattering by boron and the associated smallest mean free path
0
0001
0002
0003
0004
0005
0006
0007
0008
0009
001
250 270 290 310 330 350 370 390 410
ZT
T (K)
2B
4B
Undoped
2N
4N
65
CHAPTER 6
CONCLUSIONS
Graphene ZAZ junctions exhibit varying properties depending on the various structural
configurations In this thesis it was found that the transport properties of graphene
depend on their width the edge of GNR doping concentration and the type of dopant
used The calculations of the band structure contributed towards the determination of the
minimum length of GNR required for studying the transport properties The minimum
length had a band gap equivalent to that of germanium and hence the importance of the
width being 12 atoms wide This band gap indicated fluctuating changes when doped
with elements such as B and N The viable junction showing transistor properties was
hence created by doping the semiconductor part of ZAZ By doping the I-V
characteristics were studied which showed significant NDR which was more pronounced
in the case of nitrogen Also the changing positions of the dopants contributed towards
the I-V curve to be more ohmic The edge doping caused minimum NDR and
semiconductor behavior as compared to central doping Lastly the thermoelectric
properties were studied - the increasing concentration of N causes the Figure of Merit to
decline due to the decrease in conductivity as well as mobility of electrons
66
REFERENCES
1 Wikianswers What makes carbon unique
httpwikianswerscomQWhat_makes_carbon_so_unique (22 November)
2 Kopeliovich D D Graphite
httpwwwsubstechcomdokuwikidokuphpid=graphite (1128)
3 Barbier M Transport properties of nanostructures and superlattices on single layer and
bilayer graphene University Antwerpen Antwerpen 2012
4 Shylau A Electron transport interaction and spin in graphene and graphene
nanoribbons Linkoping Norrkoping 2012
5 HassJ R F T Li X Li Z Zong W A de Heer P N First E H Conrad C
AJeffrey and C Berger Applied Physics Letters 2006 89 (14) 143
6 Jones A Mechanical Exfoliation to Make Graphene and Visulization
httpcarbonchemwisceduFilesMechanicalExfoliationpdf (18 October)
7 Anteroinen J Structural and Electrical Characteristics of Graphene Field Effect
Transistors AALRO school of Electrical Engineering AALTO 2011
8 Novoselov K S A K G S V MorozovD JiangY Zhang S V Dubonos I V
Grigorieva A A Firsov Science 2004 306 (22)
9 Kosynkin D A L H A Sinitskii J R Lomeda A Dimiev K B Price and J M
Tour Nature 458 876
10 Yi Z Luyao Zhang Accounts of chemical research 46 (10) 2339
11 Eizenberg M B JM 1979 82 236
12 Yu Q K L J Siriponglert S Li H Chen Y P Pei S S Applied Physcis
Letters 2008 93 (113103)
13 Li X C W An J Kim S Nah J Yang D Piner R Velamakanni A Jung I
TutucE Banerjee S K Colombo L Ruoff R S Science 2009 324 1314
14 Schaefer H E Nanoscience Springer Berlin 2010
15 Levente Tapasztoacute G D Philippe Lambin amp Laacuteszloacute P Biroacute Nature Nanotechnology
2008 3 401
67
REFERENCES
16 Dacheng Wei Y L Advance Materials 2010 22 (30) 3241
17 Wei Yao K L Y GYGao Elsevier Solid State Communications 2013 153 52
18 Dacheng Wei Dagger Yunqi Liudagger Yu Wangdagger Hongliang ZhangdaggerDagger Liping HuangdaggerDagger
Yudagger a G NanoLetters 2009 9 (5) 1758
19 Nakada K M F G Dresselhaus and M S Dresselhaus PhysRevB 1996 54
(9858)
20 Son Y W C M L a L S G PhysRevLett 2006 97 (216803)
21 Raza H Graphene Nanoelectronics Springer 2012
22 Ryan W J Electronic Transport in Graphene p-n junctions Short Noise and
Nanoribbons Harvard University 2009
23 Fangping OuYang J X Rui Guo Hua Zhang and Hui Xu Nanotechnology 2009
20 6
24 Guo J Carbon nanotube electronicsModeling physics and applications Purdue
University West Lafayette IN 2005
25 Motta C S S-P MITrioni cond-matmes-hall 2012 7
26 B P Growing Graphene via Chemical Vapor Deposition Ponoma College Ponoma
2011
27 ZurichE Transport properties of three-terminal graphene devices University of
Science and Technology Norway 2008
28 Uichiro MIntroduction to the electron theory of metals
29 Robert Laughlin H S Additional background material on the Nobel Prize in Physics
1998 (410)
30 MarkGoerbig Quantum Hall Effects (11152013)
68
REFERENCES
31 Zurich E Transport properties of three-terminal graphene devices Norwegian
University of Science and Technology Norway 2008
32 Deepak R Klein Tunneling University og Tennessee Space Institute Tennessee
2011
33 Williams JR L D CMMarcus Quantum Hall Effect in a Gate-Controlled p-n
Junction in Graphene (1122013)
34 Avadhanulu MN P G K A Textbook of Engineering Physcis for BE BSc (Engg)
SChand New Delhi 1992
35 Andriotis A Applied Physics Letters 2007 91 (152105)
36 Qimin Yan B H dagger Jie Yudagger Fawei Zhengdagger Ji ZangDagger Jian Wudagger Bing-Lin Gu F
L Dagger and Wenhui Duandagger NanoLetters 2007 7 (6) 1473
37 Soler J M E A J D Gale A Garciacutea J Junquera P Ordejoacuten and D Saacutenchez-
Portal J Phys Condens Matter 2002 14 2745
vii
TABLE OF CONTENTS
(Continued)
Chapter Page
281 Seebeck Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
34
282 Peltier Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
36
29 Early Research ndash ab initio Studyhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
37
3 COMPUTATIONAL DETAILShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
31 Introductionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
311 Extended Huckel Theory helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
39
312 Introduction to NEGFhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
41
313 Electrostaticshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
42
314 Non-Equilibrium Greenrsquos Functionhelliphelliphelliphelliphelliphelliphelliphelliphellip
44
4 ATOMISTIX TOOLKIT DETAILShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
41 Introductionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
42 Device Structurehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
47
43 Transmission Spectrum Calculationhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
50
44 Calculating the Currenthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
51
45 Calculating the Transport Co-efficienthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
52
5 RESULTS AND DISCUSSIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
53
51 Band Structure Analysis helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
53
52 I-V Characteristics of GNR Junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
59
53 Thermoelectric Propertieshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
63
6 CONCLUSIONhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 65
REFERENCEShelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
66
viii
LIST OF FIGURES
Figure Page
11 (a) Chemical representation of Carbon (b) Graphite ore (c) Structure of
Graphite and a single layer Graphenhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
2
12 An optical image of Graphene flake obtained by exfoliation of
graphitehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
3
13 (a) Graphene formation on Nickel (b) Graphene atoms on Ni (111)
lattice (c)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
7
14 (a) SEM image of graphene on copper foil (b) High-resolution SEM
image of graphene on Cuhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
8
15 (a) Transfer process (b) Wafer-scale synthesis of graphene (c) Graphene
films transferred onto glass wafer (d) SiSiO2 with device patterned (e)
PET filmhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
9
16 (a) High-magnification image of the annealed sample showing that well-
defined zigzag armchair and zigzag-zigzag edges are formed (b) ) STM
image of an 8 nm wide bent junction connecting an armchair and a
zigzag graphene nanoribbon which was carved by STM
tipshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
10
17 Band structure of graphene before and after doping The image shows
shift towards the Fermi levelhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
11
18 Low resolution TEM image of N-doped graphene Background is the
lacey carbon TEM grid graphene sheet is crumpled with many
rippleshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
13
19 Zigzag and Armchair orientation of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphellip 13
110 Bandstructure of ZGNRhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 14
111 Bandstructure of AGNRhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 15
21 Left Real space Graphene lattice with basis vectors and Right
The first Brillouin zone of Graphene in reciprocal space with basis
vectors and K and Krsquo are responsible for massless transport at low
energyhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
ix
LIST OF FIGURES
(Continued)
Figure Page
22 Bandstructure of a graphene sheet showing a band gap of 0eVhelliphelliphellip 18
23 Band structure of Graphene calculated with the tight-binding modelhellip 19
24 The energy dispersion around the K pointhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 22
25 Electrons colliding with stationary ionshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 23
26 (a) 2D electrons in a perpendicular magnetic field Logitudinal resistance
measured across C5 and C6 Transverse resistance measured across C3
and C5 (b) Classical Hall resistance as a function on the magnetic field
25
27 Klein tunneling through an npn barrierhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 29
28 Electron trajectory considering the linear electrostatic potential U(x) = Fx 30
29 Electron like and hole like trajectories at same Ehelliphelliphelliphelliphelliphelliphelliphelliphellip 30
210 Quantum Hall effect in graphene 22
The Hall conductivity σxy and the
longitudinal resistivity of monolayer graphene as a function of carrier
density at B = 14T and T= 4K This shows half-integer QHE with chiral
index J= 1helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
32
211 (a) LL for Graphene bilayer (b) Schematics of Hall conductivity as a
function of nn0 for bilayer Graphene (solid line) and monolayer
Graphene (dotted line) (c) LL for monolayer Graphenehelliphelliphelliphelliphelliphelliphellip
33
212 Seebeck Effecthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 35
213 Transmission functions in units of (2e2h) for AZA structureshelliphelliphelliphellip 37
214 I-V curve for a 591nm long channel (Vbias=20mV)helliphelliphelliphelliphelliphelliphelliphellip 38
31 NEGF systemhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 42
41 Geometry of device configuration with two electrodeshelliphelliphelliphelliphelliphelliphellip 48
42 The electron distribution in a device configuration which illustrates a left
moving scattering state with origin in right electrodehelliphelliphelliphelliphelliphelliphelliphellip
48
x
LIST OF FIGURES
(Continued)
Figure Page
51 Band structure of AGNR widths (a) 4 atoms (b) 5 atomshelliphelliphelliphelliphelliphellip
53
52 Band structures of AGNR widths (a) 6 atoms (b) 7 atomshelliphelliphelliphelliphelliphellip 54
53 Band structure of AGNR widths (a) 8 atoms (b) 9 atomshelliphelliphelliphelliphelliphelliphellip 54
54 Band structures of AGNR widths (a) 10 atoms (b) 11 atomshelliphelliphelliphelliphellip 55
55 Band structure of AGNR with a width of 12 atomshelliphelliphelliphelliphelliphelliphelliphelliphellip 55
56 Variation in band gaps as the width (number of atoms) varieshelliphelliphelliphellip 55
57 Band structure of ZGNR width (a) 4 atoms (b) 6 atomshelliphelliphelliphelliphelliphelliphellip 56
58 Band structure of ZGNR width (a) 8atoms and (b) 10 atoms 57
59 Band structure of ZGNR with a width 12 atomshelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 57
510 Band structures of Doped AGNR (a) 4 N Doped (b) 4 B Doped (c)
2 N Doped (d) position of Nitrogen from (c)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
58
511 Current Vs Voltage graph for varying graphene width showing
conductivityhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
59
512 ZAZ GNR junction devicehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 60
513 I-V curve of Boron Doped ZAZ junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 61
514 I-V curve of Nitrogen Doped ZAZhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 62
515 Variation of Peltier effect coefficient with temperature for various doping 64
1
CHAPTER 1
INTRODUCTION
11 Graphene The New Carbon
Carbon (chemical symbol C atomic mass 1207amu) (Figure 11a) is a widely distributed
element in nature It is found abundantly in the sun stars comets and the atmospheres of
the planet Carbon can form up to four bonds it can bond with itself endlessly and with
most other elements in many different shapes making it a significant part of the
construction for many kinds of complex molecules1
Two allotropes of carbon are commonly used diamond and graphite (Figure
11b) The bonding structures of diamond and graphite contribute to the properties
individually In diamond all the p-orbitals are used forming a sp3
bonding whereas in
graphite only two orbitals are occupied allowing the unpaired bond for the transport of
electrons Each carbon atom in graphene possesses sp2 hybridization ie each carbon
atom is connected to three other carbon atoms via covalent bonds with a bond length of
142Å and an angle of 120deg between each bonded pair This makes graphite a better
conductor than diamond Graphite consists of many layers of 2D carbon lattices (Figure
11c) stacked on top of each other and held via Van der Waals forces A single layer of
graphite where carbon atoms are arranged in a honeycomb lattice is known as graphene
(Figure 11c)
2
Figure 11 (a) Chemical representation of Carbon (b) Graphite ore (c) Structure of
Graphite and a single layer Graphene2
Theoretical work on graphene was done specifically to study the other allotropes
The first study was done by Wallace in 1947 who calculated the band structure of
graphene3 Further the peculiar Landau levels were known by McClure in 1957 and the
relativistic Hofstadter butterfly by Ramal in 19853 Later in 1991 the invention of carbon
nanotubes by Iijima boosted the theoretical research on graphene3 Prior to the invention
of carbon nanotubes there were a few experimental papers on graphene growth via
various methods like intercalation of graphite (Shioyama 2001) free standing (Boehm
1962) epitaxial as well as graphene grown on metals (Bommel 1975 Land 1992 Itoh
1991)3 With all the various discoveries the electronic properties of graphene were not
studied until 2004 when Berger and Novoselov were able to access the electronic
properties with contact of graphene flakes3 (Figure 12)
3
Figure 12 An optical image of Graphene flake obtained by exfoliation of graphite3
The specific lattice structure of graphene possesses a number of unique electronic
properties making it an interesting material for theorists experimentalists and engineers
Utilization of graphene as a fundamental block of electronic devices requires
development of new theoretical methods for understanding the current propagations in
graphene constriction4
12 Graphene Synthesis
The discovery of graphene by mechanical exfoliation called the lsquoScotch tape methodrsquo led
to serious attempts towards the production of top quality graphene5 Graphene was first
exfoliated mechanically from graphite in 20046 The importance of high quality graphene
cannot be emphasized enough however electron transport has shown that defects play an
important role in hindering the transport properties of electrons (holes)7 The two
synthesizing methods for the large scale manufacture of graphene are chemical vapor
deposition (CVD) and silicon carbide (SiC) desorption method
4
Graphene can be synthesized by sublimation of silicon from SiC at high
temperature (1200degC) in high vacuum5 The major advantage of this method is that the
SiC provides an insulating substrate and no transfer of the graphene layer is needed Yet
the disadvantage of this method outweighs its advantages the high temperature is cost-
ineffective making it unsuitable for large scale manufacturing8 Also the crystal growth
face alters the properties of graphene Graphene grown on Si-terminated face has poor
homogeneity and is subjected to unintentional doping7 Conversely graphene grown on
C-terminated SiC has higher mobility and is often called lsquoturbostaticrsquo due to the
rotational disorder7
Unlike the SiC method the graphene produced via CVD method needs to be
transferred to a substrate making it difficult to maintain the quality of graphene Yet
CVD synthesized graphene has a larger grain size7 More research is being done on
various methods for synthesis of graphene The methods include direct chemical
synthesis ion implantation crystal sonification and lastly unzipping carbon nanotubes to
form graphene sheets9
Graphene and few-layer graphene have been grown by CVD from carbon
containing gases on catalytic metal surfaces andby surface segregation of C dissolved in
the bulk of such metals7 Growing graphene with CVD is a very attractive solution since
it is compatible with the existing semiconductor industry9 Graphene has been grown via
CVD process on metal substrates such as Nickel (Ni) and Copper (Cu)
5
121 Synthesis of Graphene on Nickel (Ni)
Polycrystalline Ni films are annealed in ArH2 atmosphere at 900-1000degC to increase
grain size and are then exposed to H2CH4 gas mixture10
In this step the hydrocarbon
decomposes and dissolves in Ni to form a solid solution Lastly the samples are cooled in
argon gas Ni has high carbon solubility at elevated temperatures and the solubility
decreases as temperature is reduced During the cooling process the carbon atoms diffuse
out from the Ni-C solid solution and precipitate on the Ni surface to form graphene films
(Figure 13a) Since Ni (111) has a lattice similar to the densely packed hexagonal lattice
of graphene (Figure 13b) they also have similar lattice constants and hence Ni surface
serves as an excellent lattice matched substrate for graphene growth11
The growth of graphene on Ni is based on carbon segregation and precipitation
process different segregation behavior is produced by different cooling rates which
affect the thickness and quality of graphene films12
Medium cooling rates lead to optimal
carbon segregation and produce few layers12
Graphene films grown on Ni are usually
continuous with monolayer and few layer regions Annealing of Ni substrates at elevated
temperatures in hydrogen atmosphere not only increases the single-crystalline Ni grain
size but also eliminates certain impurities in Ni thereby improving the graphene quality
Furthermore the graphene thickness can also be affected due to the amount of carbon
dissolved in the Ni films during the growth time
After synthesis the graphene can be transferred to other insulator substrates for
further characterization and applications Figure 13c shows the selected area electron
diffraction pattern of graphene film along the [001] direction which confirms the
graphene lattice structure shown After transfer to insulator substrates the geometry can
6
be retained as shown in Figure 13d Under optimal growth parameters graphene growth
is only limited by the Ni catalyst Lastly Figures 13e and 13f show the wafer-scale
graphene synthesis and transfer of graphene to a flexible transparent substrate
respectively
Though polycrystalline Ni is a good substrate the percentage and size of
graphene monolayer are still limited Researchers have hence tried other metal substrates
for graphene synthesis
7
Figure 13 (a) Graphene formation on Nickel (b) Graphene atoms on Ni (111) lattice
(c) Low magnification TEM image of graphene edges (d) Optical image of graphene
transferred from the Ni surface to SiO2Si substrate (e) Full-wafer scale deposition of
graphene layers on polycrystalline Ni (f) Transparent and flexible graphene films on
PDMS substrate10
8
122 Synthesis of Graphene on Copper (Cu)
Graphene films are grown on 25microm thick Cu foils in a hot wall furnace13
The Cu foil is
first annealed in hydrogen atmosphere at 1000degC and a mixture of H2CH4 is introduced
into the system to initiate graphene growth After a continuous graphene layer is formed
on the Cu foil the system is cooled to room temperature Figure 14a shows an SEM
image of graphene on Cu substrate indicating the Cu grains with contrast The Cu
surface steps are formed during thermal annealing and the darker flakes indicate multiple-
layer graphene (Figure 14b)10
The graphene wrinkles in Figure 14(b) originate from
different thermal expansion coefficient of graphene and Cu They go across the Cu grain
boundaries indicating that the graphene film is continuous
Figure 14 (a) SEM image of graphene on copper foil (b) High-resolution SEM image of
graphene on Cu10
123 Transfer of Graphene films
In order to facilitate the applications of graphene for electronic applications we need to
separate the graphene from the catalytic metal substrate Figure 15a shows the transfer
process of graphene Graphene is first coated with a thin layer of polymethyl
methacrylate (PMMA) and baked at 120degC to evaporate the solvent10
The metal layer is
then removed by Ni or Cu etchant leaving behind the PMMA graphene film The film is
then cleaned by deionized water and then transferred onto the target substrate After the
9
evaporation of water vapor the PMMA is removed by acetone leaving graphene film on
top of the target substrate Figure 15b shows a graphene wafer transferred from the
substrate onto glass and polyethylene terephthalate (PET) films
Figure 15 (a) Transfer process (b) Wafer-scale synthesis of graphene (c) Graphene
films transferred onto glass wafer (d) SiSiO2 with device patterned (e) PET film10
124 Synthesis of Graphene Junction
Graphene junctions with smooth armchair and zigzag edges are difficult to produce by
conventional methods such as mechanical exfoliation chemical exfoliation or lithography
etching14
The conventional methods can only produce rough edges Recently
Dresselhaus reported an edge reconstruction of graphene by Joule heating in a TEM-STM
10
(Figure16b) system15
An individual nanoribbon sample is attached to the sample holder
at one end and to the STM tip at the other end these ends also serve as the two
electrodes The structural transformation in the growth of graphene from armchair to zig-
zag is mainly attributed to the vaporization of carbon edges that reconstruct at high
temperatures in which resistive Joule heating and preferred current flow play an
important role This means that by controlling the flow of current a perfectly smooth
edged ribbon can be synthesized making graphene-based electronics possible16
Figure 16 (a) High-magnification image of the annealed sample showing that well-
defined zigzag armchair and zigzag-zigzag edges are formed (b) STM image of an 8 nm
wide bent junction connecting an armchair and a zigzag graphene nanoribbon which was
carved by STM tips14
125 Doping in Graphene
The doping of graphene can be roughly classified into two categories - electrical and
chemical Electrical doping involves changing gate voltages of graphene devices and
chemical doping uses chemical routes such as substitutional or interstitial This thesis
discusses chemical doping and the importance of doping sites by changing the dopant
Chemical doping is a common approach to tailor the electronic properties of
11
semiconductors Doping of graphene can cause its electronic properties to alter leading to
a metal-semiconductor transition The two means of doping graphene are interstitial and
substitutional In interstitial doping the dopant atoms or molecules are introduced as
adatoms or admolecules on the surface of graphene whereas in substitutional doping the
dopant atoms are replaced in the carbon lattice forming a bond in the lattice of
graphene16
Doping graphene results in the formation of n or p-type semiconductors
depending on the kind of dopant If the dopant is an electron donor it causes the Fermi
level to shift up resulting in n-type behavior of graphene Furthermore if the dopant is an
electron acceptor it causes the Fermi level to shift down resulting in a p-type behavior of
graphene (Figure 17)16
Figure 17 Band structure of graphene before and after doping The image shows shift
towards the Fermi level16
Graphene nanoribbons (GNR) can be made into a p- and n- type semiconductor
by doping with boron (B) and nitrogen (N) respectively In theory GNR p-n junction is
formed by doping GNR with B and N in different regions However experimentally
doping graphene with both these elements is very difficult due to the dopants reacting
with each other17
Hence most experimental studies use GNR doped by only one
12
element N-doped graphene was synthesized by Wei et al Wang and B-doped Graphene
was realized by Endo17
Many researchers have demonstrated interstitial doping of graphene by gas metal
and organic molecules16
The various gases and metals used are NO2 NH3 An-CH3 Na-
NH2 F4-TCNQ TPa TCNE and others16
Doping in graphene is hence possible by
electrons or holes in high concentration without deterioration of its mobility Interstitial
doping is highly sensitive due to most of the conducting channel being exposed to surface
absorbates and hence can be used in molecule detection
In substitutional doping the dopant atoms are included in the graphene lattice and
thus chemically bonded Substitutional doping is done via the CVD method using a
carbon and dopant source Substitutional doping opens up many applications in device
engineering making graphene a very good candidate as a semiconductor This study
involves the study of transport properties of graphene doped by substitution
126 Nitrogen (N) Doped Graphene Synthesis (Substitutional)
N-Doped graphene is prepared via a CVD process using a 25microm thick Cu film on a Si
substrate The substrate is placed in a quartz tube with the flow of hydrogen (20sccm) and
argon (100 sccm)18
When the center of the furnace reaches 800degC 60 sccm of CH4 and
60 sccm of NH3 is introduced into the flow as C source and N source respectively The
substrate is then moved to high temperature and after 10 min growth the sample is
cooled to room temperature under H2 ambient Figure 1 8 shows the growth of N-doped
graphene18
13
Figure 18 Low resolution TEM image of N-doped graphene Background is the lacey
carbon TEM grid graphene sheet is crumpled with many ripples18
13 Structure of Graphene Nanoribbon (GNR)
Graphene Nanoribbons (GNR) are strips of graphene with very thin width of lt50nm
GNRs can be terminated in three separate ways called zig-zag (0 n) armchair (m 0) and
chiral (m n) (Figure19) and this termination along the width of the ribbon dictates the
size of the band gap19
Figure 19 Zigzag and Armchair orientation of Graphene5
Due to their various edge structures GNRs exhibit different electronic properties
ranging from normal semiconductors to spin-polarized half metals which open the
possibility of GNRs as electronic devices19
14
Within a tight binding approach (AGNRs) could be metallic or semiconducting
depending on their ribbon width but all zigzag graphene nanoribbons (ZGNRs) are
metallic with a high density of electronic states at the edges Hence ZGNRs exhibit
characteristic edge effects which are not present in AGNRs These edge effects in
ZGNR create a flat band close to the Fermi level making the ZGNR edges more
reactive19
First-principles calculations show that the GNRs possess a non-zero direct
band gaps These gaps are small for ZGNR (Figure 110) caused due to spin ordering
effects at the edges For AGNRs the band gap arises from quantum confinement (Figure
111) effect that has larger magnitudes than ZGNR20
Figure 110 Band structure of ZGNR
15
Figure 111 Band structure of AGNR
For GNRs the band gap decreases as the ribbon width increases and in order to
create a semiconductor with a desirable band gap the nanoribbon width should be
adjusted accordingly This property of adjusting the band gap makes graphene an
excellent candidate for transistor switching By applying an electric field GNR can be
altered from an insulator to a conductor GNRs exhibit very intriguing properties and
have become one of the promising candidates for electronic applications
14 Overview of Graphene Junction
The invention of p-n junctions date back to 1940s which later resulted in the invention of
junction transistors One of the key technological reasons for success of the p-n junction
is mainly due to its ability to locally modulate the energy band gaps via an applied bias21
A graphene p-n junction is created via single layer of graphene in which the
carrier type and density in two adjacent regions are controlled by electrostatic gating8
For materials with a band gap the electric field can either switch lsquooffrsquo the current or
rectify it (p-n diode)22
Being a ldquogaplessrdquo material the off state is not achievable in
16
graphene In order to achieve an off state the gap can be created by doping graphene with
various elements (Group III or Group V) Doping allows p-n junctions to be
reconfigurable using a gate voltage to distinguish between graphene p- n regions within a
single sheet Many researchers have studied the electronic as well as transport properties
of doped graphene junctions
In 2009 Fangping OuYang studied the transport properties of T-shaped graphene
junctions using the ATK software and showed that the conductance depends on
geometric structures which can be controlled by selective doping23
Wei Yao in 2013
studied the transport properties in graphene p-n junctions and showed that the
rectification effect depends on boron doping density and position17
The study of transport properties in graphene p-n junctions is a recent
advancement The thesis discusses transport properties including the current-voltage (I-
V) characteristics of doped graphene junctions Moreover the software used is similar to
the software in use by current researchers since they have produced viable data using
ATK
17
CHAPTER 2
RESEARCH BACKGROUND
21 Band Structure of Graphene
The unique electronic properties of graphene were first predicted in 1946 Figure 21
shows a top view of the hexagonal arrangement of carbon atoms in real space as well as
the first Brillouin zone in reciprocal space
Figure 21 Left Real space graphene lattice with basis vectors and Right The
first Brillouin zone of graphene in reciprocal space with basis vectors and
K and
Krsquo are responsible for massless transport at low energy24
The real space basis vectors are radic
and
radic
The reciprocal space basis vectors are 1 2
0 0
4 1 3 4 1 3( )and ( )2 2 2 23 3
b x y b x ya a
where the magnitude of the basis vectors is |a0| = radic acc The distance between nearest
neighbor carbon atoms is acc=0142nm
18
The band structure can be calculated by solving the eigenvalues using the
dispersion relation E( )
1 2 3( ) 3 2cos 2cos 2cosE k t k a k a k a (21)
Transport properties of solids are closely related to the energy dispersion
relations E ( ) in the material and in particular to the behavior of E ( ) near the Fermi
level Graphene is a zero gap semimetal whose specific linear electronic band dispersion
near the Brillouin zone corners (Dirac points) gives rise to electrons and holes that
propagate as massless Fermions25
The valence and conduction bands do not overlap in
graphene they touch at the Fermi Level (Figure 22)
Figure 22 Band structure of a graphene sheet showing a band gap of 0eV
The low energy properties of graphene can be well described by making a linear
expansion of the band structure around the K and Krsquo This energy can be written as
19
E(k) = plusmnħvF|k (22)
where vF is the Fermi velocity of 1106ms given by
1F
Ev
k
ħ (23)
Figure 23 Band structure of graphene calculated with the tight-binding model
22
The Fermi surface of graphene consists of double cones with Fermi energy at the
intersection of these cones (Figure 23) The slope of the band is zero and hence the
effective mass of electrons in that region is zero which leads to an entirely new transport
mechanism in graphene26
20
22 Transport Characteristics of Graphene
Transport process usually involves a flow of charge or energy or both The flow is mainly
due to external perturbations such as electric field and temperature gradient The
relationship between forces and flow usually defines various transport coefficients that
are the characteristics of electrons and phonons in the material All modern electronics
are based on the ability to control the electronic properties of a material by applying
external voltage This is done by an electric field effect where the gate voltage changes
the carrier concentration of the material and consequently its conductivity The electric
field effect in graphene was reported by Novoselov in 2004 and is used in transport
measurements8
The electron-phonon interaction in graphene plays an important role in
understanding the photoemission spectra observed in graphene The electric field effect is
an alternative method for changing the charge carrier density in low dimensional systems
The electric field effect in graphene which was first reported by Novoselov et al in
2004 is widely used as a characterization tool in transport measurements25
The transport characteristics of the material are directly related to the
bandstructure of graphene The carriers in graphene lattice are free to move in two
dimensions In the carrier transport of graphene the carriers ndash electrons and holes ndash close
to the Dirac points are of importance The transport is described by a two component
wave function (Equation 24) which obeys the 2D Dirac-like equation for massless
particles27
21
-ivFσ nablaψ(r) = Eψ(r)
(24)
where σ is the 2D Pauli spin matrix In the continuum limit the above (Equation
24) corresponds to the effective low energy Dirac Hamiltonian (Equation 25)
0( )
0
x y
F F
x y
iH k k
i
k kv v
k k
(25)
The electronic band structure of the energy (E) versus wave vector (k) relation for
graphene is given by Equation 24
The two component wave function resembles the spin or wave function of
quantum electro dynamics (QED)27
Corresponding to the spin of particles in QED the
charge carriers of graphene can be attributed with a pseudospin σ The pseudospin is the
direct result of two different carbon sublattices corresponding to the bonding and
antibonding combinations27
22
Figure 24 The energy dispersion around the K point27
In Figure 24 the red and blue lines correspond to the antibonding and bonding
states respectively The pseudospin can have two values either in the direction of or
against the momentum It can be seen that the electrons with energy E travelling in the
positive direction originates from the same branch as a hole with energy ndashE travelling in
the negative direction giving it the same pseudospin This results in suppressed
backscattering and Klein tunneling The back scattering process requires the pseudospin
to flip which is possible in the presence of short range scatters that act differently on sub
lattices27
23 Drude Theory
The classical theory of metallic conductivity was presented by Drude in 1900 and was
elaborated by Lorentz in 190528
Drude treated the free electrons as classical ideal gas
meaning the electrons collide with stationary ions and not each other
23
Figure 25 Electrons colliding with stationary ions28
The Drude theory applied the kinetic theory of gases to a metal considered as a gas of
electrons The basic assumptions made by the Drude theory are28
When metallic elements are brought together to form a solid then the valence
electrons become freely moving through the metal whereas the ions remain intact
as nearly immobile positive particles
Between collisions the electrons move freely ie there is neither electron-
electron interaction nor electron-ion interaction
The scattering mechanism leads to instantaneous collisions of the electron with
the scatterers
The collisions are characterized by a relaxation time τ
The electrons achieve thermal equilibrium only through collisions the velocity
after a collision is randomly directed the speed is as appropriate to the
temperature
With the relaxation time Drude obtained the electrical conductivity expression
where n is the number of electrons per unit volume
σ = ne2τm
(25)
He also calculated the thermal conductivity and successfully provided the
theoretical basis for Wiedemann-Frantz law already established in 1853 which states that
24
the ratio of electrical and thermal conductivity of any metals is a universal constant at any
given temperature28
The Drude theory gives results which are qualitatively correct outside of the
quantum Hall regime28
In the Drude theory of the electrical conductivity of a metal an
electron is accelerated by the electric field for an average time τ before being scattered
by impurities lattice imperfections and phonons to a state which has zero average
velocity The average drift velocity of the electron is
d
eE mv (26)
It is assumed that all electrons drift together and hence the current density
j = -ne (27)
This Drude theory works well for fields below ~ 01T At stronger fields the Hall
resistivity becomes nearly constant over finite intervals of magnetic fields28
The QHE
reflects both novel disorder physics as well as novel interaction physics in the quantum
Hall regime
24 Quantum Hall Effect (QHE)
The discovery of QHE is a remarkable achievement in condensed matter physics The
Hall Effect was discovered by Edwin Hall in 187929
However the precise quantization
of the Hall conductance in units of e2h was not recognized until February 1980 Five
years later in 1985 Klaus von Klitzing was awarded the Nobel Prize in Physics for the
discovery of QHE29
The quantum Hall effect occurs in two-dimensional electron systems in the limit
of strong perpendicular magnetic field that stems from electronic transport
25
measurements where one drives a current I through the sample and where one measures
both the longitudinal and transverse resistance (Hall resistance) A longitudinal resistance
is a resistance measured between two contacts that may be connected by a line which
does not connect C1 and C430
Transverse resistance is measured between two contacts
connected by an imaginary line connecting C1 and C4 (Figure 26a)
Figure 26 (a) 2D electrons in a perpendicular magnetic field Logitudinal resistance
measured across C5 and C6 Transverse resistance measured across C3 and C5
(b) Classical Hall resistance as a function on the magnetic field30
Due to the existence of quantum Hall effect it is natural to expect that there exists
a classical Hall Effect Hall showed that the transverse resistance of a thin metallic plate
varies linearly with the strength B of the perpendicular magnetic field (Figure 26 b)
RH = Bqnel (28)
More quantitatively the classical Hall Effect can be understood within the Drude
model for diffusive transport in a metal Within this model one considers independent
26
charge carriers of momentum p described by the equation of motion
( )
b
dp p pe E B
dt m (29)
where E and B are the electric and magnetic field respectively The macroscopic
transport characteristics ie resistivity of the system are obtained from the static
solution of the equation of motion dpdt = 0 and one finds for 2D electrons with p =
(pxpy)
x
x yb
y
y xb
eBe
eBe
ppE
m
ppE
m
(210)
In the above expression characteristic frequency is visible as
C
b
eB
m (211)
This is known as cyclotron frequency as it characterizes the cyclotron motion of a
charged particle in a magnetic field30
With the Drude theory the conductivity can be
written as
j = -enelpmb (212)
and the mobility can be given as
micro = eτmb (213)
The transport properties in the limit of ωCτ-gt infin are entirely governed in the presence of
27
a magnetic field by the off-diagonal ie transverse components of
conductivityresistivity
The theory of quantum Hall effect subjects all physical properties of 2D electron
system in the limit where the magnetic field is strong so that the mixing of Landau levels
by disorder or electron-electron interaction is considered to be a weak perturbation30
This is known as the quantum Hall regime The ratios between the energy scales
corresponding to the two interactions are important The limit where disorder potential is
much stronger is referred to as integer quantum hall regime whereas the limit where the
interaction potential is much stronger is referred to as fractional quantum Hall regime
25 Resistivity and Resistance
The electronic transport in the framework of the Drude theory allows for the calculation
of conductivity or resistivity of a classical diffusive 2D electrons in a magnetic field30
The conductivity and conductance are related to one another but they depend on the
geometry of the conductor-the resistance R and hence the resistivity is given by
R = (LA)ρ (214)
where L is the length of the conductor and A is the cross section
For a d-dimensional conductor the cross section scales as Ld-1
such that the
scaling relation between the resistance and the resistivity is
R~ ρL2-d
(215)
From the dimension point of view resistance and resistivity are the same in 2D and the
resistance is scale-invariant Further the resistance of a 2D conductor depends in
general on the so-called aspect ratio LW via some factor f (LW)30
However for
transverse Hall resistance it is the length of the conductor that plays the role of cross
28
section such that the Hall resistivity and the Hall resistance truly coincide ie f=1 The
Quantum Hall effect is highly insensitive to the particular geometric properties of the
sample used in transport measurements Recently quantum Hall physics experienced the
discovery of ldquorelativisticrdquo quantum Hall effect in graphene The electrons in graphene
behave as if they were relativistic massless particles contributing to a very interesting
field of research30
26 Klein Tunneling
Klein tunneling in which relativistic particles penetrate through a potential barrier
without the exponential damping that is characteristic for nonrelativistic quantum
tunneling has never been observed for elementary particles The tunneling allows
transmission of a particle through a potential barrier higher than its kinetic energy
violating the principle of classical mechanics30
On the quantum scale the objects exhibit
wave-like characteristics in which the quanta move against a potential hill described by
their wave function This wave function represents the probability amplitude of finding
the object in a particular location The transmission of the object through the potential hill
is termed as tunneling When EltV then the ψ(x) over V is returned by ψrsquo(x) In quantum
mechanics an electron tunnels from the conduction into the valence band Such a
tunneling from an electron-like to hole-like state is called as Klein Tunneling in which the
electron avoids backscattering
In Figure 27 it is shown that an electron hitting a potential barrier is reflected
with 100 certainty In non-relativistic quantum mechanics the electrons can tunnel
through the barrier but the probability of tunneling exponentially decays with increasing
29
height and width of the barrier However in relativistic quantum mechanics the barrier
gets transparent even in the limit of infinite barrier height (Klein paradox)31
Figure 27 Klein tunneling through an npn barrier30
The Klein paradox in graphene can be understood in terms of electrons and holes
In graphene the massless carriers behave differently than ordinary carriers (with mass) in
the presence of an electric field A barrier which is repulsive for electrons will be
attractive for holes Since there are hole states inside the barrier with the same energy as
the electrons outside an electron arriving at the barrier can tunnel through it as a hole
before leaving again as an electron Klein tunneling for transport in graphene is that the
charge carriers cannot be confined by potential barriers The Klein tunneling effect has
been experimentally observed by Ando in 1998 in which the absence of backscattering
(Figure 28) is responsible for high conductivity in carbon nanotubes
30
Figure 28 Electron trajectory considering the linear electrostatic potential U(x) = Fx30
The electron is able to propagate through an infinitely high potential barrier since
it makes a transition from the conduction band to valence band In this transition from
conduction band to valence band its dynamics changes from electron-like to hole-like
The equation of motion is thus given by
2
2 2 2| | ( )
pdr E
dt E Up
p E U
v
v
at energy E (216)
This shows that in the conduction band (UltE) and in the valence band (UgtE)
In Klein tunneling the pairs of electron-like and hole-like trajectories at the same E and
py have turning points at dmin given by dmin=2v|py|F (Figure 29)
Figure 29 Electron like and hole like trajectories at same E21
31
The tunneling probability exponential dependence on dmin
2
min| |
( ) exp( ) exp( )2
y y
y
vT
F
p pdp
(217)
The applications of the Klein tunneling include Atomic clock Scanning tunneling
Microscope Tunnel diode Tunneling transistor and many more32
Since graphene
exhibits Klein tunneling it can be very useful to study the transport properties in
graphene and use it in such applications
27 Quantum Hall Effect in a Graphene
A monolayer graphene shows half-integer quantum Hall effects where the Hall
resistance is quantized at values of
2
1
xyh v eR
(218)
around filling factors
14( 1 2)Nv
(219)
where N is an integer e is the electron charge h is the Planckrsquos constant and the
factor 4 is due to spin and valley degeneracy QHE in graphene can be observed at room
temperature which is a very intriguing property (Figure 210) Graphene reveals
significant differences with respect to conventional 2D electron systems The Landau
quantization yields energy levels that disperse differently in graphene as well as
particular zero-energy level that is only half filled at the charge neutrality point (v=o)
32
Figure 210 Quantum Hall effect in graphene22
The Hall conductivity σxy and the
longitudinal resistivity of monolayer graphene as a function of carrier density at B = 14T
and T= 4K This shows half-integer QHE with chiral index J= 1
The QHE in graphene is not entirely similar to regular QHE since the charge
carriers in graphene are Dirac Fermions The charge carriers governed by
electrodynamics is given by (Equation 220) which does not apply for graphene and a
QED quantization of graphene electronic band structure is used
En = (n+12)ħω (220)
33
In the presence of magnetic field the nature of the Dirac Fermions in graphene
results in unevenly spaced Landau levels (LL) containing a distinctive LL at the electron-
hole degenerating a zero energy given by
2MG
MGFehn B
n vE (221)
The LL levels at high magnetic fields in MG are shown in Figure 211
Figure 211 (a) LL for Graphene bilayer (b) Schematics of Hall conductivity as a
function of nn0 for bilayer Graphene (solid line) and monolayer Graphene (dotted line)
(c) LL for monolayer Graphene33
It is found that the Hall resistance of a two dimensional electron system has
plateaus as a function of the number of electrons at low temperatures and strong magnetic
fields32
At large B the Dirac-like energy spectrum of graphene gives rise to a
characteristic series of QH plateaus in conductance reflecting the presence of a zero-
energy Landau level that include only odd multiples of 2e2h for uniform carrier density
in the sheet These plateaus of QH edge states at the edge of the sheet circulating in a
34
direction are determined by the direction of B and the carrier type33
This is why QHE in
graphene is known as Half-Integer Quantum Hall Effect
28 Thermoelectric Effect
Thermoelectricity refers to a class of phenomena in which a temperature difference
creates an electric potential or an electric potential creates a temperature difference The
principle of thermoelectric effect has been known for over 100 years Recently the
practical applications of thermoelectric effect have become more viable34
Thermoelectric effect is the direct conversion of temperature differences to
electric voltage and vice versa Joule heating is the heat generated whenever a voltage is
applied across a resistive material The Peltier-Seebeck effect is reversible whereas Joule
heating is not This effect can be used to generate electricity to measure temperature to
cool objects or to heat them Since the direction of heating and cooling is determined by
the sign of the applied voltage thermoelectric devices make very convenient temperature
controllers
281 Seebeck Coefficient
Thomas Johann Seebeck discovered that an emf appears in a circuit composed of two
dissimilar metals when the junction between the metals is held at different
temperatures34
The thermoelectric emf causes a continuous current in the circuit when a
complete loop is formed and the current is known as thermoelectric current This is
known as the Seebeck effect
35
Figure 212 Seebeck Effect34
As long as the two junctions are at different temperatures the thermoelectric emf
exists and the current will keep flowing between the hot and cold junction that are at
different temperatures The Seebeck effect is the conversion of temperature difference
directly into electricity The voltage developed in the circuit shown in Figure 212 is
proportional to the difference in temperature between the two junctions and is given by
V = α (T2-T1) (222)
This Seebeck effect is observed not only in metals but also in semiconductors
Here α is known as the Seebeck coefficient α measures the magnitude of an induced
thermoelectric voltage in response to the temperature difference across the material If the
temperature difference ∆T between the two ends of a material is small then the Seebeck
coefficient of a material is written by
α = ∆V∆T (223)
36
This can be expressed in terms of electric field as
α E∆T (224)
The units of Seebeck coefficient is given as VK The higher the Seebeck coefficient
value the better it is since it will create a very large voltage that can be used to provide
power
282 Peltier Coefficient
Peltier effect is the inverse of Seebeck effect involving a junction phenomenon There is
heat absorption or generation at the junctions depending on the direction of current flow
Heat generated by current flowing in one direction is absorbed if the current is reversed
The heat absorbed per second at a junction carrying current I is given by
Heat absorbed in t sec = πabIt (225)
Here πab is the Peltier coefficient and given by HIt Thus Peltier coefficient is
numerically equal to the applied potential difference expressed in Volts
Overall by studying the flow of electrons the values of Seebeck
coefficient and Peltier co-efficient can be estimated These values determine the various
applications of the materials In this thesis the Peltier and Seebeck coefficient of the
graphene junction and the new applications are discussed
37
29 Early Research ndash ab intio studies
In 2007 Androitis studied that the conducting properties of graphene nanoribbons and
junctions are strongly dependent on their size and geometric features35
He concluded that
there is no conductance for small AZA or ZAZ ribbons (Figure 213)
Figure 213 Transmission functions in units of (2e
2h) for AZA structures
35
Figure 213 shows that T (E) exhibits a negligible peak [T (E) = 001 in units of
2e2h] at E= -225 and 250eV However it was noted that when the width of the arm type
was increased T (E) at -225 and 250eV was 02035
Later in 2007 Qimin Yan used first principles methods to investigate the Current-
Voltage characteristics of GNR Transistors and the effect of edge doping He showed that
GNR field effect transistors can achieve high performance levels with ONOFF ratios on
the order of 103-10
436
Figure 214 is an I-V curve of AZA GNR-FET connected via
armchair metallic leads36
38
Figure 214 I-V curve for a 591nm long channel (Vbias=20mV)
36
In 2009 Fangping OuYang demonstrated the intrinsic transport properties and
effective B or N doping of the junctions by using first-principles quantum transport
simulations He concluded that the I-V characteristics of pure-carbon T-shaped junctions
exhibit metallic behavior and the current in the junction strongly depends on the height
of the stem23
He reported that the conductance of the devices depends on the geometric
structures which can be controlled by selective doping
In 2012 Wei Yao used the first principle calculations based on Density
Functional Theory (DFT) and Non-equilibrium Greens Function (NEGF) to study the
electronic as well as the transport properties of B-doped 6-GNR p-n junction His results
showed that the boron doping interval can influence the rectification effect at low bias
and also exhibit Negative Differential Resistance (NDR) phenomena at high positive
bias
39
CHAPTER 3
COMPUTATIONAL DETAILS
31 Introduction
The physical chemical electrical electronic and optical properties of a solid are
determined by their quantized electronic states The quantum states in low-dimensional
systems are produced due to the confinement of the carrier charges in one or two
dimensions Graphene is a conductor electrons are able to flow through graphene more
easily than through even copper The electrons can travel through the sheet of graphene
like mass-less particles as fast as just one hundredth that of the speed of light The ways
in which electrons behave in graphene make it very helpful to study their fundamental
physical properties Graphenersquos near perfect crystal lattice provides a very clean system
to experiment By restricting the electrons to only two dimensions they exhibit some
interesting properties such as the anomalous quantum Hall effect and Klein tunneling
In this chapter two theoretical concepts used for calculating the electronic structure
and the transport properties for graphene are described These include the Extended
Huckel Theory and Non-Equilibrium Greenrsquos Function (NEGF) method
311 Extended Huckel Theory
Erich Huumlckel was born in Germany on August 9th
1896 He studied mathematics and
physics in Berlin He is best known for his work in the field of chemistry and physics for
two contributions (1) Debye- Huumlckel theory of electrolytic solutions (2) Huumlckel
method of approximate molecular orbital calculations on electron systems In 1930 he
published his findings on systems in 1931 he generalized and expanded the system
40
theory to explain benzene Due to his poor communication skills his findings went
unrecognized for over 20 years It was in 1951 that his 4n + 2 rule was finally clarified by
Doering to show if C=C bonds would show aromaticity Huumlckel died on February 16th
1980 with very little worldwide recognition for his contributions to chemistry Today
chemistry students recognize his name and his contributions to the field are quite
substantial
One of the first semi-empirical methods to be developed was Huumlckel Molecular
Orbital Theory (HMO) HMO was developed to describe molecules containing
conjugated double bonds HMO considered only electrons in pi orbitals and ignored all
other electrons in a molecule The Extended Huumlckel Molecular Orbital Method (EH) was
developed out of the need to consider all valence electrons in a molecular orbital
calculation
By considering all the valence electrons chemists could determine molecular
structure compute energy barriers for bond rotations and determine energies and
structures of transition states for reactions By considering only the valence electrons the
computed energies could be used to choose between proposed transition states to clarify
reaction mechanisms The total valence electron wavefunction is described as a product
of the one-electron wave functions
1 2 3(1) (2) (3) ( )valence j n (31)
where n is the number of electrons and j identifies the molecular orbital Each
molecular orbital is written as a linear combination of atomic orbitals (LCAO)
1 12
N
j jr rrc j N
(32)
41
The energy of the jth
molecular orbital is given by a one-electron Schroumldinger
equation using an effective one electron Hamiltonian heff which expresses the interaction
of an electron with the rest of the molecule
eff j j jh (33)
This is the energy eigenvalue of jth
molecular orbital corresponding to the Eigen
function j The advantage of using this method is that the exact form of heff is not
required The total energy of the molecule is the sum of the single electron energies
j jj
E n (34)
where nj is the number of electrons in orbital j
In order to use the Extended Huckel method a set of calculation parameters and
approximations must be followed These parameters include the Basis set K-point and
the Brillouin Zone and lastly the Mesh cut-off
312 Introduction to NEGF
The Greenrsquos function is a function of two space-time coordinates From the knowledge of
this function one can calculate time-dependent expectation values such as currents and
densities electron addition and removal energies and the total energy of the system In
the absence of external fields the non-equilibrium Green function method reduces to the
equilibrium Green functions NEGF can be applied to both extended and finite systems
The generic system of NEGF consists of the electron dynamics of the channel described
by the Hamiltonian This channel consists of two contact reservoirs with respective
chemical potential μR and μL The NEGF assumes ballistic transport neglecting self-
42
energy from scattering The system is insulated from gate contacts whose effects are
realized via a 3D Poisson solver which solves for the potential at a given point in real
space based on electron density
22 ( ) [ ( ) ( )]D
qr N r n r
(35)
Figure 31 NEGF system
The system is easily expandable to systems with several contacts or gate
configurations by adding additional self-energy matrices to NEGF or additional sources
to the Poisson solver
313 Electrostatics
Electrostatic potential is created every time in the presence of a charge density due to an
induced electric field The Poissonrsquos equation correlates the electrostatic potential to
charge density as given in Equation 36
43
2( ( ) ( ) ( ) ( ))( )
( )( ) ( )
ADq p r n r r N rr
rr r
N
(36)
where ɛ(r) is the dielectric permittivity of the material ρ(r) n(r) ND(r) and NA(r) are the
hole electron donor and acceptor concentrations of the system respectively
Two types of boundary conditions are usually applied to the Poissonrsquos equation
Dirichlet boundary conditions
Φ (0) = F0 and Φ (L) = FL
von Neumann boundary conditions
00
( )
x
d x
dxB
and
( )L
x L
d x
dxB
For the transport problems with open boundary conditions the von Neumann
boundary conditions are used assuming that the potential vanishes at the boundary ie
B0=BL=0
The Poissonrsquos equation can hence be discretized on a grid as
2 ( )( )
( )
rx
r
= M (37)
where M is the matrix Φ and ρ are vectors containing the discretized values of
the electrostatic potential Φ and charge density ρ respectively
44
The Schroumldinger and Poisson equations are coupled since V(x) = -qΦ(x) is used
for the Schroumldinger to compute ρ(x) This self-consistent loop stops when the
convergence is reached
( )r
V(x) = -qΦ(x)
314 Non-Equilibrium Greenrsquos Function
Greenrsquos functions are a mathematical construction that are used to solve differential
equations subject to specific initial or boundary conditions They are named after the
British mathematician George Green The 1-D equation of L( )f( )=S( ) can be defined
by the Greenrsquos Function as given below
( ) ( ) ( )G x x f x x x (38)
The general Greenrsquos function is given by
( ) ( ) ( )f x dx G x x S x (39)
Applying the operator L( ) to the solution f( ) satisfies the original differential
equation The Greenrsquos Function G( ) is the propagator which propagates the influence
of a perturbation S( ) originally situated at the point to the point at which the
function f( ) is evaluated
The Greenrsquos Function G( ) can also be a correlation function If the points
and are strongly (weakly) correlated then S( ) will greatly (poorly) affect f( )
Poisson equation
2 ( )( )
( )
rr
r
Schroumldinger equation
2
2
( ( ) ) ( )
( )2
( ) | ( ) |
E H r E r S
H V rm
r dE E r
Figure 32 Self-consistent loop
45
The Schroumldinger equation with open boundaries can be written as
( )E H S (310)
Considering a 1-D and homogenous system ranging from =0 to L assuming
that Σ=0 and the form of equations is same before and after discretization then
22
2 0( ) ( ) ( )
2E x S x
m
dV
dx
(311)
The Greenrsquos function can hence be computed corresponding to the Schroumldinger
equation
22
2 0( ) ( ) ( )
2E G x x x x
m
dV
dx
(312)
Due to the delta-function at = a discontinuity is observed and hence the
Greens function is evaluated at boundary conditions
0
2
exp( ( )) x x 2 ( )( )
exp( ik(x x)) x x
ik x x m E VG x x k
A
A
(313)
By integrating the Schroumldinger equation twice and setting the lower and upper
integration boundaries to = -δ and = +δ the Greenrsquos Functions can be written as
2
( ) ( ) 0
( ) ( ) 2
x x x x
G x x G x x
dG x x dG x x m
dx dx
(314)
46
The coefficient A+ and A
- become
ik
mA A
(315)
The Greenrsquos Function takes a final form known as Retarded Greenrsquos Function and
is written as
( ) exp( | |)G x x i ik x xk
m (316)
And the wave function is
( ) ( ) ( )x dx G x x S x (317)
Retarded Greenrsquos Function propagates the wave functions generated by a source
or perturbation S from its origin at to any point
The retarded Greenrsquos Function as discretized Schroumldinger equation is written as
( )R RE H G I (318)
The wave function Φ can be calculated from the retarded Greenrsquos function and the
source vector as
Φ = GR∙S (319)
Overall in this section the Greenrsquos function approach in calculating the electron
dynamics is reviewed We defined the self-energy of each part of the system spectral
function and the probability current density the electric current is derived explicitly using
Non Equilibrium Greenrsquos function We will use this formalism to calculate the tunneling
phenomena in coupled quantum dots isolated or otherwise
47
CHAPTER 4
ATOMISTIX TOOLKIT DETAILS
41 Introduction
Virtual NanoLab (VNL) is a graphical user interface (GUI) that provides a group of
modeling tools the function of these tools involves the set-up investigation and the
study of nanoscale structures The quantum mechanical equations are solved by the
software by using the advanced software architecture and numerical methods to
implement ab initio calculations VNL simulates the electronic structure and calculates
the transport properties based on the two systems mentioned earlier NEGF and Extended
Huckel ATK is the main engine for computing the scripts and hence all the calculations
performed in VNL are done by ATK VNL is a user friendly software as it not only
allows creating a script but also helps to set up a virtual experiment
This thesis involves the use of VNL in order to study the effect of the width and
different orientations of the doped atoms Since the software allows for virtual
experiments it makes it much easier to study the I-V characteristics based on the change
in position of atoms
42 Device Structure
In this thesis AZA GNR p-n junction with boron doping (location) was created using the
ATK software which is based on NEGF and DFT Further the thesis discusses the
transport properties and the I-V curve of such junction
The input format of ATK is NanoLanguage which is an extension to Python
scripting language ATK uses the NEGF system for formalism of simulating device
48
Figure 41 Geometry of device configuration with two electrodes
37
The system is divided into three parts left central and right The implementation
relies on the screening approximation which assumes that the properties of the left and
right regions can be decribed by solving a bulk problem for fully periodic electrode cell37
This screening approximation is fulfilled when the electrode regions can be described by
an equilibrium electron distribution
Figure 42 The electron distribution in a device configuration which illustrates a left
moving scattering state with origin in right electrode37
The system assumes that in steady state the electron density of the central region
is constant in time and hence the electron density is calculated independently from each
electrode The electron density is given by the occupied eigenstates of the system
n(r) = nL(r) + n
R(r) (41)
49
The left and right densities are calculated by summing up the occupied scattering
states
nL(r) = sum
(42)
nR(r) = sum
(43)
The scattering states are usually calculated by first calculating the Bloch states in
the electrodes and then solving the Schroumldinger equation of the central region using the
Bloch state as matching boundary Instead of using the scattering states the ATK
software uses the NEGF method to calculate the non-equilibrium electron density
The electron density is given in terms of electron density matrix
D = DL + D
R (44)
The left density matrix is given by NEGF theory
DL = int
(45)
where
ρL(ɛ) =
(46)
ρL(ɛ) = is the special density matrix
Also if there is a non-equilibrium electron distribution in the central region then
the electron distribution in electrode is given by the Fermi function f with an electron
temperature TL
G(ɛ) =
(47)
G = retarded Green function
δ+ is an infinitesimal positive number and S H overlap the Hamiltonian matrices
L =
sum sum
(48)
50
L
is the broadening function of the left electrode given in terms of left electrode
self -energysum
43 Transmission Spectrum Calculations
Once the self-consistent non-equilibrium density matrix has been obtained the various
transport properties of the system can be calculated One of the most important properties
is the transmission spectrum from which the current and differential conductance can be
obtained
The transmission coefficient in ATK is obtained by the retarded Greens function
T(ɛ) = G(ɛ)ΓL(ɛ)G
ϯ(ɛ)Γ
R(ɛ) (49)
The transmission amplitude of individual scattering states may be obtained
through the Transmission Eigenvalues The ldquoTransmission Eigenvaluesrdquo is an analysis
which finds the eigenvalues of the transmission matrix
The transmission matrix at energy E and k-point is given by
Tnm(Ek) = sum (410)
where
= transmission amplitude from Bloch state ψn(k)
The transmission coefficient is given by the trace of transmission matrix
T(Ek) = sum (411)
Keeping in mind all quantities depend on the quantum numbers parametrically
Transmission eigenvalues sum up to the transmission coefficient
T = sum (412)
51
44 Calculating the Current
Current is calculated from the transmission coefficient using
I( ) ( )R L
L RL R
R LB B
eE f f dE
h
E EV V T T T
k kT T
(413)
where f is the Fermi function TRL is the electron temperature of the right or left
electrode and Tσ(E) is the transmission coefficient for the spin component σ
The chemical potentials of the left and right electrode given by
L
F R LR L
eVE
are defined relative to the Fermi level of the left electrode These chemical potential are
related to the applied bias and hencebiasR L
eV therefore bias L RV V V
The transmission spectrum itself is usually rather insensitive to temperature and is
used in self-consistent calculations but often depends strongly on the electrode voltages
Thus for an accurate estimate of the current the transmission spectrum should be
calculated self-consistently for each desired bias
ATK uses very precise method to calculate the transport properties of the system
Transmission spectra for various concentrations of boron doped graphene p-n junctions
are generated in this Chapter and various coefficients such as Seebeck Peltier and
Conductance are calculated
52
45 Calculating Transport coefficients
The linear response transport coefficient of an applied voltage difference or temperature
difference between the two electrodes is given by
Conductance
| dT 0
e
dI
dUG
(414)
Peltier coefficient
| d 0
Q
I
I
(415)
Seebeck coefficient
| 0
dUS I
dT T
(416)
These linear response coefficients are calculated by the Transport Coefficients To
perform these calculations the ATK uses the Electron Transmission Spectrum
53
CHAPTER 5
RESULTS AND DISCUSSION
51 Band Structure Analysis
The electronic bandstructure of GNR both doped and undoped are discussed in this
chapter
The armchair configuration of Pristine GNR (PGNR) has a band structure that is
dependent on its width This is explained by the fact that the sheet itself acts like a
potential well where the electrons are confined to form standing waves along Cr the
rolling vector albeit with slightly different boundary conditions (Cr = ma1 + na2
where m and n are integers and a1 and a2 are the unit cell vectors of graphene lattice) In
a GNR the two nodal points of the standing wave must be at the ribbon edge while in a
Single wall nanotube (SWNT) they can be anywhere ie a circumferential periodic
boundary condition
(a) (b)
Figure 51 Bandstructure of AGNR widths (a) 4 atoms (b) 5 atoms
54
(a) (b)
Figure 52 Bandstructure of AGNR widths (a) 6 atoms (b) 7 atoms
(a) (b)
Figure 53 Bandstructure of AGNR widths (a) 8 atoms (b) 9 atoms
55
(a) (b)
Figure 54 Bandstructure of AGNR widths (a) 10 atoms (b) 11 atoms
Figure 55 Bandstructure of AGNR with a width of 12 atoms
Figure 56 Variation in band gaps as the width (number of atoms) varies
0
05
1
15
2
25
0 2 4 6 8 10 12 14
Wdith vs Band Structure
eV
56
The band structure of 12 Atom AGNR is close to that of Ge (0626 eV) The
actual width of this nanoribbon is about 25 nm 12 AGNR has been fabricated
successfully and doped with various dopants Hence the 12 Atom AGNR has been chosen
to study the transport properties
A junction is created using ZGNR and AGNR To maintain the consistency in the
device analysis it is imperative that the band structure of ZGNR is also calculated From
the simulation it is evident that ZGNR-AGNR-ZGNR junction configuration displays the
Metal ndashSemiconductor-Metal configuration that is addressed in this work The Fermi
Level in all the Z-GNR nanoribbons of widths 4-12 lies within the conduction band
Figure 57 Band structure of ZGNR width (a) 4 atoms (b) 6 atoms
57
(a) (b)
Figure 58 Band structure of ZGNR width (a) 8 atoms and (b) 10 atoms
Figure 59 Band structure of ZGNR with a width of 12 atoms
In order to create viable junction that would show transistor properties doping of
the semiconductor part is necessary The 12 atom AGNR is doped with boron (p-type)
and nitrogen (n-type) - (Figure 510a) 4 N doped (Figure 510b) 4 B In both cases
the impurities lie on the edge of the atoms For 2 nitrogen doped GNR with the
58
impurities lying in the center of the ribbon the Fermi level is found to be in the
conduction band as shown in (Figure 510c) (Figure 510d) shows the position of N with
respect to the edge A very clear departure from the expected (the valence band extending
above Fermi level) is shown in (Figure 510a)
Figure 510 Band structures of Doped AGNR (a) 4 N Doped (b) 4 B Doped (c) 2
N Doped (d) position of Nitrogen from (c)
(a) (b)
(c) (d)
59
52 I-V Characteristics of GNR junction
In pristine graphene the chirality determines the conductivity as seen from the I-V curves
for various widths At certain widths the semiconducting properties are more
pronounced These widths determine the wavelengths of the standing waves which in
turn determine the sub-band locations in the E-k plot When the biasing potential
exceeds 012V the I-V curve shows linearity In case of the 8-atom wide PGNR the
band gap is about 03 eV and it is evident from the I-V plot that the On-State is + 033 V
The band gap of 10-atom and the 4-atom wide PGNR is large enough to show
semiconducting properties
Figure 511 Current Vs Voltage graph for varying graphene width showing
conductivity
-30000
-20000
-10000
0
10000
20000
30000
-3 -2 -1 0 1 2 3
Cu
rre
nt
(nA
)
Voltage (V) (bias)
Current (nA) Vs Voltage for varying graphene width
W=10
W=8
W=6
W=4
60
The ZAZ GNR Configurations show the properties of a semiconductor junction The 12
atom ZAZ structure is studied for its I-V characteristics In this Chapter undoped B-
doped N-Doped B and N Doped (P-N Junction) ZAZ junctions are simulated
Figure 512 ZAZ GNR junction device
61
The boron doped ZAZ junction I-V characteristics are shown below (Figure 513)
The impurity concentration is 2 and 4 Various device configurations are studied
Figure 513 I-V curve of Boron Doped ZAZ junction
-25000
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
25000
-205 -155 -105 -055 -005 045 095 145 195
Cu
rre
nt
(nA
)
VBias
2B_1G_R 2B_0G_R
4B_0G_L 4B_0G_C
4B_0G_R 4B_1G_L
4B_1G_C 4B_1G_R
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
-2 -1 0 1 2
Cu
ren
t(n
A)
VBias
4 B doped GNR Jn
62
Figure 514 I-V curve of Nitrogen Doped ZAZ
-25000
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
-2 -15 -1 -05 0 05 1 15 2
Cu
rre
nt(
nA
)
VBias
I-V Curve as function of Dopant location
2N_0G_L2N_0G_C2N_0G_R2N_1G2N_1G_C2N_1G_R
-15000
-10000
-5000
0
5000
10000
15000
-2 -1 0 1 2
Cu
rre
nt(
nA
)
VBias
2N_0G_C
2N_1G_C
63
Figure 513 and Figure 514 show the I-V characteristics of the GNR junction doped with
2 boron and nitrogen respectively The location of N and B is at the central region of
the edge of the GNR Both B doped and N doped GNR Junctions show significant
Negative Differential Resistance (NDR) This is more pronounced in case of nitrogen
doping Another interesting observation is increasing ohmic nature with the change in
location of the dopants Nitrogen doped device configuration exhibits a pronounced
semiconductor behavior and the NDR effect is observed to be minimal
53 Thermoelectric Properties
In this study the thermoelectric properties were simulated for the GNR Junctions that
displayed high NDR effect The variation in the Peltier coefficient with temperature is
shown as function of doping
When the concentration of nitrogen increases the dimensionless Figure of Merit
ZT seems to decrease considerably This is mostly explained by the decrease in both
conductivity and mobility of the electrons
ZT = S2σTk (51)
where S is the Seebeck coefficient σ is the electrical conductivity T is the
absolute temperature and k is the thermal conductivity
64
Figure 515 Variation of Peltier coefficient with temperature as function of
doping
Figure 515 shows the maximum Peltier coefficient for 2 boron This is
explained by the scattering by boron and the associated smallest mean free path
0
0001
0002
0003
0004
0005
0006
0007
0008
0009
001
250 270 290 310 330 350 370 390 410
ZT
T (K)
2B
4B
Undoped
2N
4N
65
CHAPTER 6
CONCLUSIONS
Graphene ZAZ junctions exhibit varying properties depending on the various structural
configurations In this thesis it was found that the transport properties of graphene
depend on their width the edge of GNR doping concentration and the type of dopant
used The calculations of the band structure contributed towards the determination of the
minimum length of GNR required for studying the transport properties The minimum
length had a band gap equivalent to that of germanium and hence the importance of the
width being 12 atoms wide This band gap indicated fluctuating changes when doped
with elements such as B and N The viable junction showing transistor properties was
hence created by doping the semiconductor part of ZAZ By doping the I-V
characteristics were studied which showed significant NDR which was more pronounced
in the case of nitrogen Also the changing positions of the dopants contributed towards
the I-V curve to be more ohmic The edge doping caused minimum NDR and
semiconductor behavior as compared to central doping Lastly the thermoelectric
properties were studied - the increasing concentration of N causes the Figure of Merit to
decline due to the decrease in conductivity as well as mobility of electrons
66
REFERENCES
1 Wikianswers What makes carbon unique
httpwikianswerscomQWhat_makes_carbon_so_unique (22 November)
2 Kopeliovich D D Graphite
httpwwwsubstechcomdokuwikidokuphpid=graphite (1128)
3 Barbier M Transport properties of nanostructures and superlattices on single layer and
bilayer graphene University Antwerpen Antwerpen 2012
4 Shylau A Electron transport interaction and spin in graphene and graphene
nanoribbons Linkoping Norrkoping 2012
5 HassJ R F T Li X Li Z Zong W A de Heer P N First E H Conrad C
AJeffrey and C Berger Applied Physics Letters 2006 89 (14) 143
6 Jones A Mechanical Exfoliation to Make Graphene and Visulization
httpcarbonchemwisceduFilesMechanicalExfoliationpdf (18 October)
7 Anteroinen J Structural and Electrical Characteristics of Graphene Field Effect
Transistors AALRO school of Electrical Engineering AALTO 2011
8 Novoselov K S A K G S V MorozovD JiangY Zhang S V Dubonos I V
Grigorieva A A Firsov Science 2004 306 (22)
9 Kosynkin D A L H A Sinitskii J R Lomeda A Dimiev K B Price and J M
Tour Nature 458 876
10 Yi Z Luyao Zhang Accounts of chemical research 46 (10) 2339
11 Eizenberg M B JM 1979 82 236
12 Yu Q K L J Siriponglert S Li H Chen Y P Pei S S Applied Physcis
Letters 2008 93 (113103)
13 Li X C W An J Kim S Nah J Yang D Piner R Velamakanni A Jung I
TutucE Banerjee S K Colombo L Ruoff R S Science 2009 324 1314
14 Schaefer H E Nanoscience Springer Berlin 2010
15 Levente Tapasztoacute G D Philippe Lambin amp Laacuteszloacute P Biroacute Nature Nanotechnology
2008 3 401
67
REFERENCES
16 Dacheng Wei Y L Advance Materials 2010 22 (30) 3241
17 Wei Yao K L Y GYGao Elsevier Solid State Communications 2013 153 52
18 Dacheng Wei Dagger Yunqi Liudagger Yu Wangdagger Hongliang ZhangdaggerDagger Liping HuangdaggerDagger
Yudagger a G NanoLetters 2009 9 (5) 1758
19 Nakada K M F G Dresselhaus and M S Dresselhaus PhysRevB 1996 54
(9858)
20 Son Y W C M L a L S G PhysRevLett 2006 97 (216803)
21 Raza H Graphene Nanoelectronics Springer 2012
22 Ryan W J Electronic Transport in Graphene p-n junctions Short Noise and
Nanoribbons Harvard University 2009
23 Fangping OuYang J X Rui Guo Hua Zhang and Hui Xu Nanotechnology 2009
20 6
24 Guo J Carbon nanotube electronicsModeling physics and applications Purdue
University West Lafayette IN 2005
25 Motta C S S-P MITrioni cond-matmes-hall 2012 7
26 B P Growing Graphene via Chemical Vapor Deposition Ponoma College Ponoma
2011
27 ZurichE Transport properties of three-terminal graphene devices University of
Science and Technology Norway 2008
28 Uichiro MIntroduction to the electron theory of metals
29 Robert Laughlin H S Additional background material on the Nobel Prize in Physics
1998 (410)
30 MarkGoerbig Quantum Hall Effects (11152013)
68
REFERENCES
31 Zurich E Transport properties of three-terminal graphene devices Norwegian
University of Science and Technology Norway 2008
32 Deepak R Klein Tunneling University og Tennessee Space Institute Tennessee
2011
33 Williams JR L D CMMarcus Quantum Hall Effect in a Gate-Controlled p-n
Junction in Graphene (1122013)
34 Avadhanulu MN P G K A Textbook of Engineering Physcis for BE BSc (Engg)
SChand New Delhi 1992
35 Andriotis A Applied Physics Letters 2007 91 (152105)
36 Qimin Yan B H dagger Jie Yudagger Fawei Zhengdagger Ji ZangDagger Jian Wudagger Bing-Lin Gu F
L Dagger and Wenhui Duandagger NanoLetters 2007 7 (6) 1473
37 Soler J M E A J D Gale A Garciacutea J Junquera P Ordejoacuten and D Saacutenchez-
Portal J Phys Condens Matter 2002 14 2745
viii
LIST OF FIGURES
Figure Page
11 (a) Chemical representation of Carbon (b) Graphite ore (c) Structure of
Graphite and a single layer Graphenhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
2
12 An optical image of Graphene flake obtained by exfoliation of
graphitehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
3
13 (a) Graphene formation on Nickel (b) Graphene atoms on Ni (111)
lattice (c)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
7
14 (a) SEM image of graphene on copper foil (b) High-resolution SEM
image of graphene on Cuhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
8
15 (a) Transfer process (b) Wafer-scale synthesis of graphene (c) Graphene
films transferred onto glass wafer (d) SiSiO2 with device patterned (e)
PET filmhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
9
16 (a) High-magnification image of the annealed sample showing that well-
defined zigzag armchair and zigzag-zigzag edges are formed (b) ) STM
image of an 8 nm wide bent junction connecting an armchair and a
zigzag graphene nanoribbon which was carved by STM
tipshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
10
17 Band structure of graphene before and after doping The image shows
shift towards the Fermi levelhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
11
18 Low resolution TEM image of N-doped graphene Background is the
lacey carbon TEM grid graphene sheet is crumpled with many
rippleshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
13
19 Zigzag and Armchair orientation of Graphenehelliphelliphelliphelliphelliphelliphelliphelliphellip 13
110 Bandstructure of ZGNRhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 14
111 Bandstructure of AGNRhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 15
21 Left Real space Graphene lattice with basis vectors and Right
The first Brillouin zone of Graphene in reciprocal space with basis
vectors and K and Krsquo are responsible for massless transport at low
energyhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
17
ix
LIST OF FIGURES
(Continued)
Figure Page
22 Bandstructure of a graphene sheet showing a band gap of 0eVhelliphelliphellip 18
23 Band structure of Graphene calculated with the tight-binding modelhellip 19
24 The energy dispersion around the K pointhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 22
25 Electrons colliding with stationary ionshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 23
26 (a) 2D electrons in a perpendicular magnetic field Logitudinal resistance
measured across C5 and C6 Transverse resistance measured across C3
and C5 (b) Classical Hall resistance as a function on the magnetic field
25
27 Klein tunneling through an npn barrierhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 29
28 Electron trajectory considering the linear electrostatic potential U(x) = Fx 30
29 Electron like and hole like trajectories at same Ehelliphelliphelliphelliphelliphelliphelliphelliphellip 30
210 Quantum Hall effect in graphene 22
The Hall conductivity σxy and the
longitudinal resistivity of monolayer graphene as a function of carrier
density at B = 14T and T= 4K This shows half-integer QHE with chiral
index J= 1helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
32
211 (a) LL for Graphene bilayer (b) Schematics of Hall conductivity as a
function of nn0 for bilayer Graphene (solid line) and monolayer
Graphene (dotted line) (c) LL for monolayer Graphenehelliphelliphelliphelliphelliphelliphellip
33
212 Seebeck Effecthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 35
213 Transmission functions in units of (2e2h) for AZA structureshelliphelliphelliphellip 37
214 I-V curve for a 591nm long channel (Vbias=20mV)helliphelliphelliphelliphelliphelliphelliphellip 38
31 NEGF systemhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 42
41 Geometry of device configuration with two electrodeshelliphelliphelliphelliphelliphelliphellip 48
42 The electron distribution in a device configuration which illustrates a left
moving scattering state with origin in right electrodehelliphelliphelliphelliphelliphelliphelliphellip
48
x
LIST OF FIGURES
(Continued)
Figure Page
51 Band structure of AGNR widths (a) 4 atoms (b) 5 atomshelliphelliphelliphelliphelliphellip
53
52 Band structures of AGNR widths (a) 6 atoms (b) 7 atomshelliphelliphelliphelliphelliphellip 54
53 Band structure of AGNR widths (a) 8 atoms (b) 9 atomshelliphelliphelliphelliphelliphelliphellip 54
54 Band structures of AGNR widths (a) 10 atoms (b) 11 atomshelliphelliphelliphelliphellip 55
55 Band structure of AGNR with a width of 12 atomshelliphelliphelliphelliphelliphelliphelliphelliphellip 55
56 Variation in band gaps as the width (number of atoms) varieshelliphelliphelliphellip 55
57 Band structure of ZGNR width (a) 4 atoms (b) 6 atomshelliphelliphelliphelliphelliphelliphellip 56
58 Band structure of ZGNR width (a) 8atoms and (b) 10 atoms 57
59 Band structure of ZGNR with a width 12 atomshelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 57
510 Band structures of Doped AGNR (a) 4 N Doped (b) 4 B Doped (c)
2 N Doped (d) position of Nitrogen from (c)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
58
511 Current Vs Voltage graph for varying graphene width showing
conductivityhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
59
512 ZAZ GNR junction devicehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 60
513 I-V curve of Boron Doped ZAZ junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 61
514 I-V curve of Nitrogen Doped ZAZhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 62
515 Variation of Peltier effect coefficient with temperature for various doping 64
1
CHAPTER 1
INTRODUCTION
11 Graphene The New Carbon
Carbon (chemical symbol C atomic mass 1207amu) (Figure 11a) is a widely distributed
element in nature It is found abundantly in the sun stars comets and the atmospheres of
the planet Carbon can form up to four bonds it can bond with itself endlessly and with
most other elements in many different shapes making it a significant part of the
construction for many kinds of complex molecules1
Two allotropes of carbon are commonly used diamond and graphite (Figure
11b) The bonding structures of diamond and graphite contribute to the properties
individually In diamond all the p-orbitals are used forming a sp3
bonding whereas in
graphite only two orbitals are occupied allowing the unpaired bond for the transport of
electrons Each carbon atom in graphene possesses sp2 hybridization ie each carbon
atom is connected to three other carbon atoms via covalent bonds with a bond length of
142Å and an angle of 120deg between each bonded pair This makes graphite a better
conductor than diamond Graphite consists of many layers of 2D carbon lattices (Figure
11c) stacked on top of each other and held via Van der Waals forces A single layer of
graphite where carbon atoms are arranged in a honeycomb lattice is known as graphene
(Figure 11c)
2
Figure 11 (a) Chemical representation of Carbon (b) Graphite ore (c) Structure of
Graphite and a single layer Graphene2
Theoretical work on graphene was done specifically to study the other allotropes
The first study was done by Wallace in 1947 who calculated the band structure of
graphene3 Further the peculiar Landau levels were known by McClure in 1957 and the
relativistic Hofstadter butterfly by Ramal in 19853 Later in 1991 the invention of carbon
nanotubes by Iijima boosted the theoretical research on graphene3 Prior to the invention
of carbon nanotubes there were a few experimental papers on graphene growth via
various methods like intercalation of graphite (Shioyama 2001) free standing (Boehm
1962) epitaxial as well as graphene grown on metals (Bommel 1975 Land 1992 Itoh
1991)3 With all the various discoveries the electronic properties of graphene were not
studied until 2004 when Berger and Novoselov were able to access the electronic
properties with contact of graphene flakes3 (Figure 12)
3
Figure 12 An optical image of Graphene flake obtained by exfoliation of graphite3
The specific lattice structure of graphene possesses a number of unique electronic
properties making it an interesting material for theorists experimentalists and engineers
Utilization of graphene as a fundamental block of electronic devices requires
development of new theoretical methods for understanding the current propagations in
graphene constriction4
12 Graphene Synthesis
The discovery of graphene by mechanical exfoliation called the lsquoScotch tape methodrsquo led
to serious attempts towards the production of top quality graphene5 Graphene was first
exfoliated mechanically from graphite in 20046 The importance of high quality graphene
cannot be emphasized enough however electron transport has shown that defects play an
important role in hindering the transport properties of electrons (holes)7 The two
synthesizing methods for the large scale manufacture of graphene are chemical vapor
deposition (CVD) and silicon carbide (SiC) desorption method
4
Graphene can be synthesized by sublimation of silicon from SiC at high
temperature (1200degC) in high vacuum5 The major advantage of this method is that the
SiC provides an insulating substrate and no transfer of the graphene layer is needed Yet
the disadvantage of this method outweighs its advantages the high temperature is cost-
ineffective making it unsuitable for large scale manufacturing8 Also the crystal growth
face alters the properties of graphene Graphene grown on Si-terminated face has poor
homogeneity and is subjected to unintentional doping7 Conversely graphene grown on
C-terminated SiC has higher mobility and is often called lsquoturbostaticrsquo due to the
rotational disorder7
Unlike the SiC method the graphene produced via CVD method needs to be
transferred to a substrate making it difficult to maintain the quality of graphene Yet
CVD synthesized graphene has a larger grain size7 More research is being done on
various methods for synthesis of graphene The methods include direct chemical
synthesis ion implantation crystal sonification and lastly unzipping carbon nanotubes to
form graphene sheets9
Graphene and few-layer graphene have been grown by CVD from carbon
containing gases on catalytic metal surfaces andby surface segregation of C dissolved in
the bulk of such metals7 Growing graphene with CVD is a very attractive solution since
it is compatible with the existing semiconductor industry9 Graphene has been grown via
CVD process on metal substrates such as Nickel (Ni) and Copper (Cu)
5
121 Synthesis of Graphene on Nickel (Ni)
Polycrystalline Ni films are annealed in ArH2 atmosphere at 900-1000degC to increase
grain size and are then exposed to H2CH4 gas mixture10
In this step the hydrocarbon
decomposes and dissolves in Ni to form a solid solution Lastly the samples are cooled in
argon gas Ni has high carbon solubility at elevated temperatures and the solubility
decreases as temperature is reduced During the cooling process the carbon atoms diffuse
out from the Ni-C solid solution and precipitate on the Ni surface to form graphene films
(Figure 13a) Since Ni (111) has a lattice similar to the densely packed hexagonal lattice
of graphene (Figure 13b) they also have similar lattice constants and hence Ni surface
serves as an excellent lattice matched substrate for graphene growth11
The growth of graphene on Ni is based on carbon segregation and precipitation
process different segregation behavior is produced by different cooling rates which
affect the thickness and quality of graphene films12
Medium cooling rates lead to optimal
carbon segregation and produce few layers12
Graphene films grown on Ni are usually
continuous with monolayer and few layer regions Annealing of Ni substrates at elevated
temperatures in hydrogen atmosphere not only increases the single-crystalline Ni grain
size but also eliminates certain impurities in Ni thereby improving the graphene quality
Furthermore the graphene thickness can also be affected due to the amount of carbon
dissolved in the Ni films during the growth time
After synthesis the graphene can be transferred to other insulator substrates for
further characterization and applications Figure 13c shows the selected area electron
diffraction pattern of graphene film along the [001] direction which confirms the
graphene lattice structure shown After transfer to insulator substrates the geometry can
6
be retained as shown in Figure 13d Under optimal growth parameters graphene growth
is only limited by the Ni catalyst Lastly Figures 13e and 13f show the wafer-scale
graphene synthesis and transfer of graphene to a flexible transparent substrate
respectively
Though polycrystalline Ni is a good substrate the percentage and size of
graphene monolayer are still limited Researchers have hence tried other metal substrates
for graphene synthesis
7
Figure 13 (a) Graphene formation on Nickel (b) Graphene atoms on Ni (111) lattice
(c) Low magnification TEM image of graphene edges (d) Optical image of graphene
transferred from the Ni surface to SiO2Si substrate (e) Full-wafer scale deposition of
graphene layers on polycrystalline Ni (f) Transparent and flexible graphene films on
PDMS substrate10
8
122 Synthesis of Graphene on Copper (Cu)
Graphene films are grown on 25microm thick Cu foils in a hot wall furnace13
The Cu foil is
first annealed in hydrogen atmosphere at 1000degC and a mixture of H2CH4 is introduced
into the system to initiate graphene growth After a continuous graphene layer is formed
on the Cu foil the system is cooled to room temperature Figure 14a shows an SEM
image of graphene on Cu substrate indicating the Cu grains with contrast The Cu
surface steps are formed during thermal annealing and the darker flakes indicate multiple-
layer graphene (Figure 14b)10
The graphene wrinkles in Figure 14(b) originate from
different thermal expansion coefficient of graphene and Cu They go across the Cu grain
boundaries indicating that the graphene film is continuous
Figure 14 (a) SEM image of graphene on copper foil (b) High-resolution SEM image of
graphene on Cu10
123 Transfer of Graphene films
In order to facilitate the applications of graphene for electronic applications we need to
separate the graphene from the catalytic metal substrate Figure 15a shows the transfer
process of graphene Graphene is first coated with a thin layer of polymethyl
methacrylate (PMMA) and baked at 120degC to evaporate the solvent10
The metal layer is
then removed by Ni or Cu etchant leaving behind the PMMA graphene film The film is
then cleaned by deionized water and then transferred onto the target substrate After the
9
evaporation of water vapor the PMMA is removed by acetone leaving graphene film on
top of the target substrate Figure 15b shows a graphene wafer transferred from the
substrate onto glass and polyethylene terephthalate (PET) films
Figure 15 (a) Transfer process (b) Wafer-scale synthesis of graphene (c) Graphene
films transferred onto glass wafer (d) SiSiO2 with device patterned (e) PET film10
124 Synthesis of Graphene Junction
Graphene junctions with smooth armchair and zigzag edges are difficult to produce by
conventional methods such as mechanical exfoliation chemical exfoliation or lithography
etching14
The conventional methods can only produce rough edges Recently
Dresselhaus reported an edge reconstruction of graphene by Joule heating in a TEM-STM
10
(Figure16b) system15
An individual nanoribbon sample is attached to the sample holder
at one end and to the STM tip at the other end these ends also serve as the two
electrodes The structural transformation in the growth of graphene from armchair to zig-
zag is mainly attributed to the vaporization of carbon edges that reconstruct at high
temperatures in which resistive Joule heating and preferred current flow play an
important role This means that by controlling the flow of current a perfectly smooth
edged ribbon can be synthesized making graphene-based electronics possible16
Figure 16 (a) High-magnification image of the annealed sample showing that well-
defined zigzag armchair and zigzag-zigzag edges are formed (b) STM image of an 8 nm
wide bent junction connecting an armchair and a zigzag graphene nanoribbon which was
carved by STM tips14
125 Doping in Graphene
The doping of graphene can be roughly classified into two categories - electrical and
chemical Electrical doping involves changing gate voltages of graphene devices and
chemical doping uses chemical routes such as substitutional or interstitial This thesis
discusses chemical doping and the importance of doping sites by changing the dopant
Chemical doping is a common approach to tailor the electronic properties of
11
semiconductors Doping of graphene can cause its electronic properties to alter leading to
a metal-semiconductor transition The two means of doping graphene are interstitial and
substitutional In interstitial doping the dopant atoms or molecules are introduced as
adatoms or admolecules on the surface of graphene whereas in substitutional doping the
dopant atoms are replaced in the carbon lattice forming a bond in the lattice of
graphene16
Doping graphene results in the formation of n or p-type semiconductors
depending on the kind of dopant If the dopant is an electron donor it causes the Fermi
level to shift up resulting in n-type behavior of graphene Furthermore if the dopant is an
electron acceptor it causes the Fermi level to shift down resulting in a p-type behavior of
graphene (Figure 17)16
Figure 17 Band structure of graphene before and after doping The image shows shift
towards the Fermi level16
Graphene nanoribbons (GNR) can be made into a p- and n- type semiconductor
by doping with boron (B) and nitrogen (N) respectively In theory GNR p-n junction is
formed by doping GNR with B and N in different regions However experimentally
doping graphene with both these elements is very difficult due to the dopants reacting
with each other17
Hence most experimental studies use GNR doped by only one
12
element N-doped graphene was synthesized by Wei et al Wang and B-doped Graphene
was realized by Endo17
Many researchers have demonstrated interstitial doping of graphene by gas metal
and organic molecules16
The various gases and metals used are NO2 NH3 An-CH3 Na-
NH2 F4-TCNQ TPa TCNE and others16
Doping in graphene is hence possible by
electrons or holes in high concentration without deterioration of its mobility Interstitial
doping is highly sensitive due to most of the conducting channel being exposed to surface
absorbates and hence can be used in molecule detection
In substitutional doping the dopant atoms are included in the graphene lattice and
thus chemically bonded Substitutional doping is done via the CVD method using a
carbon and dopant source Substitutional doping opens up many applications in device
engineering making graphene a very good candidate as a semiconductor This study
involves the study of transport properties of graphene doped by substitution
126 Nitrogen (N) Doped Graphene Synthesis (Substitutional)
N-Doped graphene is prepared via a CVD process using a 25microm thick Cu film on a Si
substrate The substrate is placed in a quartz tube with the flow of hydrogen (20sccm) and
argon (100 sccm)18
When the center of the furnace reaches 800degC 60 sccm of CH4 and
60 sccm of NH3 is introduced into the flow as C source and N source respectively The
substrate is then moved to high temperature and after 10 min growth the sample is
cooled to room temperature under H2 ambient Figure 1 8 shows the growth of N-doped
graphene18
13
Figure 18 Low resolution TEM image of N-doped graphene Background is the lacey
carbon TEM grid graphene sheet is crumpled with many ripples18
13 Structure of Graphene Nanoribbon (GNR)
Graphene Nanoribbons (GNR) are strips of graphene with very thin width of lt50nm
GNRs can be terminated in three separate ways called zig-zag (0 n) armchair (m 0) and
chiral (m n) (Figure19) and this termination along the width of the ribbon dictates the
size of the band gap19
Figure 19 Zigzag and Armchair orientation of Graphene5
Due to their various edge structures GNRs exhibit different electronic properties
ranging from normal semiconductors to spin-polarized half metals which open the
possibility of GNRs as electronic devices19
14
Within a tight binding approach (AGNRs) could be metallic or semiconducting
depending on their ribbon width but all zigzag graphene nanoribbons (ZGNRs) are
metallic with a high density of electronic states at the edges Hence ZGNRs exhibit
characteristic edge effects which are not present in AGNRs These edge effects in
ZGNR create a flat band close to the Fermi level making the ZGNR edges more
reactive19
First-principles calculations show that the GNRs possess a non-zero direct
band gaps These gaps are small for ZGNR (Figure 110) caused due to spin ordering
effects at the edges For AGNRs the band gap arises from quantum confinement (Figure
111) effect that has larger magnitudes than ZGNR20
Figure 110 Band structure of ZGNR
15
Figure 111 Band structure of AGNR
For GNRs the band gap decreases as the ribbon width increases and in order to
create a semiconductor with a desirable band gap the nanoribbon width should be
adjusted accordingly This property of adjusting the band gap makes graphene an
excellent candidate for transistor switching By applying an electric field GNR can be
altered from an insulator to a conductor GNRs exhibit very intriguing properties and
have become one of the promising candidates for electronic applications
14 Overview of Graphene Junction
The invention of p-n junctions date back to 1940s which later resulted in the invention of
junction transistors One of the key technological reasons for success of the p-n junction
is mainly due to its ability to locally modulate the energy band gaps via an applied bias21
A graphene p-n junction is created via single layer of graphene in which the
carrier type and density in two adjacent regions are controlled by electrostatic gating8
For materials with a band gap the electric field can either switch lsquooffrsquo the current or
rectify it (p-n diode)22
Being a ldquogaplessrdquo material the off state is not achievable in
16
graphene In order to achieve an off state the gap can be created by doping graphene with
various elements (Group III or Group V) Doping allows p-n junctions to be
reconfigurable using a gate voltage to distinguish between graphene p- n regions within a
single sheet Many researchers have studied the electronic as well as transport properties
of doped graphene junctions
In 2009 Fangping OuYang studied the transport properties of T-shaped graphene
junctions using the ATK software and showed that the conductance depends on
geometric structures which can be controlled by selective doping23
Wei Yao in 2013
studied the transport properties in graphene p-n junctions and showed that the
rectification effect depends on boron doping density and position17
The study of transport properties in graphene p-n junctions is a recent
advancement The thesis discusses transport properties including the current-voltage (I-
V) characteristics of doped graphene junctions Moreover the software used is similar to
the software in use by current researchers since they have produced viable data using
ATK
17
CHAPTER 2
RESEARCH BACKGROUND
21 Band Structure of Graphene
The unique electronic properties of graphene were first predicted in 1946 Figure 21
shows a top view of the hexagonal arrangement of carbon atoms in real space as well as
the first Brillouin zone in reciprocal space
Figure 21 Left Real space graphene lattice with basis vectors and Right The
first Brillouin zone of graphene in reciprocal space with basis vectors and
K and
Krsquo are responsible for massless transport at low energy24
The real space basis vectors are radic
and
radic
The reciprocal space basis vectors are 1 2
0 0
4 1 3 4 1 3( )and ( )2 2 2 23 3
b x y b x ya a
where the magnitude of the basis vectors is |a0| = radic acc The distance between nearest
neighbor carbon atoms is acc=0142nm
18
The band structure can be calculated by solving the eigenvalues using the
dispersion relation E( )
1 2 3( ) 3 2cos 2cos 2cosE k t k a k a k a (21)
Transport properties of solids are closely related to the energy dispersion
relations E ( ) in the material and in particular to the behavior of E ( ) near the Fermi
level Graphene is a zero gap semimetal whose specific linear electronic band dispersion
near the Brillouin zone corners (Dirac points) gives rise to electrons and holes that
propagate as massless Fermions25
The valence and conduction bands do not overlap in
graphene they touch at the Fermi Level (Figure 22)
Figure 22 Band structure of a graphene sheet showing a band gap of 0eV
The low energy properties of graphene can be well described by making a linear
expansion of the band structure around the K and Krsquo This energy can be written as
19
E(k) = plusmnħvF|k (22)
where vF is the Fermi velocity of 1106ms given by
1F
Ev
k
ħ (23)
Figure 23 Band structure of graphene calculated with the tight-binding model
22
The Fermi surface of graphene consists of double cones with Fermi energy at the
intersection of these cones (Figure 23) The slope of the band is zero and hence the
effective mass of electrons in that region is zero which leads to an entirely new transport
mechanism in graphene26
20
22 Transport Characteristics of Graphene
Transport process usually involves a flow of charge or energy or both The flow is mainly
due to external perturbations such as electric field and temperature gradient The
relationship between forces and flow usually defines various transport coefficients that
are the characteristics of electrons and phonons in the material All modern electronics
are based on the ability to control the electronic properties of a material by applying
external voltage This is done by an electric field effect where the gate voltage changes
the carrier concentration of the material and consequently its conductivity The electric
field effect in graphene was reported by Novoselov in 2004 and is used in transport
measurements8
The electron-phonon interaction in graphene plays an important role in
understanding the photoemission spectra observed in graphene The electric field effect is
an alternative method for changing the charge carrier density in low dimensional systems
The electric field effect in graphene which was first reported by Novoselov et al in
2004 is widely used as a characterization tool in transport measurements25
The transport characteristics of the material are directly related to the
bandstructure of graphene The carriers in graphene lattice are free to move in two
dimensions In the carrier transport of graphene the carriers ndash electrons and holes ndash close
to the Dirac points are of importance The transport is described by a two component
wave function (Equation 24) which obeys the 2D Dirac-like equation for massless
particles27
21
-ivFσ nablaψ(r) = Eψ(r)
(24)
where σ is the 2D Pauli spin matrix In the continuum limit the above (Equation
24) corresponds to the effective low energy Dirac Hamiltonian (Equation 25)
0( )
0
x y
F F
x y
iH k k
i
k kv v
k k
(25)
The electronic band structure of the energy (E) versus wave vector (k) relation for
graphene is given by Equation 24
The two component wave function resembles the spin or wave function of
quantum electro dynamics (QED)27
Corresponding to the spin of particles in QED the
charge carriers of graphene can be attributed with a pseudospin σ The pseudospin is the
direct result of two different carbon sublattices corresponding to the bonding and
antibonding combinations27
22
Figure 24 The energy dispersion around the K point27
In Figure 24 the red and blue lines correspond to the antibonding and bonding
states respectively The pseudospin can have two values either in the direction of or
against the momentum It can be seen that the electrons with energy E travelling in the
positive direction originates from the same branch as a hole with energy ndashE travelling in
the negative direction giving it the same pseudospin This results in suppressed
backscattering and Klein tunneling The back scattering process requires the pseudospin
to flip which is possible in the presence of short range scatters that act differently on sub
lattices27
23 Drude Theory
The classical theory of metallic conductivity was presented by Drude in 1900 and was
elaborated by Lorentz in 190528
Drude treated the free electrons as classical ideal gas
meaning the electrons collide with stationary ions and not each other
23
Figure 25 Electrons colliding with stationary ions28
The Drude theory applied the kinetic theory of gases to a metal considered as a gas of
electrons The basic assumptions made by the Drude theory are28
When metallic elements are brought together to form a solid then the valence
electrons become freely moving through the metal whereas the ions remain intact
as nearly immobile positive particles
Between collisions the electrons move freely ie there is neither electron-
electron interaction nor electron-ion interaction
The scattering mechanism leads to instantaneous collisions of the electron with
the scatterers
The collisions are characterized by a relaxation time τ
The electrons achieve thermal equilibrium only through collisions the velocity
after a collision is randomly directed the speed is as appropriate to the
temperature
With the relaxation time Drude obtained the electrical conductivity expression
where n is the number of electrons per unit volume
σ = ne2τm
(25)
He also calculated the thermal conductivity and successfully provided the
theoretical basis for Wiedemann-Frantz law already established in 1853 which states that
24
the ratio of electrical and thermal conductivity of any metals is a universal constant at any
given temperature28
The Drude theory gives results which are qualitatively correct outside of the
quantum Hall regime28
In the Drude theory of the electrical conductivity of a metal an
electron is accelerated by the electric field for an average time τ before being scattered
by impurities lattice imperfections and phonons to a state which has zero average
velocity The average drift velocity of the electron is
d
eE mv (26)
It is assumed that all electrons drift together and hence the current density
j = -ne (27)
This Drude theory works well for fields below ~ 01T At stronger fields the Hall
resistivity becomes nearly constant over finite intervals of magnetic fields28
The QHE
reflects both novel disorder physics as well as novel interaction physics in the quantum
Hall regime
24 Quantum Hall Effect (QHE)
The discovery of QHE is a remarkable achievement in condensed matter physics The
Hall Effect was discovered by Edwin Hall in 187929
However the precise quantization
of the Hall conductance in units of e2h was not recognized until February 1980 Five
years later in 1985 Klaus von Klitzing was awarded the Nobel Prize in Physics for the
discovery of QHE29
The quantum Hall effect occurs in two-dimensional electron systems in the limit
of strong perpendicular magnetic field that stems from electronic transport
25
measurements where one drives a current I through the sample and where one measures
both the longitudinal and transverse resistance (Hall resistance) A longitudinal resistance
is a resistance measured between two contacts that may be connected by a line which
does not connect C1 and C430
Transverse resistance is measured between two contacts
connected by an imaginary line connecting C1 and C4 (Figure 26a)
Figure 26 (a) 2D electrons in a perpendicular magnetic field Logitudinal resistance
measured across C5 and C6 Transverse resistance measured across C3 and C5
(b) Classical Hall resistance as a function on the magnetic field30
Due to the existence of quantum Hall effect it is natural to expect that there exists
a classical Hall Effect Hall showed that the transverse resistance of a thin metallic plate
varies linearly with the strength B of the perpendicular magnetic field (Figure 26 b)
RH = Bqnel (28)
More quantitatively the classical Hall Effect can be understood within the Drude
model for diffusive transport in a metal Within this model one considers independent
26
charge carriers of momentum p described by the equation of motion
( )
b
dp p pe E B
dt m (29)
where E and B are the electric and magnetic field respectively The macroscopic
transport characteristics ie resistivity of the system are obtained from the static
solution of the equation of motion dpdt = 0 and one finds for 2D electrons with p =
(pxpy)
x
x yb
y
y xb
eBe
eBe
ppE
m
ppE
m
(210)
In the above expression characteristic frequency is visible as
C
b
eB
m (211)
This is known as cyclotron frequency as it characterizes the cyclotron motion of a
charged particle in a magnetic field30
With the Drude theory the conductivity can be
written as
j = -enelpmb (212)
and the mobility can be given as
micro = eτmb (213)
The transport properties in the limit of ωCτ-gt infin are entirely governed in the presence of
27
a magnetic field by the off-diagonal ie transverse components of
conductivityresistivity
The theory of quantum Hall effect subjects all physical properties of 2D electron
system in the limit where the magnetic field is strong so that the mixing of Landau levels
by disorder or electron-electron interaction is considered to be a weak perturbation30
This is known as the quantum Hall regime The ratios between the energy scales
corresponding to the two interactions are important The limit where disorder potential is
much stronger is referred to as integer quantum hall regime whereas the limit where the
interaction potential is much stronger is referred to as fractional quantum Hall regime
25 Resistivity and Resistance
The electronic transport in the framework of the Drude theory allows for the calculation
of conductivity or resistivity of a classical diffusive 2D electrons in a magnetic field30
The conductivity and conductance are related to one another but they depend on the
geometry of the conductor-the resistance R and hence the resistivity is given by
R = (LA)ρ (214)
where L is the length of the conductor and A is the cross section
For a d-dimensional conductor the cross section scales as Ld-1
such that the
scaling relation between the resistance and the resistivity is
R~ ρL2-d
(215)
From the dimension point of view resistance and resistivity are the same in 2D and the
resistance is scale-invariant Further the resistance of a 2D conductor depends in
general on the so-called aspect ratio LW via some factor f (LW)30
However for
transverse Hall resistance it is the length of the conductor that plays the role of cross
28
section such that the Hall resistivity and the Hall resistance truly coincide ie f=1 The
Quantum Hall effect is highly insensitive to the particular geometric properties of the
sample used in transport measurements Recently quantum Hall physics experienced the
discovery of ldquorelativisticrdquo quantum Hall effect in graphene The electrons in graphene
behave as if they were relativistic massless particles contributing to a very interesting
field of research30
26 Klein Tunneling
Klein tunneling in which relativistic particles penetrate through a potential barrier
without the exponential damping that is characteristic for nonrelativistic quantum
tunneling has never been observed for elementary particles The tunneling allows
transmission of a particle through a potential barrier higher than its kinetic energy
violating the principle of classical mechanics30
On the quantum scale the objects exhibit
wave-like characteristics in which the quanta move against a potential hill described by
their wave function This wave function represents the probability amplitude of finding
the object in a particular location The transmission of the object through the potential hill
is termed as tunneling When EltV then the ψ(x) over V is returned by ψrsquo(x) In quantum
mechanics an electron tunnels from the conduction into the valence band Such a
tunneling from an electron-like to hole-like state is called as Klein Tunneling in which the
electron avoids backscattering
In Figure 27 it is shown that an electron hitting a potential barrier is reflected
with 100 certainty In non-relativistic quantum mechanics the electrons can tunnel
through the barrier but the probability of tunneling exponentially decays with increasing
29
height and width of the barrier However in relativistic quantum mechanics the barrier
gets transparent even in the limit of infinite barrier height (Klein paradox)31
Figure 27 Klein tunneling through an npn barrier30
The Klein paradox in graphene can be understood in terms of electrons and holes
In graphene the massless carriers behave differently than ordinary carriers (with mass) in
the presence of an electric field A barrier which is repulsive for electrons will be
attractive for holes Since there are hole states inside the barrier with the same energy as
the electrons outside an electron arriving at the barrier can tunnel through it as a hole
before leaving again as an electron Klein tunneling for transport in graphene is that the
charge carriers cannot be confined by potential barriers The Klein tunneling effect has
been experimentally observed by Ando in 1998 in which the absence of backscattering
(Figure 28) is responsible for high conductivity in carbon nanotubes
30
Figure 28 Electron trajectory considering the linear electrostatic potential U(x) = Fx30
The electron is able to propagate through an infinitely high potential barrier since
it makes a transition from the conduction band to valence band In this transition from
conduction band to valence band its dynamics changes from electron-like to hole-like
The equation of motion is thus given by
2
2 2 2| | ( )
pdr E
dt E Up
p E U
v
v
at energy E (216)
This shows that in the conduction band (UltE) and in the valence band (UgtE)
In Klein tunneling the pairs of electron-like and hole-like trajectories at the same E and
py have turning points at dmin given by dmin=2v|py|F (Figure 29)
Figure 29 Electron like and hole like trajectories at same E21
31
The tunneling probability exponential dependence on dmin
2
min| |
( ) exp( ) exp( )2
y y
y
vT
F
p pdp
(217)
The applications of the Klein tunneling include Atomic clock Scanning tunneling
Microscope Tunnel diode Tunneling transistor and many more32
Since graphene
exhibits Klein tunneling it can be very useful to study the transport properties in
graphene and use it in such applications
27 Quantum Hall Effect in a Graphene
A monolayer graphene shows half-integer quantum Hall effects where the Hall
resistance is quantized at values of
2
1
xyh v eR
(218)
around filling factors
14( 1 2)Nv
(219)
where N is an integer e is the electron charge h is the Planckrsquos constant and the
factor 4 is due to spin and valley degeneracy QHE in graphene can be observed at room
temperature which is a very intriguing property (Figure 210) Graphene reveals
significant differences with respect to conventional 2D electron systems The Landau
quantization yields energy levels that disperse differently in graphene as well as
particular zero-energy level that is only half filled at the charge neutrality point (v=o)
32
Figure 210 Quantum Hall effect in graphene22
The Hall conductivity σxy and the
longitudinal resistivity of monolayer graphene as a function of carrier density at B = 14T
and T= 4K This shows half-integer QHE with chiral index J= 1
The QHE in graphene is not entirely similar to regular QHE since the charge
carriers in graphene are Dirac Fermions The charge carriers governed by
electrodynamics is given by (Equation 220) which does not apply for graphene and a
QED quantization of graphene electronic band structure is used
En = (n+12)ħω (220)
33
In the presence of magnetic field the nature of the Dirac Fermions in graphene
results in unevenly spaced Landau levels (LL) containing a distinctive LL at the electron-
hole degenerating a zero energy given by
2MG
MGFehn B
n vE (221)
The LL levels at high magnetic fields in MG are shown in Figure 211
Figure 211 (a) LL for Graphene bilayer (b) Schematics of Hall conductivity as a
function of nn0 for bilayer Graphene (solid line) and monolayer Graphene (dotted line)
(c) LL for monolayer Graphene33
It is found that the Hall resistance of a two dimensional electron system has
plateaus as a function of the number of electrons at low temperatures and strong magnetic
fields32
At large B the Dirac-like energy spectrum of graphene gives rise to a
characteristic series of QH plateaus in conductance reflecting the presence of a zero-
energy Landau level that include only odd multiples of 2e2h for uniform carrier density
in the sheet These plateaus of QH edge states at the edge of the sheet circulating in a
34
direction are determined by the direction of B and the carrier type33
This is why QHE in
graphene is known as Half-Integer Quantum Hall Effect
28 Thermoelectric Effect
Thermoelectricity refers to a class of phenomena in which a temperature difference
creates an electric potential or an electric potential creates a temperature difference The
principle of thermoelectric effect has been known for over 100 years Recently the
practical applications of thermoelectric effect have become more viable34
Thermoelectric effect is the direct conversion of temperature differences to
electric voltage and vice versa Joule heating is the heat generated whenever a voltage is
applied across a resistive material The Peltier-Seebeck effect is reversible whereas Joule
heating is not This effect can be used to generate electricity to measure temperature to
cool objects or to heat them Since the direction of heating and cooling is determined by
the sign of the applied voltage thermoelectric devices make very convenient temperature
controllers
281 Seebeck Coefficient
Thomas Johann Seebeck discovered that an emf appears in a circuit composed of two
dissimilar metals when the junction between the metals is held at different
temperatures34
The thermoelectric emf causes a continuous current in the circuit when a
complete loop is formed and the current is known as thermoelectric current This is
known as the Seebeck effect
35
Figure 212 Seebeck Effect34
As long as the two junctions are at different temperatures the thermoelectric emf
exists and the current will keep flowing between the hot and cold junction that are at
different temperatures The Seebeck effect is the conversion of temperature difference
directly into electricity The voltage developed in the circuit shown in Figure 212 is
proportional to the difference in temperature between the two junctions and is given by
V = α (T2-T1) (222)
This Seebeck effect is observed not only in metals but also in semiconductors
Here α is known as the Seebeck coefficient α measures the magnitude of an induced
thermoelectric voltage in response to the temperature difference across the material If the
temperature difference ∆T between the two ends of a material is small then the Seebeck
coefficient of a material is written by
α = ∆V∆T (223)
36
This can be expressed in terms of electric field as
α E∆T (224)
The units of Seebeck coefficient is given as VK The higher the Seebeck coefficient
value the better it is since it will create a very large voltage that can be used to provide
power
282 Peltier Coefficient
Peltier effect is the inverse of Seebeck effect involving a junction phenomenon There is
heat absorption or generation at the junctions depending on the direction of current flow
Heat generated by current flowing in one direction is absorbed if the current is reversed
The heat absorbed per second at a junction carrying current I is given by
Heat absorbed in t sec = πabIt (225)
Here πab is the Peltier coefficient and given by HIt Thus Peltier coefficient is
numerically equal to the applied potential difference expressed in Volts
Overall by studying the flow of electrons the values of Seebeck
coefficient and Peltier co-efficient can be estimated These values determine the various
applications of the materials In this thesis the Peltier and Seebeck coefficient of the
graphene junction and the new applications are discussed
37
29 Early Research ndash ab intio studies
In 2007 Androitis studied that the conducting properties of graphene nanoribbons and
junctions are strongly dependent on their size and geometric features35
He concluded that
there is no conductance for small AZA or ZAZ ribbons (Figure 213)
Figure 213 Transmission functions in units of (2e
2h) for AZA structures
35
Figure 213 shows that T (E) exhibits a negligible peak [T (E) = 001 in units of
2e2h] at E= -225 and 250eV However it was noted that when the width of the arm type
was increased T (E) at -225 and 250eV was 02035
Later in 2007 Qimin Yan used first principles methods to investigate the Current-
Voltage characteristics of GNR Transistors and the effect of edge doping He showed that
GNR field effect transistors can achieve high performance levels with ONOFF ratios on
the order of 103-10
436
Figure 214 is an I-V curve of AZA GNR-FET connected via
armchair metallic leads36
38
Figure 214 I-V curve for a 591nm long channel (Vbias=20mV)
36
In 2009 Fangping OuYang demonstrated the intrinsic transport properties and
effective B or N doping of the junctions by using first-principles quantum transport
simulations He concluded that the I-V characteristics of pure-carbon T-shaped junctions
exhibit metallic behavior and the current in the junction strongly depends on the height
of the stem23
He reported that the conductance of the devices depends on the geometric
structures which can be controlled by selective doping
In 2012 Wei Yao used the first principle calculations based on Density
Functional Theory (DFT) and Non-equilibrium Greens Function (NEGF) to study the
electronic as well as the transport properties of B-doped 6-GNR p-n junction His results
showed that the boron doping interval can influence the rectification effect at low bias
and also exhibit Negative Differential Resistance (NDR) phenomena at high positive
bias
39
CHAPTER 3
COMPUTATIONAL DETAILS
31 Introduction
The physical chemical electrical electronic and optical properties of a solid are
determined by their quantized electronic states The quantum states in low-dimensional
systems are produced due to the confinement of the carrier charges in one or two
dimensions Graphene is a conductor electrons are able to flow through graphene more
easily than through even copper The electrons can travel through the sheet of graphene
like mass-less particles as fast as just one hundredth that of the speed of light The ways
in which electrons behave in graphene make it very helpful to study their fundamental
physical properties Graphenersquos near perfect crystal lattice provides a very clean system
to experiment By restricting the electrons to only two dimensions they exhibit some
interesting properties such as the anomalous quantum Hall effect and Klein tunneling
In this chapter two theoretical concepts used for calculating the electronic structure
and the transport properties for graphene are described These include the Extended
Huckel Theory and Non-Equilibrium Greenrsquos Function (NEGF) method
311 Extended Huckel Theory
Erich Huumlckel was born in Germany on August 9th
1896 He studied mathematics and
physics in Berlin He is best known for his work in the field of chemistry and physics for
two contributions (1) Debye- Huumlckel theory of electrolytic solutions (2) Huumlckel
method of approximate molecular orbital calculations on electron systems In 1930 he
published his findings on systems in 1931 he generalized and expanded the system
40
theory to explain benzene Due to his poor communication skills his findings went
unrecognized for over 20 years It was in 1951 that his 4n + 2 rule was finally clarified by
Doering to show if C=C bonds would show aromaticity Huumlckel died on February 16th
1980 with very little worldwide recognition for his contributions to chemistry Today
chemistry students recognize his name and his contributions to the field are quite
substantial
One of the first semi-empirical methods to be developed was Huumlckel Molecular
Orbital Theory (HMO) HMO was developed to describe molecules containing
conjugated double bonds HMO considered only electrons in pi orbitals and ignored all
other electrons in a molecule The Extended Huumlckel Molecular Orbital Method (EH) was
developed out of the need to consider all valence electrons in a molecular orbital
calculation
By considering all the valence electrons chemists could determine molecular
structure compute energy barriers for bond rotations and determine energies and
structures of transition states for reactions By considering only the valence electrons the
computed energies could be used to choose between proposed transition states to clarify
reaction mechanisms The total valence electron wavefunction is described as a product
of the one-electron wave functions
1 2 3(1) (2) (3) ( )valence j n (31)
where n is the number of electrons and j identifies the molecular orbital Each
molecular orbital is written as a linear combination of atomic orbitals (LCAO)
1 12
N
j jr rrc j N
(32)
41
The energy of the jth
molecular orbital is given by a one-electron Schroumldinger
equation using an effective one electron Hamiltonian heff which expresses the interaction
of an electron with the rest of the molecule
eff j j jh (33)
This is the energy eigenvalue of jth
molecular orbital corresponding to the Eigen
function j The advantage of using this method is that the exact form of heff is not
required The total energy of the molecule is the sum of the single electron energies
j jj
E n (34)
where nj is the number of electrons in orbital j
In order to use the Extended Huckel method a set of calculation parameters and
approximations must be followed These parameters include the Basis set K-point and
the Brillouin Zone and lastly the Mesh cut-off
312 Introduction to NEGF
The Greenrsquos function is a function of two space-time coordinates From the knowledge of
this function one can calculate time-dependent expectation values such as currents and
densities electron addition and removal energies and the total energy of the system In
the absence of external fields the non-equilibrium Green function method reduces to the
equilibrium Green functions NEGF can be applied to both extended and finite systems
The generic system of NEGF consists of the electron dynamics of the channel described
by the Hamiltonian This channel consists of two contact reservoirs with respective
chemical potential μR and μL The NEGF assumes ballistic transport neglecting self-
42
energy from scattering The system is insulated from gate contacts whose effects are
realized via a 3D Poisson solver which solves for the potential at a given point in real
space based on electron density
22 ( ) [ ( ) ( )]D
qr N r n r
(35)
Figure 31 NEGF system
The system is easily expandable to systems with several contacts or gate
configurations by adding additional self-energy matrices to NEGF or additional sources
to the Poisson solver
313 Electrostatics
Electrostatic potential is created every time in the presence of a charge density due to an
induced electric field The Poissonrsquos equation correlates the electrostatic potential to
charge density as given in Equation 36
43
2( ( ) ( ) ( ) ( ))( )
( )( ) ( )
ADq p r n r r N rr
rr r
N
(36)
where ɛ(r) is the dielectric permittivity of the material ρ(r) n(r) ND(r) and NA(r) are the
hole electron donor and acceptor concentrations of the system respectively
Two types of boundary conditions are usually applied to the Poissonrsquos equation
Dirichlet boundary conditions
Φ (0) = F0 and Φ (L) = FL
von Neumann boundary conditions
00
( )
x
d x
dxB
and
( )L
x L
d x
dxB
For the transport problems with open boundary conditions the von Neumann
boundary conditions are used assuming that the potential vanishes at the boundary ie
B0=BL=0
The Poissonrsquos equation can hence be discretized on a grid as
2 ( )( )
( )
rx
r
= M (37)
where M is the matrix Φ and ρ are vectors containing the discretized values of
the electrostatic potential Φ and charge density ρ respectively
44
The Schroumldinger and Poisson equations are coupled since V(x) = -qΦ(x) is used
for the Schroumldinger to compute ρ(x) This self-consistent loop stops when the
convergence is reached
( )r
V(x) = -qΦ(x)
314 Non-Equilibrium Greenrsquos Function
Greenrsquos functions are a mathematical construction that are used to solve differential
equations subject to specific initial or boundary conditions They are named after the
British mathematician George Green The 1-D equation of L( )f( )=S( ) can be defined
by the Greenrsquos Function as given below
( ) ( ) ( )G x x f x x x (38)
The general Greenrsquos function is given by
( ) ( ) ( )f x dx G x x S x (39)
Applying the operator L( ) to the solution f( ) satisfies the original differential
equation The Greenrsquos Function G( ) is the propagator which propagates the influence
of a perturbation S( ) originally situated at the point to the point at which the
function f( ) is evaluated
The Greenrsquos Function G( ) can also be a correlation function If the points
and are strongly (weakly) correlated then S( ) will greatly (poorly) affect f( )
Poisson equation
2 ( )( )
( )
rr
r
Schroumldinger equation
2
2
( ( ) ) ( )
( )2
( ) | ( ) |
E H r E r S
H V rm
r dE E r
Figure 32 Self-consistent loop
45
The Schroumldinger equation with open boundaries can be written as
( )E H S (310)
Considering a 1-D and homogenous system ranging from =0 to L assuming
that Σ=0 and the form of equations is same before and after discretization then
22
2 0( ) ( ) ( )
2E x S x
m
dV
dx
(311)
The Greenrsquos function can hence be computed corresponding to the Schroumldinger
equation
22
2 0( ) ( ) ( )
2E G x x x x
m
dV
dx
(312)
Due to the delta-function at = a discontinuity is observed and hence the
Greens function is evaluated at boundary conditions
0
2
exp( ( )) x x 2 ( )( )
exp( ik(x x)) x x
ik x x m E VG x x k
A
A
(313)
By integrating the Schroumldinger equation twice and setting the lower and upper
integration boundaries to = -δ and = +δ the Greenrsquos Functions can be written as
2
( ) ( ) 0
( ) ( ) 2
x x x x
G x x G x x
dG x x dG x x m
dx dx
(314)
46
The coefficient A+ and A
- become
ik
mA A
(315)
The Greenrsquos Function takes a final form known as Retarded Greenrsquos Function and
is written as
( ) exp( | |)G x x i ik x xk
m (316)
And the wave function is
( ) ( ) ( )x dx G x x S x (317)
Retarded Greenrsquos Function propagates the wave functions generated by a source
or perturbation S from its origin at to any point
The retarded Greenrsquos Function as discretized Schroumldinger equation is written as
( )R RE H G I (318)
The wave function Φ can be calculated from the retarded Greenrsquos function and the
source vector as
Φ = GR∙S (319)
Overall in this section the Greenrsquos function approach in calculating the electron
dynamics is reviewed We defined the self-energy of each part of the system spectral
function and the probability current density the electric current is derived explicitly using
Non Equilibrium Greenrsquos function We will use this formalism to calculate the tunneling
phenomena in coupled quantum dots isolated or otherwise
47
CHAPTER 4
ATOMISTIX TOOLKIT DETAILS
41 Introduction
Virtual NanoLab (VNL) is a graphical user interface (GUI) that provides a group of
modeling tools the function of these tools involves the set-up investigation and the
study of nanoscale structures The quantum mechanical equations are solved by the
software by using the advanced software architecture and numerical methods to
implement ab initio calculations VNL simulates the electronic structure and calculates
the transport properties based on the two systems mentioned earlier NEGF and Extended
Huckel ATK is the main engine for computing the scripts and hence all the calculations
performed in VNL are done by ATK VNL is a user friendly software as it not only
allows creating a script but also helps to set up a virtual experiment
This thesis involves the use of VNL in order to study the effect of the width and
different orientations of the doped atoms Since the software allows for virtual
experiments it makes it much easier to study the I-V characteristics based on the change
in position of atoms
42 Device Structure
In this thesis AZA GNR p-n junction with boron doping (location) was created using the
ATK software which is based on NEGF and DFT Further the thesis discusses the
transport properties and the I-V curve of such junction
The input format of ATK is NanoLanguage which is an extension to Python
scripting language ATK uses the NEGF system for formalism of simulating device
48
Figure 41 Geometry of device configuration with two electrodes
37
The system is divided into three parts left central and right The implementation
relies on the screening approximation which assumes that the properties of the left and
right regions can be decribed by solving a bulk problem for fully periodic electrode cell37
This screening approximation is fulfilled when the electrode regions can be described by
an equilibrium electron distribution
Figure 42 The electron distribution in a device configuration which illustrates a left
moving scattering state with origin in right electrode37
The system assumes that in steady state the electron density of the central region
is constant in time and hence the electron density is calculated independently from each
electrode The electron density is given by the occupied eigenstates of the system
n(r) = nL(r) + n
R(r) (41)
49
The left and right densities are calculated by summing up the occupied scattering
states
nL(r) = sum
(42)
nR(r) = sum
(43)
The scattering states are usually calculated by first calculating the Bloch states in
the electrodes and then solving the Schroumldinger equation of the central region using the
Bloch state as matching boundary Instead of using the scattering states the ATK
software uses the NEGF method to calculate the non-equilibrium electron density
The electron density is given in terms of electron density matrix
D = DL + D
R (44)
The left density matrix is given by NEGF theory
DL = int
(45)
where
ρL(ɛ) =
(46)
ρL(ɛ) = is the special density matrix
Also if there is a non-equilibrium electron distribution in the central region then
the electron distribution in electrode is given by the Fermi function f with an electron
temperature TL
G(ɛ) =
(47)
G = retarded Green function
δ+ is an infinitesimal positive number and S H overlap the Hamiltonian matrices
L =
sum sum
(48)
50
L
is the broadening function of the left electrode given in terms of left electrode
self -energysum
43 Transmission Spectrum Calculations
Once the self-consistent non-equilibrium density matrix has been obtained the various
transport properties of the system can be calculated One of the most important properties
is the transmission spectrum from which the current and differential conductance can be
obtained
The transmission coefficient in ATK is obtained by the retarded Greens function
T(ɛ) = G(ɛ)ΓL(ɛ)G
ϯ(ɛ)Γ
R(ɛ) (49)
The transmission amplitude of individual scattering states may be obtained
through the Transmission Eigenvalues The ldquoTransmission Eigenvaluesrdquo is an analysis
which finds the eigenvalues of the transmission matrix
The transmission matrix at energy E and k-point is given by
Tnm(Ek) = sum (410)
where
= transmission amplitude from Bloch state ψn(k)
The transmission coefficient is given by the trace of transmission matrix
T(Ek) = sum (411)
Keeping in mind all quantities depend on the quantum numbers parametrically
Transmission eigenvalues sum up to the transmission coefficient
T = sum (412)
51
44 Calculating the Current
Current is calculated from the transmission coefficient using
I( ) ( )R L
L RL R
R LB B
eE f f dE
h
E EV V T T T
k kT T
(413)
where f is the Fermi function TRL is the electron temperature of the right or left
electrode and Tσ(E) is the transmission coefficient for the spin component σ
The chemical potentials of the left and right electrode given by
L
F R LR L
eVE
are defined relative to the Fermi level of the left electrode These chemical potential are
related to the applied bias and hencebiasR L
eV therefore bias L RV V V
The transmission spectrum itself is usually rather insensitive to temperature and is
used in self-consistent calculations but often depends strongly on the electrode voltages
Thus for an accurate estimate of the current the transmission spectrum should be
calculated self-consistently for each desired bias
ATK uses very precise method to calculate the transport properties of the system
Transmission spectra for various concentrations of boron doped graphene p-n junctions
are generated in this Chapter and various coefficients such as Seebeck Peltier and
Conductance are calculated
52
45 Calculating Transport coefficients
The linear response transport coefficient of an applied voltage difference or temperature
difference between the two electrodes is given by
Conductance
| dT 0
e
dI
dUG
(414)
Peltier coefficient
| d 0
Q
I
I
(415)
Seebeck coefficient
| 0
dUS I
dT T
(416)
These linear response coefficients are calculated by the Transport Coefficients To
perform these calculations the ATK uses the Electron Transmission Spectrum
53
CHAPTER 5
RESULTS AND DISCUSSION
51 Band Structure Analysis
The electronic bandstructure of GNR both doped and undoped are discussed in this
chapter
The armchair configuration of Pristine GNR (PGNR) has a band structure that is
dependent on its width This is explained by the fact that the sheet itself acts like a
potential well where the electrons are confined to form standing waves along Cr the
rolling vector albeit with slightly different boundary conditions (Cr = ma1 + na2
where m and n are integers and a1 and a2 are the unit cell vectors of graphene lattice) In
a GNR the two nodal points of the standing wave must be at the ribbon edge while in a
Single wall nanotube (SWNT) they can be anywhere ie a circumferential periodic
boundary condition
(a) (b)
Figure 51 Bandstructure of AGNR widths (a) 4 atoms (b) 5 atoms
54
(a) (b)
Figure 52 Bandstructure of AGNR widths (a) 6 atoms (b) 7 atoms
(a) (b)
Figure 53 Bandstructure of AGNR widths (a) 8 atoms (b) 9 atoms
55
(a) (b)
Figure 54 Bandstructure of AGNR widths (a) 10 atoms (b) 11 atoms
Figure 55 Bandstructure of AGNR with a width of 12 atoms
Figure 56 Variation in band gaps as the width (number of atoms) varies
0
05
1
15
2
25
0 2 4 6 8 10 12 14
Wdith vs Band Structure
eV
56
The band structure of 12 Atom AGNR is close to that of Ge (0626 eV) The
actual width of this nanoribbon is about 25 nm 12 AGNR has been fabricated
successfully and doped with various dopants Hence the 12 Atom AGNR has been chosen
to study the transport properties
A junction is created using ZGNR and AGNR To maintain the consistency in the
device analysis it is imperative that the band structure of ZGNR is also calculated From
the simulation it is evident that ZGNR-AGNR-ZGNR junction configuration displays the
Metal ndashSemiconductor-Metal configuration that is addressed in this work The Fermi
Level in all the Z-GNR nanoribbons of widths 4-12 lies within the conduction band
Figure 57 Band structure of ZGNR width (a) 4 atoms (b) 6 atoms
57
(a) (b)
Figure 58 Band structure of ZGNR width (a) 8 atoms and (b) 10 atoms
Figure 59 Band structure of ZGNR with a width of 12 atoms
In order to create viable junction that would show transistor properties doping of
the semiconductor part is necessary The 12 atom AGNR is doped with boron (p-type)
and nitrogen (n-type) - (Figure 510a) 4 N doped (Figure 510b) 4 B In both cases
the impurities lie on the edge of the atoms For 2 nitrogen doped GNR with the
58
impurities lying in the center of the ribbon the Fermi level is found to be in the
conduction band as shown in (Figure 510c) (Figure 510d) shows the position of N with
respect to the edge A very clear departure from the expected (the valence band extending
above Fermi level) is shown in (Figure 510a)
Figure 510 Band structures of Doped AGNR (a) 4 N Doped (b) 4 B Doped (c) 2
N Doped (d) position of Nitrogen from (c)
(a) (b)
(c) (d)
59
52 I-V Characteristics of GNR junction
In pristine graphene the chirality determines the conductivity as seen from the I-V curves
for various widths At certain widths the semiconducting properties are more
pronounced These widths determine the wavelengths of the standing waves which in
turn determine the sub-band locations in the E-k plot When the biasing potential
exceeds 012V the I-V curve shows linearity In case of the 8-atom wide PGNR the
band gap is about 03 eV and it is evident from the I-V plot that the On-State is + 033 V
The band gap of 10-atom and the 4-atom wide PGNR is large enough to show
semiconducting properties
Figure 511 Current Vs Voltage graph for varying graphene width showing
conductivity
-30000
-20000
-10000
0
10000
20000
30000
-3 -2 -1 0 1 2 3
Cu
rre
nt
(nA
)
Voltage (V) (bias)
Current (nA) Vs Voltage for varying graphene width
W=10
W=8
W=6
W=4
60
The ZAZ GNR Configurations show the properties of a semiconductor junction The 12
atom ZAZ structure is studied for its I-V characteristics In this Chapter undoped B-
doped N-Doped B and N Doped (P-N Junction) ZAZ junctions are simulated
Figure 512 ZAZ GNR junction device
61
The boron doped ZAZ junction I-V characteristics are shown below (Figure 513)
The impurity concentration is 2 and 4 Various device configurations are studied
Figure 513 I-V curve of Boron Doped ZAZ junction
-25000
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
25000
-205 -155 -105 -055 -005 045 095 145 195
Cu
rre
nt
(nA
)
VBias
2B_1G_R 2B_0G_R
4B_0G_L 4B_0G_C
4B_0G_R 4B_1G_L
4B_1G_C 4B_1G_R
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
-2 -1 0 1 2
Cu
ren
t(n
A)
VBias
4 B doped GNR Jn
62
Figure 514 I-V curve of Nitrogen Doped ZAZ
-25000
-20000
-15000
-10000
-5000
0
5000
10000
15000
20000
-2 -15 -1 -05 0 05 1 15 2
Cu
rre
nt(
nA
)
VBias
I-V Curve as function of Dopant location
2N_0G_L2N_0G_C2N_0G_R2N_1G2N_1G_C2N_1G_R
-15000
-10000
-5000
0
5000
10000
15000
-2 -1 0 1 2
Cu
rre
nt(
nA
)
VBias
2N_0G_C
2N_1G_C
63
Figure 513 and Figure 514 show the I-V characteristics of the GNR junction doped with
2 boron and nitrogen respectively The location of N and B is at the central region of
the edge of the GNR Both B doped and N doped GNR Junctions show significant
Negative Differential Resistance (NDR) This is more pronounced in case of nitrogen
doping Another interesting observation is increasing ohmic nature with the change in
location of the dopants Nitrogen doped device configuration exhibits a pronounced
semiconductor behavior and the NDR effect is observed to be minimal
53 Thermoelectric Properties
In this study the thermoelectric properties were simulated for the GNR Junctions that
displayed high NDR effect The variation in the Peltier coefficient with temperature is
shown as function of doping
When the concentration of nitrogen increases the dimensionless Figure of Merit
ZT seems to decrease considerably This is mostly explained by the decrease in both
conductivity and mobility of the electrons
ZT = S2σTk (51)
where S is the Seebeck coefficient σ is the electrical conductivity T is the
absolute temperature and k is the thermal conductivity
64
Figure 515 Variation of Peltier coefficient with temperature as function of
doping
Figure 515 shows the maximum Peltier coefficient for 2 boron This is
explained by the scattering by boron and the associated smallest mean free path
0
0001
0002
0003
0004
0005
0006
0007
0008
0009
001
250 270 290 310 330 350 370 390 410
ZT
T (K)
2B
4B
Undoped
2N
4N
65
CHAPTER 6
CONCLUSIONS
Graphene ZAZ junctions exhibit varying properties depending on the various structural
configurations In this thesis it was found that the transport properties of graphene
depend on their width the edge of GNR doping concentration and the type of dopant
used The calculations of the band structure contributed towards the determination of the
minimum length of GNR required for studying the transport properties The minimum
length had a band gap equivalent to that of germanium and hence the importance of the
width being 12 atoms wide This band gap indicated fluctuating changes when doped
with elements such as B and N The viable junction showing transistor properties was
hence created by doping the semiconductor part of ZAZ By doping the I-V
characteristics were studied which showed significant NDR which was more pronounced
in the case of nitrogen Also the changing positions of the dopants contributed towards
the I-V curve to be more ohmic The edge doping caused minimum NDR and
semiconductor behavior as compared to central doping Lastly the thermoelectric
properties were studied - the increasing concentration of N causes the Figure of Merit to
decline due to the decrease in conductivity as well as mobility of electrons
66
REFERENCES
1 Wikianswers What makes carbon unique
httpwikianswerscomQWhat_makes_carbon_so_unique (22 November)
2 Kopeliovich D D Graphite
httpwwwsubstechcomdokuwikidokuphpid=graphite (1128)
3 Barbier M Transport properties of nanostructures and superlattices on single layer and
bilayer graphene University Antwerpen Antwerpen 2012
4 Shylau A Electron transport interaction and spin in graphene and graphene
nanoribbons Linkoping Norrkoping 2012
5 HassJ R F T Li X Li Z Zong W A de Heer P N First E H Conrad C
AJeffrey and C Berger Applied Physics Letters 2006 89 (14) 143
6 Jones A Mechanical Exfoliation to Make Graphene and Visulization
httpcarbonchemwisceduFilesMechanicalExfoliationpdf (18 October)
7 Anteroinen J Structural and Electrical Characteristics of Graphene Field Effect
Transistors AALRO school of Electrical Engineering AALTO 2011
8 Novoselov K S A K G S V MorozovD JiangY Zhang S V Dubonos I V
Grigorieva A A Firsov Science 2004 306 (22)
9 Kosynkin D A L H A Sinitskii J R Lomeda A Dimiev K B Price and J M
Tour Nature 458 876
10 Yi Z Luyao Zhang Accounts of chemical research 46 (10) 2339
11 Eizenberg M B JM 1979 82 236
12 Yu Q K L J Siriponglert S Li H Chen Y P Pei S S Applied Physcis
Letters 2008 93 (113103)
13 Li X C W An J Kim S Nah J Yang D Piner R Velamakanni A Jung I
TutucE Banerjee S K Colombo L Ruoff R S Science 2009 324 1314
14 Schaefer H E Nanoscience Springer Berlin 2010
15 Levente Tapasztoacute G D Philippe Lambin amp Laacuteszloacute P Biroacute Nature Nanotechnology
2008 3 401
67
REFERENCES
16 Dacheng Wei Y L Advance Materials 2010 22 (30) 3241
17 Wei Yao K L Y GYGao Elsevier Solid State Communications 2013 153 52
18 Dacheng Wei Dagger Yunqi Liudagger Yu Wangdagger Hongliang ZhangdaggerDagger Liping HuangdaggerDagger
Yudagger a G NanoLetters 2009 9 (5) 1758
19 Nakada K M F G Dresselhaus and M S Dresselhaus PhysRevB 1996 54
(9858)
20 Son Y W C M L a L S G PhysRevLett 2006 97 (216803)
21 Raza H Graphene Nanoelectronics Springer 2012
22 Ryan W J Electronic Transport in Graphene p-n junctions Short Noise and
Nanoribbons Harvard University 2009
23 Fangping OuYang J X Rui Guo Hua Zhang and Hui Xu Nanotechnology 2009
20 6
24 Guo J Carbon nanotube electronicsModeling physics and applications Purdue
University West Lafayette IN 2005
25 Motta C S S-P MITrioni cond-matmes-hall 2012 7
26 B P Growing Graphene via Chemical Vapor Deposition Ponoma College Ponoma
2011
27 ZurichE Transport properties of three-terminal graphene devices University of
Science and Technology Norway 2008
28 Uichiro MIntroduction to the electron theory of metals
29 Robert Laughlin H S Additional background material on the Nobel Prize in Physics
1998 (410)
30 MarkGoerbig Quantum Hall Effects (11152013)
68
REFERENCES
31 Zurich E Transport properties of three-terminal graphene devices Norwegian
University of Science and Technology Norway 2008
32 Deepak R Klein Tunneling University og Tennessee Space Institute Tennessee
2011
33 Williams JR L D CMMarcus Quantum Hall Effect in a Gate-Controlled p-n
Junction in Graphene (1122013)
34 Avadhanulu MN P G K A Textbook of Engineering Physcis for BE BSc (Engg)
SChand New Delhi 1992
35 Andriotis A Applied Physics Letters 2007 91 (152105)
36 Qimin Yan B H dagger Jie Yudagger Fawei Zhengdagger Ji ZangDagger Jian Wudagger Bing-Lin Gu F
L Dagger and Wenhui Duandagger NanoLetters 2007 7 (6) 1473
37 Soler J M E A J D Gale A Garciacutea J Junquera P Ordejoacuten and D Saacutenchez-
Portal J Phys Condens Matter 2002 14 2745
ix
LIST OF FIGURES
(Continued)
Figure Page
22 Bandstructure of a graphene sheet showing a band gap of 0eVhelliphelliphellip 18
23 Band structure of Graphene calculated with the tight-binding modelhellip 19
24 The energy dispersion around the K pointhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 22
25 Electrons colliding with stationary ionshelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 23
26 (a) 2D electrons in a perpendicular magnetic field Logitudinal resistance
measured across C5 and C6 Transverse resistance measured across C3
and C5 (b) Classical Hall resistance as a function on the magnetic field
25
27 Klein tunneling through an npn barrierhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 29
28 Electron trajectory considering the linear electrostatic potential U(x) = Fx 30
29 Electron like and hole like trajectories at same Ehelliphelliphelliphelliphelliphelliphelliphelliphellip 30
210 Quantum Hall effect in graphene 22
The Hall conductivity σxy and the
longitudinal resistivity of monolayer graphene as a function of carrier
density at B = 14T and T= 4K This shows half-integer QHE with chiral
index J= 1helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
32
211 (a) LL for Graphene bilayer (b) Schematics of Hall conductivity as a
function of nn0 for bilayer Graphene (solid line) and monolayer
Graphene (dotted line) (c) LL for monolayer Graphenehelliphelliphelliphelliphelliphelliphellip
33
212 Seebeck Effecthelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 35
213 Transmission functions in units of (2e2h) for AZA structureshelliphelliphelliphellip 37
214 I-V curve for a 591nm long channel (Vbias=20mV)helliphelliphelliphelliphelliphelliphelliphellip 38
31 NEGF systemhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 42
41 Geometry of device configuration with two electrodeshelliphelliphelliphelliphelliphelliphellip 48
42 The electron distribution in a device configuration which illustrates a left
moving scattering state with origin in right electrodehelliphelliphelliphelliphelliphelliphelliphellip
48
x
LIST OF FIGURES
(Continued)
Figure Page
51 Band structure of AGNR widths (a) 4 atoms (b) 5 atomshelliphelliphelliphelliphelliphellip
53
52 Band structures of AGNR widths (a) 6 atoms (b) 7 atomshelliphelliphelliphelliphelliphellip 54
53 Band structure of AGNR widths (a) 8 atoms (b) 9 atomshelliphelliphelliphelliphelliphelliphellip 54
54 Band structures of AGNR widths (a) 10 atoms (b) 11 atomshelliphelliphelliphelliphellip 55
55 Band structure of AGNR with a width of 12 atomshelliphelliphelliphelliphelliphelliphelliphelliphellip 55
56 Variation in band gaps as the width (number of atoms) varieshelliphelliphelliphellip 55
57 Band structure of ZGNR width (a) 4 atoms (b) 6 atomshelliphelliphelliphelliphelliphelliphellip 56
58 Band structure of ZGNR width (a) 8atoms and (b) 10 atoms 57
59 Band structure of ZGNR with a width 12 atomshelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 57
510 Band structures of Doped AGNR (a) 4 N Doped (b) 4 B Doped (c)
2 N Doped (d) position of Nitrogen from (c)helliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
58
511 Current Vs Voltage graph for varying graphene width showing
conductivityhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip
59
512 ZAZ GNR junction devicehelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 60
513 I-V curve of Boron Doped ZAZ junctionhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 61
514 I-V curve of Nitrogen Doped ZAZhelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphelliphellip 62
515 Variation of Peltier effect coefficient with temperature for various doping 64
1
CHAPTER 1
INTRODUCTION
11 Graphene The New Carbon
Carbon (chemical symbol C atomic mass 1207amu) (Figure 11a) is a widely distributed
element in nature It is found abundantly in the sun stars comets and the atmospheres of
the planet Carbon can form up to four bonds it can bond with itself endlessly and with
most other elements in many different shapes making it a significant part of the
construction for many kinds of complex molecules1
Two allotropes of carbon are commonly used diamond and graphite (Figure
11b) The bonding structures of diamond and graphite contribute to the properties
individually In diamond all the p-orbitals are used forming a sp3
bonding whereas in
graphite only two orbitals are occupied allowing the unpaired bond for the transport of
electrons Each carbon atom in graphene possesses sp2 hybridization ie each carbon
atom is connected to three other carbon atoms via covalent bonds with a bond length of
142Å and an angle of 120deg between each bonded pair This makes graphite a better
conductor than diamond Graphite consists of many layers of 2D carbon lattices (Figure
11c) stacked on top of each other and held via Van der Waals forces A single layer of
graphite where carbon atoms are arranged in a honeycomb lattice is known as graphene
(Figure 11c)
2
Figure 11 (a) Chemical representation of Carbon (b) Graphite ore (c) Structure of
Graphite and a single layer Graphene2
Theoretical work on graphene was done specifically to study the other allotropes
The first study was done by Wallace in 1947 who calculated the band structure of
graphene3 Further the peculiar Landau levels were known by McClure in 1957 and the
relativistic Hofstadter butterfly by Ramal in 19853 Later in 1991 the invention of carbon
nanotubes by Iijima boosted the theoretical research on graphene3 Prior to the invention
of carbon nanotubes there were a few experimental papers on graphene growth via
various methods like intercalation of graphite (Shioyama 2001) free standing (Boehm
1962) epitaxial as well as graphene grown on metals (Bommel 1975 Land 1992 Itoh
1991)3 With all the various discoveries the electronic properties of graphene were not
studied until 2004 when Berger and Novoselov were able to access the electronic
properties with contact of graphene flakes3 (Figure 12)
3
Figure 12 An optical image of Graphene flake obtained by exfoliation of graphite3
The specific lattice structure of graphene possesses a number of unique electronic
properties making it an interesting material for theorists experimentalists and engineers
Utilization of graphene as a fundamental block of electronic devices requires
development of new theoretical methods for understanding the current propagations in
graphene constriction4
12 Graphene Synthesis
The discovery of graphene by mechanical exfoliation called the lsquoScotch tape methodrsquo led
to serious attempts towards the production of top quality graphene5 Graphene was first
exfoliated mechanically from graphite in 20046 The importance of high quality graphene
cannot be emphasized enough however electron transport has shown that defects play an
important role in hindering the transport properties of electrons (holes)7 The two
synthesizing methods for the large scale manufacture of graphene are chemical vapor
deposition (CVD) and silicon carbide (SiC) desorption method
4
Graphene can be synthesized by sublimation of silicon from SiC at high
temperature (1200degC) in high vacuum5 The major advantage of this method is that the
SiC provides an insulating substrate and no transfer of the graphene layer is needed Yet
the disadvantage of this method outweighs its advantages the high temperature is cost-
ineffective making it unsuitable for large scale manufacturing8 Also the crystal growth
face alters the properties of graphene Graphene grown on Si-terminated face has poor
homogeneity and is subjected to unintentional doping7 Conversely graphene grown on
C-terminated SiC has higher mobility and is often called lsquoturbostaticrsquo due to the
rotational disorder7
Unlike the SiC method the graphene produced via CVD method needs to be
transferred to a substrate making it difficult to maintain the quality of graphene Yet
CVD synthesized graphene has a larger grain size7 More research is being done on
various methods for synthesis of graphene The methods include direct chemical
synthesis ion implantation crystal sonification and lastly unzipping carbon nanotubes to
form graphene sheets9
Graphene and few-layer graphene have been grown by CVD from carbon
containing gases on catalytic metal surfaces andby surface segregation of C dissolved in
the bulk of such metals7 Growing graphene with CVD is a very attractive solution since
it is compatible with the existing semiconductor industry9 Graphene has been grown via
CVD process on metal substrates such as Nickel (Ni) and Copper (Cu)
5
121 Synthesis of Graphene on Nickel (Ni)
Polycrystalline Ni films are annealed in ArH2 atmosphere at 900-1000degC to increase
grain size and are then exposed to H2CH4 gas mixture10
In this step the hydrocarbon
decomposes and dissolves in Ni to form a solid solution Lastly the samples are cooled in
argon gas Ni has high carbon solubility at elevated temperatures and the solubility
decreases as temperature is reduced During the cooling process the carbon atoms diffuse
out from the Ni-C solid solution and precipitate on the Ni surface to form graphene films
(Figure 13a) Since Ni (111) has a lattice similar to the densely packed hexagonal lattice
of graphene (Figure 13b) they also have similar lattice constants and hence Ni surface
serves as an excellent lattice matched substrate for graphene growth11
The growth of graphene on Ni is based on carbon segregation and precipitation
process different segregation behavior is produced by different cooling rates which
affect the thickness and quality of graphene films12
Medium cooling rates lead to optimal
carbon segregation and produce few layers12
Graphene films grown on Ni are usually
continuous with monolayer and few layer regions Annealing of Ni substrates at elevated
temperatures in hydrogen atmosphere not only increases the single-crystalline Ni grain
size but also eliminates certain impurities in Ni thereby improving the graphene quality
Furthermore the graphene thickness can also be affected due to the amount of carbon
dissolved in the Ni films during the growth time
After synthesis the graphene can be transferred to other insulator substrates for
further characterization and applications Figure 13c shows the selected area electron
diffraction pattern of graphene film along the [001] direction which confirms the
graphene lattice structure shown After transfer to insulator substrates the geometry can
6
be retained as shown in Figure 13d Under optimal growth parameters graphene growth
is only limited by the Ni catalyst Lastly Figures 13e and 13f show the wafer-scale
graphene synthesis and transfer of graphene to a flexible transparent substrate
respectively
Though polycrystalline Ni is a good substrate the percentage and size of
graphene monolayer are still limited Researchers have hence tried other metal substrates
for graphene synthesis
7
Figure 13 (a) Graphene formation on Nickel (b) Graphene atoms on Ni (111) lattice
(c) Low magnification TEM image of graphene edges (d) Optical image of graphene
transferred from the Ni surface to SiO2Si substrate (e) Full-wafer scale deposition of
graphene layers on polycrystalline Ni (f) Transparent and flexible graphene films on
PDMS substrate10
8
122 Synthesis of Graphene on Copper (Cu)
Graphene films are grown on 25microm thick Cu foils in a hot wall furnace13
The Cu foil is
first annealed in hydrogen atmosphere at 1000degC and a mixture of H2CH4 is introduced
into the system to initiate graphene growth After a continuous graphene layer is formed
on the Cu foil the system is cooled to room temperature Figure 14a shows an SEM
image of graphene on Cu substrate indicating the Cu grains with contrast The Cu
surface steps are formed during thermal annealing and the darker flakes indicate multiple-
layer graphene (Figure 14b)10
The graphene wrinkles in Figure 14(b) originate from
different thermal expansion coefficient of graphene and Cu They go across the Cu grain
boundaries indicating that the graphene film is continuous
Figure 14 (a) SEM image of graphene on copper foil (b) High-resolution SEM image of
graphene on Cu10
123 Transfer of Graphene films
In order to facilitate the applications of graphene for electronic applications we need to
separate the graphene from the catalytic metal substrate Figure 15a shows the transfer
process of graphene Graphene is first coated with a thin layer of polymethyl
methacrylate (PMMA) and baked at 120degC to evaporate the solvent10
The metal layer is
then removed by Ni or Cu etchant leaving behind the PMMA graphene film The film is
then cleaned by deionized water and then transferred onto the target substrate After the
9
evaporation of water vapor the PMMA is removed by acetone leaving graphene film on
top of the target substrate Figure 15b shows a graphene wafer transferred from the
substrate onto glass and polyethylene terephthalate (PET) films
Figure 15 (a) Transfer process (b) Wafer-scale synthesis of graphene (c) Graphene
films transferred onto glass wafer (d) SiSiO2 with device patterned (e) PET film10
124 Synthesis of Graphene Junction
Graphene junctions with smooth armchair and zigzag edges are difficult to produce by
conventional methods such as mechanical exfoliation chemical exfoliation or lithography
etching14
The conventional methods can only produce rough edges Recently
Dresselhaus reported an edge reconstruction of graphene by Joule heating in a TEM-STM
10
(Figure16b) system15
An individual nanoribbon sample is attached to the sample holder
at one end and to the STM tip at the other end these ends also serve as the two
electrodes The structural transformation in the growth of graphene from armchair to zig-
zag is mainly attributed to the vaporization of carbon edges that reconstruct at high
temperatures in which resistive Joule heating and preferred current flow play an
important role This means that by controlling the flow of current a perfectly smooth
edged ribbon can be synthesized making graphene-based electronics possible16
Figure 16 (a) High-magnification image of the annealed sample showing that well-
defined zigzag armchair and zigzag-zigzag edges are formed (b) STM image of an 8 nm
wide bent junction connecting an armchair and a zigzag graphene nanoribbon which was
carved by STM tips14
125 Doping in Graphene
The doping of graphene can be roughly classified into two categories - electrical and
chemical Electrical doping involves changing gate voltages of graphene devices and
chemical doping uses chemical routes such as substitutional or interstitial This thesis
discusses chemical doping and the importance of doping sites by changing the dopant
Chemical doping is a common approach to tailor the electronic properties of
11
semiconductors Doping of graphene can cause its electronic properties to alter leading to
a metal-semiconductor transition The two means of doping graphene are interstitial and
substitutional In interstitial doping the dopant atoms or molecules are introduced as
adatoms or admolecules on the surface of graphene whereas in substitutional doping the
dopant atoms are replaced in the carbon lattice forming a bond in the lattice of
graphene16
Doping graphene results in the formation of n or p-type semiconductors
depending on the kind of dopant If the dopant is an electron donor it causes the Fermi
level to shift up resulting in n-type behavior of graphene Furthermore if the dopant is an
electron acceptor it causes the Fermi level to shift down resulting in a p-type behavior of
graphene (Figure 17)16
Figure 17 Band structure of graphene before and after doping The image shows shift
towards the Fermi level16
Graphene nanoribbons (GNR) can be made into a p- and n- type semiconductor
by doping with boron (B) and nitrogen (N) respectively In theory GNR p-n junction is
formed by doping GNR with B and N in different regions However experimentally
doping graphene with both these elements is very difficult due to the dopants reacting
with each other17
Hence most experimental studies use GNR doped by only one
12
element N-doped graphene was synthesized by Wei et al Wang and B-doped Graphene
was realized by Endo17
Many researchers have demonstrated interstitial doping of graphene by gas metal
and organic molecules16
The various gases and metals used are NO2 NH3 An-CH3 Na-
NH2 F4-TCNQ TPa TCNE and others16
Doping in graphene is hence possible by
electrons or holes in high concentration without deterioration of its mobility Interstitial
doping is highly sensitive due to most of the conducting channel being exposed to surface
absorbates and hence can be used in molecule detection
In substitutional doping the dopant atoms are included in the graphene lattice and
thus chemically bonded Substitutional doping is done via the CVD method using a
carbon and dopant source Substitutional doping opens up many applications in device
engineering making graphene a very good candidate as a semiconductor This study
involves the study of transport properties of graphene doped by substitution
126 Nitrogen (N) Doped Graphene Synthesis (Substitutional)
N-Doped graphene is prepared via a CVD process using a 25microm thick Cu film on a Si
substrate The substrate is placed in a quartz tube with the flow of hydrogen (20sccm) and
argon (100 sccm)18
When the center of the furnace reaches 800degC 60 sccm of CH4 and
60 sccm of NH3 is introduced into the flow as C source and N source respectively The
substrate is then moved to high temperature and after 10 min growth the sample is
cooled to room temperature under H2 ambient Figure 1 8 shows the growth of N-doped
graphene18
13
Figure 18 Low resolution TEM image of N-doped graphene Background is the lacey
carbon TEM grid graphene sheet is crumpled with many ripples18
13 Structure of Graphene Nanoribbon (GNR)
Graphene Nanoribbons (GNR) are strips of graphene with very thin width of lt50nm
GNRs can be terminated in three separate ways called zig-zag (0 n) armchair (m 0) and
chiral (m n) (Figure19) and this termination along the width of the ribbon dictates the
size of the band gap19
Figure 19 Zigzag and Armchair orientation of Graphene5
Due to their various edge structures GNRs exhibit different electronic properties
ranging from normal semiconductors to spin-polarized half metals which open the
possibility of GNRs as electronic devices19
14
Within a tight binding approach (AGNRs) could be metallic or semiconducting
depending on their ribbon width but all zigzag graphene nanoribbons (ZGNRs) are
metallic with a high density of electronic states at the edges Hence ZGNRs exhibit
characteristic edge effects which are not present in AGNRs These edge effects in
ZGNR create a flat band close to the Fermi level making the ZGNR edges more
reactive19
First-principles calculations show that the GNRs possess a non-zero direct
band gaps These gaps are small for ZGNR (Figure 110) caused due to spin ordering
effects at the edges For AGNRs the band gap arises from quantum confinement (Figure
111) effect that has larger magnitudes than ZGNR20
Figure 110 Band structure of ZGNR
15
Figure 111 Band structure of AGNR
For GNRs the band gap decreases as the ribbon width increases and in order to
create a semiconductor with a desirable band gap the nanoribbon width should be
adjusted accordingly This property of adjusting the band gap makes graphene an
excellent candidate for transistor switching By applying an electric field GNR can be
altered from an insulator to a conductor GNRs exhibit very intriguing properties and
have become one of the promising candidates for electronic applications
14 Overview of Graphene Junction
The invention of p-n junctions date back to 1940s which later resulted in the invention of
junction transistors One of the key technological reasons for success of the p-n junction
is mainly due to its ability to locally modulate the energy band gaps via an applied bias21
A graphene p-n junction is created via single layer of graphene in which the
carrier type and density in two adjacent regions are controlled by electrostatic gating8
For materials with a band gap the electric field can either switch lsquooffrsquo the current or
rectify it (p-n diode)22
Being a ldquogaplessrdquo material the off state is not achievable in
16
graphene In order to achieve an off state the gap can be created by doping graphene with
various elements (Group III or Group V) Doping allows p-n junctions to be
reconfigurable using a gate voltage to distinguish between graphene p- n regions within a
single sheet Many researchers have studied the electronic as well as transport properties
of doped graphene junctions
In 2009 Fangping OuYang studied the transport properties of T-shaped graphene
junctions using the ATK software and showed that the conductance depends on
geometric structures which can be controlled by selective doping23
Wei Yao in 2013
studied the transport properties in graphene p-n junctions and showed that the
rectification effect depends on boron doping density and position17
The study of transport properties in graphene p-n junctions is a recent
advancement The thesis discusses transport properties including the current-voltage (I-
V) characteristics of doped graphene junctions Moreover the software used is similar to
the software in use by current researchers since they have produced viable data using
ATK
17
CHAPTER 2
RESEARCH BACKGROUND
21 Band Structure of Graphene
The unique electronic properties of graphene were first predicted in 1946 Figure 21
shows a top view of the hexagonal arrangement of carbon atoms in real space as well as
the first Brillouin zone in reciprocal space
Figure 21 Left Real space graphene lattice with basis vectors and Right The
first Brillouin zone of graphene in reciprocal space with basis vectors and
K and
Krsquo are responsible for massless transport at low energy24
The real space basis vectors are radic
and
radic
The reciprocal space basis vectors are 1 2
0 0
4 1 3 4 1 3( )and ( )2 2 2 23 3
b x y b x ya a
where the magnitude of the basis vectors is |a0| = radic acc The distance between nearest
neighbor carbon atoms is acc=0142nm
18
The band structure can be calculated by solving the eigenvalues using the
dispersion relation E( )
1 2 3( ) 3 2cos 2cos 2cosE k t k a k a k a (21)
Transport properties of solids are closely related to the energy dispersion
relations E ( ) in the material and in particular to the behavior of E ( ) near the Fermi
level Graphene is a zero gap semimetal whose specific linear electronic band dispersion
near the Brillouin zone corners (Dirac points) gives rise to electrons and holes that
propagate as massless Fermions25
The valence and conduction bands do not overlap in
graphene they touch at the Fermi Level (Figure 22)
Figure 22 Band structure of a graphene sheet showing a band gap of 0eV
The low energy properties of graphene can be well described by making a linear
expansion of the band structure around the K and Krsquo This energy can be written as
19
E(k) = plusmnħvF|k (22)
where vF is the Fermi velocity of 1106ms given by
1F
Ev
k
ħ (23)
Figure 23 Band structure of graphene calculated with the tight-binding model
22
The Fermi surface of graphene consists of double cones with Fermi energy at the
intersection of these cones (Figure 23) The slope of the band is zero and hence the
effective mass of electrons in that region is zero which leads to an entirely new transport
mechanism in graphene26
20
22 Transport Characteristics of Graphene
Transport process usually involves a flow of charge or energy or both The flow is mainly
due to external perturbations such as electric field and temperature gradient The
relationship between forces and flow usually defines various transport coefficients that
are the characteristics of electrons and phonons in the material All modern electronics
are based on the ability to control the electronic properties of a material by applying
external voltage This is done by an electric field effect where the gate voltage changes
the carrier concentration of the material and consequently its conductivity The electric
field effect in graphene was reported by Novoselov in 2004 and is used in transport
measurements8
The electron-phonon interaction in graphene plays an important role in
understanding the photoemission spectra observed in graphene The electric field effect is
an alternative method for changing the charge carrier density in low dimensional systems
The electric field effect in graphene which was first reported by Novoselov et al in
2004 is widely used as a characterization tool in transport measurements25
The transport characteristics of the material are directly related to the
bandstructure of graphene The carriers in graphene lattice are free to move in two
dimensions In the carrier transport of graphene the carriers ndash electrons and holes ndash close
to the Dirac points are of importance The transport is described by a two component
wave function (Equation 24) which obeys the 2D Dirac-like equation for massless
particles27
21
-ivFσ nablaψ(r) = Eψ(r)
(24)
where σ is the 2D Pauli spin matrix In the continuum limit the above (Equation
24) corresponds to the effective low energy Dirac Hamiltonian (Equation 25)
0( )
0
x y
F F
x y
iH k k
i
k kv v
k k
(25)
The electronic band structure of the energy (E) versus wave vector (k) relation for
graphene is given by Equation 24
The two component wave function resembles the spin or wave function of
quantum electro dynamics (QED)27
Corresponding to the spin of particles in QED the
charge carriers of graphene can be attributed with a pseudospin σ The pseudospin is the
direct result of two different carbon sublattices corresponding to the bonding and
antibonding combinations27
22
Figure 24 The energy dispersion around the K point27
In Figure 24 the red and blue lines correspond to the antibonding and bonding
states respectively The pseudospin can have two values either in the direction of or
against the momentum It can be seen that the electrons with energy E travelling in the
positive direction originates from the same branch as a hole with energy ndashE travelling in
the negative direction giving it the same pseudospin This results in suppressed
backscattering and Klein tunneling The back scattering process requires the pseudospin
to flip which is possible in the presence of short range scatters that act differently on sub
lattices27
23 Drude Theory
The classical theory of metallic conductivity was presented by Drude in 1900 and was
elaborated by Lorentz in 190528
Drude treated the free electrons as classical ideal gas
meaning the electrons collide with stationary ions and not each other
23
Figure 25 Electrons colliding with stationary ions28
The Drude theory applied the kinetic theory of gases to a metal considered as a gas of
electrons The basic assumptions made by the Drude theory are28
When metallic elements are brought together to form a solid then the valence
electrons become freely moving through the metal whereas the ions remain intact
as nearly immobile positive particles
Between collisions the electrons move freely ie there is neither electron-
electron interaction nor electron-ion interaction
The scattering mechanism leads to instantaneous collisions of the electron with
the scatterers
The collisions are characterized by a relaxation time τ
The elect